#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103506.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103506
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.5 La3 Nb0.5 O14'
_chemical_formula_weight         1070.65
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   7.991
_cell_length_b                   7.991
_cell_length_c                   5.037
_cell_measurement_temperature    293(2)
_cell_volume                     278.5
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         11.7E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.938
_diffrn_measured_fraction_theta_max 0.938
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0537
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            506
_diffrn_reflns_theta_full        22.99
_diffrn_reflns_theta_max         22.99
_diffrn_reflns_theta_min         3.19
_exptl_absorpt_coefficient_mu    14.491
_exptl_crystal_density_diffrn    6.383
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             474
_refine_diff_density_max         1.579
_refine_diff_density_min         -1.865
_refine_diff_density_rms         0.448
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.10(9)
_refine_ls_extinction_coef       0.025(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.991
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         506
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.991
_refine_ls_R_factor_all          0.0383
_refine_ls_R_factor_gt           0.0383
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1157
_refine_ls_wR_factor_ref         0.1157
_reflns_number_gt                506
_reflns_number_total             506
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-11.7d3.cif
_cod_data_source_block           11.7d3
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis
;
_cod_original_formula_sum        'Ga5.50 La3 Nb0.50 O14'
_cod_database_code               2103506
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.43306(11) 0.0000 0.0000 0.0133(3) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0163(6) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4769(4) 0.0127(5) Uani 1 3 d S
Ga3 Ga -0.7679(2) 0.0000 -0.5000 0.0134(4) Uani 1 2 d S
Nb Nb 0.0000 0.0000 0.0000 0.0163(6) Uani 0.50 6 d SP
O1 O -0.3333 0.3333 0.169(3) 0.015(2) Uani 1 3 d S
O3 O -0.1493(17) 0.0698(19) 0.239(2) 0.046(4) Uani 1 1 d .
O2 O -0.5470(16) 0.1485(18) -0.310(2) 0.052(4) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -0.9600 2.8600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2400 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 66.3(5) 6 .
O3 La O2 140.2(4) 6 6
O3 La O2 106.3(5) . 6
O3 La O2 106.3(5) 6 .
O3 La O2 140.2(4) . .
O2 La O2 102.4(6) 6 .
O3 La O1 79.6(3) 6 2_455
O3 La O1 122.4(3) . 2_455
O2 La O1 72.2(4) 6 2_455
O2 La O1 92.3(4) . 2_455
O3 La O1 122.4(3) 6 .
O3 La O1 79.6(3) . .
O2 La O1 92.3(4) 6 .
O2 La O1 72.2(4) . .
O1 La O1 155.45(6) 2_455 .
O3 La O2 79.4(4) 6 5_445
O3 La O2 63.8(4) . 5_445
O2 La O2 63.6(5) 6 5_445
O2 La O2 155.9(2) . 5_445
O1 La O2 65.3(4) 2_455 5_445
O1 La O2 125.2(4) . 5_445
O3 La O2 63.8(4) 6 3_565
O3 La O2 79.4(4) . 3_565
O2 La O2 155.9(2) 6 3_565
O2 La O2 63.6(5) . 3_565
O1 La O2 125.2(4) 2_455 3_565
O1 La O2 65.3(4) . 3_565
O2 La O2 136.1(4) 5_445 3_565
O3 La Ga2 110.8(4) 6 .
O3 La Ga2 84.8(4) . .
O2 La Ga2 31.1(3) 6 .
O2 La Ga2 131.1(3) . .
O1 La Ga2 65.2(3) 2_455 .
O1 La Ga2 110.6(3) . .
O2 La Ga2 32.5(2) 5_445 .
O2 La Ga2 164.2(2) 3_565 .
O3 La Ga2 84.8(4) 6 2_565
O3 La Ga2 110.8(4) . 2_565
O2 La Ga2 131.1(3) 6 2_565
O2 La Ga2 31.1(3) . 2_565
O1 La Ga2 110.6(3) 2_455 2_565
O1 La Ga2 65.2(3) . 2_565
O2 La Ga2 164.2(2) 5_445 2_565
O2 La Ga2 32.5(2) 3_565 2_565
Ga2 La Ga2 161.75(3) . 2_565
O3 La Nb 33.2(2) 6 .
O3 La Nb 33.2(2) . .
O2 La Nb 128.8(3) 6 .
O2 La Nb 128.8(3) . .
O1 La Nb 102.27(3) 2_455 .
O1 La Nb 102.27(3) . .
O2 La Nb 68.0(2) 5_445 .
O2 La Nb 68.0(2) 3_565 .
Ga2 La Nb 99.124(15) . .
Ga2 La Nb 99.125(15) 2_565 .
O3 La Ga1 33.2(2) 6 .
O3 La Ga1 33.2(2) . .
O2 La Ga1 128.8(3) 6 .
O2 La Ga1 128.8(3) . .
O1 La Ga1 102.27(3) 2_455 .
O1 La Ga1 102.27(3) . .
O2 La Ga1 68.0(2) 5_445 .
O2 La Ga1 68.0(2) 3_565 .
Ga2 La Ga1 99.124(15) . .
Ga2 La Ga1 99.125(15) 2_565 .
Nb La Ga1 0.0 . .
O3 Ga1 O3 86.2(5) 4 .
O3 Ga1 O3 86.2(5) 4 3
O3 Ga1 O3 86.2(5) . 3
O3 Ga1 O3 108.0(8) 4 2
O3 Ga1 O3 161.4(8) . 2
O3 Ga1 O3 82.9(6) 3 2
O3 Ga1 O3 82.9(6) 4 5
O3 Ga1 O3 108.0(8) . 5
O3 Ga1 O3 161.4(8) 3 5
O3 Ga1 O3 86.2(5) 2 5
O3 Ga1 O3 161.4(8) 4 6
O3 Ga1 O3 82.9(6) . 6
O3 Ga1 O3 108.0(8) 3 6
O3 Ga1 O3 86.2(5) 2 6
O3 Ga1 O3 86.2(5) 5 6
O3 Ga1 La 126.0(4) 4 .
O3 Ga1 La 41.4(3) . .
O3 Ga1 La 99.3(4) 3 .
O3 Ga1 La 126.0(4) 2 .
O3 Ga1 La 99.3(4) 5 .
O3 Ga1 La 41.4(3) 6 .
O3 Ga1 La 99.3(4) 4 2
O3 Ga1 La 126.0(4) . 2
O3 Ga1 La 41.4(3) 3 2
O3 Ga1 La 41.4(3) 2 2
O3 Ga1 La 126.0(4) 5 2
O3 Ga1 La 99.3(4) 6 2
La Ga1 La 120.0 . 2
O3 Ga1 La 41.4(3) 4 4
O3 Ga1 La 99.3(4) . 4
O3 Ga1 La 126.0(4) 3 4
O3 Ga1 La 99.3(4) 2 4
O3 Ga1 La 41.4(3) 5 4
O3 Ga1 La 126.0(4) 6 4
La Ga1 La 120.0 . 4
La Ga1 La 120.0 2 4
O3 Ga1 O2 67.5(4) 4 1_655
O3 Ga1 O2 146.8(4) . 1_655
O3 Ga1 O2 110.8(4) 3 1_655
O3 Ga1 O2 51.9(5) 2 1_655
O3 Ga1 O2 50.9(5) 5 1_655
O3 Ga1 O2 116.1(4) 6 1_655
La Ga1 O2 148.32(18) . 1_655
La Ga1 O2 79.9(2) 2 1_655
La Ga1 O2 47.5(2) 4 1_655
O3 Ga1 O2 146.8(4) 4 4_445
O3 Ga1 O2 110.8(4) . 4_445
O3 Ga1 O2 67.5(4) 3 4_445
O3 Ga1 O2 50.9(5) 2 4_445
O3 Ga1 O2 116.1(4) 5 4_445
O3 Ga1 O2 51.9(5) 6 4_445
La Ga1 O2 79.9(2) . 4_445
La Ga1 O2 47.5(2) 2 4_445
La Ga1 O2 148.32(18) 4 4_445
O2 Ga1 O2 102.2(2) 1_655 4_445
O3 Ga1 O2 50.9(5) 4 2_565
O3 Ga1 O2 51.9(5) . 2_565
O3 Ga1 O2 116.1(4) 3 2_565
O3 Ga1 O2 146.8(4) 2 2_565
O3 Ga1 O2 67.5(4) 5 2_565
O3 Ga1 O2 110.8(4) 6 2_565
La Ga1 O2 79.9(2) . 2_565
La Ga1 O2 148.32(18) 2 2_565
La Ga1 O2 47.5(2) 4 2_565
O2 Ga1 O2 95.0(5) 1_655 2_565
O2 Ga1 O2 159.8(5) 4_445 2_565
O1 Ga2 O2 117.7(4) 2_456 6
O1 Ga2 O2 117.7(4) 2_456 2_455
O2 Ga2 O2 100.1(5) 6 2_455
O1 Ga2 O2 117.7(4) 2_456 5_445
O2 Ga2 O2 100.1(5) 6 5_445
O2 Ga2 O2 100.1(5) 2_455 5_445
O1 Ga2 O1 180.0 2_456 2_455
O2 Ga2 O1 62.3(4) 6 2_455
O2 Ga2 O1 62.3(4) 2_455 2_455
O2 Ga2 O1 62.3(4) 5_445 2_455
O1 Ga2 La 135.42(2) 2_456 4_445
O2 Ga2 La 106.3(4) 6 4_445
O2 Ga2 La 56.9(5) 2_455 4_445
O2 Ga2 La 43.2(4) 5_445 4_445
O1 Ga2 La 44.58(2) 2_455 4_445
O1 Ga2 La 135.42(2) 2_456 2_455
O2 Ga2 La 56.9(5) 6 2_455
O2 Ga2 La 43.2(4) 2_455 2_455
O2 Ga2 La 106.3(4) 5_445 2_455
O1 Ga2 La 44.58(2) 2_455 2_455
La Ga2 La 74.88(4) 4_445 2_455
O1 Ga2 La 135.42(2) 2_456 .
O2 Ga2 La 43.2(4) 6 .
O2 Ga2 La 106.3(4) 2_455 .
O2 Ga2 La 56.9(5) 5_445 .
O1 Ga2 La 44.58(2) 2_455 .
La Ga2 La 74.88(4) 4_445 .
La Ga2 La 74.88(4) 2_455 .
O1 Ga2 O3 65.3(2) 2_456 6_556
O2 Ga2 O3 102.2(6) 6 6_556
O2 Ga2 O3 151.8(5) 2_455 6_556
O2 Ga2 O3 59.2(4) 5_445 6_556
O1 Ga2 O3 114.7(2) 2_455 6_556
La Ga2 O3 100.05(17) 4_445 6_556
La Ga2 O3 154.2(2) 2_455 6_556
La Ga2 O3 79.4(2) . 6_556
O1 Ga2 O3 65.3(2) 2_456 5_446
O2 Ga2 O3 151.8(5) 6 5_446
O2 Ga2 O3 59.2(4) 2_455 5_446
O2 Ga2 O3 102.2(6) 5_445 5_446
O1 Ga2 O3 114.7(2) 2_455 5_446
La Ga2 O3 79.4(2) 4_445 5_446
La Ga2 O3 100.04(17) 2_455 5_446
La Ga2 O3 154.2(2) . 5_446
O3 Ga2 O3 103.8(2) 6_556 5_446
O1 Ga2 O3 65.3(2) 2_456 2_456
O2 Ga2 O3 59.2(4) 6 2_456
O2 Ga2 O3 102.2(6) 2_455 2_456
O2 Ga2 O3 151.8(5) 5_445 2_456
O1 Ga2 O3 114.7(2) 2_455 2_456
La Ga2 O3 154.2(2) 4_445 2_456
La Ga2 O3 79.4(2) 2_455 2_456
La Ga2 O3 100.04(17) . 2_456
O3 Ga2 O3 103.8(2) 6_556 2_456
O3 Ga2 O3 103.8(2) 5_446 2_456
O1 Ga2 La 41.94(2) 2_456 4_446
O2 Ga2 La 158.3(4) 6 4_446
O2 Ga2 La 98.1(4) 2_455 4_446
O2 Ga2 La 88.1(5) 5_445 4_446
O1 Ga2 La 138.06(2) 2_455 4_446
La Ga2 La 93.472(5) 4_445 4_446
La Ga2 La 139.849(4) 2_455 4_446
La Ga2 La 139.848(4) . 4_446
O3 Ga2 La 64.7(2) 6_556 4_446
O3 Ga2 La 39.81(17) 5_446 4_446
O3 Ga2 La 105.3(2) 2_456 4_446
O3 Ga3 O3 134.5(7) 2_455 4_454
O3 Ga3 O2 100.9(5) 2_455 .
O3 Ga3 O2 107.9(5) 4_454 .
O3 Ga3 O2 107.9(5) 2_455 6_554
O3 Ga3 O2 100.9(5) 4_454 6_554
O2 Ga3 O2 100.3(11) . 6_554
O3 Ga3 O3 78.4(6) 2_455 3_454
O3 Ga3 O3 74.4(5) 4_454 3_454
O2 Ga3 O3 177.1(5) . 3_454
O2 Ga3 O3 77.3(6) 6_554 3_454
O3 Ga3 O3 74.4(5) 2_455 5_455
O3 Ga3 O3 78.4(6) 4_454 5_455
O2 Ga3 O3 77.3(6) . 5_455
O2 Ga3 O3 177.1(5) 6_554 5_455
O3 Ga3 O3 105.1(5) 3_454 5_455
O3 Ga3 Nb 110.7(4) 2_455 1_454
O3 Ga3 Nb 35.6(3) 4_454 1_454
O2 Ga3 Nb 143.3(3) . 1_454
O2 Ga3 Nb 87.6(5) 6_554 1_454
O3 Ga3 Nb 38.8(2) 3_454 1_454
O3 Ga3 Nb 93.3(2) 5_455 1_454
O3 Ga3 Nb 35.6(3) 2_455 1_455
O3 Ga3 Nb 110.7(4) 4_454 1_455
O2 Ga3 Nb 87.6(5) . 1_455
O2 Ga3 Nb 143.3(3) 6_554 1_455
O3 Ga3 Nb 93.3(2) 3_454 1_455
O3 Ga3 Nb 38.8(2) 5_455 1_455
Nb Ga3 Nb 107.26(5) 1_454 1_455
O3 Ga3 O1 160.3(5) 2_455 1_554
O3 Ga3 O1 61.6(4) 4_454 1_554
O2 Ga3 O1 59.8(4) . 1_554
O2 Ga3 O1 74.5(4) 6_554 1_554
O3 Ga3 O1 120.7(3) 3_454 1_554
O3 Ga3 O1 102.7(3) 5_455 1_554
Nb Ga3 O1 88.8(2) 1_454 1_554
Nb Ga3 O1 137.17(17) 1_455 1_554
O3 Ga3 O1 61.6(4) 2_455 2_455
O3 Ga3 O1 160.3(5) 4_454 2_455
O2 Ga3 O1 74.5(4) . 2_455
O2 Ga3 O1 59.8(4) 6_554 2_455
O3 Ga3 O1 102.7(3) 3_454 2_455
O3 Ga3 O1 120.7(3) 5_455 2_455
Nb Ga3 O1 137.17(17) 1_454 2_455
Nb Ga3 O1 88.8(2) 1_455 2_455
O1 Ga3 O1 106.12(18) 1_554 2_455
O3 Ga3 O3 45.9(3) 2_455 6_455
O3 Ga3 O3 89.0(6) 4_454 6_455
O2 Ga3 O3 118.4(6) . 6_455
O2 Ga3 O3 134.9(5) 6_554 6_455
O3 Ga3 O3 63.1(4) 3_454 6_455
O3 Ga3 O3 48.0(2) 5_455 6_455
Nb Ga3 O3 75.3(2) 1_454 6_455
Nb Ga3 O3 32.91(17) 1_455 6_455
O1 Ga3 O3 144.2(2) 1_554 6_455
O1 Ga3 O3 107.3(3) 2_455 6_455
O3 Ga3 O3 89.0(6) 2_455 1_454
O3 Ga3 O3 45.9(3) 4_454 1_454
O2 Ga3 O3 134.9(5) . 1_454
O2 Ga3 O3 118.4(6) 6_554 1_454
O3 Ga3 O3 48.0(2) 3_454 1_454
O3 Ga3 O3 63.1(4) 5_455 1_454
Nb Ga3 O3 32.91(17) 1_454 1_454
Nb Ga3 O3 75.3(2) 1_455 1_454
O1 Ga3 O3 107.3(3) 1_554 1_454
O1 Ga3 O3 144.2(2) 2_455 1_454
O3 Ga3 O3 45.6(4) 6_455 1_454
O3 Nb O3 86.2(5) 4 .
O3 Nb O3 86.2(5) 4 3
O3 Nb O3 86.2(5) . 3
O3 Nb O3 108.0(8) 4 2
O3 Nb O3 161.4(8) . 2
O3 Nb O3 82.9(6) 3 2
O3 Nb O3 82.9(6) 4 5
O3 Nb O3 108.0(8) . 5
O3 Nb O3 161.4(8) 3 5
O3 Nb O3 86.2(5) 2 5
O3 Nb O3 161.4(8) 4 6
O3 Nb O3 82.9(6) . 6
O3 Nb O3 108.0(8) 3 6
O3 Nb O3 86.2(5) 2 6
O3 Nb O3 86.2(5) 5 6
O3 Nb Ga3 159.9(4) 4 4_445
O3 Nb Ga3 113.5(3) . 4_445
O3 Nb Ga3 98.4(4) 3 4_445
O3 Nb Ga3 53.8(4) 2 4_445
O3 Nb Ga3 87.1(3) 5 4_445
O3 Nb Ga3 32.5(3) 6 4_445
O3 Nb Ga3 87.1(3) 4 4_446
O3 Nb Ga3 53.8(4) . 4_446
O3 Nb Ga3 32.5(3) 3 4_446
O3 Nb Ga3 113.5(3) 2 4_446
O3 Nb Ga3 159.9(4) 5 4_446
O3 Nb Ga3 98.4(4) 6 4_446
Ga3 Nb Ga3 107.26(5) 4_445 4_446
O3 Nb Ga3 53.8(4) 4 2_565
O3 Nb Ga3 32.5(3) . 2_565
O3 Nb Ga3 87.1(3) 3 2_565
O3 Nb Ga3 159.9(4) 2 2_565
O3 Nb Ga3 98.4(4) 5 2_565
O3 Nb Ga3 113.5(3) 6 2_565
Ga3 Nb Ga3 145.51(2) 4_445 2_565
Ga3 Nb Ga3 61.80(4) 4_446 2_565
O3 Nb Ga3 113.5(3) 4 2_564
O3 Nb Ga3 98.4(4) . 2_564
O3 Nb Ga3 159.9(4) 3 2_564
O3 Nb Ga3 87.1(3) 2 2_564
O3 Nb Ga3 32.5(3) 5 2_564
O3 Nb Ga3 53.8(4) 6 2_564
Ga3 Nb Ga3 61.80(4) 4_445 2_564
Ga3 Nb Ga3 145.51(2) 4_446 2_564
Ga3 Nb Ga3 107.26(5) 2_565 2_564
O3 Nb Ga3 32.5(3) 4 1_656
O3 Nb Ga3 87.1(3) . 1_656
O3 Nb Ga3 53.8(4) 3 1_656
O3 Nb Ga3 98.4(4) 2 1_656
O3 Nb Ga3 113.5(3) 5 1_656
O3 Nb Ga3 159.9(4) 6 1_656
Ga3 Nb Ga3 145.51(2) 4_445 1_656
Ga3 Nb Ga3 61.80(4) 4_446 1_656
Ga3 Nb Ga3 61.80(4) 2_565 1_656
Ga3 Nb Ga3 145.50(2) 2_564 1_656
O3 Nb Ga3 98.4(4) 4 1_655
O3 Nb Ga3 159.9(4) . 1_655
O3 Nb Ga3 113.5(3) 3 1_655
O3 Nb Ga3 32.5(3) 2 1_655
O3 Nb Ga3 53.8(4) 5 1_655
O3 Nb Ga3 87.1(3) 6 1_655
Ga3 Nb Ga3 61.80(4) 4_445 1_655
Ga3 Nb Ga3 145.51(2) 4_446 1_655
Ga3 Nb Ga3 145.50(2) 2_565 1_655
Ga3 Nb Ga3 61.80(4) 2_564 1_655
Ga3 Nb Ga3 107.26(5) 1_656 1_655
Ga2 O1 La 109.8(3) 2_566 .
Ga2 O1 La 109.8(3) 2_566 2_565
La O1 La 109.2(3) . 2_565
Ga2 O1 La 109.8(3) 2_566 4_455
La O1 La 109.2(3) . 4_455
La O1 La 109.2(3) 2_565 4_455
Ga2 O1 O2 146.4(3) 2_566 3_565
La O1 O2 62.5(4) . 3_565
La O1 O2 52.0(3) 2_565 3_565
La O1 O2 103.4(5) 4_455 3_565
Ga2 O1 O2 146.4(3) 2_566 .
La O1 O2 52.0(3) . .
La O1 O2 103.4(5) 2_565 .
La O1 O2 62.5(4) 4_455 .
O2 O1 O2 57.3(4) 3_565 .
Ga2 O1 O2 146.4(3) 2_566 4_455
La O1 O2 103.4(5) . 4_455
La O1 O2 62.5(4) 2_565 4_455
La O1 O2 52.0(3) 4_455 4_455
O2 O1 O2 57.3(4) 3_565 4_455
O2 O1 O2 57.3(4) . 4_455
Ga2 O1 O2 31.4(3) 2_566 3_566
La O1 O2 96.9(3) . 3_566
La O1 O2 88.5(4) 2_565 3_566
La O1 O2 140.5(5) 4_455 3_566
O2 O1 O2 114.9(3) 3_565 3_566
O2 O1 O2 148.74(14) . 3_566
O2 O1 O2 148.74(14) 4_455 3_566
Ga2 O1 O2 31.4(3) 2_566 1_556
La O1 O2 88.5(4) . 1_556
La O1 O2 140.5(5) 2_565 1_556
La O1 O2 96.9(3) 4_455 1_556
O2 O1 O2 148.75(14) 3_565 1_556
O2 O1 O2 114.9(3) . 1_556
O2 O1 O2 148.74(14) 4_455 1_556
O2 O1 O2 53.7(4) 3_566 1_556
Ga2 O1 O2 31.4(3) 2_566 4_456
La O1 O2 140.5(5) . 4_456
La O1 O2 96.9(3) 2_565 4_456
La O1 O2 88.5(4) 4_455 4_456
O2 O1 O2 148.74(14) 3_565 4_456
O2 O1 O2 148.74(14) . 4_456
O2 O1 O2 114.9(3) 4_455 4_456
O2 O1 O2 53.7(4) 3_566 4_456
O2 O1 O2 53.7(4) 1_556 4_456
Ga2 O1 O3 83.5(3) 2_566 .
La O1 O3 48.2(2) . .
La O1 O3 81.9(3) 2_565 .
La O1 O3 157.3(4) 4_455 .
O2 O1 O3 67.2(4) 3_565 .
O2 O1 O3 96.1(4) . .
O2 O1 O3 124.4(5) 4_455 .
O2 O1 O3 56.6(3) 3_566 .
O2 O1 O3 85.1(5) 1_556 .
O2 O1 O3 110.3(5) 4_456 .
Ga2 O1 O3 83.5(3) 2_566 3_565
La O1 O3 157.3(4) . 3_565
La O1 O3 48.2(2) 2_565 3_565
La O1 O3 81.9(3) 4_455 3_565
O2 O1 O3 96.1(4) 3_565 3_565
O2 O1 O3 124.4(5) . 3_565
O2 O1 O3 67.2(4) 4_455 3_565
O2 O1 O3 85.1(5) 3_566 3_565
O2 O1 O3 110.2(5) 1_556 3_565
O2 O1 O3 56.6(3) 4_456 3_565
O3 O1 O3 118.73(13) . 3_565
Ga2 O1 O3 83.5(3) 2_566 4_455
La O1 O3 81.9(3) . 4_455
La O1 O3 157.3(4) 2_565 4_455
La O1 O3 48.2(2) 4_455 4_455
O2 O1 O3 124.4(5) 3_565 4_455
O2 O1 O3 67.2(4) . 4_455
O2 O1 O3 96.1(4) 4_455 4_455
O2 O1 O3 110.3(5) 3_566 4_455
O2 O1 O3 56.6(3) 1_556 4_455
O2 O1 O3 85.1(5) 4_456 4_455
O3 O1 O3 118.74(13) . 4_455
O3 O1 O3 118.73(13) 3_565 4_455
Ga2 O1 Ga2 180.0 2_566 2_565
La O1 Ga2 70.2(3) . 2_565
La O1 Ga2 70.2(3) 2_565 2_565
La O1 Ga2 70.2(3) 4_455 2_565
O2 O1 Ga2 33.6(3) 3_565 2_565
O2 O1 Ga2 33.6(3) . 2_565
O2 O1 Ga2 33.6(3) 4_455 2_565
O2 O1 Ga2 148.6(3) 3_566 2_565
O2 O1 Ga2 148.6(3) 1_556 2_565
O2 O1 Ga2 148.6(3) 4_456 2_565
O3 O1 Ga2 96.5(3) . 2_565
O3 O1 Ga2 96.5(3) 3_565 2_565
O3 O1 Ga2 96.5(3) 4_455 2_565
Ga2 O1 Ga3 62.1(2) 2_566 1_556
La O1 Ga3 72.08(9) . 1_556
La O1 Ga3 171.0(5) 2_565 1_556
La O1 Ga3 78.17(9) 4_455 1_556
O2 O1 Ga3 132.5(4) 3_565 1_556
O2 O1 Ga3 84.4(2) . 1_556
O2 O1 Ga3 126.2(4) 4_455 1_556
O2 O1 Ga3 82.5(4) 3_566 1_556
O2 O1 Ga3 30.9(2) 1_556 1_556
O2 O1 Ga3 77.9(4) 4_456 1_556
O3 O1 Ga3 93.1(3) . 1_556
O3 O1 Ga3 130.4(4) 3_565 1_556
O3 O1 Ga3 30.6(2) 4_455 1_556
Ga2 O1 Ga3 117.9(2) 2_565 1_556
Ga2 O1 Ga3 62.1(2) 2_566 2_565
La O1 Ga3 78.17(9) . 2_565
La O1 Ga3 72.08(9) 2_565 2_565
La O1 Ga3 171.0(5) 4_455 2_565
O2 O1 Ga3 84.4(2) 3_565 2_565
O2 O1 Ga3 126.2(4) . 2_565
O2 O1 Ga3 132.5(4) 4_455 2_565
O2 O1 Ga3 30.9(2) 3_566 2_565
O2 O1 Ga3 77.9(4) 1_556 2_565
O2 O1 Ga3 82.5(4) 4_456 2_565
O3 O1 Ga3 30.6(2) . 2_565
O3 O1 Ga3 93.1(3) 3_565 2_565
O3 O1 Ga3 130.4(4) 4_455 2_565
Ga2 O1 Ga3 117.9(2) 2_565 2_565
Ga3 O1 Ga3 99.9(3) 1_556 2_565
Ga2 O1 Ga3 62.1(2) 2_566 4_456
La O1 Ga3 171.0(5) . 4_456
La O1 Ga3 78.17(9) 2_565 4_456
La O1 Ga3 72.08(9) 4_455 4_456
O2 O1 Ga3 126.2(4) 3_565 4_456
O2 O1 Ga3 132.5(4) . 4_456
O2 O1 Ga3 84.4(2) 4_455 4_456
O2 O1 Ga3 77.9(4) 3_566 4_456
O2 O1 Ga3 82.5(4) 1_556 4_456
O2 O1 Ga3 30.9(2) 4_456 4_456
O3 O1 Ga3 130.4(4) . 4_456
O3 O1 Ga3 30.6(2) 3_565 4_456
O3 O1 Ga3 93.1(3) 4_455 4_456
Ga2 O1 Ga3 117.9(2) 2_565 4_456
Ga3 O1 Ga3 99.9(3) 1_556 4_456
Ga3 O1 Ga3 99.9(3) 2_565 4_456
Ga2 O1 O2 78.5(3) 2_566 6
La O1 O2 42.54(18) . 6
La O1 O2 149.3(2) 2_565 6
La O1 O2 94.6(2) 4_455 6
O2 O1 O2 104.6(4) 3_565 6
O2 O1 O2 70.1(3) . 6
O2 O1 O2 126.0(3) 4_455 6
O2 O1 O2 84.8(3) 3_566 6
O2 O1 O2 49.6(4) 1_556 6
O2 O1 O2 103.1(4) 4_456 6
O3 O1 O2 69.5(3) . 6
O3 O1 O2 159.2(5) 3_565 6
O3 O1 O2 49.3(3) 4_455 6
Ga2 O1 O2 101.5(3) 2_565 6
Ga3 O1 O2 29.85(17) 1_556 6
Ga3 O1 O2 87.5(3) 2_565 6
Ga3 O1 O2 129.0(4) 4_456 6
Ga2 O1 O2 78.5(3) 2_566 5_455
La O1 O2 149.3(2) . 5_455
La O1 O2 94.6(2) 2_565 5_455
La O1 O2 42.54(18) 4_455 5_455
O2 O1 O2 126.0(3) 3_565 5_455
O2 O1 O2 104.6(4) . 5_455
O2 O1 O2 70.1(3) 4_455 5_455
O2 O1 O2 103.1(4) 3_566 5_455
O2 O1 O2 84.8(3) 1_556 5_455
O2 O1 O2 49.6(4) 4_456 5_455
O3 O1 O2 159.2(5) . 5_455
O3 O1 O2 49.3(3) 3_565 5_455
O3 O1 O2 69.5(3) 4_455 5_455
Ga2 O1 O2 101.5(3) 2_565 5_455
Ga3 O1 O2 87.5(3) 1_556 5_455
Ga3 O1 O2 129.0(4) 2_565 5_455
Ga3 O1 O2 29.85(17) 4_456 5_455
O2 O1 O2 116.1(2) 6 5_455
Ga2 O1 O2 78.5(3) 2_566 2_565
La O1 O2 94.6(2) . 2_565
La O1 O2 42.54(18) 2_565 2_565
La O1 O2 149.3(2) 4_455 2_565
O2 O1 O2 70.1(3) 3_565 2_565
O2 O1 O2 126.0(3) . 2_565
O2 O1 O2 104.6(4) 4_455 2_565
O2 O1 O2 49.6(4) 3_566 2_565
O2 O1 O2 103.1(4) 1_556 2_565
O2 O1 O2 84.8(3) 4_456 2_565
O3 O1 O2 49.3(3) . 2_565
O3 O1 O2 69.5(3) 3_565 2_565
O3 O1 O2 159.2(5) 4_455 2_565
Ga2 O1 O2 101.5(3) 2_565 2_565
Ga3 O1 O2 129.0(4) 1_556 2_565
Ga3 O1 O2 29.85(17) 2_565 2_565
Ga3 O1 O2 87.5(3) 4_456 2_565
O2 O1 O2 116.1(2) 6 2_565
O2 O1 O2 116.1(2) 5_455 2_565
Ga2 O1 O3 118.7(3) 2_566 6
La O1 O3 27.88(17) . 6
La O1 O3 81.4(3) 2_565 6
La O1 O3 123.1(5) 4_455 6
O2 O1 O3 39.9(4) 3_565 6
O2 O1 O3 60.7(4) . 6
O2 O1 O3 93.4(4) 4_455 6
O2 O1 O3 93.6(3) 3_566 6
O2 O1 O3 108.9(4) 1_556 6
O2 O1 O3 147.3(4) 4_456 6
O3 O1 O3 37.0(3) . 6
O3 O1 O3 129.6(4) 3_565 6
O3 O1 O3 108.9(3) 4_455 6
Ga2 O1 O3 61.3(3) 2_565 6
Ga3 O1 O3 99.03(17) 1_556 6
Ga3 O1 O3 65.78(15) 2_565 6
Ga3 O1 O3 158.03(14) 4_456 6
O2 O1 O3 69.2(3) 6 6
O2 O1 O3 162.8(5) 5_455 6
O2 O1 O3 71.8(3) 2_565 6
Ga2 O1 O3 118.7(3) 2_566 2_565
La O1 O3 123.1(5) . 2_565
La O1 O3 27.88(17) 2_565 2_565
La O1 O3 81.4(3) 4_455 2_565
O2 O1 O3 60.7(4) 3_565 2_565
O2 O1 O3 93.4(4) . 2_565
O2 O1 O3 39.8(4) 4_455 2_565
O2 O1 O3 108.9(4) 3_566 2_565
O2 O1 O3 147.3(4) 1_556 2_565
O2 O1 O3 93.6(3) 4_456 2_565
O3 O1 O3 108.9(3) . 2_565
O3 O1 O3 37.0(3) 3_565 2_565
O3 O1 O3 129.6(4) 4_455 2_565
Ga2 O1 O3 61.3(3) 2_565 2_565
Ga3 O1 O3 158.03(14) 1_556 2_565
Ga3 O1 O3 99.03(17) 2_565 2_565
Ga3 O1 O3 65.78(15) 4_456 2_565
O2 O1 O3 162.8(5) 6 2_565
O2 O1 O3 71.8(3) 5_455 2_565
O2 O1 O3 69.2(3) 2_565 2_565
O3 O1 O3 98.9(4) 6 2_565
Ga2 O1 O3 118.7(3) 2_566 5_455
La O1 O3 81.4(3) . 5_455
La O1 O3 123.1(5) 2_565 5_455
La O1 O3 27.88(17) 4_455 5_455
O2 O1 O3 93.4(4) 3_565 5_455
O2 O1 O3 39.9(4) . 5_455
O2 O1 O3 60.7(4) 4_455 5_455
O2 O1 O3 147.3(4) 3_566 5_455
O2 O1 O3 93.6(3) 1_556 5_455
O2 O1 O3 108.9(4) 4_456 5_455
O3 O1 O3 129.6(4) . 5_455
O3 O1 O3 108.9(3) 3_565 5_455
O3 O1 O3 37.0(3) 4_455 5_455
Ga2 O1 O3 61.3(3) 2_565 5_455
Ga3 O1 O3 65.78(15) 1_556 5_455
Ga3 O1 O3 158.03(14) 2_565 5_455
Ga3 O1 O3 99.03(16) 4_456 5_455
O2 O1 O3 71.8(3) 6 5_455
O2 O1 O3 69.2(3) 5_455 5_455
O2 O1 O3 162.8(5) 2_565 5_455
O3 O1 O3 98.9(4) 6 5_455
O3 O1 O3 98.9(4) 2_565 5_455
Ga2 O1 Ga3 136.96(13) 2_566 .
La O1 Ga3 52.6(2) . .
La O1 Ga3 113.2(5) 2_565 .
La O1 Ga3 58.1(2) 4_455 .
O2 O1 Ga3 67.2(3) 3_565 .
O2 O1 Ga3 10.0(3) . .
O2 O1 Ga3 63.1(4) 4_455 .
O2 O1 Ga3 146.3(3) 3_566 .
O2 O1 Ga3 105.6(2) 1_556 .
O2 O1 Ga3 140.4(3) 4_456 .
O3 O1 Ga3 99.5(3) . .
O3 O1 Ga3 128.6(4) 3_565 .
O3 O1 Ga3 57.2(3) 4_455 .
Ga2 O1 Ga3 43.04(13) 2_565 .
Ga3 O1 Ga3 74.88(9) 1_556 .
Ga3 O1 Ga3 130.07(14) 2_565 .
Ga3 O1 Ga3 130.07(14) 4_456 .
O2 O1 Ga3 63.2(3) 6 .
O2 O1 Ga3 100.7(2) 5_455 .
O2 O1 Ga3 134.8(4) 2_565 .
O3 O1 Ga3 66.2(2) 6 .
O3 O1 Ga3 101.1(4) 2_565 .
O3 O1 Ga3 32.7(2) 5_455 .
Ga2 O1 Ga3 136.96(13) 2_566 2_564
La O1 Ga3 58.1(2) . 2_564
La O1 Ga3 52.6(2) 2_565 2_564
La O1 Ga3 113.2(5) 4_455 2_564
O2 O1 Ga3 10.0(3) 3_565 2_564
O2 O1 Ga3 63.1(4) . 2_564
O2 O1 Ga3 67.2(3) 4_455 2_564
O2 O1 Ga3 105.6(2) 3_566 2_564
O2 O1 Ga3 140.4(3) 1_556 2_564
O2 O1 Ga3 146.3(3) 4_456 2_564
O3 O1 Ga3 57.2(3) . 2_564
O3 O1 Ga3 99.5(3) 3_565 2_564
O3 O1 Ga3 128.6(4) 4_455 2_564
Ga2 O1 Ga3 43.04(13) 2_565 2_564
Ga3 O1 Ga3 130.07(14) 1_556 2_564
Ga3 O1 Ga3 74.88(9) 2_565 2_564
Ga3 O1 Ga3 130.07(14) 4_456 2_564
O2 O1 Ga3 100.7(2) 6 2_564
O2 O1 Ga3 134.8(4) 5_455 2_564
O2 O1 Ga3 63.2(3) 2_565 2_564
O3 O1 Ga3 32.7(2) 6 2_564
O3 O1 Ga3 66.2(2) 2_565 2_564
O3 O1 Ga3 101.1(4) 5_455 2_564
Ga3 O1 Ga3 72.5(2) . 2_564
Ga2 O1 Ga3 136.96(13) 2_566 4_455
La O1 Ga3 113.2(5) . 4_455
La O1 Ga3 58.1(2) 2_565 4_455
La O1 Ga3 52.6(2) 4_455 4_455
O2 O1 Ga3 63.1(4) 3_565 4_455
O2 O1 Ga3 67.2(3) . 4_455
O2 O1 Ga3 10.0(3) 4_455 4_455
O2 O1 Ga3 140.3(3) 3_566 4_455
O2 O1 Ga3 146.3(3) 1_556 4_455
O2 O1 Ga3 105.6(2) 4_456 4_455
O3 O1 Ga3 128.6(4) . 4_455
O3 O1 Ga3 57.2(3) 3_565 4_455
O3 O1 Ga3 99.5(3) 4_455 4_455
Ga2 O1 Ga3 43.04(13) 2_565 4_455
Ga3 O1 Ga3 130.07(14) 1_556 4_455
Ga3 O1 Ga3 130.07(14) 2_565 4_455
Ga3 O1 Ga3 74.88(9) 4_456 4_455
O2 O1 Ga3 134.8(4) 6 4_455
O2 O1 Ga3 63.2(3) 5_455 4_455
O2 O1 Ga3 100.7(2) 2_565 4_455
O3 O1 Ga3 101.1(4) 6 4_455
O3 O1 Ga3 32.7(2) 2_565 4_455
O3 O1 Ga3 66.2(2) 5_455 4_455
Ga3 O1 Ga3 72.5(2) . 4_455
Ga3 O1 Ga3 72.5(2) 2_564 4_455
Ga2 O1 Ga1 100.45(18) 2_566 1_455
La O1 Ga1 70.66(8) . 1_455
La O1 Ga1 147.2(5) 2_565 1_455
La O1 Ga1 46.12(4) 4_455 1_455
O2 O1 Ga1 106.5(4) 3_565 1_455
O2 O1 Ga1 49.2(3) . 1_455
O2 O1 Ga1 85.2(4) 4_455 1_455
O2 O1 Ga1 124.3(4) 3_566 1_455
O2 O1 Ga1 71.5(2) 1_556 1_455
O2 O1 Ga1 102.6(4) 4_456 1_455
O3 O1 Ga1 114.8(2) . 1_455
O3 O1 Ga1 126.4(2) 3_565 1_455
O3 O1 Ga1 17.9(2) 4_455 1_455
Ga2 O1 Ga1 79.54(18) 2_565 1_455
Ga3 O1 Ga1 41.81(3) 1_556 1_455
Ga3 O1 Ga1 136.21(15) 2_565 1_455
Ga3 O1 Ga1 106.16(7) 4_456 1_455
O2 O1 Ga1 48.8(2) 6 1_455
O2 O1 Ga1 78.84(19) 5_455 1_455
O2 O1 Ga1 164.1(2) 2_565 1_455
O3 O1 Ga1 95.40(19) 6 1_455
O3 O1 Ga1 123.6(3) 2_565 1_455
O3 O1 Ga1 24.74(13) 5_455 1_455
Ga3 O1 Ga1 39.29(6) . 1_455
Ga3 O1 Ga1 111.1(3) 2_564 1_455
Ga3 O1 Ga1 90.96(18) 4_455 1_455
Ga2 O1 Nb 100.45(18) 2_566 1_455
La O1 Nb 70.66(8) . 1_455
La O1 Nb 147.2(5) 2_565 1_455
La O1 Nb 46.12(4) 4_455 1_455
O2 O1 Nb 106.5(4) 3_565 1_455
O2 O1 Nb 49.2(3) . 1_455
O2 O1 Nb 85.2(4) 4_455 1_455
O2 O1 Nb 124.3(4) 3_566 1_455
O2 O1 Nb 71.5(2) 1_556 1_455
O2 O1 Nb 102.6(4) 4_456 1_455
O3 O1 Nb 114.8(2) . 1_455
O3 O1 Nb 126.4(2) 3_565 1_455
O3 O1 Nb 17.9(2) 4_455 1_455
Ga2 O1 Nb 79.54(18) 2_565 1_455
Ga3 O1 Nb 41.81(3) 1_556 1_455
Ga3 O1 Nb 136.21(15) 2_565 1_455
Ga3 O1 Nb 106.16(7) 4_456 1_455
O2 O1 Nb 48.8(2) 6 1_455
O2 O1 Nb 78.84(19) 5_455 1_455
O2 O1 Nb 164.1(2) 2_565 1_455
O3 O1 Nb 95.40(19) 6 1_455
O3 O1 Nb 123.6(3) 2_565 1_455
O3 O1 Nb 24.74(13) 5_455 1_455
Ga3 O1 Nb 39.29(6) . 1_455
Ga3 O1 Nb 111.1(3) 2_564 1_455
Ga3 O1 Nb 90.96(18) 4_455 1_455
Ga1 O1 Nb 0.0 1_455 1_455
Ga2 O1 Nb 100.46(18) 2_566 .
La O1 Nb 46.12(4) . .
La O1 Nb 70.66(8) 2_565 .
La O1 Nb 147.2(5) 4_455 .
O2 O1 Nb 49.2(3) 3_565 .
O2 O1 Nb 85.2(4) . .
O2 O1 Nb 106.5(4) 4_455 .
O2 O1 Nb 71.5(2) 3_566 .
O2 O1 Nb 102.6(4) 1_556 .
O2 O1 Nb 124.3(4) 4_456 .
O3 O1 Nb 17.9(2) . .
O3 O1 Nb 114.8(2) 3_565 .
O3 O1 Nb 126.4(2) 4_455 .
Ga2 O1 Nb 79.55(18) 2_565 .
Ga3 O1 Nb 106.16(7) 1_556 .
Ga3 O1 Nb 41.81(3) 2_565 .
Ga3 O1 Nb 136.21(15) 4_456 .
O2 O1 Nb 78.84(19) 6 .
O2 O1 Nb 164.1(2) 5_455 .
O2 O1 Nb 48.8(2) 2_565 .
O3 O1 Nb 24.74(13) 6 .
O3 O1 Nb 95.40(19) 2_565 .
O3 O1 Nb 123.6(3) 5_455 .
Ga3 O1 Nb 90.96(18) . .
Ga3 O1 Nb 39.29(6) 2_564 .
Ga3 O1 Nb 111.1(3) 4_455 .
Ga1 O1 Nb 116.78(11) 1_455 .
Nb O1 Nb 116.78(11) 1_455 .
Ga2 O1 Ga1 100.46(18) 2_566 .
La O1 Ga1 46.12(4) . .
La O1 Ga1 70.66(8) 2_565 .
La O1 Ga1 147.2(5) 4_455 .
O2 O1 Ga1 49.2(3) 3_565 .
O2 O1 Ga1 85.2(4) . .
O2 O1 Ga1 106.5(4) 4_455 .
O2 O1 Ga1 71.5(2) 3_566 .
O2 O1 Ga1 102.6(4) 1_556 .
O2 O1 Ga1 124.3(4) 4_456 .
O3 O1 Ga1 17.9(2) . .
O3 O1 Ga1 114.8(2) 3_565 .
O3 O1 Ga1 126.4(2) 4_455 .
Ga2 O1 Ga1 79.55(18) 2_565 .
Ga3 O1 Ga1 106.16(7) 1_556 .
Ga3 O1 Ga1 41.81(3) 2_565 .
Ga3 O1 Ga1 136.21(15) 4_456 .
O2 O1 Ga1 78.84(19) 6 .
O2 O1 Ga1 164.1(2) 5_455 .
O2 O1 Ga1 48.8(2) 2_565 .
O3 O1 Ga1 24.74(13) 6 .
O3 O1 Ga1 95.40(19) 2_565 .
O3 O1 Ga1 123.6(3) 5_455 .
Ga3 O1 Ga1 90.96(18) . .
Ga3 O1 Ga1 39.29(6) 2_564 .
Ga3 O1 Ga1 111.1(3) 4_455 .
Ga1 O1 Ga1 116.78(11) 1_455 .
Nb O1 Ga1 116.78(11) 1_455 .
Nb O1 Ga1 0.0 . .
Ga2 O1 Ga1 100.45(18) 2_566 1_565
La O1 Ga1 147.2(5) . 1_565
La O1 Ga1 46.12(4) 2_565 1_565
La O1 Ga1 70.66(8) 4_455 1_565
O2 O1 Ga1 85.2(4) 3_565 1_565
O2 O1 Ga1 106.5(4) . 1_565
O2 O1 Ga1 49.2(3) 4_455 1_565
O2 O1 Ga1 102.6(4) 3_566 1_565
O2 O1 Ga1 124.3(4) 1_556 1_565
O2 O1 Ga1 71.5(2) 4_456 1_565
O3 O1 Ga1 126.4(2) . 1_565
O3 O1 Ga1 17.9(2) 3_565 1_565
O3 O1 Ga1 114.8(2) 4_455 1_565
Ga2 O1 Ga1 79.54(18) 2_565 1_565
Ga3 O1 Ga1 136.21(15) 1_556 1_565
Ga3 O1 Ga1 106.16(7) 2_565 1_565
Ga3 O1 Ga1 41.81(3) 4_456 1_565
O2 O1 Ga1 164.1(2) 6 1_565
O2 O1 Ga1 48.8(2) 5_455 1_565
O2 O1 Ga1 78.84(19) 2_565 1_565
O3 O1 Ga1 123.6(3) 6 1_565
O3 O1 Ga1 24.74(13) 2_565 1_565
O3 O1 Ga1 95.40(19) 5_455 1_565
Ga3 O1 Ga1 111.1(3) . 1_565
Ga3 O1 Ga1 90.96(18) 2_564 1_565
Ga3 O1 Ga1 39.29(6) 4_455 1_565
Ga1 O1 Ga1 116.78(11) 1_455 1_565
Nb O1 Ga1 116.78(11) 1_455 1_565
Nb O1 Ga1 116.78(11) . 1_565
Ga1 O1 Ga1 116.78(11) . 1_565
Ga2 O1 Nb 100.45(18) 2_566 1_565
La O1 Nb 147.2(5) . 1_565
La O1 Nb 46.12(4) 2_565 1_565
La O1 Nb 70.66(8) 4_455 1_565
O2 O1 Nb 85.2(4) 3_565 1_565
O2 O1 Nb 106.5(4) . 1_565
O2 O1 Nb 49.2(3) 4_455 1_565
O2 O1 Nb 102.6(4) 3_566 1_565
O2 O1 Nb 124.3(4) 1_556 1_565
O2 O1 Nb 71.5(2) 4_456 1_565
O3 O1 Nb 126.4(2) . 1_565
O3 O1 Nb 17.9(2) 3_565 1_565
O3 O1 Nb 114.8(2) 4_455 1_565
Ga2 O1 Nb 79.54(18) 2_565 1_565
Ga3 O1 Nb 136.21(15) 1_556 1_565
Ga3 O1 Nb 106.16(7) 2_565 1_565
Ga3 O1 Nb 41.81(3) 4_456 1_565
O2 O1 Nb 164.1(2) 6 1_565
O2 O1 Nb 48.8(2) 5_455 1_565
O2 O1 Nb 78.84(19) 2_565 1_565
O3 O1 Nb 123.6(3) 6 1_565
O3 O1 Nb 24.74(13) 2_565 1_565
O3 O1 Nb 95.40(19) 5_455 1_565
Ga3 O1 Nb 111.1(3) . 1_565
Ga3 O1 Nb 90.96(18) 2_564 1_565
Ga3 O1 Nb 39.29(6) 4_455 1_565
Ga1 O1 Nb 116.78(11) 1_455 1_565
Nb O1 Nb 116.78(11) 1_455 1_565
Nb O1 Nb 116.78(11) . 1_565
Ga1 O1 Nb 116.78(11) . 1_565
Ga1 O1 Nb 0.0 1_565 1_565
Ga2 O1 O2 81.4(2) 2_566 2_465
La O1 O2 114.67(14) . 2_465
La O1 O2 127.42(14) 2_565 2_465
La O1 O2 29.1(2) 4_455 2_465
O2 O1 O2 132.2(4) 3_565 2_465
O2 O1 O2 82.9(4) . 2_465
O2 O1 O2 80.0(3) 4_455 2_465
O2 O1 O2 112.8(4) 3_566 2_465
O2 O1 O2 68.8(3) 1_556 2_465
O2 O1 O2 65.9(4) 4_456 2_465
O3 O1 O2 150.3(3) . 2_465
O3 O1 O2 84.8(3) 3_565 2_465
O3 O1 O2 34.1(3) 4_455 2_465
Ga2 O1 O2 98.6(2) 2_565 2_465
Ga3 O1 O2 57.19(13) 1_556 2_465
Ga3 O1 O2 143.4(4) 2_565 2_465
Ga3 O1 O2 61.91(15) 4_456 2_465
O2 O1 O2 82.4(3) 6 2_465
O2 O1 O2 35.6(3) 5_455 2_465
O2 O1 O2 148.8(5) 2_565 2_465
O3 O1 O2 139.3(3) 6 2_465
O3 O1 O2 100.84(18) 2_565 2_465
O3 O1 O2 43.0(2) 5_455 2_465
Ga3 O1 O2 75.21(16) . 2_465
Ga3 O1 O2 141.6(3) 2_564 2_465
Ga3 O1 O2 78.44(15) 4_455 2_465
Ga1 O1 O2 44.28(13) 1_455 2_465
Nb O1 O2 44.28(13) 1_455 2_465
Nb O1 O2 160.36(13) . 2_465
Ga1 O1 O2 160.36(13) . 2_465
Ga1 O1 O2 81.69(12) 1_565 2_465
Nb O1 O2 81.69(12) 1_565 2_465
Ga2 O1 O2 81.4(2) 2_566 5_445
La O1 O2 29.14(19) . 5_445
La O1 O2 114.67(14) 2_565 5_445
La O1 O2 127.42(14) 4_455 5_445
O2 O1 O2 82.9(4) 3_565 5_445
O2 O1 O2 80.0(3) . 5_445
O2 O1 O2 132.2(4) 4_455 5_445
O2 O1 O2 68.8(3) 3_566 5_445
O2 O1 O2 65.9(4) 1_556 5_445
O2 O1 O2 112.8(4) 4_456 5_445
O3 O1 O2 34.1(3) . 5_445
O3 O1 O2 150.3(3) 3_565 5_445
O3 O1 O2 84.8(3) 4_455 5_445
Ga2 O1 O2 98.6(2) 2_565 5_445
Ga3 O1 O2 61.91(15) 1_556 5_445
Ga3 O1 O2 57.19(13) 2_565 5_445
Ga3 O1 O2 143.4(4) 4_456 5_445
O2 O1 O2 35.6(3) 6 5_445
O2 O1 O2 148.8(5) 5_455 5_445
O2 O1 O2 82.4(3) 2_565 5_445
O3 O1 O2 43.0(2) 6 5_445
O3 O1 O2 139.3(3) 2_565 5_445
O3 O1 O2 100.84(18) 5_455 5_445
Ga3 O1 O2 78.44(15) . 5_445
Ga3 O1 O2 75.21(16) 2_564 5_445
Ga3 O1 O2 141.6(3) 4_455 5_445
Ga1 O1 O2 81.69(12) 1_455 5_445
Nb O1 O2 81.69(12) 1_455 5_445
Nb O1 O2 44.28(13) . 5_445
Ga1 O1 O2 44.28(13) . 5_445
Ga1 O1 O2 160.36(13) 1_565 5_445
Nb O1 O2 160.36(13) 1_565 5_445
O2 O1 O2 117.81(11) 2_465 5_445
Ga2 O1 O2 81.4(2) 2_566 6_665
La O1 O2 127.42(14) . 6_665
La O1 O2 29.14(19) 2_565 6_665
La O1 O2 114.67(14) 4_455 6_665
O2 O1 O2 80.0(3) 3_565 6_665
O2 O1 O2 132.2(4) . 6_665
O2 O1 O2 82.9(4) 4_455 6_665
O2 O1 O2 65.9(4) 3_566 6_665
O2 O1 O2 112.8(4) 1_556 6_665
O2 O1 O2 68.8(3) 4_456 6_665
O3 O1 O2 84.8(3) . 6_665
O3 O1 O2 34.1(3) 3_565 6_665
O3 O1 O2 150.3(3) 4_455 6_665
Ga2 O1 O2 98.6(2) 2_565 6_665
Ga3 O1 O2 143.4(4) 1_556 6_665
Ga3 O1 O2 61.91(15) 2_565 6_665
Ga3 O1 O2 57.19(13) 4_456 6_665
O2 O1 O2 148.8(5) 6 6_665
O2 O1 O2 82.4(3) 5_455 6_665
O2 O1 O2 35.6(3) 2_565 6_665
O3 O1 O2 100.83(18) 6 6_665
O3 O1 O2 43.0(2) 2_565 6_665
O3 O1 O2 139.3(3) 5_455 6_665
Ga3 O1 O2 141.6(3) . 6_665
Ga3 O1 O2 78.44(15) 2_564 6_665
Ga3 O1 O2 75.21(16) 4_455 6_665
Ga1 O1 O2 160.36(13) 1_455 6_665
Nb O1 O2 160.36(13) 1_455 6_665
Nb O1 O2 81.69(12) . 6_665
Ga1 O1 O2 81.69(12) . 6_665
Ga1 O1 O2 44.28(13) 1_565 6_665
Nb O1 O2 44.28(13) 1_565 6_665
O2 O1 O2 117.81(11) 2_465 6_665
O2 O1 O2 117.81(11) 5_445 6_665
Ga2 O1 O3 51.6(2) 2_566 6_556
La O1 O3 64.2(2) . 6_556
La O1 O3 102.8(2) 2_565 6_556
La O1 O3 147.4(3) 4_455 6_556
O2 O1 O3 100.8(3) 3_565 6_556
O2 O1 O3 115.9(3) . 6_556
O2 O1 O3 158.0(4) 4_455 6_556
O2 O1 O3 32.9(3) 3_566 6_556
O2 O1 O3 52.7(4) 1_556 6_556
O2 O1 O3 81.7(4) 4_456 6_556
O3 O1 O3 33.7(3) . 6_556
O3 O1 O3 116.8(4) 3_565 6_556
O3 O1 O3 99.8(3) 4_455 6_556
Ga2 O1 O3 128.4(2) 2_565 6_556
Ga3 O1 O3 69.4(2) 1_556 6_556
Ga3 O1 O3 30.91(14) 2_565 6_556
Ga3 O1 O3 109.7(4) 4_456 6_556
O2 O1 O3 58.2(3) 6 6_556
O2 O1 O3 130.0(5) 5_455 6_556
O2 O1 O3 60.8(2) 2_565 6_556
O3 O1 O3 67.07(19) 6 6_556
O3 O1 O3 129.93(11) 2_565 6_556
O3 O1 O3 129.93(11) 5_455 6_556
Ga3 O1 O3 114.02(13) . 6_556
Ga3 O1 O3 90.90(12) 2_564 6_556
Ga3 O1 O3 159.84(17) 4_455 6_556
Ga1 O1 O3 105.94(17) 1_455 6_556
Nb O1 O3 105.94(17) 1_455 6_556
Nb O1 O3 51.62(12) . 6_556
Ga1 O1 O3 51.62(12) . 6_556
Ga1 O1 O3 133.2(2) 1_565 6_556
Nb O1 O3 133.2(2) 1_565 6_556
O2 O1 O3 121.4(3) 2_465 6_556
O2 O1 O3 35.92(18) 5_445 6_556
O2 O1 O3 90.6(2) 6_665 6_556
Ga2 O1 O3 51.6(2) 2_566 2_566
La O1 O3 147.4(3) . 2_566
La O1 O3 64.2(2) 2_565 2_566
La O1 O3 102.8(2) 4_455 2_566
O2 O1 O3 115.9(3) 3_565 2_566
O2 O1 O3 158.0(4) . 2_566
O2 O1 O3 100.8(3) 4_455 2_566
O2 O1 O3 52.7(4) 3_566 2_566
O2 O1 O3 81.7(4) 1_556 2_566
O2 O1 O3 32.9(3) 4_456 2_566
O3 O1 O3 99.8(3) . 2_566
O3 O1 O3 33.7(3) 3_565 2_566
O3 O1 O3 116.8(4) 4_455 2_566
Ga2 O1 O3 128.4(2) 2_565 2_566
Ga3 O1 O3 109.7(4) 1_556 2_566
Ga3 O1 O3 69.4(2) 2_565 2_566
Ga3 O1 O3 30.91(14) 4_456 2_566
O2 O1 O3 130.0(5) 6 2_566
O2 O1 O3 60.8(2) 5_455 2_566
O2 O1 O3 58.2(3) 2_565 2_566
O3 O1 O3 129.93(11) 6 2_566
O3 O1 O3 67.07(19) 2_565 2_566
O3 O1 O3 129.93(11) 5_455 2_566
Ga3 O1 O3 159.84(17) . 2_566
Ga3 O1 O3 114.02(13) 2_564 2_566
Ga3 O1 O3 90.90(13) 4_455 2_566
Ga1 O1 O3 133.2(2) 1_455 2_566
Nb O1 O3 133.2(2) 1_455 2_566
Nb O1 O3 105.94(17) . 2_566
Ga1 O1 O3 105.94(17) . 2_566
Ga1 O1 O3 51.62(12) 1_565 2_566
Nb O1 O3 51.62(12) 1_565 2_566
O2 O1 O3 90.6(2) 2_465 2_566
O2 O1 O3 121.4(3) 5_445 2_566
O2 O1 O3 35.92(18) 6_665 2_566
O3 O1 O3 85.5(3) 6_556 2_566
Ga2 O1 O3 51.6(2) 2_566 5_456
La O1 O3 102.83(19) . 5_456
La O1 O3 147.4(3) 2_565 5_456
La O1 O3 64.2(2) 4_455 5_456
O2 O1 O3 158.0(4) 3_565 5_456
O2 O1 O3 100.8(3) . 5_456
O2 O1 O3 115.9(3) 4_455 5_456
O2 O1 O3 81.7(4) 3_566 5_456
O2 O1 O3 32.9(3) 1_556 5_456
O2 O1 O3 52.7(4) 4_456 5_456
O3 O1 O3 116.8(4) . 5_456
O3 O1 O3 99.8(3) 3_565 5_456
O3 O1 O3 33.7(3) 4_455 5_456
Ga2 O1 O3 128.4(2) 2_565 5_456
Ga3 O1 O3 30.91(14) 1_556 5_456
Ga3 O1 O3 109.7(4) 2_565 5_456
Ga3 O1 O3 69.4(2) 4_456 5_456
O2 O1 O3 60.8(2) 6 5_456
O2 O1 O3 58.2(3) 5_455 5_456
O2 O1 O3 130.0(5) 2_565 5_456
O3 O1 O3 129.93(11) 6 5_456
O3 O1 O3 129.93(11) 2_565 5_456
O3 O1 O3 67.07(19) 5_455 5_456
Ga3 O1 O3 90.90(13) . 5_456
Ga3 O1 O3 159.84(17) 2_564 5_456
Ga3 O1 O3 114.02(13) 4_455 5_456
Ga1 O1 O3 51.62(13) 1_455 5_456
Nb O1 O3 51.62(13) 1_455 5_456
Nb O1 O3 133.2(2) . 5_456
Ga1 O1 O3 133.2(2) . 5_456
Ga1 O1 O3 105.94(17) 1_565 5_456
Nb O1 O3 105.94(17) 1_565 5_456
O2 O1 O3 35.92(18) 2_465 5_456
O2 O1 O3 90.6(2) 5_445 5_456
O2 O1 O3 121.4(3) 6_665 5_456
O3 O1 O3 85.5(3) 6_556 5_456
O3 O1 O3 85.5(3) 2_566 5_456
Ga2 O1 La 29.50(9) 2_566 1_556
La O1 La 80.3(2) . 1_556
La O1 La 121.7(3) 2_565 1_556
La O1 La 121.7(3) 4_455 1_556
O2 O1 La 129.1(3) 3_565 1_556
O2 O1 La 123.4(2) . 1_556
O2 O1 La 173.4(3) 4_455 1_556
O2 O1 La 33.8(3) 3_566 1_556
O2 O1 La 24.9(3) 1_556 1_556
O2 O1 La 60.7(3) 4_456 1_556
O3 O1 La 62.1(3) . 1_556
O3 O1 La 111.4(4) 3_565 1_556
O3 O1 La 78.9(3) 4_455 1_556
Ga2 O1 La 150.51(9) 2_565 1_556
Ga3 O1 La 49.36(16) 1_556 1_556
Ga3 O1 La 53.30(17) 2_565 1_556
Ga3 O1 La 91.5(3) 4_456 1_556
O2 O1 La 53.5(3) 6 1_556
O2 O1 La 103.9(4) 5_455 1_556
O2 O1 La 80.3(3) 2_565 1_556
O3 O1 La 92.3(2) 6 1_556
O3 O1 La 142.0(3) 2_565 1_556
O3 O1 La 115.1(2) 5_455 1_556
Ga3 O1 La 116.61(5) . 1_556
Ga3 O1 La 119.30(5) 2_564 1_556
Ga3 O1 La 166.2(2) 4_455 1_556
Ga1 O1 La 90.96(13) 1_455 1_556
Nb O1 La 90.96(13) 1_455 1_556
Nb O1 La 80.06(11) . 1_556
Ga1 O1 La 80.06(11) . 1_556
Ga1 O1 La 129.0(3) 1_565 1_556
Nb O1 La 129.0(3) 1_565 1_556
O2 O1 La 93.5(2) 2_465 1_556
O2 O1 La 52.16(16) 5_445 1_556
O2 O1 La 99.3(3) 6_665 1_556
O3 O1 La 28.62(14) 6_556 1_556
O3 O1 La 77.9(3) 2_566 1_556
O3 O1 La 57.7(2) 5_456 1_556
Ga2 O1 La 29.50(9) 2_566 2_566
La O1 La 121.7(3) . 2_566
La O1 La 80.3(2) 2_565 2_566
La O1 La 121.7(3) 4_455 2_566
O2 O1 La 123.4(2) 3_565 2_566
O2 O1 La 173.4(3) . 2_566
O2 O1 La 129.1(3) 4_455 2_566
O2 O1 La 24.9(3) 3_566 2_566
O2 O1 La 60.7(3) 1_556 2_566
O2 O1 La 33.8(3) 4_456 2_566
O3 O1 La 78.9(3) . 2_566
O3 O1 La 62.1(3) 3_565 2_566
O3 O1 La 111.4(4) 4_455 2_566
Ga2 O1 La 150.51(9) 2_565 2_566
Ga3 O1 La 91.5(3) 1_556 2_566
Ga3 O1 La 49.36(16) 2_565 2_566
Ga3 O1 La 53.30(17) 4_456 2_566
O2 O1 La 103.9(4) 6 2_566
O2 O1 La 80.3(3) 5_455 2_566
O2 O1 La 53.5(3) 2_565 2_566
O3 O1 La 115.1(2) 6 2_566
O3 O1 La 92.3(2) 2_565 2_566
O3 O1 La 142.0(3) 5_455 2_566
Ga3 O1 La 166.2(2) . 2_566
Ga3 O1 La 116.61(5) 2_564 2_566
Ga3 O1 La 119.30(5) 4_455 2_566
Ga1 O1 La 129.0(3) 1_455 2_566
Nb O1 La 129.0(3) 1_455 2_566
Nb O1 La 90.96(13) . 2_566
Ga1 O1 La 90.96(13) . 2_566
Ga1 O1 La 80.06(11) 1_565 2_566
Nb O1 La 80.06(11) 1_565 2_566
O2 O1 La 99.3(3) 2_465 2_566
O2 O1 La 93.6(2) 5_445 2_566
O2 O1 La 52.16(16) 6_665 2_566
O3 O1 La 57.7(2) 6_556 2_566
O3 O1 La 28.62(14) 2_566 2_566
O3 O1 La 77.9(3) 5_456 2_566
La O1 La 50.48(15) 1_556 2_566
Ga2 O1 La 29.49(9) 2_566 4_456
La O1 La 121.7(3) . 4_456
La O1 La 121.7(3) 2_565 4_456
La O1 La 80.3(2) 4_455 4_456
O2 O1 La 173.4(3) 3_565 4_456
O2 O1 La 129.1(3) . 4_456
O2 O1 La 123.4(2) 4_455 4_456
O2 O1 La 60.7(3) 3_566 4_456
O2 O1 La 33.8(3) 1_556 4_456
O2 O1 La 24.9(3) 4_456 4_456
O3 O1 La 111.4(4) . 4_456
O3 O1 La 78.9(3) 3_565 4_456
O3 O1 La 62.1(3) 4_455 4_456
Ga2 O1 La 150.50(9) 2_565 4_456
Ga3 O1 La 53.30(17) 1_556 4_456
Ga3 O1 La 91.5(3) 2_565 4_456
Ga3 O1 La 49.36(16) 4_456 4_456
O2 O1 La 80.3(3) 6 4_456
O2 O1 La 53.5(3) 5_455 4_456
O2 O1 La 103.9(4) 2_565 4_456
O3 O1 La 142.0(3) 6 4_456
O3 O1 La 115.1(2) 2_565 4_456
O3 O1 La 92.3(2) 5_455 4_456
Ga3 O1 La 119.30(5) . 4_456
Ga3 O1 La 166.2(2) 2_564 4_456
Ga3 O1 La 116.61(5) 4_455 4_456
Ga1 O1 La 80.06(11) 1_455 4_456
Nb O1 La 80.06(11) 1_455 4_456
Nb O1 La 129.0(3) . 4_456
Ga1 O1 La 129.0(3) . 4_456
Ga1 O1 La 90.96(13) 1_565 4_456
Nb O1 La 90.96(13) 1_565 4_456
O2 O1 La 52.16(16) 2_465 4_456
O2 O1 La 99.3(3) 5_445 4_456
O2 O1 La 93.6(2) 6_665 4_456
O3 O1 La 77.9(3) 6_556 4_456
O3 O1 La 57.7(2) 2_566 4_456
O3 O1 La 28.62(14) 5_456 4_456
La O1 La 50.48(15) 1_556 4_456
La O1 La 50.48(15) 2_566 4_456
Ga2 O1 O3 115.1(2) 2_566 5
La O1 O3 61.15(18) . 5
La O1 O3 49.37(16) 2_565 5
La O1 O3 134.6(5) 4_455 5
O2 O1 O3 31.3(2) 3_565 5
O2 O1 O3 82.6(4) . 5
O2 O1 O3 85.5(4) 4_455 5
O2 O1 O3 83.8(2) 3_566 5
O2 O1 O3 125.1(4) 1_556 5
O2 O1 O3 128.4(4) 4_456 5
O3 O1 O3 40.2(3) . 5
O3 O1 O3 96.8(3) 3_565 5
O3 O1 O3 142.1(3) 4_455 5
Ga2 O1 O3 64.9(2) 2_565 5
Ga3 O1 O3 128.93(11) 1_556 5
Ga3 O1 O3 53.11(13) 2_565 5
Ga3 O1 O3 124.65(11) 4_456 5
O2 O1 O3 100.1(2) 6 5
O2 O1 O3 143.5(3) 5_455 5
O2 O1 O3 43.6(3) 2_565 5
O3 O1 O3 33.5(2) 6 5
O3 O1 O3 72.1(3) 2_565 5
O3 O1 O3 122.0(4) 5_455 5
Ga3 O1 O3 91.2(3) . 5
Ga3 O1 O3 21.91(13) 2_564 5
Ga3 O1 O3 88.6(2) 4_455 5
Ga1 O1 O3 126.9(3) 1_455 5
Nb O1 O3 126.9(3) 1_455 5
Nb O1 O3 23.70(11) . 5
Ga1 O1 O3 23.70(11) . 5
Ga1 O1 O3 94.78(17) 1_565 5
Nb O1 O3 94.78(17) 1_565 5
O2 O1 O3 163.5(4) 2_465 5
O2 O1 O3 67.23(18) 5_445 5
O2 O1 O3 67.59(18) 6_665 5
O3 O1 O3 72.59(14) 6_556 5
O3 O1 O3 99.86(19) 2_566 5
O3 O1 O3 156.8(3) 5_456 5
La O1 O3 101.10(16) 1_556 5
La O1 O3 95.98(16) 2_566 5
La O1 O3 144.3(3) 4_456 5
Ga2 O1 O3 115.1(2) 2_566 2_455
La O1 O3 49.37(16) . 2_455
La O1 O3 134.6(5) 2_565 2_455
La O1 O3 61.15(18) 4_455 2_455
O2 O1 O3 85.5(4) 3_565 2_455
O2 O1 O3 31.3(2) . 2_455
O2 O1 O3 82.6(4) 4_455 2_455
O2 O1 O3 128.4(4) 3_566 2_455
O2 O1 O3 83.8(2) 1_556 2_455
O2 O1 O3 125.1(4) 4_456 2_455
O3 O1 O3 96.8(3) . 2_455
O3 O1 O3 142.1(3) 3_565 2_455
O3 O1 O3 40.2(3) 4_455 2_455
Ga2 O1 O3 64.9(2) 2_565 2_455
Ga3 O1 O3 53.11(13) 1_556 2_455
Ga3 O1 O3 124.65(11) 2_565 2_455
Ga3 O1 O3 128.93(11) 4_456 2_455
O2 O1 O3 43.6(3) 6 2_455
O2 O1 O3 100.1(2) 5_455 2_455
O2 O1 O3 143.5(3) 2_565 2_455
O3 O1 O3 72.1(3) 6 2_455
O3 O1 O3 122.0(4) 2_565 2_455
O3 O1 O3 33.5(2) 5_455 2_455
Ga3 O1 O3 21.91(13) . 2_455
Ga3 O1 O3 88.6(2) 2_564 2_455
Ga3 O1 O3 91.2(3) 4_455 2_455
Ga1 O1 O3 23.70(11) 1_455 2_455
Nb O1 O3 23.70(11) 1_455 2_455
Nb O1 O3 94.78(17) . 2_455
Ga1 O1 O3 94.78(17) . 2_455
Ga1 O1 O3 126.9(3) 1_565 2_455
Nb O1 O3 126.9(3) 1_565 2_455
O2 O1 O3 67.23(18) 2_465 2_455
O2 O1 O3 67.59(18) 5_445 2_455
O2 O1 O3 163.5(4) 6_665 2_455
O3 O1 O3 99.86(19) 6_556 2_455
O3 O1 O3 156.8(3) 2_566 2_455
O3 O1 O3 72.59(14) 5_456 2_455
La O1 O3 95.98(16) 1_556 2_455
La O1 O3 144.3(3) 2_566 2_455
La O1 O3 101.10(16) 4_456 2_455
O3 O1 O3 103.3(3) 5 2_455
Ga2 O1 O3 115.1(2) 2_566 6_565
La O1 O3 134.6(5) . 6_565
La O1 O3 61.15(18) 2_565 6_565
La O1 O3 49.37(16) 4_455 6_565
O2 O1 O3 82.6(4) 3_565 6_565
O2 O1 O3 85.5(4) . 6_565
O2 O1 O3 31.3(2) 4_455 6_565
O2 O1 O3 125.1(4) 3_566 6_565
O2 O1 O3 128.4(4) 1_556 6_565
O2 O1 O3 83.8(2) 4_456 6_565
O3 O1 O3 142.1(3) . 6_565
O3 O1 O3 40.2(3) 3_565 6_565
O3 O1 O3 96.8(3) 4_455 6_565
Ga2 O1 O3 64.9(2) 2_565 6_565
Ga3 O1 O3 124.65(11) 1_556 6_565
Ga3 O1 O3 128.93(11) 2_565 6_565
Ga3 O1 O3 53.11(13) 4_456 6_565
O2 O1 O3 143.5(3) 6 6_565
O2 O1 O3 43.6(3) 5_455 6_565
O2 O1 O3 100.1(2) 2_565 6_565
O3 O1 O3 122.0(4) 6 6_565
O3 O1 O3 33.5(2) 2_565 6_565
O3 O1 O3 72.1(3) 5_455 6_565
Ga3 O1 O3 88.6(2) . 6_565
Ga3 O1 O3 91.2(3) 2_564 6_565
Ga3 O1 O3 21.91(13) 4_455 6_565
Ga1 O1 O3 94.78(17) 1_455 6_565
Nb O1 O3 94.78(17) 1_455 6_565
Nb O1 O3 126.9(3) . 6_565
Ga1 O1 O3 126.9(3) . 6_565
Ga1 O1 O3 23.70(11) 1_565 6_565
Nb O1 O3 23.70(11) 1_565 6_565
O2 O1 O3 67.59(18) 2_465 6_565
O2 O1 O3 163.5(4) 5_445 6_565
O2 O1 O3 67.23(18) 6_665 6_565
O3 O1 O3 156.8(3) 6_556 6_565
O3 O1 O3 72.59(14) 2_566 6_565
O3 O1 O3 99.86(19) 5_456 6_565
La O1 O3 144.3(3) 1_556 6_565
La O1 O3 101.09(16) 2_566 6_565
La O1 O3 95.98(16) 4_456 6_565
O3 O1 O3 103.3(3) 5 6_565
O3 O1 O3 103.3(3) 2_455 6_565
Ga2 O1 Ga2 71.42(17) 2_566 1_665
La O1 Ga2 111.58(3) . 1_665
La O1 Ga2 40.44(15) 2_565 1_665
La O1 Ga2 135.79(2) 4_455 1_665
O2 O1 Ga2 81.2(2) 3_565 1_665
O2 O1 Ga2 138.5(4) . 1_665
O2 O1 Ga2 101.5(4) 4_455 1_665
O2 O1 Ga2 48.2(3) 3_566 1_665
O2 O1 Ga2 100.6(4) 1_556 1_665
O2 O1 Ga2 70.5(3) 4_456 1_665
O3 O1 Ga2 65.1(2) . 1_665
O3 O1 Ga2 54.0(3) 3_565 1_665
O3 O1 Ga2 154.3(5) 4_455 1_665
Ga2 O1 Ga2 108.59(17) 2_565 1_665
Ga3 O1 Ga2 130.6(4) 1_556 1_665
Ga3 O1 Ga2 40.26(5) 2_565 1_665
Ga3 O1 Ga2 70.39(11) 4_456 1_665
O2 O1 Ga2 127.3(3) 6 1_665
O2 O1 Ga2 99.1(2) 5_455 1_665
O2 O1 Ga2 17.1(2) 2_565 1_665
O3 O1 Ga2 88.75(13) 6 1_665
O3 O1 Ga2 62.37(18) 2_565 1_665
O3 O1 Ga2 160.8(2) 5_455 1_665
Ga3 O1 Ga2 148.3(3) . 1_665
Ga3 O1 Ga2 76.04(6) 2_564 1_665
Ga3 O1 Ga2 95.10(8) 4_455 1_665
Ga1 O1 Ga2 171.9(4) 1_455 1_665
Nb O1 Ga2 171.9(4) 1_455 1_665
Nb O1 Ga2 65.91(2) . 1_665
Ga1 O1 Ga2 65.91(2) . 1_665
Ga1 O1 Ga2 65.91(2) 1_565 1_665
Nb O1 Ga2 65.91(2) 1_565 1_665
O2 O1 Ga2 132.0(2) 2_465 1_665
O2 O1 Ga2 96.77(15) 5_445 1_665
O2 O1 Ga2 21.68(13) 6_665 1_665
O3 O1 Ga2 69.27(17) 6_556 1_665
O3 O1 Ga2 41.50(14) 2_566 1_665
O3 O1 Ga2 120.6(3) 5_456 1_665
La O1 Ga2 81.87(19) 1_556 1_665
La O1 Ga2 42.94(9) 2_566 1_665
La O1 Ga2 92.4(2) 4_456 1_665
O3 O1 Ga2 58.78(12) 5 1_665
O3 O1 Ga2 160.68(16) 2_455 1_665
O3 O1 Ga2 88.90(11) 6_565 1_665
Ga2 O1 Ga2 71.42(17) 2_566 .
La O1 Ga2 40.44(15) . .
La O1 Ga2 135.79(2) 2_565 .
La O1 Ga2 111.58(3) 4_455 .
O2 O1 Ga2 101.5(4) 3_565 .
O2 O1 Ga2 81.2(2) . .
O2 O1 Ga2 138.5(4) 4_455 .
O2 O1 Ga2 70.5(3) 3_566 .
O2 O1 Ga2 48.2(3) 1_556 .
O2 O1 Ga2 100.6(4) 4_456 .
O3 O1 Ga2 54.0(3) . .
O3 O1 Ga2 154.3(5) 3_565 .
O3 O1 Ga2 65.1(2) 4_455 .
Ga2 O1 Ga2 108.59(17) 2_565 .
Ga3 O1 Ga2 40.26(5) 1_556 .
Ga3 O1 Ga2 70.39(11) 2_565 .
Ga3 O1 Ga2 130.6(4) 4_456 .
O2 O1 Ga2 17.1(2) 6 .
O2 O1 Ga2 127.3(3) 5_455 .
O2 O1 Ga2 99.1(2) 2_565 .
O3 O1 Ga2 62.37(18) 6 .
O3 O1 Ga2 160.8(2) 2_565 .
O3 O1 Ga2 88.75(13) 5_455 .
Ga3 O1 Ga2 76.04(6) . .
Ga3 O1 Ga2 95.11(8) 2_564 .
Ga3 O1 Ga2 148.3(3) 4_455 .
Ga1 O1 Ga2 65.91(2) 1_455 .
Nb O1 Ga2 65.91(2) 1_455 .
Nb O1 Ga2 65.91(2) . .
Ga1 O1 Ga2 65.91(2) . .
Ga1 O1 Ga2 171.9(4) 1_565 .
Nb O1 Ga2 171.9(4) 1_565 .
O2 O1 Ga2 96.77(15) 2_465 .
O2 O1 Ga2 21.68(13) 5_445 .
O2 O1 Ga2 132.0(2) 6_665 .
O3 O1 Ga2 41.50(14) 6_556 .
O3 O1 Ga2 120.6(3) 2_566 .
O3 O1 Ga2 69.27(17) 5_456 .
La O1 Ga2 42.94(9) 1_556 .
La O1 Ga2 92.4(2) 2_566 .
La O1 Ga2 81.87(19) 4_456 .
O3 O1 Ga2 88.90(11) 5 .
O3 O1 Ga2 58.78(12) 2_455 .
O3 O1 Ga2 160.68(16) 6_565 .
Ga2 O1 Ga2 110.34(17) 1_665 .
Ga2 O1 Ga2 71.41(17) 2_566 1_565
La O1 Ga2 135.79(2) . 1_565
La O1 Ga2 111.58(3) 2_565 1_565
La O1 Ga2 40.44(15) 4_455 1_565
O2 O1 Ga2 138.5(4) 3_565 1_565
O2 O1 Ga2 101.5(4) . 1_565
O2 O1 Ga2 81.2(2) 4_455 1_565
O2 O1 Ga2 100.6(4) 3_566 1_565
O2 O1 Ga2 70.5(3) 1_556 1_565
O2 O1 Ga2 48.2(3) 4_456 1_565
O3 O1 Ga2 154.3(5) . 1_565
O3 O1 Ga2 65.1(2) 3_565 1_565
O3 O1 Ga2 54.0(3) 4_455 1_565
Ga2 O1 Ga2 108.58(17) 2_565 1_565
Ga3 O1 Ga2 70.39(11) 1_556 1_565
Ga3 O1 Ga2 130.6(4) 2_565 1_565
Ga3 O1 Ga2 40.26(5) 4_456 1_565
O2 O1 Ga2 99.1(2) 6 1_565
O2 O1 Ga2 17.1(2) 5_455 1_565
O2 O1 Ga2 127.3(3) 2_565 1_565
O3 O1 Ga2 160.8(2) 6 1_565
O3 O1 Ga2 88.75(13) 2_565 1_565
O3 O1 Ga2 62.37(18) 5_455 1_565
Ga3 O1 Ga2 95.11(8) . 1_565
Ga3 O1 Ga2 148.3(3) 2_564 1_565
Ga3 O1 Ga2 76.04(6) 4_455 1_565
Ga1 O1 Ga2 65.91(2) 1_455 1_565
Nb O1 Ga2 65.91(2) 1_455 1_565
Nb O1 Ga2 171.9(4) . 1_565
Ga1 O1 Ga2 171.9(4) . 1_565
Ga1 O1 Ga2 65.91(2) 1_565 1_565
Nb O1 Ga2 65.91(2) 1_565 1_565
O2 O1 Ga2 21.68(13) 2_465 1_565
O2 O1 Ga2 132.0(2) 5_445 1_565
O2 O1 Ga2 96.77(15) 6_665 1_565
O3 O1 Ga2 120.6(3) 6_556 1_565
O3 O1 Ga2 69.27(17) 2_566 1_565
O3 O1 Ga2 41.50(14) 5_456 1_565
La O1 Ga2 92.4(2) 1_556 1_565
La O1 Ga2 81.87(19) 2_566 1_565
La O1 Ga2 42.94(9) 4_456 1_565
O3 O1 Ga2 160.68(16) 5 1_565
O3 O1 Ga2 88.90(11) 2_455 1_565
O3 O1 Ga2 58.78(12) 6_565 1_565
Ga2 O1 Ga2 110.34(17) 1_665 1_565
Ga2 O1 Ga2 110.34(17) . 1_565
Ga2 O1 O1 110.3(3) 2_566 2_565
La O1 O1 98.1(3) . 2_565
La O1 O1 12.27(3) 2_565 2_565
La O1 O1 119.1(4) 4_455 2_565
O2 O1 O1 45.4(3) 3_565 2_565
O2 O1 O1 101.0(5) . 2_565
O2 O1 O1 69.3(5) 4_455 2_565
O2 O1 O1 84.6(3) 3_566 2_565
O2 O1 O1 138.3(5) 1_556 2_565
O2 O1 O1 103.6(4) 4_456 2_565
O3 O1 O1 70.0(3) . 2_565
O3 O1 O1 59.5(2) 3_565 2_565
O3 O1 O1 165.1(6) 4_455 2_565
Ga2 O1 O1 69.7(3) 2_565 2_565
Ga3 O1 O1 162.6(3) 1_556 2_565
Ga3 O1 O1 63.54(10) 2_565 2_565
Ga3 O1 O1 88.72(9) 4_456 2_565
O2 O1 O1 137.1(2) 6 2_565
O2 O1 O1 106.8(2) 5_455 2_565
O2 O1 O1 35.6(2) 2_565 2_565
O3 O1 O1 70.2(2) 6 2_565
O3 O1 O1 39.05(17) 2_565 2_565
O3 O1 O1 128.1(5) 5_455 2_565
Ga3 O1 O1 111.0(5) . 2_565
Ga3 O1 O1 43.7(2) 2_564 2_565
Ga3 O1 O1 66.7(2) 4_455 2_565
Ga1 O1 O1 149.3(5) 1_455 2_565
Nb O1 O1 149.3(5) 1_455 2_565
Nb O1 O1 58.39(6) . 2_565
Ga1 O1 O1 58.39(6) . 2_565
Ga1 O1 O1 58.39(6) 1_565 2_565
Nb O1 O1 58.39(6) 1_565 2_565
O2 O1 O1 139.51(17) 2_465 2_565
O2 O1 O1 102.44(13) 5_445 2_565
O2 O1 O1 34.83(18) 6_665 2_565
O3 O1 O1 93.47(19) 6_556 2_565
O3 O1 O1 70.7(2) 2_566 2_565
O3 O1 O1 156.2(4) 5_456 2_565
La O1 O1 115.8(3) 1_556 2_565
La O1 O1 81.5(2) 2_566 2_565
La O1 O1 128.1(3) 4_456 2_565
O3 O1 O1 37.44(14) 5 2_565
O3 O1 O1 130.8(5) 2_455 2_565
O3 O1 O1 72.5(2) 6_565 2_565
Ga2 O1 O1 38.84(17) 1_665 2_565
Ga2 O1 O1 123.708(18) . 2_565
Ga2 O1 O1 123.708(19) 1_565 2_565
Ga2 O1 O1 110.3(3) 2_566 2_455
La O1 O1 12.27(3) . 2_455
La O1 O1 119.1(4) 2_565 2_455
La O1 O1 98.1(3) 4_455 2_455
O2 O1 O1 69.3(5) 3_565 2_455
O2 O1 O1 45.4(3) . 2_455
O2 O1 O1 101.0(5) 4_455 2_455
O2 O1 O1 103.6(4) 3_566 2_455
O2 O1 O1 84.6(3) 1_556 2_455
O2 O1 O1 138.3(5) 4_456 2_455
O3 O1 O1 59.5(2) . 2_455
O3 O1 O1 165.1(6) 3_565 2_455
O3 O1 O1 70.0(3) 4_455 2_455
Ga2 O1 O1 69.7(3) 2_565 2_455
Ga3 O1 O1 63.54(10) 1_556 2_455
Ga3 O1 O1 88.72(9) 2_565 2_455
Ga3 O1 O1 162.6(3) 4_456 2_455
O2 O1 O1 35.6(2) 6 2_455
O2 O1 O1 137.1(2) 5_455 2_455
O2 O1 O1 106.8(2) 2_565 2_455
O3 O1 O1 39.05(17) 6 2_455
O3 O1 O1 128.1(5) 2_565 2_455
O3 O1 O1 70.2(2) 5_455 2_455
Ga3 O1 O1 43.7(2) . 2_455
Ga3 O1 O1 66.7(2) 2_564 2_455
Ga3 O1 O1 111.0(5) 4_455 2_455
Ga1 O1 O1 58.39(6) 1_455 2_455
Nb O1 O1 58.39(6) 1_455 2_455
Nb O1 O1 58.39(6) . 2_455
Ga1 O1 O1 58.39(6) . 2_455
Ga1 O1 O1 149.3(5) 1_565 2_455
Nb O1 O1 149.3(5) 1_565 2_455
O2 O1 O1 102.44(13) 2_465 2_455
O2 O1 O1 34.83(18) 5_445 2_455
O2 O1 O1 139.51(17) 6_665 2_455
O3 O1 O1 70.7(2) 6_556 2_455
O3 O1 O1 156.2(4) 2_566 2_455
O3 O1 O1 93.47(19) 5_456 2_455
La O1 O1 81.5(2) 1_556 2_455
La O1 O1 128.1(3) 2_566 2_455
La O1 O1 115.8(3) 4_456 2_455
O3 O1 O1 72.5(2) 5 2_455
O3 O1 O1 37.44(14) 2_455 2_455
O3 O1 O1 130.8(5) 6_565 2_455
Ga2 O1 O1 123.708(18) 1_665 2_455
Ga2 O1 O1 38.84(17) . 2_455
Ga2 O1 O1 123.708(19) 1_565 2_455
O1 O1 O1 108.7(3) 2_565 2_455
Ga2 O1 O1 110.3(3) 2_566 2_465
La O1 O1 119.1(4) . 2_465
La O1 O1 98.1(3) 2_565 2_465
La O1 O1 12.27(3) 4_455 2_465
O2 O1 O1 101.0(5) 3_565 2_465
O2 O1 O1 69.3(5) . 2_465
O2 O1 O1 45.4(3) 4_455 2_465
O2 O1 O1 138.3(5) 3_566 2_465
O2 O1 O1 103.6(4) 1_556 2_465
O2 O1 O1 84.6(3) 4_456 2_465
O3 O1 O1 165.1(6) . 2_465
O3 O1 O1 70.0(3) 3_565 2_465
O3 O1 O1 59.5(2) 4_455 2_465
Ga2 O1 O1 69.7(3) 2_565 2_465
Ga3 O1 O1 88.72(9) 1_556 2_465
Ga3 O1 O1 162.6(3) 2_565 2_465
Ga3 O1 O1 63.54(10) 4_456 2_465
O2 O1 O1 106.8(2) 6 2_465
O2 O1 O1 35.6(2) 5_455 2_465
O2 O1 O1 137.1(2) 2_565 2_465
O3 O1 O1 128.1(5) 6 2_465
O3 O1 O1 70.2(2) 2_565 2_465
O3 O1 O1 39.05(17) 5_455 2_465
Ga3 O1 O1 66.7(2) . 2_465
Ga3 O1 O1 111.0(5) 2_564 2_465
Ga3 O1 O1 43.7(2) 4_455 2_465
Ga1 O1 O1 58.39(6) 1_455 2_465
Nb O1 O1 58.39(6) 1_455 2_465
Nb O1 O1 149.3(5) . 2_465
Ga1 O1 O1 149.3(5) . 2_465
Ga1 O1 O1 58.39(6) 1_565 2_465
Nb O1 O1 58.39(6) 1_565 2_465
O2 O1 O1 34.83(18) 2_465 2_465
O2 O1 O1 139.51(17) 5_445 2_465
O2 O1 O1 102.44(13) 6_665 2_465
O3 O1 O1 156.2(4) 6_556 2_465
O3 O1 O1 93.47(19) 2_566 2_465
O3 O1 O1 70.7(2) 5_456 2_465
La O1 O1 128.1(3) 1_556 2_465
La O1 O1 115.8(3) 2_566 2_465
La O1 O1 81.5(2) 4_456 2_465
O3 O1 O1 130.8(5) 5 2_465
O3 O1 O1 72.5(2) 2_455 2_465
O3 O1 O1 37.44(14) 6_565 2_465
Ga2 O1 O1 123.708(19) 1_665 2_465
Ga2 O1 O1 123.708(19) . 2_465
Ga2 O1 O1 38.84(17) 1_565 2_465
O1 O1 O1 108.7(3) 2_565 2_465
O1 O1 O1 108.7(3) 2_455 2_465
Ga2 O1 O1 0.0 2_566 1_556
La O1 O1 109.8(3) . 1_556
La O1 O1 109.8(3) 2_565 1_556
La O1 O1 109.8(3) 4_455 1_556
O2 O1 O1 146.4(3) 3_565 1_556
O2 O1 O1 146.4(3) . 1_556
O2 O1 O1 146.4(3) 4_455 1_556
O2 O1 O1 31.4(3) 3_566 1_556
O2 O1 O1 31.4(3) 1_556 1_556
O2 O1 O1 31.4(3) 4_456 1_556
O3 O1 O1 83.5(3) . 1_556
O3 O1 O1 83.5(3) 3_565 1_556
O3 O1 O1 83.5(3) 4_455 1_556
Ga2 O1 O1 179.997(1) 2_565 1_556
Ga3 O1 O1 62.1(2) 1_556 1_556
Ga3 O1 O1 62.1(2) 2_565 1_556
Ga3 O1 O1 62.1(2) 4_456 1_556
O2 O1 O1 78.5(3) 6 1_556
O2 O1 O1 78.5(3) 5_455 1_556
O2 O1 O1 78.5(3) 2_565 1_556
O3 O1 O1 118.7(3) 6 1_556
O3 O1 O1 118.7(3) 2_565 1_556
O3 O1 O1 118.7(3) 5_455 1_556
Ga3 O1 O1 136.96(13) . 1_556
Ga3 O1 O1 136.96(13) 2_564 1_556
Ga3 O1 O1 136.96(13) 4_455 1_556
Ga1 O1 O1 100.45(19) 1_455 1_556
Nb O1 O1 100.45(19) 1_455 1_556
Nb O1 O1 100.46(18) . 1_556
Ga1 O1 O1 100.46(18) . 1_556
Ga1 O1 O1 100.45(18) 1_565 1_556
Nb O1 O1 100.45(18) 1_565 1_556
O2 O1 O1 81.4(2) 2_465 1_556
O2 O1 O1 81.4(2) 5_445 1_556
O2 O1 O1 81.4(2) 6_665 1_556
O3 O1 O1 51.6(2) 6_556 1_556
O3 O1 O1 51.6(2) 2_566 1_556
O3 O1 O1 51.6(2) 5_456 1_556
La O1 O1 29.49(9) 1_556 1_556
La O1 O1 29.50(9) 2_566 1_556
La O1 O1 29.49(9) 4_456 1_556
O3 O1 O1 115.1(2) 5 1_556
O3 O1 O1 115.1(2) 2_455 1_556
O3 O1 O1 115.1(2) 6_565 1_556
Ga2 O1 O1 71.42(17) 1_665 1_556
Ga2 O1 O1 71.42(17) . 1_556
Ga2 O1 O1 71.41(17) 1_565 1_556
O1 O1 O1 110.3(3) 2_565 1_556
O1 O1 O1 110.3(3) 2_455 1_556
O1 O1 O1 110.3(3) 2_465 1_556
Ga2 O1 O1 179.996(1) 2_566 1_554
La O1 O1 70.2(3) . 1_554
La O1 O1 70.2(3) 2_565 1_554
La O1 O1 70.2(3) 4_455 1_554
O2 O1 O1 33.6(3) 3_565 1_554
O2 O1 O1 33.6(3) . 1_554
O2 O1 O1 33.6(3) 4_455 1_554
O2 O1 O1 148.6(3) 3_566 1_554
O2 O1 O1 148.6(3) 1_556 1_554
O2 O1 O1 148.6(3) 4_456 1_554
O3 O1 O1 96.5(3) . 1_554
O3 O1 O1 96.5(3) 3_565 1_554
O3 O1 O1 96.5(3) 4_455 1_554
Ga2 O1 O1 0.0 2_565 1_554
Ga3 O1 O1 117.9(2) 1_556 1_554
Ga3 O1 O1 117.9(2) 2_565 1_554
Ga3 O1 O1 117.9(2) 4_456 1_554
O2 O1 O1 101.5(3) 6 1_554
O2 O1 O1 101.5(3) 5_455 1_554
O2 O1 O1 101.5(3) 2_565 1_554
O3 O1 O1 61.3(3) 6 1_554
O3 O1 O1 61.3(3) 2_565 1_554
O3 O1 O1 61.3(3) 5_455 1_554
Ga3 O1 O1 43.04(13) . 1_554
Ga3 O1 O1 43.04(13) 2_564 1_554
Ga3 O1 O1 43.04(13) 4_455 1_554
Ga1 O1 O1 79.54(18) 1_455 1_554
Nb O1 O1 79.54(18) 1_455 1_554
Nb O1 O1 79.55(19) . 1_554
Ga1 O1 O1 79.55(19) . 1_554
Ga1 O1 O1 79.55(18) 1_565 1_554
Nb O1 O1 79.55(18) 1_565 1_554
O2 O1 O1 98.6(2) 2_465 1_554
O2 O1 O1 98.6(2) 5_445 1_554
O2 O1 O1 98.6(2) 6_665 1_554
O3 O1 O1 128.4(2) 6_556 1_554
O3 O1 O1 128.4(2) 2_566 1_554
O3 O1 O1 128.4(2) 5_456 1_554
La O1 O1 150.51(9) 1_556 1_554
La O1 O1 150.51(9) 2_566 1_554
La O1 O1 150.50(9) 4_456 1_554
O3 O1 O1 64.9(2) 5 1_554
O3 O1 O1 64.9(2) 2_455 1_554
O3 O1 O1 64.9(2) 6_565 1_554
Ga2 O1 O1 108.59(17) 1_665 1_554
Ga2 O1 O1 108.59(17) . 1_554
Ga2 O1 O1 108.58(17) 1_565 1_554
O1 O1 O1 69.7(3) 2_565 1_554
O1 O1 O1 69.7(3) 2_455 1_554
O1 O1 O1 69.7(3) 2_465 1_554
O1 O1 O1 180.0 1_556 1_554
Ga2 O1 Ga3 71.46(16) 2_566 2_465
La O1 Ga3 100.64(5) . 2_465
La O1 Ga3 147.01(3) 2_565 2_465
La O1 Ga3 45.51(14) 4_455 2_465
O2 O1 Ga3 140.5(4) 3_565 2_465
O2 O1 Ga3 83.8(3) . 2_465
O2 O1 Ga3 97.5(3) 4_455 2_465
O2 O1 Ga3 101.9(4) 3_566 2_465
O2 O1 Ga3 51.5(3) 1_556 2_465
O2 O1 Ga3 66.6(3) 4_456 2_465
O3 O1 Ga3 129.9(3) . 2_465
O3 O1 Ga3 101.0(3) 3_565 2_465
O3 O1 Ga3 19.7(3) 4_455 2_465
Ga2 O1 Ga3 108.54(16) 2_565 2_465
Ga3 O1 Ga3 36.92(5) 1_556 2_465
Ga3 O1 Ga3 129.3(3) 2_565 2_465
Ga3 O1 Ga3 73.71(12) 4_456 2_465
O2 O1 Ga3 63.53(19) 6 2_465
O2 O1 Ga3 52.7(2) 5_455 2_465
O2 O1 Ga3 149.4(5) 2_565 2_465
O3 O1 Ga3 128.18(15) 6 2_465
O3 O1 Ga3 121.12(14) 2_565 2_465
O3 O1 Ga3 47.38(19) 5_455 2_465
Ga3 O1 Ga3 74.33(5) . 2_465
Ga3 O1 Ga3 146.8(2) 2_564 2_465
Ga3 O1 Ga3 97.51(8) 4_455 2_465
Ga1 O1 Ga3 36.16(2) 1_455 2_465
Nb O1 Ga3 36.16(2) 1_455 2_465
Nb O1 Ga3 142.32(8) . 2_465
Ga1 O1 Ga3 142.32(8) . 2_465
Ga1 O1 Ga3 100.89(4) 1_565 2_465
Nb O1 Ga3 100.89(4) 1_565 2_465
O2 O1 Ga3 20.33(13) 2_465 2_465
O2 O1 Ga3 98.23(17) 5_445 2_465
O2 O1 Ga3 130.7(2) 6_665 2_465
O3 O1 Ga3 102.6(2) 6_556 2_465
O3 O1 Ga3 97.4(2) 2_566 2_465
O3 O1 Ga3 20.16(12) 5_456 2_465
La O1 Ga3 76.33(16) 1_556 2_465
La O1 Ga3 96.1(2) 2_566 2_465
La O1 Ga3 45.60(8) 4_456 2_465
O3 O1 Ga3 161.65(16) 5 2_465
O3 O1 Ga3 59.50(11) 2_455 2_465
O3 O1 Ga3 87.91(11) 6_565 2_465
Ga2 O1 Ga3 137.1(3) 1_665 2_465
Ga2 O1 Ga3 76.83(9) . 2_465
Ga2 O1 Ga3 36.04(4) 1_565 2_465
O1 O1 Ga3 159.28(4) 2_565 2_465
O1 O1 Ga3 89.13(6) 2_455 2_465
O1 O1 Ga3 53.85(12) 2_465 2_465
O1 O1 Ga3 71.46(16) 1_556 2_465
O1 O1 Ga3 108.54(16) 1_554 2_465
Ga2 O1 Ga3 71.46(16) 2_566 4_446
La O1 Ga3 45.51(14) . 4_446
La O1 Ga3 100.64(5) 2_565 4_446
La O1 Ga3 147.01(3) 4_455 4_446
O2 O1 Ga3 83.8(3) 3_565 4_446
O2 O1 Ga3 97.5(3) . 4_446
O2 O1 Ga3 140.5(4) 4_455 4_446
O2 O1 Ga3 51.5(3) 3_566 4_446
O2 O1 Ga3 66.6(3) 1_556 4_446
O2 O1 Ga3 101.9(4) 4_456 4_446
O3 O1 Ga3 19.7(3) . 4_446
O3 O1 Ga3 129.9(3) 3_565 4_446
O3 O1 Ga3 101.0(3) 4_455 4_446
Ga2 O1 Ga3 108.54(16) 2_565 4_446
Ga3 O1 Ga3 73.71(12) 1_556 4_446
Ga3 O1 Ga3 36.92(5) 2_565 4_446
Ga3 O1 Ga3 129.3(3) 4_456 4_446
O2 O1 Ga3 52.7(2) 6 4_446
O2 O1 Ga3 149.4(5) 5_455 4_446
O2 O1 Ga3 63.53(19) 2_565 4_446
O3 O1 Ga3 47.38(19) 6 4_446
O3 O1 Ga3 128.18(15) 2_565 4_446
O3 O1 Ga3 121.12(14) 5_455 4_446
Ga3 O1 Ga3 97.51(8) . 4_446
Ga3 O1 Ga3 74.33(5) 2_564 4_446
Ga3 O1 Ga3 146.8(2) 4_455 4_446
Ga1 O1 Ga3 100.90(4) 1_455 4_446
Nb O1 Ga3 100.90(4) 1_455 4_446
Nb O1 Ga3 36.16(3) . 4_446
Ga1 O1 Ga3 36.16(3) . 4_446
Ga1 O1 Ga3 142.32(8) 1_565 4_446
Nb O1 Ga3 142.32(8) 1_565 4_446
O2 O1 Ga3 130.7(2) 2_465 4_446
O2 O1 Ga3 20.33(13) 5_445 4_446
O2 O1 Ga3 98.23(17) 6_665 4_446
O3 O1 Ga3 20.16(12) 6_556 4_446
O3 O1 Ga3 102.6(2) 2_566 4_446
O3 O1 Ga3 97.4(2) 5_456 4_446
La O1 Ga3 45.60(8) 1_556 4_446
La O1 Ga3 76.33(16) 2_566 4_446
La O1 Ga3 96.1(2) 4_456 4_446
O3 O1 Ga3 59.50(11) 5 4_446
O3 O1 Ga3 87.92(11) 2_455 4_446
O3 O1 Ga3 161.65(16) 6_565 4_446
Ga2 O1 Ga3 76.83(9) 1_665 4_446
Ga2 O1 Ga3 36.04(4) . 4_446
Ga2 O1 Ga3 137.1(3) 1_565 4_446
O1 O1 Ga3 89.13(6) 2_565 4_446
O1 O1 Ga3 53.85(12) 2_455 4_446
O1 O1 Ga3 159.28(4) 2_465 4_446
O1 O1 Ga3 71.46(16) 1_556 4_446
O1 O1 Ga3 108.54(16) 1_554 4_446
Ga3 O1 Ga3 110.39(15) 2_465 4_446
Ga2 O1 Ga3 71.46(16) 2_566 1_666
La O1 Ga3 147.01(3) . 1_666
La O1 Ga3 45.51(14) 2_565 1_666
La O1 Ga3 100.64(5) 4_455 1_666
O2 O1 Ga3 97.5(3) 3_565 1_666
O2 O1 Ga3 140.5(4) . 1_666
O2 O1 Ga3 83.8(3) 4_455 1_666
O2 O1 Ga3 66.6(3) 3_566 1_666
O2 O1 Ga3 101.9(4) 1_556 1_666
O2 O1 Ga3 51.5(3) 4_456 1_666
O3 O1 Ga3 101.0(3) . 1_666
O3 O1 Ga3 19.7(3) 3_565 1_666
O3 O1 Ga3 129.9(3) 4_455 1_666
Ga2 O1 Ga3 108.54(16) 2_565 1_666
Ga3 O1 Ga3 129.3(3) 1_556 1_666
Ga3 O1 Ga3 73.71(12) 2_565 1_666
Ga3 O1 Ga3 36.92(5) 4_456 1_666
O2 O1 Ga3 149.4(5) 6 1_666
O2 O1 Ga3 63.53(19) 5_455 1_666
O2 O1 Ga3 52.7(2) 2_565 1_666
O3 O1 Ga3 121.12(14) 6 1_666
O3 O1 Ga3 47.38(19) 2_565 1_666
O3 O1 Ga3 128.18(15) 5_455 1_666
Ga3 O1 Ga3 146.8(2) . 1_666
Ga3 O1 Ga3 97.51(8) 2_564 1_666
Ga3 O1 Ga3 74.33(5) 4_455 1_666
Ga1 O1 Ga3 142.32(8) 1_455 1_666
Nb O1 Ga3 142.32(8) 1_455 1_666
Nb O1 Ga3 100.89(4) . 1_666
Ga1 O1 Ga3 100.89(4) . 1_666
Ga1 O1 Ga3 36.16(3) 1_565 1_666
Nb O1 Ga3 36.16(3) 1_565 1_666
O2 O1 Ga3 98.23(17) 2_465 1_666
O2 O1 Ga3 130.7(2) 5_445 1_666
O2 O1 Ga3 20.33(13) 6_665 1_666
O3 O1 Ga3 97.4(2) 6_556 1_666
O3 O1 Ga3 20.16(12) 2_566 1_666
O3 O1 Ga3 102.6(2) 5_456 1_666
La O1 Ga3 96.1(2) 1_556 1_666
La O1 Ga3 45.60(8) 2_566 1_666
La O1 Ga3 76.33(16) 4_456 1_666
O3 O1 Ga3 87.91(11) 5 1_666
O3 O1 Ga3 161.65(16) 2_455 1_666
O3 O1 Ga3 59.50(11) 6_565 1_666
Ga2 O1 Ga3 36.04(4) 1_665 1_666
Ga2 O1 Ga3 137.1(3) . 1_666
Ga2 O1 Ga3 76.83(9) 1_565 1_666
O1 O1 Ga3 53.85(12) 2_565 1_666
O1 O1 Ga3 159.28(4) 2_455 1_666
O1 O1 Ga3 89.13(6) 2_465 1_666
O1 O1 Ga3 71.46(16) 1_556 1_666
O1 O1 Ga3 108.54(16) 1_554 1_666
Ga3 O1 Ga3 110.39(15) 2_465 1_666
Ga3 O1 Ga3 110.39(15) 4_446 1_666
Ga2 O1 O3 55.8(2) 2_566 5_556
La O1 O3 83.14(18) . 5_556
La O1 O3 74.13(18) 2_565 5_556
La O1 O3 164.4(5) 4_455 5_556
O2 O1 O3 90.6(3) 3_565 5_556
O2 O1 O3 132.4(4) . 5_556
O2 O1 O3 136.0(4) 4_455 5_556
O2 O1 O3 24.5(2) 3_566 5_556
O2 O1 O3 73.4(4) 1_556 5_556
O2 O1 O3 75.9(4) 4_456 5_556
O3 O1 O3 36.3(3) . 5_556
O3 O1 O3 90.1(3) 3_565 5_556
O3 O1 O3 127.8(4) 4_455 5_556
Ga2 O1 O3 124.2(2) 2_565 5_556
Ga3 O1 O3 97.4(3) 1_556 5_556
Ga3 O1 O3 6.63(16) 2_565 5_556
Ga3 O1 O3 94.3(3) 4_456 5_556
O2 O1 O3 88.3(3) 6 5_556
O2 O1 O3 123.0(4) 5_455 5_556
O2 O1 O3 31.6(2) 2_565 5_556
O3 O1 O3 72.18(15) 6 5_556
O3 O1 O3 100.1(2) 2_565 5_556
O3 O1 O3 160.1(2) 5_455 5_556
Ga3 O1 O3 135.55(15) . 5_556
Ga3 O1 O3 81.19(15) 2_564 5_556
Ga3 O1 O3 132.20(14) 4_455 5_556
Ga1 O1 O3 136.2(2) 1_455 5_556
Nb O1 O3 136.2(2) 1_455 5_556
Nb O1 O3 48.38(15) . 5_556
Ga1 O1 O3 48.38(15) . 5_556
Ga1 O1 O3 104.39(13) 1_565 5_556
Nb O1 O3 104.39(13) 1_565 5_556
O2 O1 O3 137.2(4) 2_465 5_556
O2 O1 O3 60.30(19) 5_445 5_556
O2 O1 O3 60.64(19) 6_665 5_556
O3 O1 O3 30.3(2) 6_556 5_556
O3 O1 O3 64.3(3) 2_566 5_556
O3 O1 O3 104.5(4) 5_456 5_556
La O1 O3 49.37(18) 1_556 5_556
La O1 O3 42.96(18) 2_566 5_556
La O1 O3 85.1(3) 4_456 5_556
O3 O1 O3 59.34(14) 5 5_556
O3 O1 O3 127.82(7) 2_455 5_556
O3 O1 O3 127.82(7) 6_565 5_556
Ga2 O1 O3 39.08(12) 1_665 5_556
Ga2 O1 O3 71.31(15) . 5_556
Ga2 O1 O3 124.0(3) 1_565 5_556
O1 O1 O3 66.6(2) 2_565 5_556
O1 O1 O3 93.14(18) 2_455 5_556
O1 O1 O3 157.7(3) 2_465 5_556
O1 O1 O3 55.8(2) 1_556 5_556
O1 O1 O3 124.2(2) 1_554 5_556
Ga3 O1 O3 124.4(3) 2_465 5_556
Ga3 O1 O3 40.02(12) 4_446 5_556
Ga3 O1 O3 70.41(15) 1_666 5_556
Ga2 O1 O3 55.8(2) 2_566 2_456
La O1 O3 74.13(18) . 2_456
La O1 O3 164.4(5) 2_565 2_456
La O1 O3 83.14(18) 4_455 2_456
O2 O1 O3 136.0(4) 3_565 2_456
O2 O1 O3 90.6(3) . 2_456
O2 O1 O3 132.4(4) 4_455 2_456
O2 O1 O3 75.9(4) 3_566 2_456
O2 O1 O3 24.5(2) 1_556 2_456
O2 O1 O3 73.4(4) 4_456 2_456
O3 O1 O3 90.1(3) . 2_456
O3 O1 O3 127.8(4) 3_565 2_456
O3 O1 O3 36.3(3) 4_455 2_456
Ga2 O1 O3 124.2(2) 2_565 2_456
Ga3 O1 O3 6.63(16) 1_556 2_456
Ga3 O1 O3 94.3(3) 2_565 2_456
Ga3 O1 O3 97.4(3) 4_456 2_456
O2 O1 O3 31.6(2) 6 2_456
O2 O1 O3 88.3(3) 5_455 2_456
O2 O1 O3 123.0(4) 2_565 2_456
O3 O1 O3 100.1(2) 6 2_456
O3 O1 O3 160.1(2) 2_565 2_456
O3 O1 O3 72.18(15) 5_455 2_456
Ga3 O1 O3 81.19(16) . 2_456
Ga3 O1 O3 132.20(14) 2_564 2_456
Ga3 O1 O3 135.55(15) 4_455 2_456
Ga1 O1 O3 48.38(15) 1_455 2_456
Nb O1 O3 48.38(15) 1_455 2_456
Nb O1 O3 104.39(13) . 2_456
Ga1 O1 O3 104.39(13) . 2_456
Ga1 O1 O3 136.2(2) 1_565 2_456
Nb O1 O3 136.2(2) 1_565 2_456
O2 O1 O3 60.30(19) 2_465 2_456
O2 O1 O3 60.64(19) 5_445 2_456
O2 O1 O3 137.2(4) 6_665 2_456
O3 O1 O3 64.3(3) 6_556 2_456
O3 O1 O3 104.5(4) 2_566 2_456
O3 O1 O3 30.3(2) 5_456 2_456
La O1 O3 42.96(18) 1_556 2_456
La O1 O3 85.1(3) 2_566 2_456
La O1 O3 49.37(18) 4_456 2_456
O3 O1 O3 127.82(7) 5 2_456
O3 O1 O3 59.34(15) 2_455 2_456
O3 O1 O3 127.82(7) 6_565 2_456
Ga2 O1 O3 124.0(3) 1_665 2_456
Ga2 O1 O3 39.08(12) . 2_456
Ga2 O1 O3 71.31(15) 1_565 2_456
O1 O1 O3 157.7(3) 2_565 2_456
O1 O1 O3 66.6(2) 2_455 2_456
O1 O1 O3 93.14(18) 2_465 2_456
O1 O1 O3 55.8(2) 1_556 2_456
O1 O1 O3 124.2(2) 1_554 2_456
Ga3 O1 O3 40.02(12) 2_465 2_456
Ga3 O1 O3 70.41(15) 4_446 2_456
Ga3 O1 O3 124.4(3) 1_666 2_456
O3 O1 O3 91.5(3) 5_556 2_456
Ga2 O1 O3 55.8(2) 2_566 6_566
La O1 O3 164.4(5) . 6_566
La O1 O3 83.14(18) 2_565 6_566
La O1 O3 74.13(18) 4_455 6_566
O2 O1 O3 132.4(4) 3_565 6_566
O2 O1 O3 136.0(4) . 6_566
O2 O1 O3 90.6(3) 4_455 6_566
O2 O1 O3 73.4(4) 3_566 6_566
O2 O1 O3 75.9(4) 1_556 6_566
O2 O1 O3 24.5(2) 4_456 6_566
O3 O1 O3 127.8(4) . 6_566
O3 O1 O3 36.3(3) 3_565 6_566
O3 O1 O3 90.1(3) 4_455 6_566
Ga2 O1 O3 124.2(2) 2_565 6_566
Ga3 O1 O3 94.3(3) 1_556 6_566
Ga3 O1 O3 97.4(3) 2_565 6_566
Ga3 O1 O3 6.63(16) 4_456 6_566
O2 O1 O3 123.0(4) 6 6_566
O2 O1 O3 31.6(2) 5_455 6_566
O2 O1 O3 88.3(3) 2_565 6_566
O3 O1 O3 160.1(2) 6 6_566
O3 O1 O3 72.18(15) 2_565 6_566
O3 O1 O3 100.1(2) 5_455 6_566
Ga3 O1 O3 132.20(14) . 6_566
Ga3 O1 O3 135.55(15) 2_564 6_566
Ga3 O1 O3 81.19(15) 4_455 6_566
Ga1 O1 O3 104.39(13) 1_455 6_566
Nb O1 O3 104.39(13) 1_455 6_566
Nb O1 O3 136.2(2) . 6_566
Ga1 O1 O3 136.2(2) . 6_566
Ga1 O1 O3 48.38(15) 1_565 6_566
Nb O1 O3 48.38(15) 1_565 6_566
O2 O1 O3 60.64(19) 2_465 6_566
O2 O1 O3 137.2(4) 5_445 6_566
O2 O1 O3 60.30(19) 6_665 6_566
O3 O1 O3 104.5(4) 6_556 6_566
O3 O1 O3 30.3(2) 2_566 6_566
O3 O1 O3 64.3(3) 5_456 6_566
La O1 O3 85.1(3) 1_556 6_566
La O1 O3 49.37(18) 2_566 6_566
La O1 O3 42.96(18) 4_456 6_566
O3 O1 O3 127.82(7) 5 6_566
O3 O1 O3 127.82(7) 2_455 6_566
O3 O1 O3 59.34(14) 6_565 6_566
Ga2 O1 O3 71.31(15) 1_665 6_566
Ga2 O1 O3 124.0(3) . 6_566
Ga2 O1 O3 39.08(12) 1_565 6_566
O1 O1 O3 93.14(18) 2_565 6_566
O1 O1 O3 157.7(3) 2_455 6_566
O1 O1 O3 66.6(2) 2_465 6_566
O1 O1 O3 55.8(2) 1_556 6_566
O1 O1 O3 124.2(2) 1_554 6_566
Ga3 O1 O3 70.41(15) 2_465 6_566
Ga3 O1 O3 124.4(3) 4_446 6_566
Ga3 O1 O3 40.02(12) 1_666 6_566
O3 O1 O3 91.5(3) 5_556 6_566
O3 O1 O3 91.5(3) 2_456 6_566
Ga2 O1 O3 86.2(2) 2_566 4
La O1 O3 66.24(13) . 4
La O1 O3 60.69(11) 2_565 4
La O1 O3 163.8(5) 4_455 4
O2 O1 O3 60.4(2) 3_565 4
O2 O1 O3 105.9(4) . 4
O2 O1 O3 112.7(4) 4_455 4
O2 O1 O3 55.0(2) 3_566 4
O2 O1 O3 98.5(4) 1_556 4
O2 O1 O3 104.7(4) 4_456 4
O3 O1 O3 22.0(3) . 4
O3 O1 O3 97.5(3) 3_565 4
O3 O1 O3 140.7(3) 4_455 4
Ga2 O1 O3 93.83(19) 2_565 4
Ga3 O1 O3 113.31(19) 1_556 4
Ga3 O1 O3 24.11(15) 2_565 4
Ga3 O1 O3 115.0(2) 4_456 4
O2 O1 O3 91.5(2) 6 4
O2 O1 O3 144.4(3) 5_455 4
O2 O1 O3 28.5(3) 2_565 4
O3 O1 O3 46.1(3) 6 4
O3 O1 O3 88.3(2) 2_565 4
O3 O1 O3 145.0(3) 5_455 4
Ga3 O1 O3 112.2(2) . 4
Ga3 O1 O3 50.80(13) 2_564 4
Ga3 O1 O3 113.6(2) 4_455 4
Ga1 O1 O3 135.99(12) 1_455 4
Nb O1 O3 135.99(12) 1_455 4
Nb O1 O3 21.48(14) . 4
Ga1 O1 O3 21.48(14) . 4
Ga1 O1 O3 104.34(11) 1_565 4
Nb O1 O3 104.34(11) 1_565 4
O2 O1 O3 167.0(4) 2_465 4
O2 O1 O3 56.11(17) 5_445 4
O2 O1 O3 63.46(18) 6_665 4
O3 O1 O3 46.4(2) 6_556 4
O3 O1 O3 84.5(2) 2_566 4
O3 O1 O3 131.4(3) 5_456 4
La O1 O3 73.70(15) 1_556 4
La O1 O3 70.97(16) 2_566 4
La O1 O3 115.6(3) 4_456 4
O3 O1 O3 29.2(2) 5 4
O3 O1 O3 115.55(14) 2_455 4
O3 O1 O3 121.80(13) 6_565 4
Ga2 O1 O3 45.34(12) 1_665 4
Ga2 O1 O3 75.63(12) . 4
Ga2 O1 O3 152.5(3) 1_565 4
O1 O1 O3 49.34(12) 2_565 4
O1 O1 O3 78.37(12) 2_455 4
O1 O1 O3 157.3(4) 2_465 4
O1 O1 O3 86.17(19) 1_556 4
O1 O1 O3 93.8(2) 1_554 4
Ga3 O1 O3 148.9(2) 2_465 4
Ga3 O1 O3 39.96(11) 4_446 4
Ga3 O1 O3 81.19(13) 1_666 4
O3 O1 O3 30.5(3) 5_556 4
O3 O1 O3 109.31(17) 2_456 4
O3 O1 O3 114.71(17) 6_566 4
Ga2 O1 O3 86.2(2) 2_566 3_455
La O1 O3 60.69(11) . 3_455
La O1 O3 163.8(5) 2_565 3_455
La O1 O3 66.24(13) 4_455 3_455
O2 O1 O3 112.7(4) 3_565 3_455
O2 O1 O3 60.4(2) . 3_455
O2 O1 O3 105.9(4) 4_455 3_455
O2 O1 O3 104.7(4) 3_566 3_455
O2 O1 O3 55.0(2) 1_556 3_455
O2 O1 O3 98.5(4) 4_456 3_455
O3 O1 O3 97.5(3) . 3_455
O3 O1 O3 140.7(3) 3_565 3_455
O3 O1 O3 22.0(3) 4_455 3_455
Ga2 O1 O3 93.83(19) 2_565 3_455
Ga3 O1 O3 24.11(15) 1_556 3_455
Ga3 O1 O3 115.0(2) 2_565 3_455
Ga3 O1 O3 113.32(19) 4_456 3_455
O2 O1 O3 28.5(3) 6 3_455
O2 O1 O3 91.5(3) 5_455 3_455
O2 O1 O3 144.4(3) 2_565 3_455
O3 O1 O3 88.3(2) 6 3_455
O3 O1 O3 145.0(3) 2_565 3_455
O3 O1 O3 46.1(3) 5_455 3_455
Ga3 O1 O3 50.80(13) . 3_455
Ga3 O1 O3 113.6(2) 2_564 3_455
Ga3 O1 O3 112.2(2) 4_455 3_455
Ga1 O1 O3 21.48(14) 1_455 3_455
Nb O1 O3 21.48(14) 1_455 3_455
Nb O1 O3 104.34(11) . 3_455
Ga1 O1 O3 104.34(11) . 3_455
Ga1 O1 O3 135.99(12) 1_565 3_455
Nb O1 O3 135.99(12) 1_565 3_455
O2 O1 O3 56.11(17) 2_465 3_455
O2 O1 O3 63.46(18) 5_445 3_455
O2 O1 O3 167.0(4) 6_665 3_455
O3 O1 O3 84.5(2) 6_556 3_455
O3 O1 O3 131.4(3) 2_566 3_455
O3 O1 O3 46.4(2) 5_456 3_455
La O1 O3 70.97(16) 1_556 3_455
La O1 O3 115.6(3) 2_566 3_455
La O1 O3 73.70(15) 4_456 3_455
O3 O1 O3 121.80(13) 5 3_455
O3 O1 O3 29.2(2) 2_455 3_455
O3 O1 O3 115.55(14) 6_565 3_455
Ga2 O1 O3 152.5(3) 1_665 3_455
Ga2 O1 O3 45.34(12) . 3_455
Ga2 O1 O3 75.63(12) 1_565 3_455
O1 O1 O3 157.3(4) 2_565 3_455
O1 O1 O3 49.34(12) 2_455 3_455
O1 O1 O3 78.37(12) 2_465 3_455
O1 O1 O3 86.2(2) 1_556 3_455
O1 O1 O3 93.83(19) 1_554 3_455
Ga3 O1 O3 39.96(11) 2_465 3_455
Ga3 O1 O3 81.19(13) 4_446 3_455
Ga3 O1 O3 148.9(2) 1_666 3_455
O3 O1 O3 114.71(17) 5_556 3_455
O3 O1 O3 30.5(3) 2_456 3_455
O3 O1 O3 109.31(17) 6_566 3_455
O3 O1 O3 119.56(5) 4 3_455
Ga2 O1 O3 86.17(19) 2_566 1_565
La O1 O3 163.8(5) . 1_565
La O1 O3 66.24(13) 2_565 1_565
La O1 O3 60.69(11) 4_455 1_565
O2 O1 O3 105.9(4) 3_565 1_565
O2 O1 O3 112.7(4) . 1_565
O2 O1 O3 60.4(2) 4_455 1_565
O2 O1 O3 98.5(4) 3_566 1_565
O2 O1 O3 104.7(4) 1_556 1_565
O2 O1 O3 55.0(2) 4_456 1_565
O3 O1 O3 140.7(3) . 1_565
O3 O1 O3 22.0(3) 3_565 1_565
O3 O1 O3 97.5(3) 4_455 1_565
Ga2 O1 O3 93.83(19) 2_565 1_565
Ga3 O1 O3 115.0(2) 1_556 1_565
Ga3 O1 O3 113.31(19) 2_565 1_565
Ga3 O1 O3 24.11(15) 4_456 1_565
O2 O1 O3 144.4(3) 6 1_565
O2 O1 O3 28.5(3) 5_455 1_565
O2 O1 O3 91.5(2) 2_565 1_565
O3 O1 O3 145.0(3) 6 1_565
O3 O1 O3 46.1(2) 2_565 1_565
O3 O1 O3 88.3(2) 5_455 1_565
Ga3 O1 O3 113.6(2) . 1_565
Ga3 O1 O3 112.2(2) 2_564 1_565
Ga3 O1 O3 50.80(13) 4_455 1_565
Ga1 O1 O3 104.34(11) 1_455 1_565
Nb O1 O3 104.34(11) 1_455 1_565
Nb O1 O3 135.99(12) . 1_565
Ga1 O1 O3 135.99(12) . 1_565
Ga1 O1 O3 21.48(14) 1_565 1_565
Nb O1 O3 21.48(14) 1_565 1_565
O2 O1 O3 63.46(18) 2_465 1_565
O2 O1 O3 167.0(4) 5_445 1_565
O2 O1 O3 56.11(17) 6_665 1_565
O3 O1 O3 131.4(3) 6_556 1_565
O3 O1 O3 46.4(2) 2_566 1_565
O3 O1 O3 84.5(2) 5_456 1_565
La O1 O3 115.6(3) 1_556 1_565
La O1 O3 73.70(15) 2_566 1_565
La O1 O3 70.97(16) 4_456 1_565
O3 O1 O3 115.55(14) 5 1_565
O3 O1 O3 121.80(13) 2_455 1_565
O3 O1 O3 29.2(2) 6_565 1_565
Ga2 O1 O3 75.63(12) 1_665 1_565
Ga2 O1 O3 152.5(3) . 1_565
Ga2 O1 O3 45.34(12) 1_565 1_565
O1 O1 O3 78.37(12) 2_565 1_565
O1 O1 O3 157.3(4) 2_455 1_565
O1 O1 O3 49.34(12) 2_465 1_565
O1 O1 O3 86.17(19) 1_556 1_565
O1 O1 O3 93.83(19) 1_554 1_565
Ga3 O1 O3 81.19(13) 2_465 1_565
Ga3 O1 O3 148.9(2) 4_446 1_565
Ga3 O1 O3 39.96(11) 1_666 1_565
O3 O1 O3 109.31(17) 5_556 1_565
O3 O1 O3 114.71(17) 2_456 1_565
O3 O1 O3 30.5(3) 6_566 1_565
O3 O1 O3 119.56(5) 4 1_565
O3 O1 O3 119.56(5) 3_455 1_565
Ga2 O1 O2 141.27(14) 2_566 6_554
La O1 O2 39.0(2) . 6_554
La O1 O2 104.0(4) 2_565 6_554
La O1 O2 75.2(3) 4_455 6_554
O2 O1 O2 53.5(2) 3_565 6_554
O2 O1 O2 13.3(3) . 6_554
O2 O1 O2 67.6(3) 4_455 6_554
O2 O1 O2 135.8(2) 3_566 6_554
O2 O1 O2 111.2(2) 1_556 6_554
O2 O1 O2 156.8(2) 4_456 6_554
O3 O1 O2 83.1(3) . 6_554
O3 O1 O2 134.4(4) 3_565 6_554
O3 O1 O2 71.7(3) 4_455 6_554
Ga2 O1 O2 38.73(14) 2_565 6_554
Ga3 O1 O2 82.60(18) 1_556 6_554
Ga3 O1 O2 113.42(17) 2_565 6_554
Ga3 O1 O2 145.8(3) 4_456 6_554
O2 O1 O2 62.8(3) 6 6_554
O2 O1 O2 117.6(3) 5_455 6_554
O2 O1 O2 117.6(3) 2_565 6_554
O3 O1 O2 48.5(2) 6 6_554
O3 O1 O2 100.0(4) 2_565 6_554
O3 O1 O2 50.6(3) 5_455 6_554
Ga3 O1 O2 17.87(15) . 6_554
Ga3 O1 O2 56.96(19) 2_564 6_554
Ga3 O1 O2 77.7(2) 4_455 6_554
Ga1 O1 O2 54.15(18) 1_455 6_554
Nb O1 O2 54.15(18) 1_455 6_554
Nb O1 O2 73.24(18) . 6_554
Ga1 O1 O2 73.24(18) . 6_554
Ga1 O1 O2 116.7(3) 1_565 6_554
Nb O1 O2 116.7(3) 1_565 6_554
O2 O1 O2 93.0(3) 2_465 6_554
O2 O1 O2 67.43(17) 5_445 6_554
O2 O1 O2 133.0(3) 6_665 6_554
O3 O1 O2 103.11(17) 6_556 6_554
O3 O1 O2 167.1(3) 2_566 6_554
O3 O1 O2 104.6(2) 5_456 6_554
La O1 O2 114.22(10) 1_556 6_554
La O1 O2 160.68(14) 2_566 6_554
La O1 O2 133.08(14) 4_456 6_554
O3 O1 O2 74.1(2) 5 6_554
O3 O1 O2 32.0(2) 2_455 6_554
O3 O1 O2 97.4(3) 6_565 6_554
Ga2 O1 O2 132.6(2) 1_665 6_554
Ga2 O1 O2 71.28(13) . 6_554
Ga2 O1 O2 112.96(19) 1_565 6_554
O1 O1 O2 98.8(4) 2_565 6_554
O1 O1 O2 33.5(3) 2_455 6_554
O1 O1 O2 82.5(3) 2_465 6_554
O1 O1 O2 141.27(15) 1_556 6_554
O1 O1 O2 38.73(14) 1_554 6_554
Ga3 O1 O2 90.23(17) 2_465 6_554
Ga3 O1 O2 84.36(12) 4_446 6_554
Ga3 O1 O2 147.0(3) 1_666 6_554
O3 O1 O2 119.40(17) 5_556 6_554
O3 O1 O2 88.1(2) 2_456 6_554
O3 O1 O2 149.1(2) 6_566 6_554
O3 O1 O2 94.4(2) 4 6_554
O3 O1 O2 60.0(2) 3_455 6_554
O3 O1 O2 125.4(3) 1_565 6_554
Ga2 O1 O2 141.26(14) 2_566 5_454
La O1 O2 104.0(4) . 5_454
La O1 O2 75.2(3) 2_565 5_454
La O1 O2 39.0(2) 4_455 5_454
O2 O1 O2 67.6(3) 3_565 5_454
O2 O1 O2 53.5(2) . 5_454
O2 O1 O2 13.3(3) 4_455 5_454
O2 O1 O2 156.8(2) 3_566 5_454
O2 O1 O2 135.8(2) 1_556 5_454
O2 O1 O2 111.2(2) 4_456 5_454
O3 O1 O2 134.4(4) . 5_454
O3 O1 O2 71.7(3) 3_565 5_454
O3 O1 O2 83.1(3) 4_455 5_454
Ga2 O1 O2 38.73(14) 2_565 5_454
Ga3 O1 O2 113.42(17) 1_556 5_454
Ga3 O1 O2 145.8(3) 2_565 5_454
Ga3 O1 O2 82.60(18) 4_456 5_454
O2 O1 O2 117.6(3) 6 5_454
O2 O1 O2 62.8(3) 5_455 5_454
O2 O1 O2 117.6(3) 2_565 5_454
O3 O1 O2 100.0(4) 6 5_454
O3 O1 O2 50.6(3) 2_565 5_454
O3 O1 O2 48.5(2) 5_455 5_454
Ga3 O1 O2 56.96(19) . 5_454
Ga3 O1 O2 77.7(2) 2_564 5_454
Ga3 O1 O2 17.87(15) 4_455 5_454
Ga1 O1 O2 73.24(18) 1_455 5_454
Nb O1 O2 73.24(18) 1_455 5_454
Nb O1 O2 116.7(3) . 5_454
Ga1 O1 O2 116.7(3) . 5_454
Ga1 O1 O2 54.15(18) 1_565 5_454
Nb O1 O2 54.15(18) 1_565 5_454
O2 O1 O2 67.43(17) 2_465 5_454
O2 O1 O2 133.0(3) 5_445 5_454
O2 O1 O2 93.0(3) 6_665 5_454
O3 O1 O2 167.1(3) 6_556 5_454
O3 O1 O2 104.6(2) 2_566 5_454
O3 O1 O2 103.11(17) 5_456 5_454
La O1 O2 160.68(14) 1_556 5_454
La O1 O2 133.08(14) 2_566 5_454
La O1 O2 114.22(10) 4_456 5_454
O3 O1 O2 97.4(3) 5 5_454
O3 O1 O2 74.1(2) 2_455 5_454
O3 O1 O2 32.00(19) 6_565 5_454
Ga2 O1 O2 113.0(2) 1_665 5_454
Ga2 O1 O2 132.6(2) . 5_454
Ga2 O1 O2 71.28(13) 1_565 5_454
O1 O1 O2 82.5(3) 2_565 5_454
O1 O1 O2 98.8(4) 2_455 5_454
O1 O1 O2 33.5(3) 2_465 5_454
O1 O1 O2 141.26(14) 1_556 5_454
O1 O1 O2 38.73(14) 1_554 5_454
Ga3 O1 O2 84.36(13) 2_465 5_454
Ga3 O1 O2 147.0(3) 4_446 5_454
Ga3 O1 O2 90.23(17) 1_666 5_454
O3 O1 O2 149.1(2) 5_556 5_454
O3 O1 O2 119.40(17) 2_456 5_454
O3 O1 O2 88.1(2) 6_566 5_454
O3 O1 O2 125.4(3) 4 5_454
O3 O1 O2 94.4(2) 3_455 5_454
O3 O1 O2 60.0(2) 1_565 5_454
O2 O1 O2 65.6(2) 6_554 5_454
Ga2 O1 O2 141.27(15) 2_566 2_564
La O1 O2 75.2(3) . 2_564
La O1 O2 39.0(2) 2_565 2_564
La O1 O2 104.0(4) 4_455 2_564
O2 O1 O2 13.3(3) 3_565 2_564
O2 O1 O2 67.6(3) . 2_564
O2 O1 O2 53.5(2) 4_455 2_564
O2 O1 O2 111.2(2) 3_566 2_564
O2 O1 O2 156.8(2) 1_556 2_564
O2 O1 O2 135.8(2) 4_456 2_564
O3 O1 O2 71.7(3) . 2_564
O3 O1 O2 83.1(3) 3_565 2_564
O3 O1 O2 134.4(4) 4_455 2_564
Ga2 O1 O2 38.74(14) 2_565 2_564
Ga3 O1 O2 145.8(3) 1_556 2_564
Ga3 O1 O2 82.60(18) 2_565 2_564
Ga3 O1 O2 113.42(17) 4_456 2_564
O2 O1 O2 117.6(3) 6 2_564
O2 O1 O2 117.6(3) 5_455 2_564
O2 O1 O2 62.8(3) 2_565 2_564
O3 O1 O2 50.6(3) 6 2_564
O3 O1 O2 48.5(2) 2_565 2_564
O3 O1 O2 100.0(4) 5_455 2_564
Ga3 O1 O2 77.7(2) . 2_564
Ga3 O1 O2 17.87(15) 2_564 2_564
Ga3 O1 O2 56.96(19) 4_455 2_564
Ga1 O1 O2 116.7(3) 1_455 2_564
Nb O1 O2 116.7(3) 1_455 2_564
Nb O1 O2 54.15(18) . 2_564
Ga1 O1 O2 54.15(18) . 2_564
Ga1 O1 O2 73.24(18) 1_565 2_564
Nb O1 O2 73.24(18) 1_565 2_564
O2 O1 O2 133.0(3) 2_465 2_564
O2 O1 O2 93.0(3) 5_445 2_564
O2 O1 O2 67.43(17) 6_665 2_564
O3 O1 O2 104.58(19) 6_556 2_564
O3 O1 O2 103.11(17) 2_566 2_564
O3 O1 O2 167.1(3) 5_456 2_564
La O1 O2 133.08(14) 1_556 2_564
La O1 O2 114.22(10) 2_566 2_564
La O1 O2 160.68(14) 4_456 2_564
O3 O1 O2 32.00(19) 5 2_564
O3 O1 O2 97.4(3) 2_455 2_564
O3 O1 O2 74.1(2) 6_565 2_564
Ga2 O1 O2 71.28(13) 1_665 2_564
Ga2 O1 O2 113.0(2) . 2_564
Ga2 O1 O2 132.6(2) 1_565 2_564
O1 O1 O2 33.5(3) 2_565 2_564
O1 O1 O2 82.5(3) 2_455 2_564
O1 O1 O2 98.8(4) 2_465 2_564
O1 O1 O2 141.27(14) 1_556 2_564
O1 O1 O2 38.74(14) 1_554 2_564
Ga3 O1 O2 147.0(3) 2_465 2_564
Ga3 O1 O2 90.23(17) 4_446 2_564
Ga3 O1 O2 84.36(13) 1_666 2_564
O3 O1 O2 88.1(2) 5_556 2_564
O3 O1 O2 149.1(2) 2_456 2_564
O3 O1 O2 119.40(18) 6_566 2_564
O3 O1 O2 60.0(2) 4 2_564
O3 O1 O2 125.4(3) 3_455 2_564
O3 O1 O2 94.4(2) 1_565 2_564
O2 O1 O2 65.6(2) 6_554 2_564
O2 O1 O2 65.6(2) 5_454 2_564
Ga2 O1 O3 146.38(14) 2_566 1_554
La O1 O3 47.6(3) . 1_554
La O1 O3 67.5(3) 2_565 1_554
La O1 O3 102.2(4) 4_455 1_554
O2 O1 O3 15.8(3) 3_565 1_554
O2 O1 O3 46.6(3) . 1_554
O2 O1 O3 64.5(3) 4_455 1_554
O2 O1 O3 117.2(2) 3_566 1_554
O2 O1 O3 135.8(3) 1_556 1_554
O2 O1 O3 163.2(3) 4_456 1_554
O3 O1 O3 62.9(2) . 1_554
O3 O1 O3 111.7(3) 3_565 1_554
O3 O1 O3 111.7(3) 4_455 1_554
Ga2 O1 O3 33.62(14) 2_565 1_554
Ga3 O1 O3 116.7(2) 1_556 1_554
Ga3 O1 O3 86.54(17) 2_565 1_554
Ga3 O1 O3 141.3(3) 4_456 1_554
O2 O1 O3 89.1(3) 6 1_554
O2 O1 O3 134.4(4) 5_455 1_554
O2 O1 O3 79.4(3) 2_565 1_554
O3 O1 O3 29.0(3) 6 1_554
O3 O1 O3 75.5(2) 2_565 1_554
O3 O1 O3 85.7(3) 5_455 1_554
Ga3 O1 O3 55.76(19) . 1_554
Ga3 O1 O3 16.97(12) 2_564 1_554
Ga3 O1 O3 72.1(2) 4_455 1_554
Ga1 O1 O3 94.1(2) 1_455 1_554
Nb O1 O3 94.1(2) 1_455 1_554
Nb O1 O3 46.15(15) . 1_554
Ga1 O1 O3 46.15(15) . 1_554
Ga1 O1 O3 99.7(2) 1_565 1_554
Nb O1 O3 99.7(2) 1_565 1_554
O2 O1 O3 128.2(3) 2_465 1_554
O2 O1 O3 70.9(2) 5_445 1_554
O2 O1 O3 94.8(2) 6_665 1_554
O3 O1 O3 95.3(2) 6_556 1_554
O3 O1 O3 130.6(2) 2_566 1_554
O3 O1 O3 143.9(2) 5_456 1_554
La O1 O3 121.29(13) 1_556 1_554
La O1 O3 132.25(10) 2_566 1_554
La O1 O3 169.32(15) 4_456 1_554
O3 O1 O3 36.3(2) 5 1_554
O3 O1 O3 71.7(2) 2_455 1_554
O3 O1 O3 93.4(3) 6_565 1_554
Ga2 O1 O3 92.91(15) 1_665 1_554
Ga2 O1 O3 87.59(18) . 1_554
Ga2 O1 O3 141.9(3) 1_565 1_554
O1 O1 O3 60.0(3) 2_565 1_554
O1 O1 O3 53.7(3) 2_455 1_554
O1 O1 O3 103.2(4) 2_465 1_554
O1 O1 O3 146.38(14) 1_556 1_554
O1 O1 O3 33.62(14) 1_554 1_554
Ga3 O1 O3 130.0(2) 2_465 1_554
Ga3 O1 O3 76.13(16) 4_446 1_554
Ga3 O1 O3 113.04(18) 1_666 1_554
O3 O1 O3 93.1(2) 5_556 1_554
O3 O1 O3 120.3(3) 2_456 1_554
O3 O1 O3 147.71(18) 6_566 1_554
O3 O1 O3 62.83(15) 4 1_554
O3 O1 O3 97.6(2) 3_455 1_554
O3 O1 O3 119.4(3) 1_565 1_554
O2 O1 O3 39.99(19) 6_554 1_554
O2 O1 O3 72.0(2) 5_454 1_554
O2 O1 O3 29.09(18) 2_564 1_554
Ga2 O1 O3 146.38(14) 2_566 4_454
La O1 O3 67.5(3) . 4_454
La O1 O3 102.2(4) 2_565 4_454
La O1 O3 47.6(3) 4_455 4_454
O2 O1 O3 64.5(3) 3_565 4_454
O2 O1 O3 15.8(3) . 4_454
O2 O1 O3 46.6(3) 4_455 4_454
O2 O1 O3 163.2(3) 3_566 4_454
O2 O1 O3 117.2(2) 1_556 4_454
O2 O1 O3 135.8(3) 4_456 4_454
O3 O1 O3 111.7(3) . 4_454
O3 O1 O3 111.7(3) 3_565 4_454
O3 O1 O3 62.9(2) 4_455 4_454
Ga2 O1 O3 33.62(14) 2_565 4_454
Ga3 O1 O3 86.54(17) 1_556 4_454
Ga3 O1 O3 141.3(3) 2_565 4_454
Ga3 O1 O3 116.7(2) 4_456 4_454
O2 O1 O3 79.4(3) 6 4_454
O2 O1 O3 89.1(3) 5_455 4_454
O2 O1 O3 134.4(4) 2_565 4_454
O3 O1 O3 75.5(2) 6 4_454
O3 O1 O3 85.7(3) 2_565 4_454
O3 O1 O3 29.0(3) 5_455 4_454
Ga3 O1 O3 16.97(12) . 4_454
Ga3 O1 O3 72.1(2) 2_564 4_454
Ga3 O1 O3 55.76(19) 4_455 4_454
Ga1 O1 O3 46.15(15) 1_455 4_454
Nb O1 O3 46.15(15) 1_455 4_454
Nb O1 O3 99.7(2) . 4_454
Ga1 O1 O3 99.7(2) . 4_454
Ga1 O1 O3 94.1(2) 1_565 4_454
Nb O1 O3 94.1(2) 1_565 4_454
O2 O1 O3 70.9(2) 2_465 4_454
O2 O1 O3 94.8(2) 5_445 4_454
O2 O1 O3 128.2(3) 6_665 4_454
O3 O1 O3 130.6(2) 6_556 4_454
O3 O1 O3 143.9(2) 2_566 4_454
O3 O1 O3 95.3(2) 5_456 4_454
La O1 O3 132.25(10) 1_556 4_454
La O1 O3 169.32(15) 2_566 4_454
La O1 O3 121.29(13) 4_456 4_454
O3 O1 O3 93.4(3) 5 4_454
O3 O1 O3 36.3(2) 2_455 4_454
O3 O1 O3 71.7(2) 6_565 4_454
Ga2 O1 O3 141.9(3) 1_665 4_454
Ga2 O1 O3 92.91(15) . 4_454
Ga2 O1 O3 87.59(19) 1_565 4_454
O1 O1 O3 103.2(4) 2_565 4_454
O1 O1 O3 60.0(3) 2_455 4_454
O1 O1 O3 53.7(3) 2_465 4_454
O1 O1 O3 146.38(14) 1_556 4_454
O1 O1 O3 33.62(14) 1_554 4_454
Ga3 O1 O3 76.13(16) 2_465 4_454
Ga3 O1 O3 113.04(18) 4_446 4_454
Ga3 O1 O3 130.0(2) 1_666 4_454
O3 O1 O3 147.71(18) 5_556 4_454
O3 O1 O3 93.1(2) 2_456 4_454
O3 O1 O3 120.3(3) 6_566 4_454
O3 O1 O3 119.4(3) 4 4_454
O3 O1 O3 62.83(15) 3_455 4_454
O3 O1 O3 97.6(2) 1_565 4_454
O2 O1 O3 29.10(18) 6_554 4_454
O2 O1 O3 39.99(19) 5_454 4_454
O2 O1 O3 72.0(2) 2_564 4_454
O3 O1 O3 57.3(2) 1_554 4_454
Ga2 O1 O3 146.38(14) 2_566 3_564
La O1 O3 102.2(4) . 3_564
La O1 O3 47.6(3) 2_565 3_564
La O1 O3 67.5(3) 4_455 3_564
O2 O1 O3 46.6(3) 3_565 3_564
O2 O1 O3 64.5(3) . 3_564
O2 O1 O3 15.8(3) 4_455 3_564
O2 O1 O3 135.8(3) 3_566 3_564
O2 O1 O3 163.2(3) 1_556 3_564
O2 O1 O3 117.2(2) 4_456 3_564
O3 O1 O3 111.7(3) . 3_564
O3 O1 O3 62.9(2) 3_565 3_564
O3 O1 O3 111.7(3) 4_455 3_564
Ga2 O1 O3 33.62(14) 2_565 3_564
Ga3 O1 O3 141.3(3) 1_556 3_564
Ga3 O1 O3 116.7(2) 2_565 3_564
Ga3 O1 O3 86.54(17) 4_456 3_564
O2 O1 O3 134.4(4) 6 3_564
O2 O1 O3 79.4(3) 5_455 3_564
O2 O1 O3 89.1(3) 2_565 3_564
O3 O1 O3 85.7(3) 6 3_564
O3 O1 O3 29.0(3) 2_565 3_564
O3 O1 O3 75.5(2) 5_455 3_564
Ga3 O1 O3 72.1(2) . 3_564
Ga3 O1 O3 55.76(19) 2_564 3_564
Ga3 O1 O3 16.97(12) 4_455 3_564
Ga1 O1 O3 99.7(2) 1_455 3_564
Nb O1 O3 99.7(2) 1_455 3_564
Nb O1 O3 94.1(2) . 3_564
Ga1 O1 O3 94.1(2) . 3_564
Ga1 O1 O3 46.15(15) 1_565 3_564
Nb O1 O3 46.15(15) 1_565 3_564
O2 O1 O3 94.8(2) 2_465 3_564
O2 O1 O3 128.2(3) 5_445 3_564
O2 O1 O3 70.9(2) 6_665 3_564
O3 O1 O3 143.9(2) 6_556 3_564
O3 O1 O3 95.3(2) 2_566 3_564
O3 O1 O3 130.6(2) 5_456 3_564
La O1 O3 169.32(15) 1_556 3_564
La O1 O3 121.29(13) 2_566 3_564
La O1 O3 132.25(10) 4_456 3_564
O3 O1 O3 71.7(2) 5 3_564
O3 O1 O3 93.4(3) 2_455 3_564
O3 O1 O3 36.3(2) 6_565 3_564
Ga2 O1 O3 87.59(18) 1_665 3_564
Ga2 O1 O3 141.9(3) . 3_564
Ga2 O1 O3 92.91(15) 1_565 3_564
O1 O1 O3 53.7(3) 2_565 3_564
O1 O1 O3 103.2(4) 2_455 3_564
O1 O1 O3 60.0(3) 2_465 3_564
O1 O1 O3 146.38(14) 1_556 3_564
O1 O1 O3 33.62(14) 1_554 3_564
Ga3 O1 O3 113.04(18) 2_465 3_564
Ga3 O1 O3 130.0(2) 4_446 3_564
Ga3 O1 O3 76.13(16) 1_666 3_564
O3 O1 O3 120.3(3) 5_556 3_564
O3 O1 O3 147.71(18) 2_456 3_564
O3 O1 O3 93.1(2) 6_566 3_564
O3 O1 O3 97.6(2) 4 3_564
O3 O1 O3 119.4(3) 3_455 3_564
O3 O1 O3 62.83(15) 1_565 3_564
O2 O1 O3 72.0(2) 6_554 3_564
O2 O1 O3 29.09(18) 5_454 3_564
O2 O1 O3 39.99(19) 2_564 3_564
O3 O1 O3 57.3(2) 1_554 3_564
O3 O1 O3 57.3(2) 4_454 3_564
Ga2 O1 O1 54.1(3) 2_566 2_566
La O1 O1 114.86(14) . 2_566
La O1 O1 56.99(8) 2_565 2_566
La O1 O1 136.0(2) 4_455 2_566
O2 O1 O1 97.5(2) 3_565 2_566
O2 O1 O1 154.3(4) . 2_566
O2 O1 O1 115.6(4) 4_455 2_566
O2 O1 O1 33.2(3) 3_566 2_566
O2 O1 O1 83.7(5) 1_556 2_566
O2 O1 O1 56.5(4) 4_456 2_566
O3 O1 O1 66.7(2) . 2_566
O3 O1 O1 57.4(3) 3_565 2_566
O3 O1 O1 137.3(5) 4_455 2_566
Ga2 O1 O1 125.9(3) 2_565 2_566
Ga3 O1 O1 114.2(5) 1_556 2_566
Ga3 O1 O1 36.94(9) 2_565 2_566
Ga3 O1 O1 64.30(18) 4_456 2_566
O2 O1 O1 117.1(4) 6 2_566
O2 O1 O1 94.1(3) 5_455 2_566
O2 O1 O1 28.4(2) 2_565 2_566
O3 O1 O1 97.57(13) 6 2_566
O3 O1 O1 75.75(19) 2_565 2_566
O3 O1 O1 163.3(3) 5_455 2_566
Ga3 O1 O1 163.1(3) . 2_566
Ga3 O1 O1 91.30(11) 2_564 2_566
Ga3 O1 O1 107.76(11) 4_455 2_566
Ga1 O1 O1 154.6(4) 1_455 2_566
Nb O1 O1 154.6(4) 1_455 2_566
Nb O1 O1 73.011(11) . 2_566
Ga1 O1 O1 73.011(11) . 2_566
Ga1 O1 O1 73.011(11) 1_565 2_566
Nb O1 O1 73.011(11) 1_565 2_566
O2 O1 O1 121.7(3) 2_465 2_566
O2 O1 O1 93.1(2) 5_445 2_566
O2 O1 O1 32.72(14) 6_665 2_566
O3 O1 O1 60.2(2) 6_556 2_566
O3 O1 O1 33.39(16) 2_566 2_566
O3 O1 O1 103.9(4) 5_456 2_566
La O1 O1 66.8(3) 1_556 2_566
La O1 O1 26.02(16) 2_566 2_566
La O1 O1 76.3(3) 4_456 2_566
O3 O1 O1 71.94(13) 5 2_566
O3 O1 O1 160.0(2) 2_455 2_566
O3 O1 O1 96.70(11) 6_565 2_566
Ga2 O1 O1 17.28(8) 1_665 2_566
Ga2 O1 O1 101.4(3) . 2_566
Ga2 O1 O1 101.4(3) 1_565 2_566
O1 O1 O1 56.12(9) 2_565 2_566
O1 O1 O1 125.66(17) 2_455 2_566
O1 O1 O1 125.66(17) 2_465 2_566
O1 O1 O1 54.1(3) 1_556 2_566
O1 O1 O1 125.9(3) 1_554 2_566
Ga3 O1 O1 121.8(4) 2_465 2_566
Ga3 O1 O1 72.87(14) 4_446 2_566
Ga3 O1 O1 37.73(2) 1_666 2_566
O3 O1 O1 32.87(13) 5_556 2_566
O3 O1 O1 107.6(4) 2_456 2_566
O3 O1 O1 63.3(2) 6_566 2_566
O3 O1 O1 51.55(14) 4 2_566
O3 O1 O1 137.5(4) 3_455 2_566
O3 O1 O1 76.52(13) 1_565 2_566
O2 O1 O1 145.4(2) 6_554 2_566
O2 O1 O1 125.3(2) 5_454 2_566
O2 O1 O1 88.28(19) 2_564 2_566
O3 O1 O1 107.72(19) 1_554 2_566
O3 O1 O1 159.1(3) 4_454 2_566
O3 O1 O1 103.0(2) 3_564 2_566
Ga2 O1 O1 54.1(3) 2_566 2_456
La O1 O1 56.99(8) . 2_456
La O1 O1 136.0(2) 2_565 2_456
La O1 O1 114.86(14) 4_455 2_456
O2 O1 O1 115.6(4) 3_565 2_456
O2 O1 O1 97.5(2) . 2_456
O2 O1 O1 154.3(4) 4_455 2_456
O2 O1 O1 56.5(4) 3_566 2_456
O2 O1 O1 33.2(3) 1_556 2_456
O2 O1 O1 83.7(5) 4_456 2_456
O3 O1 O1 57.4(3) . 2_456
O3 O1 O1 137.3(5) 3_565 2_456
O3 O1 O1 66.7(2) 4_455 2_456
Ga2 O1 O1 125.9(3) 2_565 2_456
Ga3 O1 O1 36.94(9) 1_556 2_456
Ga3 O1 O1 64.30(18) 2_565 2_456
Ga3 O1 O1 114.2(5) 4_456 2_456
O2 O1 O1 28.4(2) 6 2_456
O2 O1 O1 117.1(4) 5_455 2_456
O2 O1 O1 94.1(3) 2_565 2_456
O3 O1 O1 75.75(19) 6 2_456
O3 O1 O1 163.3(3) 2_565 2_456
O3 O1 O1 97.57(13) 5_455 2_456
Ga3 O1 O1 91.30(11) . 2_456
Ga3 O1 O1 107.76(11) 2_564 2_456
Ga3 O1 O1 163.1(3) 4_455 2_456
Ga1 O1 O1 73.011(11) 1_455 2_456
Nb O1 O1 73.011(11) 1_455 2_456
Nb O1 O1 73.011(11) . 2_456
Ga1 O1 O1 73.011(11) . 2_456
Ga1 O1 O1 154.6(4) 1_565 2_456
Nb O1 O1 154.6(4) 1_565 2_456
O2 O1 O1 93.1(2) 2_465 2_456
O2 O1 O1 32.72(14) 5_445 2_456
O2 O1 O1 121.7(3) 6_665 2_456
O3 O1 O1 33.39(16) 6_556 2_456
O3 O1 O1 103.9(4) 2_566 2_456
O3 O1 O1 60.2(2) 5_456 2_456
La O1 O1 26.02(16) 1_556 2_456
La O1 O1 76.3(3) 2_566 2_456
La O1 O1 66.8(3) 4_456 2_456
O3 O1 O1 96.70(11) 5 2_456
O3 O1 O1 71.94(13) 2_455 2_456
O3 O1 O1 160.0(3) 6_565 2_456
Ga2 O1 O1 101.4(3) 1_665 2_456
Ga2 O1 O1 17.28(8) . 2_456
Ga2 O1 O1 101.4(3) 1_565 2_456
O1 O1 O1 125.66(17) 2_565 2_456
O1 O1 O1 56.12(8) 2_455 2_456
O1 O1 O1 125.66(17) 2_465 2_456
O1 O1 O1 54.1(3) 1_556 2_456
O1 O1 O1 125.9(3) 1_554 2_456
Ga3 O1 O1 72.87(14) 2_465 2_456
Ga3 O1 O1 37.73(2) 4_446 2_456
Ga3 O1 O1 121.8(4) 1_666 2_456
O3 O1 O1 63.3(2) 5_556 2_456
O3 O1 O1 32.87(13) 2_456 2_456
O3 O1 O1 107.6(4) 6_566 2_456
O3 O1 O1 76.52(13) 4 2_456
O3 O1 O1 51.55(13) 3_455 2_456
O3 O1 O1 137.5(4) 1_565 2_456
O2 O1 O1 88.28(19) 6_554 2_456
O2 O1 O1 145.4(2) 5_454 2_456
O2 O1 O1 125.3(2) 2_564 2_456
O3 O1 O1 103.0(2) 1_554 2_456
O3 O1 O1 107.72(19) 4_454 2_456
O3 O1 O1 159.1(3) 3_564 2_456
O1 O1 O1 89.2(4) 2_566 2_456
Ga2 O1 O1 54.1(3) 2_566 2_466
La O1 O1 136.0(2) . 2_466
La O1 O1 114.86(14) 2_565 2_466
La O1 O1 56.99(8) 4_455 2_466
O2 O1 O1 154.3(4) 3_565 2_466
O2 O1 O1 115.6(4) . 2_466
O2 O1 O1 97.5(2) 4_455 2_466
O2 O1 O1 83.6(5) 3_566 2_466
O2 O1 O1 56.5(4) 1_556 2_466
O2 O1 O1 33.2(3) 4_456 2_466
O3 O1 O1 137.3(5) . 2_466
O3 O1 O1 66.7(2) 3_565 2_466
O3 O1 O1 57.4(3) 4_455 2_466
Ga2 O1 O1 125.9(3) 2_565 2_466
Ga3 O1 O1 64.30(18) 1_556 2_466
Ga3 O1 O1 114.2(5) 2_565 2_466
Ga3 O1 O1 36.94(9) 4_456 2_466
O2 O1 O1 94.1(3) 6 2_466
O2 O1 O1 28.4(2) 5_455 2_466
O2 O1 O1 117.1(4) 2_565 2_466
O3 O1 O1 163.3(3) 6 2_466
O3 O1 O1 97.57(13) 2_565 2_466
O3 O1 O1 75.75(19) 5_455 2_466
Ga3 O1 O1 107.76(11) . 2_466
Ga3 O1 O1 163.1(3) 2_564 2_466
Ga3 O1 O1 91.30(11) 4_455 2_466
Ga1 O1 O1 73.011(11) 1_455 2_466
Nb O1 O1 73.011(11) 1_455 2_466
Nb O1 O1 154.6(4) . 2_466
Ga1 O1 O1 154.6(4) . 2_466
Ga1 O1 O1 73.011(11) 1_565 2_466
Nb O1 O1 73.011(11) 1_565 2_466
O2 O1 O1 32.72(14) 2_465 2_466
O2 O1 O1 121.7(3) 5_445 2_466
O2 O1 O1 93.1(2) 6_665 2_466
O3 O1 O1 103.9(4) 6_556 2_466
O3 O1 O1 60.2(2) 2_566 2_466
O3 O1 O1 33.39(16) 5_456 2_466
La O1 O1 76.3(3) 1_556 2_466
La O1 O1 66.8(3) 2_566 2_466
La O1 O1 26.02(16) 4_456 2_466
O3 O1 O1 160.0(3) 5 2_466
O3 O1 O1 96.70(11) 2_455 2_466
O3 O1 O1 71.94(13) 6_565 2_466
Ga2 O1 O1 101.4(3) 1_665 2_466
Ga2 O1 O1 101.4(3) . 2_466
Ga2 O1 O1 17.28(8) 1_565 2_466
O1 O1 O1 125.66(17) 2_565 2_466
O1 O1 O1 125.66(17) 2_455 2_466
O1 O1 O1 56.12(8) 2_465 2_466
O1 O1 O1 54.1(3) 1_556 2_466
O1 O1 O1 125.9(3) 1_554 2_466
Ga3 O1 O1 37.72(2) 2_465 2_466
Ga3 O1 O1 121.8(4) 4_446 2_466
Ga3 O1 O1 72.87(14) 1_666 2_466
O3 O1 O1 107.6(4) 5_556 2_466
O3 O1 O1 63.3(2) 2_456 2_466
O3 O1 O1 32.87(13) 6_566 2_466
O3 O1 O1 137.5(4) 4 2_466
O3 O1 O1 76.52(13) 3_455 2_466
O3 O1 O1 51.55(13) 1_565 2_466
O2 O1 O1 125.3(2) 6_554 2_466
O2 O1 O1 88.28(19) 5_454 2_466
O2 O1 O1 145.4(2) 2_564 2_466
O3 O1 O1 159.1(3) 1_554 2_466
O3 O1 O1 103.0(2) 4_454 2_466
O3 O1 O1 107.72(19) 3_564 2_466
O1 O1 O1 89.2(4) 2_566 2_466
O1 O1 O1 89.2(4) 2_456 2_466
Ga2 O1 O3 86.48(18) 2_566 3
La O1 O3 41.85(16) . 3
La O1 O3 86.13(11) 2_565 3
La O1 O3 151.0(3) 4_455 3
O2 O1 O3 66.1(3) 3_565 3
O2 O1 O3 90.5(4) . 3
O2 O1 O3 123.4(4) 4_455 3
O2 O1 O3 61.2(3) 3_566 3
O2 O1 O3 84.7(4) 1_556 3
O2 O1 O3 114.6(4) 4_456 3
O3 O1 O3 6.4(3) . 3
O3 O1 O3 124.9(4) 3_565 3
O3 O1 O3 113.7(3) 4_455 3
Ga2 O1 O3 93.53(18) 2_565 3
Ga3 O1 O3 89.50(14) 1_556 3
Ga3 O1 O3 36.64(14) 2_565 3
Ga3 O1 O3 136.4(3) 4_456 3
O2 O1 O3 64.5(3) 6 3
O2 O1 O3 164.2(4) 5_455 3
O2 O1 O3 55.4(3) 2_565 3
O3 O1 O3 32.8(3) 6 3
O3 O1 O3 112.41(13) 2_565 3
O3 O1 O3 123.24(14) 5_455 3
Ga3 O1 O3 93.46(16) . 3
Ga3 O1 O3 56.45(11) 2_564 3
Ga3 O1 O3 128.8(2) 4_455 3
Ga1 O1 O3 108.77(13) 1_455 3
Nb O1 O3 108.77(13) 1_455 3
Nb O1 O3 18.10(10) . 3
Ga1 O1 O3 18.10(10) . 3
Ga1 O1 O3 131.47(13) 1_565 3
Nb O1 O3 131.47(13) 1_565 3
O2 O1 O3 146.44(19) 2_465 3
O2 O1 O3 28.89(15) 5_445 3
O2 O1 O3 90.84(17) 6_665 3
O3 O1 O3 35.3(2) 6_556 3
O3 O1 O3 106.02(16) 2_566 3
O3 O1 O3 115.16(18) 5_456 3
La O1 O3 62.99(12) 1_556 3
La O1 O3 84.28(17) 2_566 3
La O1 O3 113.2(2) 4_456 3
O3 O1 O3 41.7(2) 5 3
O3 O1 O3 90.4(2) 2_455 3
O3 O1 O3 144.9(2) 6_565 3
Ga2 O1 O3 71.40(13) 1_665 3
Ga2 O1 O3 49.67(11) . 3
Ga2 O1 O3 155.1(3) 1_565 3
O1 O1 O3 74.04(11) 2_565 3
O1 O1 O3 53.14(15) 2_455 3
O1 O1 O3 159.8(4) 2_465 3
O1 O1 O3 86.48(18) 1_556 3
O1 O1 O3 93.52(18) 1_554 3
Ga3 O1 O3 126.38(16) 2_465 3
Ga3 O1 O3 18.11(10) 4_446 3
Ga3 O1 O3 107.38(15) 1_666 3
O3 O1 O3 42.2(3) 5_556 3
O3 O1 O3 87.05(19) 2_456 3
O3 O1 O3 133.5(3) 6_566 3
O3 O1 O3 27.61(14) 4 3
O3 O1 O3 92.09(14) 3_455 3
O3 O1 O3 146.86(17) 1_565 3
O2 O1 O3 77.3(2) 6_554 3
O2 O1 O3 132.1(3) 5_454 3
O2 O1 O3 72.1(2) 2_564 3
O3 O1 O3 60.09(11) 1_554 3
O3 O1 O3 106.2(3) 4_454 3
O3 O1 O3 111.9(2) 3_564 3
O1 O1 O3 73.02(14) 2_566 3
O1 O1 O3 55.07(10) 2_456 3
O1 O1 O3 139.2(4) 2_466 3
Ga2 O1 O3 86.48(18) 2_566 4_565
La O1 O3 151.0(3) . 4_565
La O1 O3 41.85(16) 2_565 4_565
La O1 O3 86.13(11) 4_455 4_565
O2 O1 O3 90.5(4) 3_565 4_565
O2 O1 O3 123.4(4) . 4_565
O2 O1 O3 66.1(3) 4_455 4_565
O2 O1 O3 84.7(4) 3_566 4_565
O2 O1 O3 114.6(4) 1_556 4_565
O2 O1 O3 61.2(3) 4_456 4_565
O3 O1 O3 113.7(3) . 4_565
O3 O1 O3 6.4(3) 3_565 4_565
O3 O1 O3 124.9(4) 4_455 4_565
Ga2 O1 O3 93.52(18) 2_565 4_565
Ga3 O1 O3 136.4(3) 1_556 4_565
Ga3 O1 O3 89.50(14) 2_565 4_565
Ga3 O1 O3 36.64(14) 4_456 4_565
O2 O1 O3 164.2(4) 6 4_565
O2 O1 O3 55.4(3) 5_455 4_565
O2 O1 O3 64.5(3) 2_565 4_565
O3 O1 O3 123.24(14) 6 4_565
O3 O1 O3 32.8(3) 2_565 4_565
O3 O1 O3 112.41(13) 5_455 4_565
Ga3 O1 O3 128.8(2) . 4_565
Ga3 O1 O3 93.46(16) 2_564 4_565
Ga3 O1 O3 56.45(11) 4_455 4_565
Ga1 O1 O3 131.47(13) 1_455 4_565
Nb O1 O3 131.47(13) 1_455 4_565
Nb O1 O3 108.77(13) . 4_565
Ga1 O1 O3 108.77(13) . 4_565
Ga1 O1 O3 18.10(10) 1_565 4_565
Nb O1 O3 18.10(10) 1_565 4_565
O2 O1 O3 90.84(17) 2_465 4_565
O2 O1 O3 146.44(19) 5_445 4_565
O2 O1 O3 28.89(15) 6_665 4_565
O3 O1 O3 115.16(18) 6_556 4_565
O3 O1 O3 35.3(2) 2_566 4_565
O3 O1 O3 106.02(16) 5_456 4_565
La O1 O3 113.2(2) 1_556 4_565
La O1 O3 62.99(12) 2_566 4_565
La O1 O3 84.28(17) 4_456 4_565
O3 O1 O3 90.4(2) 5 4_565
O3 O1 O3 144.9(2) 2_455 4_565
O3 O1 O3 41.7(2) 6_565 4_565
Ga2 O1 O3 49.67(11) 1_665 4_565
Ga2 O1 O3 155.1(3) . 4_565
Ga2 O1 O3 71.40(13) 1_565 4_565
O1 O1 O3 53.14(15) 2_565 4_565
O1 O1 O3 159.8(4) 2_455 4_565
O1 O1 O3 74.04(11) 2_465 4_565
O1 O1 O3 86.48(18) 1_556 4_565
O1 O1 O3 93.52(18) 1_554 4_565
Ga3 O1 O3 107.38(15) 2_465 4_565
Ga3 O1 O3 126.38(16) 4_446 4_565
Ga3 O1 O3 18.11(10) 1_666 4_565
O3 O1 O3 87.05(19) 5_556 4_565
O3 O1 O3 133.5(3) 2_456 4_565
O3 O1 O3 42.2(3) 6_566 4_565
O3 O1 O3 92.09(14) 4 4_565
O3 O1 O3 146.86(16) 3_455 4_565
O3 O1 O3 27.61(14) 1_565 4_565
O2 O1 O3 132.1(3) 6_554 4_565
O2 O1 O3 72.1(2) 5_454 4_565
O2 O1 O3 77.3(2) 2_564 4_565
O3 O1 O3 106.2(3) 1_554 4_565
O3 O1 O3 111.9(2) 4_454 4_565
O3 O1 O3 60.09(11) 3_564 4_565
O1 O1 O3 55.07(10) 2_566 4_565
O1 O1 O3 139.2(4) 2_456 4_565
O1 O1 O3 73.02(14) 2_466 4_565
O3 O1 O3 119.63(4) 3 4_565
Ga2 O1 O3 86.47(18) 2_566 1_455
La O1 O3 86.13(11) . 1_455
La O1 O3 151.0(3) 2_565 1_455
La O1 O3 41.85(16) 4_455 1_455
O2 O1 O3 123.4(4) 3_565 1_455
O2 O1 O3 66.1(3) . 1_455
O2 O1 O3 90.5(4) 4_455 1_455
O2 O1 O3 114.6(4) 3_566 1_455
O2 O1 O3 61.2(3) 1_556 1_455
O2 O1 O3 84.7(4) 4_456 1_455
O3 O1 O3 124.9(4) . 1_455
O3 O1 O3 113.7(3) 3_565 1_455
O3 O1 O3 6.4(3) 4_455 1_455
Ga2 O1 O3 93.52(18) 2_565 1_455
Ga3 O1 O3 36.64(14) 1_556 1_455
Ga3 O1 O3 136.4(3) 2_565 1_455
Ga3 O1 O3 89.50(14) 4_456 1_455
O2 O1 O3 55.4(3) 6 1_455
O2 O1 O3 64.5(3) 5_455 1_455
O2 O1 O3 164.2(4) 2_565 1_455
O3 O1 O3 112.41(13) 6 1_455
O3 O1 O3 123.24(14) 2_565 1_455
O3 O1 O3 32.8(3) 5_455 1_455
Ga3 O1 O3 56.45(11) . 1_455
Ga3 O1 O3 128.8(2) 2_564 1_455
Ga3 O1 O3 93.47(16) 4_455 1_455
Ga1 O1 O3 18.10(10) 1_455 1_455
Nb O1 O3 18.10(10) 1_455 1_455
Nb O1 O3 131.47(13) . 1_455
Ga1 O1 O3 131.47(13) . 1_455
Ga1 O1 O3 108.77(13) 1_565 1_455
Nb O1 O3 108.77(13) 1_565 1_455
O2 O1 O3 28.89(15) 2_465 1_455
O2 O1 O3 90.84(17) 5_445 1_455
O2 O1 O3 146.44(19) 6_665 1_455
O3 O1 O3 106.02(16) 6_556 1_455
O3 O1 O3 115.16(18) 2_566 1_455
O3 O1 O3 35.3(2) 5_456 1_455
La O1 O3 84.28(17) 1_556 1_455
La O1 O3 113.2(2) 2_566 1_455
La O1 O3 62.99(12) 4_456 1_455
O3 O1 O3 144.9(2) 5 1_455
O3 O1 O3 41.7(2) 2_455 1_455
O3 O1 O3 90.4(2) 6_565 1_455
Ga2 O1 O3 155.1(3) 1_665 1_455
Ga2 O1 O3 71.40(13) . 1_455
Ga2 O1 O3 49.67(11) 1_565 1_455
O1 O1 O3 159.8(4) 2_565 1_455
O1 O1 O3 74.04(11) 2_455 1_455
O1 O1 O3 53.14(15) 2_465 1_455
O1 O1 O3 86.48(18) 1_556 1_455
O1 O1 O3 93.52(18) 1_554 1_455
Ga3 O1 O3 18.11(10) 2_465 1_455
Ga3 O1 O3 107.38(15) 4_446 1_455
Ga3 O1 O3 126.38(16) 1_666 1_455
O3 O1 O3 133.5(3) 5_556 1_455
O3 O1 O3 42.2(3) 2_456 1_455
O3 O1 O3 87.05(19) 6_566 1_455
O3 O1 O3 146.86(16) 4 1_455
O3 O1 O3 27.61(14) 3_455 1_455
O3 O1 O3 92.09(14) 1_565 1_455
O2 O1 O3 72.1(2) 6_554 1_455
O2 O1 O3 77.3(2) 5_454 1_455
O2 O1 O3 132.1(3) 2_564 1_455
O3 O1 O3 111.9(2) 1_554 1_455
O3 O1 O3 60.09(11) 4_454 1_455
O3 O1 O3 106.2(3) 3_564 1_455
O1 O1 O3 139.2(4) 2_566 1_455
O1 O1 O3 73.03(14) 2_456 1_455
O1 O1 O3 55.07(10) 2_466 1_455
O3 O1 O3 119.63(4) 3 1_455
O3 O1 O3 119.63(4) 4_565 1_455
Ga2 O1 La 98.40(15) 2_566 4
La O1 La 81.39(9) . 4
La O1 La 36.79(3) 2_565 4
La O1 La 143.3(4) 4_455 4
O2 O1 La 49.21(19) 3_565 4
O2 O1 La 105.0(4) . 4
O2 O1 La 91.7(4) 4_455 4
O2 O1 La 67.9(2) 3_566 4
O2 O1 La 118.9(4) 1_556 4
O2 O1 La 105.5(3) 4_456 4
O3 O1 La 45.1(3) . 4
O3 O1 La 78.5(2) 3_565 4
O3 O1 La 162.8(2) 4_455 4
Ga2 O1 La 81.60(15) 2_565 4
Ga3 O1 La 137.34(15) 1_556 4
Ga3 O1 La 41.02(6) 2_565 4
Ga3 O1 La 102.96(6) 4_456 4
O2 O1 La 114.1(2) 6 4
O2 O1 La 127.7(2) 5_455 4
O2 O1 La 21.1(3) 2_565 4
O3 O1 La 55.18(14) 6 4
O3 O1 La 64.32(15) 2_565 4
O3 O1 La 142.6(4) 5_455 4
Ga3 O1 La 114.1(2) . 4
Ga3 O1 La 42.08(3) 2_564 4
Ga3 O1 La 90.78(14) 4_455 4
Ga1 O1 La 150.2(2) 1_455 4
Nb O1 La 150.2(2) 1_455 4
Nb O1 La 36.414(18) . 4
Ga1 O1 La 36.414(18) . 4
Ga1 O1 La 81.78(5) 1_565 4
Nb O1 La 81.78(5) 1_565 4
O2 O1 La 163.15(13) 2_465 4
O2 O1 La 78.61(13) 5_445 4
O2 O1 La 46.05(12) 6_665 4
O3 O1 La 69.09(12) 6_556 4
O3 O1 La 76.47(13) 2_566 4
O3 O1 La 149.6(3) 5_456 4
La O1 La 94.28(12) 1_556 4
La O1 La 74.57(7) 2_566 4
La O1 La 124.9(2) 4_456 4
O3 O1 La 23.46(12) 5 4
O3 O1 La 126.6(2) 2_455 4
O3 O1 La 97.79(15) 6_565 4
Ga2 O1 La 35.33(2) 1_665 4
Ga2 O1 La 99.13(3) . 4
Ga2 O1 La 142.81(8) 1_565 4
O1 O1 La 25.30(7) 2_565 4
O1 O1 La 93.47(11) 2_455 4
O1 O1 La 133.8(3) 2_465 4
O1 O1 La 98.40(15) 1_556 4
O1 O1 La 81.60(15) 1_554 4
Ga3 O1 La 169.8(3) 2_465 4
Ga3 O1 La 63.91(2) 4_446 4
Ga3 O1 La 66.10(2) 1_666 4
O3 O1 La 45.63(14) 5_556 4
O3 O1 La 133.08(19) 2_456 4
O3 O1 La 105.22(13) 6_566 4
O3 O1 La 24.04(11) 4 4
O3 O1 La 140.74(12) 3_455 4
O3 O1 La 99.69(12) 1_565 4
O2 O1 La 97.4(2) 6_554 4
O2 O1 La 105.0(2) 5_454 4
O2 O1 La 43.25(13) 2_564 4
O3 O1 La 58.40(13) 1_554 4
O3 O1 La 113.7(3) 4_454 4
O3 O1 La 75.98(19) 3_564 4
O1 O1 La 49.33(8) 2_566 4
O1 O1 La 100.46(7) 2_456 4
O1 O1 La 136.6(2) 2_466 4
O3 O1 La 49.74(11) 3 4
O3 O1 La 72.35(13) 4_565 4
O3 O1 La 167.50(16) 1_455 4
Ga2 O1 La 98.40(15) 2_566 2_455
La O1 La 36.79(3) . 2_455
La O1 La 143.3(4) 2_565 2_455
La O1 La 81.39(9) 4_455 2_455
O2 O1 La 91.7(4) 3_565 2_455
O2 O1 La 49.21(19) . 2_455
O2 O1 La 105.0(4) 4_455 2_455
O2 O1 La 105.5(3) 3_566 2_455
O2 O1 La 67.9(2) 1_556 2_455
O2 O1 La 118.9(4) 4_456 2_455
O3 O1 La 78.5(2) . 2_455
O3 O1 La 162.8(2) 3_565 2_455
O3 O1 La 45.1(3) 4_455 2_455
Ga2 O1 La 81.60(15) 2_565 2_455
Ga3 O1 La 41.02(6) 1_556 2_455
Ga3 O1 La 102.96(6) 2_565 2_455
Ga3 O1 La 137.34(15) 4_456 2_455
O2 O1 La 21.1(3) 6 2_455
O2 O1 La 114.1(2) 5_455 2_455
O2 O1 La 127.7(2) 2_565 2_455
O3 O1 La 64.32(15) 6 2_455
O3 O1 La 142.6(4) 2_565 2_455
O3 O1 La 55.18(13) 5_455 2_455
Ga3 O1 La 42.08(3) . 2_455
Ga3 O1 La 90.78(14) 2_564 2_455
Ga3 O1 La 114.1(2) 4_455 2_455
Ga1 O1 La 36.414(19) 1_455 2_455
Nb O1 La 36.414(19) 1_455 2_455
Nb O1 La 81.78(5) . 2_455
Ga1 O1 La 81.78(5) . 2_455
Ga1 O1 La 150.2(2) 1_565 2_455
Nb O1 La 150.2(2) 1_565 2_455
O2 O1 La 78.61(13) 2_465 2_455
O2 O1 La 46.05(12) 5_445 2_455
O2 O1 La 163.15(13) 6_665 2_455
O3 O1 La 76.47(13) 6_556 2_455
O3 O1 La 149.6(3) 2_566 2_455
O3 O1 La 69.09(12) 5_456 2_455
La O1 La 74.57(7) 1_556 2_455
La O1 La 124.9(2) 2_566 2_455
La O1 La 94.28(11) 4_456 2_455
O3 O1 La 97.79(15) 5 2_455
O3 O1 La 23.46(12) 2_455 2_455
O3 O1 La 126.6(2) 6_565 2_455
Ga2 O1 La 142.81(8) 1_665 2_455
Ga2 O1 La 35.33(2) . 2_455
Ga2 O1 La 99.13(3) 1_565 2_455
O1 O1 La 133.8(3) 2_565 2_455
O1 O1 La 25.30(7) 2_455 2_455
O1 O1 La 93.47(12) 2_465 2_455
O1 O1 La 98.40(15) 1_556 2_455
O1 O1 La 81.60(15) 1_554 2_455
Ga3 O1 La 63.91(2) 2_465 2_455
Ga3 O1 La 66.10(2) 4_446 2_455
Ga3 O1 La 169.8(3) 1_666 2_455
O3 O1 La 105.22(13) 5_556 2_455
O3 O1 La 45.63(14) 2_456 2_455
O3 O1 La 133.08(19) 6_566 2_455
O3 O1 La 99.69(12) 4 2_455
O3 O1 La 24.04(11) 3_455 2_455
O3 O1 La 140.74(12) 1_565 2_455
O2 O1 La 43.25(13) 6_554 2_455
O2 O1 La 97.4(2) 5_454 2_455
O2 O1 La 105.0(2) 2_564 2_455
O3 O1 La 75.98(19) 1_554 2_455
O3 O1 La 58.40(13) 4_454 2_455
O3 O1 La 113.7(3) 3_564 2_455
O1 O1 La 136.6(2) 2_566 2_455
O1 O1 La 49.33(8) 2_456 2_455
O1 O1 La 100.46(7) 2_466 2_455
O3 O1 La 72.35(13) 3 2_455
O3 O1 La 167.50(16) 4_565 2_455
O3 O1 La 49.74(11) 1_455 2_455
La O1 La 117.91(7) 4 2_455
Ga2 O1 La 98.39(15) 2_566 1_565
La O1 La 143.3(4) . 1_565
La O1 La 81.39(9) 2_565 1_565
La O1 La 36.79(3) 4_455 1_565
O2 O1 La 105.0(4) 3_565 1_565
O2 O1 La 91.7(4) . 1_565
O2 O1 La 49.21(19) 4_455 1_565
O2 O1 La 118.9(4) 3_566 1_565
O2 O1 La 105.5(3) 1_556 1_565
O2 O1 La 67.9(2) 4_456 1_565
O3 O1 La 162.8(2) . 1_565
O3 O1 La 45.1(3) 3_565 1_565
O3 O1 La 78.5(2) 4_455 1_565
Ga2 O1 La 81.60(15) 2_565 1_565
Ga3 O1 La 102.96(6) 1_556 1_565
Ga3 O1 La 137.34(15) 2_565 1_565
Ga3 O1 La 41.02(6) 4_456 1_565
O2 O1 La 127.7(2) 6 1_565
O2 O1 La 21.1(3) 5_455 1_565
O2 O1 La 114.1(2) 2_565 1_565
O3 O1 La 142.6(4) 6 1_565
O3 O1 La 55.18(13) 2_565 1_565
O3 O1 La 64.32(15) 5_455 1_565
Ga3 O1 La 90.78(14) . 1_565
Ga3 O1 La 114.1(2) 2_564 1_565
Ga3 O1 La 42.08(3) 4_455 1_565
Ga1 O1 La 81.78(5) 1_455 1_565
Nb O1 La 81.78(5) 1_455 1_565
Nb O1 La 150.2(2) . 1_565
Ga1 O1 La 150.2(2) . 1_565
Ga1 O1 La 36.414(19) 1_565 1_565
Nb O1 La 36.414(19) 1_565 1_565
O2 O1 La 46.05(12) 2_465 1_565
O2 O1 La 163.15(13) 5_445 1_565
O2 O1 La 78.61(13) 6_665 1_565
O3 O1 La 149.6(3) 6_556 1_565
O3 O1 La 69.09(12) 2_566 1_565
O3 O1 La 76.47(13) 5_456 1_565
La O1 La 124.9(2) 1_556 1_565
La O1 La 94.28(11) 2_566 1_565
La O1 La 74.57(7) 4_456 1_565
O3 O1 La 126.6(2) 5 1_565
O3 O1 La 97.79(15) 2_455 1_565
O3 O1 La 23.46(12) 6_565 1_565
Ga2 O1 La 99.13(3) 1_665 1_565
Ga2 O1 La 142.81(8) . 1_565
Ga2 O1 La 35.33(2) 1_565 1_565
O1 O1 La 93.47(12) 2_565 1_565
O1 O1 La 133.8(3) 2_455 1_565
O1 O1 La 25.30(7) 2_465 1_565
O1 O1 La 98.40(15) 1_556 1_565
O1 O1 La 81.60(15) 1_554 1_565
Ga3 O1 La 66.10(2) 2_465 1_565
Ga3 O1 La 169.8(3) 4_446 1_565
Ga3 O1 La 63.91(2) 1_666 1_565
O3 O1 La 133.08(19) 5_556 1_565
O3 O1 La 105.22(13) 2_456 1_565
O3 O1 La 45.63(14) 6_566 1_565
O3 O1 La 140.74(12) 4 1_565
O3 O1 La 99.69(12) 3_455 1_565
O3 O1 La 24.04(11) 1_565 1_565
O2 O1 La 105.0(2) 6_554 1_565
O2 O1 La 43.25(13) 5_454 1_565
O2 O1 La 97.4(2) 2_564 1_565
O3 O1 La 113.7(3) 1_554 1_565
O3 O1 La 75.98(19) 4_454 1_565
O3 O1 La 58.40(13) 3_564 1_565
O1 O1 La 100.46(7) 2_566 1_565
O1 O1 La 136.6(2) 2_456 1_565
O1 O1 La 49.33(8) 2_466 1_565
O3 O1 La 167.50(16) 3 1_565
O3 O1 La 49.74(11) 4_565 1_565
O3 O1 La 72.35(13) 1_455 1_565
La O1 La 117.91(7) 4 1_565
La O1 La 117.91(7) 2_455 1_565
Ga2 O1 O2 83.39(18) 2_566 6_565
La O1 O2 138.0(2) . 6_565
La O1 O2 102.64(13) 2_565 6_565
La O1 O2 32.3(2) 4_455 6_565
O2 O1 O2 125.3(4) 3_565 6_565
O2 O1 O2 94.8(5) . 6_565
O2 O1 O2 68.0(3) 4_455 6_565
O2 O1 O2 110.9(4) 3_566 6_565
O2 O1 O2 83.7(4) 1_556 6_565
O2 O1 O2 57.3(4) 4_456 6_565
O3 O1 O2 166.9(5) . 6_565
O3 O1 O2 59.6(3) 3_565 6_565
O3 O1 O2 59.6(3) 4_455 6_565
Ga2 O1 O2 96.60(18) 2_565 6_565
Ga3 O1 O2 80.73(14) 1_556 6_565
Ga3 O1 O2 139.0(3) 2_565 6_565
Ga3 O1 O2 41.00(16) 4_456 6_565
O2 O1 O2 107.7(3) 6 6_565
O2 O1 O2 11.3(3) 5_455 6_565
O2 O1 O2 127.4(4) 2_565 6_565
O3 O1 O2 155.2(4) 6 6_565
O3 O1 O2 77.66(16) 2_565 6_565
O3 O1 O2 58.1(2) 5_455 6_565
Ga3 O1 O2 90.07(18) . 6_565
Ga3 O1 O2 135.1(3) 2_564 6_565
Ga3 O1 O2 62.79(10) 4_455 6_565
Ga1 O1 O2 67.74(16) 1_455 6_565
Nb O1 O2 67.74(16) 1_455 6_565
Nb O1 O2 173.1(2) . 6_565
Ga1 O1 O2 173.1(2) . 6_565
Ga1 O1 O2 56.55(13) 1_565 6_565
Nb O1 O2 56.55(13) 1_565 6_565
O2 O1 O2 25.52(17) 2_465 6_565
O2 O1 O2 142.6(2) 5_445 6_565
O2 O1 O2 93.26(19) 6_665 6_565
O3 O1 O2 133.6(3) 6_556 6_565
O3 O1 O2 71.8(2) 2_566 6_565
O3 O1 O2 53.65(15) 5_456 6_565
La O1 O2 105.6(2) 1_556 6_565
La O1 O2 89.7(2) 2_566 6_565
La O1 O2 55.75(11) 4_456 6_565
O3 O1 O2 149.4(2) 5 6_565
O3 O1 O2 88.7(2) 2_455 6_565
O3 O1 O2 46.22(15) 6_565 6_565
Ga2 O1 O2 110.4(2) 1_665 6_565
Ga2 O1 O2 120.98(16) . 6_565
Ga2 O1 O2 13.26(10) 1_565 6_565
O1 O1 O2 114.91(14) 2_565 6_565
O1 O1 O2 125.84(19) 2_455 6_565
O1 O1 O2 27.5(2) 2_465 6_565
O1 O1 O2 83.39(18) 1_556 6_565
O1 O1 O2 96.60(18) 1_554 6_565
Ga3 O1 O2 44.38(13) 2_465 6_565
Ga3 O1 O2 150.3(3) 4_446 6_565
Ga3 O1 O2 74.72(17) 1_666 6_565
O3 O1 O2 132.6(3) 5_556 6_565
O3 O1 O2 82.55(17) 2_456 6_565
O3 O1 O2 42.15(19) 6_566 6_565
O3 O1 O2 155.7(2) 4 6_565
O3 O1 O2 81.58(17) 3_455 6_565
O3 O1 O2 37.98(18) 1_565 6_565
O2 O1 O2 107.4(3) 6_554 6_565
O2 O1 O2 58.55(11) 5_454 6_565
O2 O1 O2 119.5(3) 2_564 6_565
O3 O1 O2 130.2(3) 1_554 6_565
O3 O1 O2 79.7(2) 4_454 6_565
O3 O1 O2 79.68(16) 3_564 6_565
O1 O1 O2 105.2(2) 2_566 6_565
O1 O1 O2 113.8(2) 2_456 6_565
O1 O1 O2 29.74(15) 2_466 6_565
O3 O1 O2 168.4(3) 3 6_565
O3 O1 O2 65.48(18) 4_565 6_565
O3 O1 O2 54.14(18) 1_455 6_565
La O1 O2 137.63(14) 4 6_565
La O1 O2 103.48(16) 2_455 6_565
La O1 O2 22.85(11) 1_565 6_565
Ga2 O1 O2 83.40(18) 2_566 5
La O1 O2 102.64(13) . 5
La O1 O2 32.3(2) 2_565 5
La O1 O2 138.0(2) 4_455 5
O2 O1 O2 68.0(3) 3_565 5
O2 O1 O2 125.3(4) . 5
O2 O1 O2 94.8(5) 4_455 5
O2 O1 O2 57.3(4) 3_566 5
O2 O1 O2 110.9(4) 1_556 5
O2 O1 O2 83.7(4) 4_456 5
O3 O1 O2 59.6(3) . 5
O3 O1 O2 59.6(3) 3_565 5
O3 O1 O2 166.9(5) 4_455 5
Ga2 O1 O2 96.61(18) 2_565 5
Ga3 O1 O2 139.0(3) 1_556 5
Ga3 O1 O2 41.00(16) 2_565 5
Ga3 O1 O2 80.73(14) 4_456 5
O2 O1 O2 127.4(4) 6 5
O2 O1 O2 107.7(3) 5_455 5
O2 O1 O2 11.3(3) 2_565 5
O3 O1 O2 77.66(16) 6 5
O3 O1 O2 58.1(2) 2_565 5
O3 O1 O2 155.2(4) 5_455 5
Ga3 O1 O2 135.1(3) . 5
Ga3 O1 O2 62.79(10) 2_564 5
Ga3 O1 O2 90.07(18) 4_455 5
Ga1 O1 O2 173.1(2) 1_455 5
Nb O1 O2 173.1(2) 1_455 5
Nb O1 O2 56.55(13) . 5
Ga1 O1 O2 56.55(13) . 5
Ga1 O1 O2 67.74(16) 1_565 5
Nb O1 O2 67.74(16) 1_565 5
O2 O1 O2 142.6(2) 2_465 5
O2 O1 O2 93.26(19) 5_445 5
O2 O1 O2 25.52(17) 6_665 5
O3 O1 O2 71.8(2) 6_556 5
O3 O1 O2 53.65(15) 2_566 5
O3 O1 O2 133.6(3) 5_456 5
La O1 O2 89.7(2) 1_556 5
La O1 O2 55.75(11) 2_566 5
La O1 O2 105.6(2) 4_456 5
O3 O1 O2 46.22(15) 5 5
O3 O1 O2 149.4(2) 2_455 5
O3 O1 O2 88.7(2) 6_565 5
Ga2 O1 O2 13.26(10) 1_665 5
Ga2 O1 O2 110.4(2) . 5
Ga2 O1 O2 120.98(16) 1_565 5
O1 O1 O2 27.5(2) 2_565 5
O1 O1 O2 114.91(14) 2_455 5
O1 O1 O2 125.84(19) 2_465 5
O1 O1 O2 83.40(18) 1_556 5
O1 O1 O2 96.61(18) 1_554 5
Ga3 O1 O2 150.3(3) 2_465 5
Ga3 O1 O2 74.72(17) 4_446 5
Ga3 O1 O2 44.38(13) 1_666 5
O3 O1 O2 42.15(19) 5_556 5
O3 O1 O2 132.6(3) 2_456 5
O3 O1 O2 82.55(17) 6_566 5
O3 O1 O2 37.98(18) 4 5
O3 O1 O2 155.7(2) 3_455 5
O3 O1 O2 81.58(17) 1_565 5
O2 O1 O2 119.5(3) 6_554 5
O2 O1 O2 107.4(3) 5_454 5
O2 O1 O2 58.55(11) 2_564 5
O3 O1 O2 79.68(16) 1_554 5
O3 O1 O2 130.2(3) 4_454 5
O3 O1 O2 79.7(2) 3_564 5
O1 O1 O2 29.74(15) 2_566 5
O1 O1 O2 105.2(2) 2_456 5
O1 O1 O2 113.8(2) 2_466 5
O3 O1 O2 65.48(18) 3 5
O3 O1 O2 54.14(18) 4_565 5
O3 O1 O2 168.4(3) 1_455 5
La O1 O2 22.85(10) 4 5
La O1 O2 137.63(14) 2_455 5
La O1 O2 103.48(16) 1_565 5
O2 O1 O2 118.70(7) 6_565 5
Ga2 O1 O2 83.40(18) 2_566 2_455
La O1 O2 32.3(2) . 2_455
La O1 O2 138.0(2) 2_565 2_455
La O1 O2 102.64(13) 4_455 2_455
O2 O1 O2 94.8(5) 3_565 2_455
O2 O1 O2 68.0(3) . 2_455
O2 O1 O2 125.3(4) 4_455 2_455
O2 O1 O2 83.7(4) 3_566 2_455
O2 O1 O2 57.3(4) 1_556 2_455
O2 O1 O2 110.9(4) 4_456 2_455
O3 O1 O2 59.6(3) . 2_455
O3 O1 O2 166.9(5) 3_565 2_455
O3 O1 O2 59.6(3) 4_455 2_455
Ga2 O1 O2 96.61(18) 2_565 2_455
Ga3 O1 O2 41.00(16) 1_556 2_455
Ga3 O1 O2 80.73(14) 2_565 2_455
Ga3 O1 O2 139.0(3) 4_456 2_455
O2 O1 O2 11.3(3) 6 2_455
O2 O1 O2 127.4(4) 5_455 2_455
O2 O1 O2 107.7(3) 2_565 2_455
O3 O1 O2 58.1(2) 6 2_455
O3 O1 O2 155.2(4) 2_565 2_455
O3 O1 O2 77.66(16) 5_455 2_455
Ga3 O1 O2 62.79(10) . 2_455
Ga3 O1 O2 90.07(18) 2_564 2_455
Ga3 O1 O2 135.1(3) 4_455 2_455
Ga1 O1 O2 56.55(13) 1_455 2_455
Nb O1 O2 56.55(13) 1_455 2_455
Nb O1 O2 67.74(16) . 2_455
Ga1 O1 O2 67.74(16) . 2_455
Ga1 O1 O2 173.1(2) 1_565 2_455
Nb O1 O2 173.1(2) 1_565 2_455
O2 O1 O2 93.26(19) 2_465 2_455
O2 O1 O2 25.52(17) 5_445 2_455
O2 O1 O2 142.6(2) 6_665 2_455
O3 O1 O2 53.65(15) 6_556 2_455
O3 O1 O2 133.6(3) 2_566 2_455
O3 O1 O2 71.8(2) 5_456 2_455
La O1 O2 55.75(11) 1_556 2_455
La O1 O2 105.6(2) 2_566 2_455
La O1 O2 89.7(2) 4_456 2_455
O3 O1 O2 88.7(2) 5 2_455
O3 O1 O2 46.22(15) 2_455 2_455
O3 O1 O2 149.4(2) 6_565 2_455
Ga2 O1 O2 120.98(16) 1_665 2_455
Ga2 O1 O2 13.26(10) . 2_455
Ga2 O1 O2 110.4(2) 1_565 2_455
O1 O1 O2 125.84(19) 2_565 2_455
O1 O1 O2 27.5(2) 2_455 2_455
O1 O1 O2 114.91(14) 2_465 2_455
O1 O1 O2 83.40(18) 1_556 2_455
O1 O1 O2 96.60(18) 1_554 2_455
Ga3 O1 O2 74.72(17) 2_465 2_455
Ga3 O1 O2 44.38(13) 4_446 2_455
Ga3 O1 O2 150.3(3) 1_666 2_455
O3 O1 O2 82.55(17) 5_556 2_455
O3 O1 O2 42.15(19) 2_456 2_455
O3 O1 O2 132.6(3) 6_566 2_455
O3 O1 O2 81.58(17) 4 2_455
O3 O1 O2 37.98(18) 3_455 2_455
O3 O1 O2 155.7(2) 1_565 2_455
O2 O1 O2 58.55(11) 6_554 2_455
O2 O1 O2 119.5(3) 5_454 2_455
O2 O1 O2 107.4(3) 2_564 2_455
O3 O1 O2 79.7(2) 1_554 2_455
O3 O1 O2 79.68(16) 4_454 2_455
O3 O1 O2 130.2(3) 3_564 2_455
O1 O1 O2 113.8(2) 2_566 2_455
O1 O1 O2 29.74(15) 2_456 2_455
O1 O1 O2 105.2(2) 2_466 2_455
O3 O1 O2 54.14(18) 3 2_455
O3 O1 O2 168.4(3) 4_565 2_455
O3 O1 O2 65.49(18) 1_455 2_455
La O1 O2 103.48(16) 4 2_455
La O1 O2 22.85(11) 2_455 2_455
La O1 O2 137.63(14) 1_565 2_455
O2 O1 O2 118.70(7) 6_565 2_455
O2 O1 O2 118.70(7) 5 2_455
Ga2 O1 O3 30.00(11) 2_566 1_556
La O1 O3 86.5(3) . 1_556
La O1 O3 101.7(3) 2_565 1_556
La O1 O3 137.6(4) 4_455 1_556
O2 O1 O3 118.6(3) 3_565 1_556
O2 O1 O3 136.6(3) . 1_556
O2 O1 O3 163.3(3) 4_455 1_556
O2 O1 O3 14.6(3) 3_566 1_556
O2 O1 O3 42.8(3) 1_556 1_556
O2 O1 O3 58.9(3) 4_456 1_556
O3 O1 O3 53.5(3) . 1_556
O3 O1 O3 98.6(3) 3_565 1_556
O3 O1 O3 98.6(3) 4_455 1_556
Ga2 O1 O3 150.00(11) 2_565 1_556
Ga3 O1 O3 69.4(2) 1_556 1_556
Ga3 O1 O3 35.69(19) 2_565 1_556
Ga3 O1 O3 87.0(3) 4_456 1_556
O2 O1 O3 70.2(3) 6 1_556
O2 O1 O3 108.0(4) 5_455 1_556
O2 O1 O3 60.6(3) 2_565 1_556
O3 O1 O3 89.2(3) 6 1_556
O3 O1 O3 123.4(3) 2_565 1_556
O3 O1 O3 135.2(2) 5_455 1_556
Ga3 O1 O3 132.42(13) . 1_556
Ga3 O1 O3 108.59(11) 2_564 1_556
Ga3 O1 O3 154.89(17) 4_455 1_556
Ga1 O1 O3 111.0(2) 1_455 1_556
Nb O1 O3 111.0(2) 1_455 1_556
Nb O1 O3 70.61(15) . 1_556
Ga1 O1 O3 70.61(15) . 1_556
Ga1 O1 O3 116.4(2) 1_565 1_556
Nb O1 O3 116.4(2) 1_565 1_556
O2 O1 O3 108.4(3) 2_465 1_556
O2 O1 O3 57.5(2) 5_445 1_556
O2 O1 O3 80.4(3) 6_665 1_556
O3 O1 O3 22.9(2) 6_556 1_556
O3 O1 O3 65.4(2) 2_566 1_556
O3 O1 O3 74.0(2) 5_456 1_556
La O1 O3 20.06(12) 1_556 1_556
La O1 O3 36.76(15) 2_566 1_556
La O1 O3 58.61(17) 4_456 1_556
O3 O1 O3 87.7(2) 5 1_556
O3 O1 O3 113.8(2) 2_455 1_556
O3 O1 O3 137.8(2) 6_565 1_556
Ga2 O1 O3 61.98(19) 1_665 1_556
Ga2 O1 O3 56.38(17) . 1_556
Ga2 O1 O3 101.3(3) 1_565 1_556
O1 O1 O3 96.2(3) 2_565 1_556
O1 O1 O3 91.4(3) 2_455 1_556
O1 O1 O3 140.0(4) 2_465 1_556
O1 O1 O3 30.00(11) 1_556 1_556
O1 O1 O3 150.00(11) 1_554 1_556
Ga3 O1 O3 93.8(2) 2_465 1_556
Ga3 O1 O3 43.04(13) 4_446 1_556
Ga3 O1 O3 80.7(2) 1_666 1_556
O3 O1 O3 30.7(3) 5_556 1_556
O3 O1 O3 62.99(19) 2_456 1_556
O3 O1 O3 81.6(3) 6_566 1_556
O3 O1 O3 58.64(15) 4 1_556
O3 O1 O3 90.7(3) 3_455 1_556
O3 O1 O3 109.6(3) 1_565 1_556
O2 O1 O3 124.77(15) 6_554 1_556
O2 O1 O3 169.5(2) 5_454 1_556
O2 O1 O3 118.23(16) 2_564 1_556
O3 O1 O3 116.38(16) 1_554 1_556
O3 O1 O3 149.27(8) 4_454 1_556
O3 O1 O3 149.27(8) 3_564 1_556
O1 O1 O3 47.7(2) 2_566 1_556
O1 O1 O3 41.9(2) 2_456 1_556
O1 O1 O3 84.0(3) 2_466 1_556
O3 O1 O3 56.65(14) 3 1_556
O3 O1 O3 98.8(2) 4_565 1_556
O3 O1 O3 103.8(3) 1_455 1_556
La O1 O3 76.30(14) 4 1_556
La O1 O3 91.00(16) 2_455 1_556
La O1 O3 126.8(2) 1_565 1_556
O2 O1 O3 113.4(3) 6_565 1_556
O2 O1 O3 69.6(2) 5 1_556
O2 O1 O3 69.63(17) 2_455 1_556
Ga3 O3 Nb 111.8(5) 2_565 .
Ga3 O3 Ga1 111.8(5) 2_565 .
Nb O3 Ga1 0.0 . .
Ga3 O3 La 138.2(5) 2_565 .
Nb O3 La 105.4(4) . .
Ga1 O3 La 105.4(4) . .
Ga3 O3 Ga3 94.1(5) 2_565 4_446
Nb O3 Ga3 87.4(4) . 4_446
Ga1 O3 Ga3 87.4(4) . 4_446
La O3 Ga3 106.0(5) . 4_446
Ga3 O3 O3 154.6(8) 2_565 6
Nb O3 O3 48.6(3) . 6
Ga1 O3 O3 48.6(3) . 6
La O3 O3 56.8(2) . 6
Ga3 O3 O3 100.1(7) 4_446 6
Ga3 O3 O3 65.1(5) 2_565 4
Nb O3 O3 46.9(2) . 4
Ga1 O3 O3 46.9(2) . 4
La O3 O3 149.4(3) . 4
Ga3 O3 O3 87.6(3) 4_446 4
O3 O3 O3 94.37(8) 6 4
Ga3 O3 O3 105.2(3) 2_565 3
Nb O3 O3 46.9(2) . 3
Ga1 O3 O3 46.9(2) . 3
La O3 O3 114.0(7) . 3
Ga3 O3 O3 40.5(3) 4_446 3
O3 O3 O3 73.9(6) 6 3
O3 O3 O3 60.0 4 3
Ga3 O3 O2 126.0(7) 2_565 5_445
Nb O3 O2 95.8(5) . 5_445
Ga1 O3 O2 95.8(5) . 5_445
La O3 O2 66.1(4) . 5_445
Ga3 O3 O2 40.0(3) 4_446 5_445
O3 O3 O2 76.8(6) 6 5_445
O3 O3 O2 121.3(6) 4 5_445
O3 O3 O2 61.9(6) 3 5_445
Ga3 O3 O3 62.2(4) 2_565 6_556
Nb O3 O3 119.4(5) . 6_556
Ga1 O3 O3 119.4(5) . 6_556
La O3 O3 114.0(5) . 6_556
Ga3 O3 O3 39.4(4) 4_446 6_556
O3 O3 O3 138.0(11) 6 6_556
O3 O3 O3 94.06(9) 4 6_556
O3 O3 O3 75.1(5) 3 6_556
O2 O3 O3 63.8(5) 5_445 6_556
Ga3 O3 O2 39.8(4) 2_565 2_565
Nb O3 O2 94.8(6) . 2_565
Ga1 O3 O2 94.8(6) . 2_565
La O3 O2 120.6(5) . 2_565
Ga3 O3 O2 130.6(5) 4_446 2_565
O3 O3 O2 117.9(8) 6 2_565
O3 O3 O2 60.7(7) 4 2_565
O3 O3 O2 120.1(7) 3 2_565
O2 O3 O2 165.3(7) 5_445 2_565
O3 O3 O2 102.0(5) 6_556 2_565
Ga3 O3 O2 36.3(3) 2_565 3_566
Nb O3 O2 147.9(5) . 3_566
Ga1 O3 O2 147.9(5) . 3_566
La O3 O2 103.8(3) . 3_566
Ga3 O3 O2 97.1(5) 4_446 3_566
O3 O3 O2 157.1(5) 6 3_566
O3 O3 O2 101.3(5) 4 3_566
O3 O3 O2 128.5(3) 3 3_566
O2 O3 O2 108.1(6) 5_445 3_566
O3 O3 O2 57.8(5) 6_556 3_566
O2 O3 O2 58.5(6) 2_565 3_566
Ga3 O3 O1 87.9(4) 2_565 .
Nb O3 O1 132.6(6) . .
Ga1 O3 O1 132.6(6) . .
La O3 O1 52.2(2) . .
Ga3 O3 O1 135.5(5) 4_446 .
O3 O3 O1 96.4(5) 6 .
O3 O3 O1 132.0(7) 4 .
O3 O3 O1 166.1(6) 3 .
O2 O3 O1 106.7(4) 5_445 .
O3 O3 O1 107.9(4) 6_556 .
O2 O3 O1 73.0(4) 2_565 .
O2 O3 O1 60.8(4) 3_566 .
Ga3 O3 O3 100.3(6) 2_565 5
Nb O3 O3 36.0(4) . 5
Ga1 O3 O3 36.0(4) . 5
La O3 O3 98.8(5) . 5
Ga3 O3 O3 122.8(2) 4_446 5
O3 O3 O3 54.3(5) 6 5
O3 O3 O3 51.8(4) 4 5
O3 O3 O3 82.3(4) 3 5
O2 O3 O3 126.1(4) 5_445 5
O3 O3 O3 145.6(3) 6_556 5
O2 O3 O3 67.5(5) 2_565 5
O2 O3 O3 125.8(5) 3_566 5
O1 O3 O3 100.3(3) . 5
Ga3 O3 O2 112.5(6) 2_565 3_565
Nb O3 O2 79.6(5) . 3_565
Ga1 O3 O2 79.6(5) . 3_565
La O3 O2 56.3(3) . 3_565
Ga3 O3 O2 153.2(4) 4_446 3_565
O3 O3 O2 54.0(6) 6 3_565
O3 O3 O2 100.0(5) 4 3_565
O3 O3 O2 123.2(2) 3 3_565
O2 O3 O2 117.8(5) 5_445 3_565
O3 O3 O2 160.9(4) 6_556 3_565
O2 O3 O2 74.3(5) 2_565 3_565
O2 O3 O2 106.4(5) 3_566 3_565
O1 O3 O2 53.0(4) . 3_565
O3 O3 O2 50.9(3) 5 3_565
Ga3 O3 O3 22.7(4) 2_565 5_556
Nb O3 O3 99.0(5) . 5_556
Ga1 O3 O3 99.0(5) . 5_556
La O3 O3 155.6(6) . 5_556
Ga3 O3 O3 74.5(3) 4_446 5_556
O3 O3 O3 147.6(4) 6 5_556
O3 O3 O3 54.0(5) 4 5_556
O3 O3 O3 82.7(4) 3 5_556
O2 O3 O3 111.6(5) 5_445 5_556
O3 O3 O3 50.9(4) 6_556 5_556
O2 O3 O3 56.4(3) 2_565 5_556
O2 O3 O3 52.6(3) 3_566 5_556
O1 O3 O3 109.9(3) . 5_556
O3 O3 O3 101.2(6) 5 5_556
O2 O3 O3 130.5(5) 3_565 5_556
Ga3 O3 Ga2 65.7(3) 2_565 2_566
Nb O3 Ga2 160.0(7) . 2_566
Ga1 O3 Ga2 160.0(7) . 2_566
La O3 Ga2 72.8(2) . 2_566
Ga3 O3 Ga2 112.5(4) 4_446 2_566
O3 O3 Ga2 125.8(4) 6 2_566
O3 O3 Ga2 127.7(6) 4 2_566
O3 O3 Ga2 152.6(4) 3 2_566
O2 O3 Ga2 101.3(4) 5_445 2_566
O3 O3 Ga2 78.0(3) 6_556 2_566
O2 O3 Ga2 70.6(4) 2_565 2_566
O2 O3 Ga2 31.9(2) 3_566 2_566
O1 O3 Ga2 31.2(3) . 2_566
O3 O3 Ga2 124.0(2) 5 2_566
O2 O3 Ga2 83.2(3) 3_565 2_566
O3 O3 Ga2 84.4(3) 5_556 2_566
Ga3 O3 Ga3 62.8(3) 2_565 1_656
Nb O3 Ga3 60.0(2) . 1_656
Ga1 O3 Ga3 60.0(2) . 1_656
La O3 Ga3 158.3(4) . 1_656
Ga3 O3 Ga3 60.1(2) 4_446 1_656
O3 O3 Ga3 106.7(2) 6 1_656
O3 O3 Ga3 28.98(18) 4 1_656
O3 O3 Ga3 44.4(3) 3 1_656
O2 O3 Ga3 97.9(4) 5_445 1_656
O3 O3 Ga3 67.2(2) 6_556 1_656
O2 O3 Ga3 78.6(4) 2_565 1_656
O2 O3 Ga3 94.9(3) 3_566 1_656
O1 O3 Ga3 149.5(4) . 1_656
O3 O3 Ga3 78.5(3) 5 1_656
O2 O3 Ga3 128.5(4) 3_565 1_656
O3 O3 Ga3 42.4(2) 5_556 1_656
Ga2 O3 Ga3 126.8(3) 2_566 1_656
Ga3 O3 La 74.1(4) 2_565 2_565
Nb O3 La 100.8(5) . 2_565
Ga1 O3 La 100.8(5) . 2_565
La O3 La 81.1(3) . 2_565
Ga3 O3 La 167.5(4) 4_446 2_565
O3 O3 La 92.4(7) 6 2_565
O3 O3 La 91.1(6) 4 2_565
O3 O3 La 146.0(5) 3 2_565
O2 O3 La 146.2(4) 5_445 2_565
O3 O3 La 128.4(5) 6_556 2_565
O2 O3 La 40.0(3) 2_565 2_565
O2 O3 La 70.9(4) 3_566 2_565
O1 O3 La 41.89(18) . 2_565
O3 O3 La 64.80(17) 5 2_565
O2 O3 La 39.2(3) 3_565 2_565
O3 O3 La 94.7(2) 5_556 2_565
Ga2 O3 La 59.16(18) 2_566 2_565
Ga3 O3 La 115.9(3) 1_656 2_565
Ga3 O3 O2 116.9(5) 2_565 6
Nb O3 O2 130.2(5) . 6
Ga1 O3 O2 130.2(5) . 6
La O3 O2 37.0(2) . 6
Ga3 O3 O2 79.7(4) 4_446 6
O3 O3 O2 86.5(3) 6 6
O3 O3 O2 167.3(6) 4 6
O3 O3 O2 108.4(7) 3 6
O2 O3 O2 46.6(4) 5_445 6
O3 O3 O2 77.1(3) 6_556 6
O2 O3 O2 129.7(5) 2_565 6
O2 O3 O2 81.8(3) 3_566 6
O1 O3 O2 60.3(2) . 6
O3 O3 O2 135.6(5) 5 6
O2 O3 O2 90.8(3) 3_565 6
O3 O3 O2 122.6(6) 5_556 6
Ga2 O3 O2 59.9(3) 2_566 6
Ga3 O3 O2 139.1(5) 1_656 6
La O3 O2 101.6(3) 2_565 6
Ga3 O3 O3 119.3(4) 2_565 2
Nb O3 O3 9.3(4) . 2
Ga1 O3 O3 9.3(4) . 2
La O3 O3 99.9(4) . 2
Ga3 O3 O3 81.6(3) 4_446 2
O3 O3 O3 43.7(2) 6 2
O3 O3 O3 54.3(4) 4 2
O3 O3 O3 42.0(3) 3 2
O2 O3 O3 86.7(3) 5_445 2
O3 O3 O3 116.7(5) 6_556 2
O2 O3 O3 104.1(4) 2_565 2
O2 O3 O3 155.6(4) 3_566 2
O1 O3 O3 134.7(6) . 2
O3 O3 O3 43.3(2) 5 2
O2 O3 O3 82.2(4) 3_565 2
O3 O3 O3 104.3(3) 5_556 2
Ga2 O3 O3 165.3(5) 2_566 2
Ga3 O3 O3 63.2(3) 1_656 2
La O3 O3 107.7(3) 2_565 2
O2 O3 O3 121.5(3) 6 2
Ga3 O3 Ga3 117.9(6) 2_565 2_564
Nb O3 Ga3 52.0(3) . 2_564
Ga1 O3 Ga3 52.0(3) . 2_564
La O3 Ga3 72.1(3) . 2_564
Ga3 O3 Ga3 134.4(3) 4_446 2_564
O3 O3 Ga3 39.3(5) 6 2_564
O3 O3 Ga3 78.8(2) 4 2_564
O3 O3 Ga3 96.92(13) 3 2_564
O2 O3 Ga3 115.7(4) 5_445 2_564
O3 O3 Ga3 171.3(3) 6_556 2_564
O2 O3 Ga3 78.9(4) 2_565 2_564
O2 O3 Ga3 128.1(5) 3_566 2_564
O1 O3 Ga3 80.7(4) . 2_564
O3 O3 Ga3 27.0(2) 5 2_564
O2 O3 Ga3 27.7(2) 3_565 2_564
O3 O3 Ga3 125.6(6) 5_556 2_564
Ga2 O3 Ga3 110.2(3) 2_566 2_564
Ga3 O3 Ga3 104.8(3) 1_656 2_564
La O3 Ga3 57.3(2) 2_565 2_564
O2 O3 Ga3 109.1(3) 6 2_564
O3 O3 Ga3 55.1(3) 2 2_564
Ga3 O3 Ga2 114.3(5) 2_565 .
Nb O3 Ga2 119.4(5) . .
Ga1 O3 Ga2 119.4(5) . .
La O3 Ga2 58.3(3) . .
Ga3 O3 Ga2 52.8(2) 4_446 .
O3 O3 Ga2 91.1(5) 6 .
O3 O3 Ga2 140.4(5) 4 .
O3 O3 Ga2 84.3(6) 3 .
O2 O3 Ga2 24.1(2) 5_445 .
O3 O3 Ga2 58.1(3) 6_556 .
O2 O3 Ga2 145.4(5) 2_565 .
O2 O3 Ga2 87.4(4) 3_566 .
O1 O3 Ga2 86.0(2) . .
O3 O3 Ga2 145.1(4) 5 .
O2 O3 Ga2 114.6(3) 3_565 .
O3 O3 Ga2 108.8(5) 5_556 .
Ga2 O3 Ga2 77.2(2) 2_566 .
Ga3 O3 Ga2 112.6(3) 1_656 .
La O3 Ga2 127.9(2) 2_565 .
O2 O3 Ga2 26.92(17) 6 .
O3 O3 Ga2 110.20(15) 2 .
Ga3 O3 Ga2 125.3(3) 2_564 .
Ga3 O3 O3 64.1(4) 2_565 2_556
Nb O3 O3 79.5(4) . 2_556
Ga1 O3 O3 79.5(4) . 2_556
La O3 O3 143.5(4) . 2_556
Ga3 O3 O3 37.5(2) 4_446 2_556
O3 O3 O3 117.8(4) 6 2_556
O3 O3 O3 55.7(3) 4 2_556
O3 O3 O3 44.1(3) 3 2_556
O2 O3 O3 77.5(3) 5_445 2_556
O3 O3 O3 41.9(2) 6_556 2_556
O2 O3 O3 94.4(3) 2_565 2_556
O2 O3 O3 84.9(4) 3_566 2_556
O1 O3 O3 145.2(5) . 2_556
O3 O3 O3 104.5(3) 5 2_556
O2 O3 O3 155.3(4) 3_565 2_556
O3 O3 O3 41.6(2) 5_556 2_556
Ga2 O3 O3 114.2(4) 2_566 2_556
Ga3 O3 O3 26.84(19) 1_656 2_556
La O3 O3 134.37(18) 2_565 2_556
O2 O3 O3 112.8(3) 6 2_556
O3 O3 O3 79.4(4) 2 2_556
Ga3 O3 O3 129.6(3) 2_564 2_556
Ga2 O3 O3 87.3(2) . 2_556
Ga3 O3 Ga1 45.1(3) 2_565 1_556
Nb O3 Ga1 105.9(4) . 1_556
Ga1 O3 Ga1 105.9(4) . 1_556
La O3 Ga1 138.2(5) . 1_556
Ga3 O3 Ga1 49.1(2) 4_446 1_556
O3 O3 Ga1 144.8(6) 6 1_556
O3 O3 Ga1 71.05(11) 4 1_556
O3 O3 Ga1 71.05(11) 3 1_556
O2 O3 Ga1 83.8(4) 5_445 1_556
O3 O3 Ga1 24.44(18) 6_556 1_556
O2 O3 Ga1 83.4(3) 2_565 1_556
O2 O3 Ga1 57.4(3) 3_566 1_556
O1 O3 Ga1 117.4(4) . 1_556
O3 O3 Ga1 122.8(4) 5 1_556
O2 O3 Ga1 157.5(4) 3_565 1_556
O3 O3 Ga1 28.0(2) 5_556 1_556
Ga2 O3 Ga1 86.4(2) 2_566 1_556
Ga3 O3 Ga1 47.06(13) 1_656 1_556
La O3 Ga1 118.9(3) 2_565 1_556
O2 O3 Ga1 101.2(4) 6 1_556
O3 O3 Ga1 106.9(4) 2 1_556
Ga3 O3 Ga1 149.7(3) 2_564 1_556
Ga2 O3 Ga1 82.2(3) . 1_556
O3 O3 Ga1 27.9(2) 2_556 1_556
Ga3 O3 Nb 45.1(3) 2_565 1_556
Nb O3 Nb 105.9(4) . 1_556
Ga1 O3 Nb 105.9(4) . 1_556
La O3 Nb 138.2(5) . 1_556
Ga3 O3 Nb 49.1(2) 4_446 1_556
O3 O3 Nb 144.8(6) 6 1_556
O3 O3 Nb 71.05(11) 4 1_556
O3 O3 Nb 71.05(11) 3 1_556
O2 O3 Nb 83.8(4) 5_445 1_556
O3 O3 Nb 24.44(18) 6_556 1_556
O2 O3 Nb 83.4(3) 2_565 1_556
O2 O3 Nb 57.4(3) 3_566 1_556
O1 O3 Nb 117.4(4) . 1_556
O3 O3 Nb 122.8(4) 5 1_556
O2 O3 Nb 157.5(4) 3_565 1_556
O3 O3 Nb 28.0(2) 5_556 1_556
Ga2 O3 Nb 86.4(2) 2_566 1_556
Ga3 O3 Nb 47.06(13) 1_656 1_556
La O3 Nb 118.9(3) 2_565 1_556
O2 O3 Nb 101.2(4) 6 1_556
O3 O3 Nb 106.9(4) 2 1_556
Ga3 O3 Nb 149.7(3) 2_564 1_556
Ga2 O3 Nb 82.2(3) . 1_556
O3 O3 Nb 27.9(2) 2_556 1_556
Ga1 O3 Nb 0.0 1_556 1_556
Ga3 O3 O2 77.2(3) 2_565 1_556
Nb O3 O2 170.8(5) . 1_556
Ga1 O3 O2 170.8(5) . 1_556
La O3 O2 66.7(3) . 1_556
Ga3 O3 O2 90.3(4) 4_446 1_556
O3 O3 O2 123.4(2) 6 1_556
O3 O3 O2 141.9(4) 4 1_556
O3 O3 O2 130.6(6) 3 1_556
O2 O3 O2 76.9(3) 5_445 1_556
O3 O3 O2 62.4(2) 6_556 1_556
O2 O3 O2 93.5(3) 2_565 1_556
O2 O3 O2 41.3(4) 3_566 1_556
O1 O3 O2 46.9(3) . 1_556
O3 O3 O2 146.8(3) 5 1_556
O2 O3 O2 98.8(3) 3_565 1_556
O3 O3 O2 88.9(4) 5_556 1_556
Ga2 O3 O2 24.94(18) 2_566 1_556
Ga3 O3 O2 125.9(3) 1_656 1_556
La O3 O2 83.0(2) 2_565 1_556
O2 O3 O2 40.7(4) 6 1_556
O3 O3 O2 161.9(2) 2 1_556
Ga3 O3 O2 126.2(3) 2_564 1_556
Ga2 O3 O2 52.9(2) . 1_556
O3 O3 O2 103.9(4) 2_556 1_556
Ga1 O3 O2 79.1(2) 1_556 1_556
Nb O3 O2 79.1(2) 1_556 1_556
Ga3 O3 La 67.2(4) 2_565 4
Nb O3 La 53.5(3) . 4
Ga1 O3 La 53.5(3) . 4
La O3 La 127.4(5) . 4
Ga3 O3 La 118.3(3) 4_446 4
O3 O3 La 87.5(5) 6 4
O3 O3 La 30.7(3) 4 4
O3 O3 La 86.4(4) 3 4
O2 O3 La 147.3(4) 5_445 4
O3 O3 La 118.1(3) 6_556 4
O2 O3 La 41.3(4) 2_565 4
O2 O3 La 97.5(4) 3_566 4
O1 O3 La 103.3(4) . 4
O3 O3 La 33.6(3) 5 4
O2 O3 La 71.8(3) 3_565 4
O3 O3 La 68.7(4) 5_556 4
Ga2 O3 La 111.0(3) 2_566 4
Ga3 O3 La 59.15(16) 1_656 4
La O3 La 61.5(2) 2_565 4
O2 O3 La 161.7(4) 6 4
O3 O3 La 62.85(14) 2 4
Ga3 O3 La 57.10(19) 2_564 4
Ga2 O3 La 170.6(3) . 4
O3 O3 La 85.17(17) 2_556 4
Ga1 O3 La 93.7(2) 1_556 4
Nb O3 La 93.7(2) 1_556 4
O2 O3 La 134.7(3) 1_556 4
Ga3 O3 O1 158.2(6) 2_565 2_455
Nb O3 O1 89.2(4) . 2_455
Ga1 O3 O1 89.2(4) . 2_455
La O3 O1 29.70(17) . 2_455
Ga3 O3 O1 80.7(3) 4_446 2_455
O3 O3 O1 46.6(3) 6 2_455
O3 O3 O1 135.2(4) 4 2_455
O3 O3 O1 84.7(5) 3 2_455
O2 O3 O1 42.0(3) 5_445 2_455
O3 O3 O1 103.0(5) 6_556 2_455
O2 O3 O1 148.6(5) 2_565 2_455
O2 O3 O1 122.9(4) 3_566 2_455
O1 O3 O1 81.4(2) . 2_455
O3 O3 O1 100.3(5) 5 2_455
O2 O3 O1 75.8(3) 3_565 2_455
O3 O3 O1 153.3(6) 5_556 2_455
Ga2 O3 O1 96.5(2) 2_566 2_455
Ga3 O3 O1 129.0(3) 1_656 2_455
La O3 O1 108.7(3) 2_565 2_455
O2 O3 O1 41.4(3) 6 2_455
O3 O3 O1 81.1(3) 2 2_455
Ga3 O3 O1 79.2(3) 2_564 2_455
Ga2 O3 O1 46.3(2) . 2_455
O3 O3 O1 117.0(2) 2_556 2_455
Ga1 O3 O1 125.3(4) 1_556 2_455
Nb O3 O1 125.3(4) 1_556 2_455
O2 O3 O1 81.6(3) 1_556 2_455
La O3 O1 133.8(4) 4 2_455
Ga3 O3 Ga3 152.8(5) 2_565 4_445
Nb O3 Ga3 41.8(2) . 4_445
Ga1 O3 Ga3 41.8(2) . 4_445
La O3 Ga3 64.4(2) . 4_445
Ga3 O3 Ga3 91.2(3) 4_446 4_445
O3 O3 Ga3 10.4(3) 6 4_445
O3 O3 Ga3 88.61(19) 4 4_445
O3 O3 Ga3 63.5(2) 3 4_445
O2 O3 Ga3 72.5(3) 5_445 4_445
O3 O3 Ga3 130.1(6) 6_556 4_445
O2 O3 Ga3 122.0(5) 2_565 4_445
O2 O3 Ga3 167.3(4) 3_566 4_445
O1 O3 Ga3 106.6(4) . 4_445
O3 O3 Ga3 55.2(3) 5 4_445
O2 O3 Ga3 63.6(3) 3_565 4_445
O3 O3 Ga3 139.6(4) 5_556 4_445
Ga2 O3 Ga3 135.4(3) 2_566 4_445
Ga3 O3 Ga3 97.6(2) 1_656 4_445
La O3 Ga3 101.2(3) 2_565 4_445
O2 O3 Ga3 90.2(3) 6 4_445
O3 O3 Ga3 35.5(2) 2 4_445
Ga3 O3 Ga3 45.65(13) 2_564 4_445
Ga2 O3 Ga3 90.0(2) . 4_445
O3 O3 Ga3 107.5(3) 2_556 4_445
Ga1 O3 Ga3 134.4(3) 1_556 4_445
Nb O3 Ga3 134.4(3) 1_556 4_445
O2 O3 Ga3 129.5(3) 1_556 4_445
La O3 Ga3 86.9(2) 4 4_445
O1 O3 Ga3 49.0(2) 2_455 4_445
Ga3 O3 La 64.4(4) 2_565 1_556
Nb O3 La 149.1(5) . 1_556
Ga1 O3 La 149.1(5) . 1_556
La O3 La 92.4(3) . 1_556
Ga3 O3 La 63.2(3) 4_446 1_556
O3 O3 La 141.0(5) 6 1_556
O3 O3 La 118.09(12) 4 1_556
O3 O3 La 102.9(3) 3 1_556
O2 O3 La 68.3(3) 5_445 1_556
O3 O3 La 29.98(18) 6_556 1_556
O2 O3 La 97.6(4) 2_565 1_556
O2 O3 La 40.2(4) 3_566 1_556
O1 O3 La 78.2(3) . 1_556
O3 O3 La 164.6(4) 5 1_556
O2 O3 La 131.1(3) 3_565 1_556
O3 O3 La 65.6(4) 5_556 1_556
Ga2 O3 La 49.77(15) 2_566 1_556
Ga3 O3 La 95.0(3) 1_656 1_556
La O3 La 106.9(2) 2_565 1_556
O2 O3 La 57.0(3) 6 1_556
O3 O3 La 144.7(4) 2 1_556
Ga3 O3 La 158.7(3) 2_564 1_556
Ga2 O3 La 50.32(16) . 1_556
O3 O3 La 71.4(3) 2_556 1_556
Ga1 O3 La 48.11(14) 1_556 1_556
Nb O3 La 48.11(14) 1_556 1_556
O2 O3 La 32.54(16) 1_556 1_556
La O3 La 131.4(3) 4 1_556
O1 O3 La 94.7(3) 2_455 1_556
Ga3 O3 La 140.1(3) 4_445 1_556
Ga3 O3 O2 94.5(5) 2_565 4_446
Nb O3 O2 88.3(4) . 4_446
Ga1 O3 O2 88.3(4) . 4_446
La O3 O2 105.0(5) . 4_446
Ga3 O3 O2 1.2(2) 4_446 4_446
O3 O3 O2 100.1(7) 6 4_446
O3 O3 O2 88.8(4) 4 4_446
O3 O3 O2 41.5(3) 3 4_446
O2 O3 O2 39.1(5) 5_445 4_446
O3 O3 O2 39.1(4) 6_556 4_446
O2 O3 O2 131.3(5) 2_565 4_446
O2 O3 O2 96.8(5) 3_566 4_446
O1 O3 O2 134.4(4) . 4_446
O3 O3 O2 123.8(2) 5 4_446
O2 O3 O2 152.9(4) 3_565 4_446
O3 O3 O2 75.1(3) 5_556 4_446
Ga2 O3 O2 111.6(4) 2_566 4_446
Ga3 O3 O2 61.3(3) 1_656 4_446
La O3 O2 167.4(3) 2_565 4_446
O2 O3 O2 78.5(4) 6 4_446
O3 O3 O2 82.4(3) 2 4_446
Ga3 O3 O2 134.8(3) 2_564 4_446
Ga2 O3 O2 51.6(3) . 4_446
O3 O3 O2 38.5(3) 2_556 4_446
Ga1 O3 O2 49.5(2) 1_556 4_446
Nb O3 O2 49.5(2) 1_556 4_446
O2 O3 O2 89.3(4) 1_556 4_446
La O3 O2 119.5(3) 4 4_446
O1 O3 O2 79.9(4) 2_455 4_446
Ga3 O3 O2 91.3(3) 4_445 4_446
La O3 O2 62.4(2) 1_556 4_446
Ga3 O3 O2 127.3(5) 2_565 .
Nb O3 O2 103.6(4) . .
Ga1 O3 O2 103.6(4) . .
La O3 O2 20.0(2) . .
Ga3 O3 O2 126.0(4) 4_446 .
O3 O3 O2 58.2(3) 6 .
O3 O3 O2 137.4(4) 4 .
O3 O3 O2 127.5(5) 3 .
O2 O3 O2 86.0(3) 5_445 .
O3 O3 O2 128.3(2) 6_556 .
O2 O3 O2 101.4(4) 2_565 .
O2 O3 O2 99.4(3) 3_566 .
O1 O3 O2 39.9(3) . .
O3 O3 O2 86.0(4) 5 .
O2 O3 O2 38.2(3) 3_565 .
O3 O3 O2 149.7(3) 5_556 .
Ga2 O3 O2 67.6(3) 2_566 .
Ga3 O3 O2 163.3(4) 1_656 .
La O3 O2 61.5(2) 2_565 .
O2 O3 O2 52.7(3) 6 .
O3 O3 O2 101.0(4) 2 .
Ga3 O3 O2 59.3(2) 2_564 .
Ga2 O3 O2 77.0(2) . .
O3 O3 O2 163.5(2) 2_556 .
Ga1 O3 O2 149.6(3) 1_556 .
Nb O3 O2 149.6(3) 1_556 .
O2 O3 O2 70.8(3) 1_556 .
La O3 O2 109.9(3) 4 .
O1 O3 O2 47.6(2) 2_455 .
Ga3 O3 O2 67.9(3) 4_445 .
La O3 O2 101.6(3) 1_556 .
O2 O3 O2 125.0(4) 4_446 .
Ga3 O3 Ga2 31.6(3) 2_565 1_665
Nb O3 Ga2 98.2(4) . 1_665
Ga1 O3 Ga2 98.2(4) . 1_665
La O3 Ga2 126.1(4) . 1_665
Ga3 O3 Ga2 123.0(3) 4_446 1_665
O3 O3 Ga2 125.6(7) 6 1_665
O3 O3 Ga2 59.8(5) 4 1_665
O3 O3 Ga2 117.5(5) 3 1_665
O2 O3 Ga2 157.4(5) 5_445 1_665
O3 O3 Ga2 93.8(4) 6_556 1_665
O2 O3 Ga2 8.2(2) 2_565 1_665
O2 O3 Ga2 53.0(3) 3_566 1_665
O1 O3 Ga2 76.2(3) . 1_665
O3 O3 Ga2 73.8(3) 5 1_665
O2 O3 Ga2 82.3(3) 3_565 1_665
O3 O3 Ga2 48.59(19) 5_556 1_665
Ga2 O3 Ga2 69.20(19) 2_566 1_665
Ga3 O3 Ga2 74.17(19) 1_656 1_665
La O3 Ga2 46.84(15) 2_565 1_665
O2 O3 Ga2 129.1(3) 6 1_665
O3 O3 Ga2 107.45(12) 2 1_665
Ga3 O3 Ga2 86.8(3) 2_564 1_665
Ga2 O3 Ga2 140.3(3) . 1_665
O3 O3 Ga2 87.66(19) 2_556 1_665
Ga1 O3 Ga2 75.33(17) 1_556 1_665
Nb O3 Ga2 75.33(17) 1_556 1_665
O2 O3 Ga2 90.5(2) 1_556 1_665
La O3 Ga2 44.97(13) 4 1_665
O1 O3 Ga2 155.3(3) 2_455 1_665
Ga3 O3 Ga2 128.9(3) 4_445 1_665
La O3 Ga2 90.98(19) 1_556 1_665
O2 O3 Ga2 123.7(3) 4_446 1_665
O2 O3 Ga2 107.7(3) . 1_665
Ga3 O3 La 146.0(6) 2_565 4_445
Nb O3 La 74.6(3) . 4_445
Ga1 O3 La 74.6(3) . 4_445
La O3 La 62.1(3) . 4_445
Ga3 O3 La 52.1(2) 4_446 4_445
O3 O3 La 53.5(5) 6 4_445
O3 O3 La 111.2(5) 4 4_445
O3 O3 La 53.6(5) 3 4_445
O2 O3 La 24.3(2) 5_445 4_445
O3 O3 La 85.2(5) 6_556 4_445
O2 O3 La 169.2(5) 2_565 4_445
O2 O3 La 132.2(5) 3_566 4_445
O1 O3 La 112.7(3) . 4_445
O3 O3 La 102.0(3) 5 4_445
O2 O3 La 101.5(3) 3_565 4_445
O3 O3 La 126.2(3) 5_556 4_445
Ga2 O3 La 119.2(3) 2_566 4_445
Ga3 O3 La 97.2(2) 1_656 4_445
La O3 La 139.1(3) 2_565 4_445
O2 O3 La 59.5(2) 6 4_445
O3 O3 La 65.30(13) 2 4_445
Ga3 O3 La 92.8(2) 2_564 4_445
Ga2 O3 La 45.40(14) . 4_445
O3 O3 La 85.58(16) 2_556 4_445
Ga1 O3 La 101.0(3) 1_556 4_445
Nb O3 La 101.0(3) 1_556 4_445
O2 O3 La 97.0(3) 1_556 4_445
La O3 La 128.1(2) 4 4_445
O1 O3 La 32.45(11) 2_455 4_445
Ga3 O3 La 48.35(12) 4_445 4_445
La O3 La 92.6(3) 1_556 4_445
O2 O3 La 51.6(3) 4_446 4_445
O2 O3 La 79.7(3) . 4_445
Ga2 O3 La 170.9(2) 1_665 4_445
Ga3 O3 O2 149.5(5) 2_565 4_445
Nb O3 O2 45.9(3) . 4_445
Ga1 O3 O2 45.9(3) . 4_445
La O3 O2 72.0(3) . 4_445
Ga3 O3 O2 68.0(3) 4_446 4_445
O3 O3 O2 32.4(5) 6 4_445
O3 O3 O2 88.9(4) 4 4_445
O3 O3 O2 45.3(4) 3 4_445
O2 O3 O2 53.8(4) 5_445 4_445
O3 O3 O2 106.9(6) 6_556 4_445
O2 O3 O2 139.3(6) 2_565 4_445
O2 O3 O2 161.8(5) 3_566 4_445
O1 O3 O2 122.3(4) . 4_445
O3 O3 O2 72.4(3) 5 4_445
O2 O3 O2 86.4(3) 3_565 4_445
O3 O3 O2 127.8(3) 5_556 4_445
Ga2 O3 O2 143.1(4) 2_566 4_445
Ga3 O3 O2 86.8(3) 1_656 4_445
La O3 O2 124.5(3) 2_565 4_445
O2 O3 O2 85.1(3) 6 4_445
O3 O3 O2 36.7(3) 2 4_445
Ga3 O3 O2 68.4(2) 2_564 4_445
Ga2 O3 O2 75.3(3) . 4_445
O3 O3 O2 88.6(3) 2_556 4_445
Ga1 O3 O2 113.4(3) 1_556 4_445
Nb O3 O2 113.4(3) 1_556 4_445
O2 O3 O2 125.2(4) 1_556 4_445
La O3 O2 98.9(3) 4 4_445
O1 O3 O2 46.6(3) 2_455 4_445
Ga3 O3 O2 23.25(15) 4_445 4_445
La O3 O2 121.6(4) 1_556 4_445
O2 O3 O2 68.1(2) 4_446 4_445
O2 O3 O2 82.5(5) . 4_445
Ga2 O3 O2 143.9(3) 1_665 4_445
La O3 O2 29.99(19) 4_445 4_445
Ga3 O3 Ga2 118.1(5) 2_565 2_565
Nb O3 Ga2 91.5(4) . 2_565
Ga1 O3 Ga2 91.5(4) . 2_565
La O3 Ga2 41.4(2) . 2_565
Ga3 O3 Ga2 145.5(4) 4_446 2_565
O3 O3 Ga2 55.9(5) 6 2_565
O3 O3 Ga2 116.1(4) 4 2_565
O3 O3 Ga2 129.66(18) 3 2_565
O2 O3 Ga2 106.0(3) 5_445 2_565
O3 O3 Ga2 147.43(15) 6_556 2_565
O2 O3 Ga2 83.9(4) 2_565 2_565
O2 O3 Ga2 101.9(3) 3_566 2_565
O1 O3 Ga2 42.7(3) . 2_565
O3 O3 Ga2 66.3(3) 5 2_565
O2 O3 Ga2 16.1(2) 3_565 2_565
O3 O3 Ga2 139.5(3) 5_556 2_565
Ga2 O3 Ga2 73.87(19) 2_566 2_565
Ga3 O3 Ga2 144.5(4) 1_656 2_565
La O3 Ga2 44.75(13) 2_565 2_565
O2 O3 Ga2 74.8(2) 6 2_565
O3 O3 Ga2 92.1(4) 2 2_565
Ga3 O3 Ga2 41.07(12) 2_564 2_565
Ga2 O3 Ga2 99.3(2) . 2_565
O3 O3 Ga2 170.7(4) 2_556 2_565
Ga1 O3 Ga2 159.3(3) 1_556 2_565
Nb O3 Ga2 159.3(3) 1_556 2_565
O2 O3 Ga2 85.4(2) 1_556 2_565
La O3 Ga2 87.6(3) 4 2_565
O1 O3 Ga2 64.8(2) 2_455 2_565
Ga3 O3 Ga2 66.27(16) 4_445 2_565
La O3 Ga2 117.9(2) 1_556 2_565
O2 O3 Ga2 144.7(4) 4_446 2_565
O2 O3 Ga2 22.32(13) . 2_565
Ga2 O3 Ga2 91.3(2) 1_665 2_565
La O3 Ga2 94.37(18) 4_445 2_565
O2 O3 Ga2 86.8(3) 4_445 2_565
Ga3 O3 O2 81.9(3) 2_565 6_655
Nb O3 O2 42.2(3) . 6_655
Ga1 O3 O2 42.2(3) . 6_655
La O3 O2 139.9(4) . 6_655
Ga3 O3 O2 59.7(2) 4_446 6_655
O3 O3 O2 87.2(3) 6 6_655
O3 O3 O2 30.7(4) 4 6_655
O3 O3 O2 29.9(4) 3 6_655
O2 O3 O2 90.7(3) 5_445 6_655
O3 O3 O2 79.7(3) 6_556 6_655
O2 O3 O2 90.3(3) 2_565 6_655
O2 O3 O2 114.6(3) 3_566 6_655
O1 O3 O2 162.6(4) . 6_655
O3 O3 O2 68.1(3) 5 6_655
O2 O3 O2 118.7(4) 3_565 6_655
O3 O3 O2 62.2(3) 5_556 6_655
Ga2 O3 O2 146.5(3) 2_566 6_655
Ga3 O3 O2 19.77(18) 1_656 6_655
La O3 O2 121.2(3) 2_565 6_655
O2 O3 O2 137.0(4) 6 6_655
O3 O3 O2 44.1(3) 2 6_655
Ga3 O3 O2 91.7(2) 2_564 6_655
Ga2 O3 O2 110.9(3) . 6_655
O3 O3 O2 38.0(2) 2_556 6_655
Ga1 O3 O2 63.71(19) 1_556 6_655
Nb O3 O2 63.71(19) 1_556 6_655
O2 O3 O2 141.9(3) 1_556 6_655
La O3 O2 59.74(19) 4 6_655
O1 O3 O2 112.7(3) 2_455 6_655
Ga3 O3 O2 77.9(2) 4_445 6_655
La O3 O2 109.4(3) 1_556 6_655
O2 O3 O2 60.9(3) 4_446 6_655
O2 O3 O2 145.1(3) . 6_655
Ga2 O3 O2 87.9(2) 1_665 6_655
La O3 O2 83.1(2) 4_445 6_655
O2 O3 O2 67.9(4) 4_445 6_655
Ga2 O3 O2 132.7(3) 2_565 6_655
Ga3 O3 O1 93.9(5) 2_565 2_456
Nb O3 O1 129.2(5) . 2_456
Ga1 O3 O1 129.2(5) . 2_456
La O3 O1 75.9(3) . 2_456
Ga3 O3 O1 46.4(2) 4_446 2_456
O3 O3 O1 111.1(6) 6 2_456
O3 O3 O1 129.3(4) 4 2_456
O3 O3 O1 85.3(5) 3 2_456
O2 O3 O1 37.0(3) 5_445 2_456
O3 O3 O1 38.4(3) 6_556 2_456
O2 O3 O1 129.0(5) 2_565 2_456
O2 O3 O1 71.1(4) 3_566 2_456
O1 O3 O1 89.2(3) . 2_456
O3 O3 O1 163.1(3) 5 2_456
O2 O3 O1 130.6(3) 3_565 2_456
O3 O3 O1 88.5(5) 5_556 2_456
Ga2 O3 O1 70.3(2) 2_566 2_456
Ga3 O3 O1 100.4(3) 1_656 2_456
La O3 O1 128.7(2) 2_565 2_456
O2 O3 O1 39.8(2) 6 2_456
O3 O3 O1 121.0(2) 2 2_456
Ga3 O3 O1 145.9(3) 2_564 2_456
Ga2 O3 O1 20.74(15) . 2_456
O3 O3 O1 73.6(2) 2_556 2_456
Ga1 O3 O1 62.9(2) 1_556 2_456
Nb O3 O1 62.9(2) 1_556 2_456
O2 O3 O1 45.8(2) 1_556 2_456
La O3 O1 156.5(3) 4 2_456
O1 O3 O1 67.07(19) 2_455 2_456
Ga3 O3 O1 108.8(3) 4_445 2_456
La O3 O1 31.45(17) 1_556 2_456
O2 O3 O1 45.2(2) 4_446 2_456
O2 O3 O1 92.5(3) . 2_456
Ga2 O3 O1 122.4(3) 1_665 2_456
La O3 O1 61.3(2) 4_445 2_456
O2 O3 O1 90.8(3) 4_445 2_456
Ga2 O3 O1 114.5(2) 2_565 2_456
O2 O3 O1 105.4(3) 6_655 2_456
Ga3 O3 Ga3 98.9(4) 2_565 1_556
Nb O3 Ga3 149.2(4) . 1_556
Ga1 O3 Ga3 149.2(4) . 1_556
La O3 Ga3 46.8(2) . 1_556
Ga3 O3 Ga3 89.1(3) 4_446 1_556
O3 O3 Ga3 102.32(17) 6 1_556
O3 O3 Ga3 163.3(2) 4 1_556
O3 O3 Ga3 124.4(6) 3 1_556
O2 O3 Ga3 63.4(3) 5_445 1_556
O3 O3 Ga3 73.31(15) 6_556 1_556
O2 O3 Ga3 110.4(4) 2_565 1_556
O2 O3 Ga3 62.9(3) 3_566 1_556
O1 O3 Ga3 46.92(19) . 1_556
O3 O3 Ga3 141.0(4) 5 1_556
O2 O3 Ga3 90.3(2) 3_565 1_556
O3 O3 Ga3 109.4(5) 5_556 1_556
Ga2 O3 Ga3 40.08(12) 2_566 1_556
Ga3 O3 Ga3 140.5(3) 1_656 1_556
La O3 Ga3 88.57(18) 2_565 1_556
O2 O3 Ga3 20.03(19) 6 1_556
O3 O3 Ga3 141.1(2) 2 1_556
Ga3 O3 Ga3 114.6(2) 2_564 1_556
Ga2 O3 Ga3 40.17(10) . 1_556
O3 O3 Ga3 114.4(3) 2_556 1_556
Ga1 O3 Ga3 94.6(2) 1_556 1_556
Nb O3 Ga3 94.6(2) 1_556 1_556
O2 O3 Ga3 21.71(16) 1_556 1_556
La O3 Ga3 149.1(3) 4 1_556
O1 O3 Ga3 60.07(19) 2_455 1_556
Ga3 O3 Ga3 107.8(2) 4_445 1_556
La O3 Ga3 46.58(11) 1_556 1_556
O2 O3 Ga3 87.9(3) 4_446 1_556
O2 O3 Ga3 55.5(2) . 1_556
Ga2 O3 Ga3 109.23(19) 1_665 1_556
La O3 Ga3 79.17(19) 4_445 1_556
O2 O3 Ga3 105.0(3) 4_445 1_556
Ga2 O3 Ga3 74.63(14) 2_565 1_556
O2 O3 Ga3 148.6(4) 6_655 1_556
O1 O3 Ga3 43.22(11) 2_456 1_556
Ga3 O3 O1 71.8(4) 2_565 2_565
Nb O3 O1 73.8(4) . 2_565
Ga1 O3 O1 73.8(4) . 2_565
La O3 O1 102.2(4) . 2_565
Ga3 O3 O1 149.3(3) 4_446 2_565
O3 O3 O1 85.6(7) 6 2_565
O3 O3 O1 61.8(4) 4 2_565
O3 O3 O1 115.6(4) 3 2_565
O2 O3 O1 162.2(5) 5_445 2_565
O3 O3 O1 133.9(5) 6_556 2_565
O2 O3 O1 32.4(3) 2_565 2_565
O2 O3 O1 87.3(4) 3_566 2_565
O1 O3 O1 72.6(3) . 2_565
O3 O3 O1 39.53(19) 5 2_565
O2 O3 O1 47.0(3) 3_565 2_565
O3 O3 O1 84.7(4) 5_556 2_565
Ga2 O3 O1 87.0(3) 2_566 2_565
Ga3 O3 O1 89.3(2) 1_656 2_565
La O3 O1 30.79(11) 2_565 2_565
O2 O3 O1 130.9(3) 6 2_565
O3 O3 O1 82.1(2) 2 2_565
Ga3 O3 O1 46.5(2) 2_564 2_565
Ga2 O3 O1 157.8(3) . 2_565
O3 O3 O1 113.66(16) 2_556 2_565
Ga1 O3 O1 112.7(3) 1_556 2_565
Nb O3 O1 112.7(3) 1_556 2_565
O2 O3 O1 111.8(3) 1_556 2_565
La O3 O1 31.27(10) 4 2_565
O1 O3 O1 122.0(4) 2_455 2_565
Ga3 O3 O1 90.5(3) 4_445 2_565
La O3 O1 127.5(3) 1_556 2_565
O2 O3 O1 150.5(3) 4_446 2_565
O2 O3 O1 82.6(3) . 2_565
Ga2 O3 O1 40.40(19) 1_665 2_565
La O3 O1 138.8(3) 4_445 2_565
O2 O3 O1 110.9(3) 4_445 2_565
Ga2 O3 O1 60.9(2) 2_565 2_565
O2 O3 O1 90.9(2) 6_655 2_565
O1 O3 O1 156.8(3) 2_456 2_565
Ga3 O3 O1 119.4(2) 1_556 2_565
Ga3 O3 La 115.1(4) 2_565 2
Nb O3 La 35.0(3) . 2
Ga1 O3 La 35.0(3) . 2
La O3 La 106.2(3) . 2
Ga3 O3 La 52.94(17) 4_446 2
O3 O3 La 60.4(4) 6 2
O3 O3 La 60.3(4) 4 2
O3 O3 La 14.33(14) 3 2
O2 O3 La 65.6(3) 5_445 2
O3 O3 La 89.2(4) 6_556 2
O2 O3 La 120.4(5) 2_565 2
O2 O3 La 142.4(4) 3_566 2
O1 O3 La 156.3(4) . 2
O3 O3 La 71.01(17) 5 2
O2 O3 La 109.0(3) 3_565 2
O3 O3 La 93.62(18) 5_556 2
Ga2 O3 La 165.0(4) 2_566 2
Ga3 O3 La 52.38(12) 1_656 2
La O3 La 135.8(3) 2_565 2
O2 O3 La 109.9(3) 6 2
O3 O3 La 28.65(17) 2 2
Ga3 O3 La 83.03(18) 2_564 2
Ga2 O3 La 89.5(2) . 2
O3 O3 La 57.5(2) 2_556 2
Ga1 O3 La 84.95(19) 1_556 2
Nb O3 La 84.95(19) 1_556 2
O2 O3 La 140.5(4) 1_556 2
La O3 La 81.78(16) 4 2
O1 O3 La 78.68(18) 2_455 2
Ga3 O3 La 50.00(10) 4_445 2
La O3 La 116.0(3) 1_556 2
O2 O3 La 53.75(18) 4_446 2
O2 O3 La 116.4(3) . 2
Ga2 O3 La 120.0(2) 1_665 2
La O3 La 50.98(12) 4_445 2
O2 O3 La 34.5(2) 4_445 2
Ga2 O3 La 115.7(2) 2_565 2
O2 O3 La 34.1(2) 6_655 2
O1 O3 La 94.8(2) 2_456 2
Ga3 O3 La 128.6(3) 1_556 2
O1 O3 La 107.7(2) 2_565 2
Ga3 O3 Ga3 113.5(4) 2_565 1_655
Nb O3 Ga3 12.4(2) . 1_655
Ga1 O3 Ga3 12.4(2) . 1_655
La O3 Ga3 99.1(3) . 1_655
Ga3 O3 Ga3 99.4(3) 4_446 1_655
O3 O3 Ga3 43.54(18) 6 1_655
O3 O3 Ga3 51.01(14) 4 1_655
O3 O3 Ga3 59.07(16) 3 1_655
O2 O3 Ga3 103.1(3) 5_445 1_655
O3 O3 Ga3 131.6(3) 6_556 1_655
O2 O3 Ga3 89.1(5) 2_565 1_655
O2 O3 Ga3 146.7(4) 3_566 1_655
O1 O3 Ga3 120.4(4) . 1_655
O3 O3 Ga3 25.04(16) 5 1_655
O2 O3 Ga3 67.5(3) 3_565 1_655
O3 O3 Ga3 104.9(4) 5_556 1_655
Ga2 O3 Ga3 148.1(4) 2_566 1_655
Ga3 O3 Ga3 69.26(16) 1_656 1_655
La O3 Ga3 89.4(3) 2_565 1_655
O2 O3 Ga3 129.5(3) 6 1_655
O3 O3 Ga3 18.34(15) 2 1_655
Ga3 O3 Ga3 39.80(11) 2_564 1_655
Ga2 O3 Ga3 125.5(3) . 1_655
O3 O3 Ga3 90.9(3) 2_556 1_655
Ga1 O3 Ga3 116.2(2) 1_556 1_655
Nb O3 Ga3 116.2(2) 1_556 1_655
O2 O3 Ga3 164.8(3) 1_556 1_655
La O3 Ga3 49.16(12) 4 1_655
O1 O3 Ga3 88.4(2) 2_455 1_655
Ga3 O3 Ga3 39.39(10) 4_445 1_655
La O3 Ga3 161.4(3) 1_556 1_655
O2 O3 Ga3 100.2(2) 4_446 1_655
O2 O3 Ga3 94.0(3) . 1_655
Ga2 O3 Ga3 93.9(2) 1_665 1_655
La O3 Ga3 80.14(15) 4_445 1_655
O2 O3 Ga3 50.22(18) 4_445 1_655
Ga2 O3 Ga3 79.97(19) 2_565 1_655
O2 O3 Ga3 52.97(17) 6_655 1_655
O1 O3 Ga3 138.9(3) 2_456 1_655
Ga3 O3 Ga3 145.7(2) 1_556 1_655
O1 O3 Ga3 64.2(2) 2_565 1_655
La O3 Ga3 46.59(9) 2 1_655
Ga3 O3 O3 136.4(5) 2_565 1_554
Nb O3 O3 52.1(3) . 1_554
Ga1 O3 O3 52.1(3) . 1_554
La O3 O3 59.5(3) . 1_554
Ga3 O3 O3 121.3(2) 4_446 1_554
O3 O3 O3 21.8(6) 6 1_554
O3 O3 O3 90.001(1) 4 1_554
O3 O3 O3 90.001(1) 3 1_554
O2 O3 O3 97.3(3) 5_445 1_554
O3 O3 O3 159.8(5) 6_556 1_554
O2 O3 O3 97.2(4) 2_565 1_554
O2 O3 O3 140.5(4) 3_566 1_554
O1 O3 O3 83.5(3) . 1_554
O3 O3 O3 40.6(4) 5 1_554
O2 O3 O3 34.1(2) 3_565 1_554
O3 O3 O3 141.8(4) 5_556 1_554
Ga2 O3 O3 114.7(2) 2_566 1_554
Ga3 O3 O3 111.33(19) 1_656 1_554
La O3 O3 71.14(16) 2_565 1_554
O2 O3 O3 95.3(3) 6 1_554
O3 O3 O3 51.5(3) 2 1_554
Ga3 O3 O3 18.53(18) 2_564 1_554
Ga2 O3 O3 107.64(16) . 1_554
O3 O3 O3 130.9(3) 2_556 1_554
Ga1 O3 O3 157.98(13) 1_556 1_554
Nb O3 O3 157.98(13) 1_556 1_554
O2 O3 O3 122.7(2) 1_556 1_554
La O3 O3 73.50(15) 4 1_554
O1 O3 O3 61.3(3) 2_455 1_554
Ga3 O3 O3 30.10(18) 4_445 1_554
La O3 O3 151.90(13) 1_556 1_554
O2 O3 O3 121.4(2) 4_446 1_554
O2 O3 O3 51.9(2) . 1_554
Ga2 O3 O3 105.26(16) 1_665 1_554
La O3 O3 74.92(16) 4_445 1_554
O2 O3 O3 53.3(2) 4_445 1_554
Ga2 O3 O3 40.78(12) 2_565 1_554
O2 O3 O3 94.3(2) 6_655 1_554
O1 O3 O3 128.4(2) 2_456 1_554
Ga3 O3 O3 105.64(13) 1_556 1_554
O1 O3 O3 64.9(2) 2_565 1_554
La O3 O3 75.69(14) 2 1_554
Ga3 O3 O3 42.07(12) 1_655 1_554
Ga3 O3 O3 43.6(5) 2_565 1_556
Nb O3 O3 127.9(3) . 1_556
Ga1 O3 O3 127.9(3) . 1_556
La O3 O3 120.5(3) . 1_556
Ga3 O3 O3 58.7(2) 4_446 1_556
O3 O3 O3 158.2(6) 6 1_556
O3 O3 O3 90.000(1) 4 1_556
O3 O3 O3 90.000(1) 3 1_556
O2 O3 O3 82.7(3) 5_445 1_556
O3 O3 O3 20.2(5) 6_556 1_556
O2 O3 O3 82.8(4) 2_565 1_556
O2 O3 O3 39.5(4) 3_566 1_556
O1 O3 O3 96.5(3) . 1_556
O3 O3 O3 139.4(4) 5 1_556
O2 O3 O3 145.9(2) 3_565 1_556
O3 O3 O3 38.2(4) 5_556 1_556
Ga2 O3 O3 65.3(2) 2_566 1_556
Ga3 O3 O3 68.67(18) 1_656 1_556
La O3 O3 108.86(16) 2_565 1_556
O2 O3 O3 84.7(3) 6 1_556
O3 O3 O3 128.5(3) 2 1_556
Ga3 O3 O3 161.47(18) 2_564 1_556
Ga2 O3 O3 72.36(16) . 1_556
O3 O3 O3 49.1(3) 2_556 1_556
Ga1 O3 O3 22.02(13) 1_556 1_556
Nb O3 O3 22.02(13) 1_556 1_556
O2 O3 O3 57.3(2) 1_556 1_556
La O3 O3 106.50(15) 4 1_556
O1 O3 O3 118.7(3) 2_455 1_556
Ga3 O3 O3 149.90(18) 4_445 1_556
La O3 O3 28.10(13) 1_556 1_556
O2 O3 O3 58.6(2) 4_446 1_556
O2 O3 O3 128.1(2) . 1_556
Ga2 O3 O3 74.74(16) 1_665 1_556
La O3 O3 105.08(16) 4_445 1_556
O2 O3 O3 126.7(2) 4_445 1_556
Ga2 O3 O3 139.21(12) 2_565 1_556
O2 O3 O3 85.7(2) 6_655 1_556
O1 O3 O3 51.6(2) 2_456 1_556
Ga3 O3 O3 74.36(13) 1_556 1_556
O1 O3 O3 115.1(2) 2_565 1_556
La O3 O3 104.31(14) 2 1_556
Ga3 O3 O3 137.93(12) 1_655 1_556
O3 O3 O3 179.999(2) 1_554 1_556
Ga3 O3 O2 57.4(3) 2_565 4_456
Nb O3 O2 153.7(6) . 4_456
Ga1 O3 O2 153.7(6) . 4_456
La O3 O2 80.9(3) . 4_456
Ga3 O3 O2 115.9(4) 4_446 4_456
O3 O3 O2 130.9(5) 6 4_456
O3 O3 O2 118.1(6) 4 4_456
O3 O3 O2 153.5(2) 3 4_456
O2 O3 O2 109.9(4) 5_445 4_456
O3 O3 O2 78.8(4) 6_556 4_456
O2 O3 O2 61.2(3) 2_565 4_456
O2 O3 O2 26.24(19) 3_566 4_456
O1 O3 O2 34.5(3) . 4_456
O3 O3 O2 118.4(2) 5 4_456
O2 O3 O2 83.2(2) 3_565 4_456
O3 O3 O2 77.3(3) 5_556 4_456
Ga2 O3 O2 9.66(19) 2_566 4_456
Ga3 O3 O2 119.6(3) 1_656 4_456
La O3 O2 54.22(19) 2_565 4_456
O2 O3 O2 69.5(3) 6 4_456
O3 O3 O2 161.7(4) 2 4_456
Ga3 O3 O2 108.8(3) 2_564 4_456
Ga2 O3 O2 85.9(2) . 4_456
O3 O3 O2 111.0(4) 2_556 4_456
Ga1 O3 O2 83.3(2) 1_556 4_456
Nb O3 O2 83.3(2) 1_556 4_456
O2 O3 O2 33.04(18) 1_556 4_456
La O3 O2 102.0(3) 4 4_456
O1 O3 O2 105.8(3) 2_455 4_456
Ga3 O3 O2 141.1(3) 4_445 4_456
La O3 O2 52.86(15) 1_556 4_456
O2 O3 O2 115.2(3) 4_446 4_456
O2 O3 O2 73.48(14) . 4_456
Ga2 O3 O2 59.6(2) 1_665 4_456
La O3 O2 128.8(3) 4_445 4_456
O2 O3 O2 152.3(5) 4_445 4_456
Ga2 O3 O2 76.3(2) 2_565 4_456
O2 O3 O2 139.1(2) 6_655 4_456
O1 O3 O2 77.0(2) 2_456 4_456
Ga3 O3 O2 49.65(19) 1_556 4_456
O1 O3 O2 79.9(3) 2_565 4_456
La O3 O2 167.8(3) 2 4_456
Ga3 O3 O2 143.4(3) 1_655 4_456
O3 O3 O2 116.5(2) 1_554 4_456
O3 O3 O2 63.5(2) 1_556 4_456
Ga3 O3 O2 48.8(3) 2_565 1_656
Nb O3 O2 68.7(3) . 1_656
Ga1 O3 O2 68.7(3) . 1_656
La O3 O2 172.9(4) . 1_656
Ga3 O3 O2 70.4(2) 4_446 1_656
O3 O3 O2 117.1(2) 6 1_656
O3 O3 O2 27.04(18) 4 1_656
O3 O3 O2 59.2(3) 3 1_656
O2 O3 O2 109.9(5) 5_445 1_656
O3 O3 O2 67.5(2) 6_556 1_656
O2 O3 O2 64.8(5) 2_565 1_656
O2 O3 O2 82.9(3) 3_566 1_656
O1 O3 O2 134.7(4) . 1_656
O3 O3 O2 78.8(4) 5 1_656
O2 O3 O2 124.5(4) 3_565 1_656
O3 O3 O2 30.6(3) 5_556 1_656
Ga2 O3 O2 114.2(3) 2_566 1_656
Ga3 O3 O2 14.82(17) 1_656 1_656
La O3 O2 103.6(3) 2_565 1_656
O2 O3 O2 144.3(4) 6 1_656
O3 O3 O2 73.7(3) 2 1_656
Ga3 O3 O2 105.7(3) 2_564 1_656
Ga2 O3 O2 120.5(3) . 1_656
O3 O3 O2 33.51(19) 2_556 1_656
Ga1 O3 O2 44.03(17) 1_556 1_656
Nb O3 O2 44.03(17) 1_556 1_656
O2 O3 O2 118.8(4) 1_556 1_656
La O3 O2 52.72(16) 4 1_656
O1 O3 O2 143.8(3) 2_455 1_656
Ga3 O3 O2 109.1(3) 4_445 1_656
La O3 O2 91.3(2) 1_556 1_656
O2 O3 O2 71.5(2) 4_446 1_656
O2 O3 O2 162.5(4) . 1_656
Ga2 O3 O2 59.8(2) 1_665 1_656
La O3 O2 111.7(3) 4_445 1_656
O2 O3 O2 100.89(17) 4_445 1_656
Ga2 O3 O2 140.2(3) 2_565 1_656
O2 O3 O2 33.0(4) 6_655 1_656
O1 O3 O2 104.5(3) 2_456 1_656
Ga3 O3 O2 137.7(3) 1_556 1_656
O1 O3 O2 80.1(2) 2_565 1_656
La O3 O2 66.7(2) 2 1_656
Ga3 O3 O2 75.8(2) 1_655 1_656
O3 O3 O2 116.6(2) 1_554 1_656
O3 O3 O2 63.4(2) 1_556 1_656
O2 O3 O2 106.2(5) 4_456 1_656
Ga3 O3 La 26.3(2) 2_565 2_566
Nb O3 La 136.7(4) . 2_566
Ga1 O3 La 136.7(4) . 2_566
La O3 La 112.4(3) . 2_566
Ga3 O3 La 101.4(3) 4_446 2_566
O3 O3 La 158.1(7) 6 2_566
O3 O3 La 90.8(4) 4 2_566
O3 O3 La 126.40(18) 3 2_566
O2 O3 La 118.1(4) 5_445 2_566
O3 O3 La 62.5(4) 6_556 2_566
O2 O3 La 47.9(3) 2_565 2_566
O2 O3 La 11.5(3) 3_566 2_566
O1 O3 La 64.9(3) . 2_566
O3 O3 La 115.4(3) 5 2_566
O2 O3 La 104.2(3) 3_565 2_566
O3 O3 La 45.5(2) 5_556 2_566
Ga2 O3 La 39.61(11) 2_566 2_566
Ga3 O3 La 87.78(19) 1_656 2_566
La O3 La 66.20(16) 2_565 2_566
O2 O3 La 93.1(3) 6 2_566
O3 O3 La 145.0(2) 2 2_566
Ga3 O3 La 122.0(3) 2_564 2_566
Ga2 O3 La 98.4(2) . 2_566
O3 O3 La 82.4(3) 2_556 2_566
Ga1 O3 La 56.61(12) 1_556 2_566
Nb O3 La 56.61(12) 1_556 2_566
O2 O3 La 52.43(19) 1_556 2_566
La O3 La 86.1(2) 4 2_566
O1 O3 La 133.9(3) 2_455 2_566
Ga3 O3 La 167.4(3) 4_445 2_566
La O3 La 49.84(11) 1_556 2_566
O2 O3 La 101.2(3) 4_446 2_566
O2 O3 La 104.8(3) . 2_566
Ga2 O3 La 41.90(9) 1_665 2_566
La O3 La 142.4(3) 4_445 2_566
O2 O3 La 169.3(4) 4_445 2_566
Ga2 O3 La 102.9(2) 2_565 2_566
O2 O3 La 107.4(2) 6_655 2_566
O1 O3 La 81.2(2) 2_456 2_566
Ga3 O3 La 73.83(13) 1_556 2_566
O1 O3 La 78.2(2) 2_565 2_566
La O3 La 138.8(2) 2 2_566
Ga3 O3 La 135.3(3) 1_655 2_566
O3 O3 La 137.34(15) 1_554 2_566
O3 O3 La 42.66(15) 1_556 2_566
O2 O3 La 31.8(2) 4_456 2_566
O2 O3 La 74.6(3) 1_656 2_566
Ga3 O3 O2 128.9(6) 2_565 2_455
Nb O3 O2 106.7(4) . 2_455
Ga1 O3 O2 106.7(4) . 2_455
La O3 O2 51.3(3) . 2_455
Ga3 O3 O2 55.2(3) 4_446 2_455
O3 O3 O2 76.3(5) 6 2_455
O3 O3 O2 138.1(5) 4 2_455
O3 O3 O2 78.3(5) 3 2_455
O2 O3 O2 16.9(4) 5_445 2_455
O3 O3 O2 70.1(4) 6_556 2_455
O2 O3 O2 158.3(6) 2_565 2_455
O2 O3 O2 101.8(4) 3_566 2_455
O1 O3 O2 89.9(3) . 2_455
O3 O3 O2 130.2(4) 5 2_455
O2 O3 O2 106.3(3) 3_565 2_455
O3 O3 O2 120.9(5) 5_556 2_455
Ga2 O3 O2 87.9(3) 2_566 2_455
Ga3 O3 O2 114.5(3) 1_656 2_455
La O3 O2 129.5(3) 2_565 2_455
O2 O3 O2 30.1(2) 6 2_455
O3 O3 O2 97.4(2) 2 2_455
Ga3 O3 O2 112.0(2) 2_564 2_455
Ga2 O3 O2 14.92(17) . 2_455
O3 O3 O2 92.32(18) 2_556 2_455
Ga1 O3 O2 93.2(3) 1_556 2_455
Nb O3 O2 93.2(3) 1_556 2_455
O2 O3 O2 64.9(4) 1_556 2_455
La O3 O2 160.2(3) 4 2_455
O1 O3 O2 33.0(2) 2_455 2_455
Ga3 O3 O2 75.1(2) 4_445 2_455
La O3 O2 65.2(2) 1_556 2_455
O2 O3 O2 54.1(2) 4_446 2_455
O2 O3 O2 71.2(3) . 2_455
Ga2 O3 O2 154.7(3) 1_665 2_455
La O3 O2 32.10(19) 4_445 2_455
O2 O3 O2 61.4(2) 4_445 2_455
Ga2 O3 O2 92.5(2) 2_565 2_455
O2 O3 O2 107.5(4) 6_655 2_455
O1 O3 O2 35.0(2) 2_456 2_455
Ga3 O3 O2 48.3(2) 1_556 2_455
O1 O3 O2 153.3(3) 2_565 2_455
La O3 O2 80.4(2) 2 2_455
Ga3 O3 O2 111.4(2) 1_655 2_455
O3 O3 O2 93.82(18) 1_554 2_455
O3 O3 O2 86.18(18) 1_556 2_455
O2 O3 O2 97.2(4) 4_456 2_455
O2 O3 O2 125.6(3) 1_656 2_455
La O3 O2 113.0(3) 2_566 2_455
Ga3 O3 O2 99.7(5) 2_565 4_455
Nb O3 O2 106.0(5) . 4_455
Ga1 O3 O2 106.0(5) . 4_455
La O3 O2 50.9(3) . 4_455
Ga3 O3 O2 155.3(4) 4_446 4_455
O3 O3 O2 75.4(5) 6 4_455
O3 O3 O2 116.8(6) 4 4_455
O3 O3 O2 148.72(16) 3 4_455
O2 O3 O2 116.5(3) 5_445 4_455
O3 O3 O2 134.5(3) 6_556 4_455
O2 O3 O2 70.1(3) 2_565 4_455
O2 O3 O2 82.6(3) 3_566 4_455
O1 O3 O2 26.6(3) . 4_455
O3 O3 O2 74.8(2) 5 4_455
O2 O3 O2 26.51(18) 3_565 4_455
O3 O3 O2 122.1(2) 5_556 4_455
Ga2 O3 O2 56.8(2) 2_566 4_455
Ga3 O3 O2 144.6(4) 1_656 4_455
La O3 O2 30.3(2) 2_565 4_455
O2 O3 O2 75.7(3) 6 4_455
O3 O3 O2 108.6(4) 2 4_455
Ga3 O3 O2 54.06(19) 2_564 4_455
Ga2 O3 O2 102.6(2) . 4_455
O3 O3 O2 163.7(3) 2_556 4_455
Ga1 O3 O2 139.7(3) 1_556 4_455
Nb O3 O2 139.7(3) 1_556 4_455
O2 O3 O2 73.13(15) 1_556 4_455
La O3 O2 86.0(3) 4 4_455
O1 O3 O2 78.9(2) 2_455 4_455
Ga3 O3 O2 85.8(2) 4_445 4_455
La O3 O2 104.8(2) 1_556 4_455
O2 O3 O2 154.1(5) 4_446 4_455
O2 O3 O2 31.38(18) . 4_455
Ga2 O3 O2 76.4(3) 1_665 4_455
La O3 O2 110.6(3) 4_445 4_455
O2 O3 O2 106.4(3) 4_445 4_455
Ga2 O3 O2 19.65(13) 2_565 4_455
O2 O3 O2 142.4(3) 6_655 4_455
O1 O3 O2 111.8(2) 2_456 4_455
Ga3 O3 O2 68.67(18) 1_556 4_455
O1 O3 O2 55.3(3) 2_565 4_455
La O3 O2 134.4(3) 2 4_455
Ga3 O3 O2 93.8(2) 1_655 4_455
O3 O3 O2 58.76(15) 1_554 4_455
O3 O3 O2 121.24(15) 1_556 4_455
O2 O3 O2 57.71(17) 4_456 4_455
O2 O3 O2 133.6(4) 1_656 4_455
La O3 O2 83.3(2) 2_566 4_455
O2 O3 O2 100.5(3) 2_455 4_455
Ga3 O3 O1 13.1(3) 2_565 2_566
Nb O3 O1 109.2(4) . 2_566
Ga1 O3 O1 109.2(4) . 2_566
La O3 O1 132.6(3) . 2_566
Ga3 O3 O1 107.0(3) 4_446 2_566
O3 O3 O1 144.2(7) 6 2_566
O3 O3 O1 64.4(4) 4 2_566
O3 O3 O1 113.3(4) 3 2_566
O2 O3 O1 138.5(5) 5_445 2_566
O3 O3 O1 75.0(4) 6_556 2_566
O2 O3 O1 27.0(3) 2_565 2_566
O2 O3 O1 39.1(3) 3_566 2_566
O1 O3 O1 80.4(3) . 2_566
O3 O3 O1 91.0(4) 5 2_566
O2 O3 O1 99.4(4) 3_565 2_566
O3 O3 O1 33.76(15) 5_556 2_566
Ga2 O3 O1 63.60(17) 2_566 2_566
Ga3 O3 O1 69.14(17) 1_656 2_566
La O3 O1 61.5(2) 2_565 2_566
O2 O3 O1 120.6(3) 6 2_566
O3 O3 O1 117.81(17) 2 2_566
Ga3 O3 O1 105.8(3) 2_564 2_566
Ga2 O3 O1 123.9(3) . 2_566
O3 O3 O1 75.2(2) 2_556 2_566
Ga1 O3 O1 58.06(18) 1_556 2_566
Nb O3 O1 58.06(18) 1_556 2_566
O2 O3 O1 80.0(2) 1_556 2_566
La O3 O1 59.27(19) 4 2_566
O1 O3 O1 160.1(2) 2_455 2_566
Ga3 O3 O1 146.0(3) 4_445 2_566
La O3 O1 73.6(2) 1_556 2_566
O2 O3 O1 107.5(3) 4_446 2_566
O2 O3 O1 117.9(3) . 2_566
Ga2 O3 O1 18.94(14) 1_665 2_566
La O3 O1 159.1(3) 4_445 2_566
O2 O3 O1 153.3(3) 4_445 2_566
Ga2 O3 O1 105.9(3) 2_565 2_566
O2 O3 O1 86.7(2) 6_655 2_566
O1 O3 O1 104.5(4) 2_456 2_566
Ga3 O3 O1 101.05(19) 1_556 2_566
O1 O3 O1 59.34(14) 2_565 2_566
La O3 O1 120.81(19) 2 2_566
Ga3 O3 O1 107.9(3) 1_655 2_566
O3 O3 O1 124.2(2) 1_554 2_566
O3 O3 O1 55.8(2) 1_556 2_566
O2 O3 O1 54.3(2) 4_456 2_566
O2 O3 O1 54.4(2) 1_656 2_566
La O3 O1 27.68(10) 2_566 2_566
O2 O3 O1 138.8(3) 2_455 2_566
O2 O3 O1 88.5(3) 4_455 2_566
Ga3 O3 O2 93.4(4) 2_565 1_655
Nb O3 O2 21.5(3) . 1_655
Ga1 O3 O2 21.5(3) . 1_655
La O3 O2 117.7(4) . 1_655
Ga3 O3 O2 99.9(3) 4_446 1_655
O3 O3 O2 63.5(3) 6 1_655
O3 O3 O2 31.75(17) 4 1_655
O3 O3 O2 60.7(3) 3 1_655
O2 O3 O2 116.5(4) 5_445 1_655
O3 O3 O2 121.63(19) 6_556 1_655
O2 O3 O2 73.3(6) 2_565 1_655
O2 O3 O2 127.8(3) 3_566 1_655
O1 O3 O2 124.3(4) . 1_655
O3 O3 O2 25.0(3) 5 1_655
O2 O3 O2 75.8(3) 3_565 1_655
O3 O3 O2 85.6(4) 5_556 1_655
Ga2 O3 O2 141.9(4) 2_566 1_655
Ga3 O3 O2 54.69(18) 1_656 1_655
La O3 O2 85.2(3) 2_565 1_655
O2 O3 O2 149.7(3) 6 1_655
O3 O3 O2 30.8(2) 2 1_655
Ga3 O3 O2 50.14(17) 2_564 1_655
Ga2 O3 O2 140.5(3) . 1_655
O3 O3 O2 79.9(3) 2_556 1_655
Ga1 O3 O2 101.1(2) 1_556 1_655
Nb O3 O2 101.1(2) 1_556 1_655
O2 O3 O2 166.6(5) 1_556 1_655
La O3 O2 32.03(17) 4 1_655
O1 O3 O2 108.4(3) 2_455 1_655
Ga3 O3 O2 59.46(18) 4_445 1_655
La O3 O2 149.2(3) 1_556 1_655
O2 O3 O2 101.06(18) 4_446 1_655
O2 O3 O2 109.0(3) . 1_655
Ga2 O3 O2 76.7(2) 1_665 1_655
La O3 O2 96.1(2) 4_445 1_655
O2 O3 O2 67.28(19) 4_445 1_655
Ga2 O3 O2 90.9(2) 2_565 1_655
O2 O3 O2 43.1(3) 6_655 1_655
O1 O3 O2 146.0(3) 2_456 1_655
Ga3 O3 O2 164.2(3) 1_556 1_655
O1 O3 O2 55.5(2) 2_565 1_655
La O3 O2 52.29(17) 2 1_655
Ga3 O3 O2 20.15(13) 1_655 1_655
O3 O3 O2 58.60(16) 1_554 1_655
O3 O3 O2 121.40(16) 1_556 1_655
O2 O3 O2 133.6(4) 4_456 1_655
O2 O3 O2 58.02(19) 1_656 1_655
La O3 O2 116.4(3) 2_566 1_655
O2 O3 O2 128.2(2) 2_455 1_655
O2 O3 O2 99.6(4) 4_455 1_655
O1 O3 O2 88.7(3) 2_566 1_655
Ga3 O3 O1 124.0(5) 2_565 1_545
Nb O3 O1 61.0(4) . 1_545
Ga1 O3 O1 61.0(4) . 1_545
La O3 O1 90.2(3) . 1_545
Ga3 O3 O1 35.2(2) 4_446 1_545
O3 O3 O1 65.3(6) 6 1_545
O3 O3 O1 85.7(4) 4 1_545
O3 O3 O1 26.0(4) 3 1_545
O2 O3 O1 37.5(3) 5_445 1_545
O3 O3 O1 74.4(5) 6_556 1_545
O2 O3 O1 146.1(4) 2_565 1_545
O2 O3 O1 131.9(5) 3_566 1_545
O1 O3 O1 140.7(3) . 1_545
O3 O3 O1 96.04(19) 5 1_545
O2 O3 O1 119.2(3) 3_565 1_545
O3 O3 O1 101.57(18) 5_556 1_545
Ga2 O3 O1 137.9(4) 2_566 1_545
Ga3 O3 O1 68.95(19) 1_656 1_545
La O3 O1 157.1(3) 2_565 1_545
O2 O3 O1 83.1(3) 6 1_545
O3 O3 O1 52.82(19) 2 1_545
Ga3 O3 O1 99.9(2) 2_564 1_545
Ga2 O3 O1 61.30(18) . 1_545
O3 O3 O1 60.0(2) 2_556 1_545
Ga1 O3 O1 81.4(2) 1_556 1_545
Nb O3 O1 81.4(2) 1_556 1_545
O2 O3 O1 113.0(3) 1_556 1_545
La O3 O1 109.86(19) 4 1_545
O1 O3 O1 60.5(2) 2_455 1_545
Ga3 O3 O1 56.1(2) 4_445 1_545
La O3 O1 94.5(3) 1_556 1_545
O2 O3 O1 35.4(2) 4_446 1_545
O2 O3 O1 106.9(3) . 1_545
Ga2 O3 O1 143.0(2) 1_665 1_545
La O3 O1 28.24(10) 4_445 1_545
O2 O3 O1 32.9(2) 4_445 1_545
Ga2 O3 O1 117.6(2) 2_565 1_545
O2 O3 O1 55.9(2) 6_655 1_545
O1 O3 O1 68.3(2) 2_456 1_545
Ga3 O3 O1 100.8(2) 1_556 1_545
O1 O3 O1 134.8(2) 2_565 1_545
La O3 O1 28.16(10) 2 1_545
Ga3 O3 O1 71.01(17) 1_655 1_545
O3 O3 O1 86.17(19) 1_554 1_545
O3 O3 O1 93.83(19) 1_556 1_545
O2 O3 O1 145.3(3) 4_456 1_545
O2 O3 O1 83.5(2) 1_656 1_545
La O3 O1 136.4(3) 2_566 1_545
O2 O3 O1 53.0(2) 2_455 1_545
O2 O3 O1 136.2(3) 4_455 1_545
O1 O3 O1 135.0(2) 2_566 1_545
O2 O3 O1 80.1(2) 1_655 1_545
Ga3 O3 O2 43.4(4) 2_565 5
Nb O3 O2 79.0(4) . 5
Ga1 O3 O2 79.0(4) . 5
La O3 O2 133.0(5) . 5
Ga3 O3 O2 121.0(3) 4_446 5
O3 O3 O2 111.4(6) 6 5
O3 O3 O2 43.0(5) 4 5
O3 O3 O2 102.8(5) 3 5
O2 O3 O2 160.9(5) 5_445 5
O3 O3 O2 102.6(4) 6_556 5
O2 O3 O2 17.8(5) 2_565 5
O2 O3 O2 71.4(3) 3_566 5
O1 O3 O2 89.9(3) . 5
O3 O3 O2 57.4(3) 5 5
O2 O3 O2 79.6(3) 3_565 5
O3 O3 O2 52.2(3) 5_556 5
Ga2 O3 O2 87.9(3) 2_566 5
Ga3 O3 O2 63.5(2) 1_656 5
La O3 O2 52.6(2) 2_565 5
O2 O3 O2 147.4(3) 6 5
O3 O3 O2 88.25(15) 2 5
Ga3 O3 O2 75.5(3) 2_564 5
Ga2 O3 O2 157.5(3) . 5
O3 O3 O2 83.5(2) 2_556 5
Ga1 O3 O2 80.1(2) 1_556 5
Nb O3 O2 80.1(2) 1_556 5
O2 O3 O2 109.7(3) 1_556 5
La O3 O2 26.11(13) 4 5
O1 O3 O2 154.3(4) 2_455 5
Ga3 O3 O2 112.3(3) 4_445 5
La O3 O2 107.2(2) 1_556 5
O2 O3 O2 122.0(2) 4_446 5
O2 O3 O2 113.0(4) . 5
Ga2 O3 O2 19.21(13) 1_665 5
La O3 O2 152.9(2) 4_445 5
O2 O3 O2 124.8(3) 4_445 5
Ga2 O3 O2 92.5(3) 2_565 5
O2 O3 O2 73.1(3) 6_655 5
O1 O3 O2 137.3(3) 2_456 5
Ga3 O3 O2 127.9(2) 1_556 5
O1 O3 O2 32.7(2) 2_565 5
La O3 O2 102.6(2) 2 5
Ga3 O3 O2 75.3(2) 1_655 5
O3 O3 O2 93.82(19) 1_554 5
O3 O3 O2 86.18(19) 1_556 5
O2 O3 O2 78.4(3) 4_456 5
O2 O3 O2 51.03(14) 1_656 5
La O3 O2 60.06(17) 2_566 5
O2 O3 O2 172.3(4) 2_455 5
O2 O3 O2 82.6(4) 4_455 5
O1 O3 O2 33.69(18) 2_566 5
O2 O3 O2 57.5(2) 1_655 5
O1 O3 O2 128.7(2) 1_545 5
Ga3 O3 O3 63.7(5) 2_565 3_565
Nb O3 O3 122.1(6) . 3_565
Ga1 O3 O3 122.1(6) . 3_565
La O3 O3 80.98(18) . 3_565
Ga3 O3 O3 147.4(2) 4_446 3_565
O3 O3 O3 109.8(5) 6 3_565
O3 O3 O3 102.3(7) 4 3_565
O3 O3 O3 162.3(7) 3 3_565
O2 O3 O3 135.6(4) 5_445 3_565
O3 O3 O3 108.4(4) 6_556 3_565
O2 O3 O3 42.4(4) 2_565 3_565
O2 O3 O3 50.7(4) 3_566 3_565
O1 O3 O3 30.63(6) . 3_565
O3 O3 O3 86.19(17) 5 3_565
O2 O3 O3 56.1(2) 3_565 3_565
O3 O3 O3 86.38(18) 5_556 3_565
Ga2 O3 O3 38.08(12) 2_566 3_565
Ga3 O3 O3 119.9(4) 1_656 3_565
La O3 O3 21.81(16) 2_565 3_565
O2 O3 O3 89.3(2) 6 3_565
O3 O3 O3 129.4(3) 2 3_565
Ga3 O3 O3 78.2(2) 2_564 3_565
Ga2 O3 O3 112.6(2) . 3_565
O3 O3 O3 127.8(2) 2_556 3_565
Ga1 O3 O3 104.6(2) 1_556 3_565
Nb O3 O3 104.6(2) 1_556 3_565
O2 O3 O3 62.73(17) 1_556 3_565
La O3 O3 76.6(3) 4 3_565
O1 O3 O3 110.68(18) 2_455 3_565
Ga3 O3 O3 119.64(16) 4_445 3_565
La O3 O3 85.08(11) 1_556 3_565
O2 O3 O3 146.9(2) 4_446 3_565
O2 O3 O3 64.6(2) . 3_565
Ga2 O3 O3 45.8(3) 1_665 3_565
La O3 O3 142.9(3) 4_445 3_565
O2 O3 O3 142.0(2) 4_445 3_565
Ga2 O3 O3 55.55(9) 2_565 3_565
O2 O3 O3 132.6(4) 6_655 3_565
O1 O3 O3 108.39(17) 2_456 3_565
Ga3 O3 O3 72.47(12) 1_556 3_565
O1 O3 O3 49.2(2) 2_565 3_565
La O3 O3 156.8(3) 2 3_565
Ga3 O3 O3 111.0(3) 1_655 3_565
O3 O3 O3 90.0 1_554 3_565
O3 O3 O3 90.0 1_556 3_565
O2 O3 O3 32.44(15) 4_456 3_565
O2 O3 O3 105.4(4) 1_656 3_565
La O3 O3 48.33(17) 2_566 3_565
O2 O3 O3 119.4(3) 2_455 3_565
O2 O3 O3 36.28(17) 4_455 3_565
O1 O3 O3 53.3(3) 2_566 3_565
O2 O3 O3 104.7(4) 1_655 3_565
O1 O3 O3 171.1(3) 1_545 3_565
O2 O3 O3 59.5(3) 5 3_565
Ga3 O3 O3 103.6(3) 2_565 4_455
Nb O3 O3 140.4(3) . 4_455
Ga1 O3 O3 140.4(3) . 4_455
La O3 O3 35.7(3) . 4_455
Ga3 O3 O3 107.4(4) 4_446 4_455
O3 O3 O3 92.17(5) 6 4_455
O3 O3 O3 162.3(7) 4 4_455
O3 O3 O3 137.7(7) 3 4_455
O2 O3 O3 76.2(4) 5_445 4_455
O3 O3 O3 92.02(5) 6_556 4_455
O2 O3 O3 101.8(4) 2_565 4_455
O2 O3 O3 68.2(2) 3_566 4_455
O1 O3 O3 30.63(6) . 4_455
O3 O3 O3 121.8(2) 5 4_455
O2 O3 O3 70.9(2) 3_565 4_455
O3 O3 O3 120.1(3) 5_556 4_455
Ga2 O3 O3 38.08(12) 2_566 4_455
Ga3 O3 O3 158.5(2) 1_656 4_455
La O3 O3 72.21(14) 2_565 4_455
O2 O3 O3 29.7(2) 6 4_455
O3 O3 O3 135.6(3) 2 4_455
Ga3 O3 O3 96.24(13) 2_564 4_455
Ga2 O3 O3 55.7(2) . 4_455
O3 O3 O3 133.6(3) 2_556 4_455
Ga1 O3 O3 111.49(15) 1_556 4_455
Nb O3 O3 111.49(15) 1_556 4_455
O2 O3 O3 32.8(2) 1_556 4_455
La O3 O3 133.6(3) 4 4_455
O1 O3 O3 58.7(2) 2_455 4_455
Ga3 O3 O3 100.1(2) 4_445 4_455
La O3 O3 63.64(14) 1_556 4_455
O2 O3 O3 106.2(4) 4_446 4_455
O2 O3 O3 38.2(2) . 4_455
Ga2 O3 O3 103.3(2) 1_665 4_455
La O3 O3 85.8(3) 4_445 4_455
O2 O3 O3 105.2(4) 4_445 4_455
Ga2 O3 O3 55.55(9) 2_565 4_455
O2 O3 O3 166.6(4) 6_655 4_455
O1 O3 O3 62.4(2) 2_456 4_455
Ga3 O3 O3 19.49(13) 1_556 4_455
O1 O3 O3 102.4(2) 2_565 4_455
La O3 O3 136.5(4) 2 4_455
Ga3 O3 O3 132.02(12) 1_655 4_455
O3 O3 O3 90.0 1_554 4_455
O3 O3 O3 90.0 1_556 4_455
O2 O3 O3 47.1(2) 4_456 4_455
O2 O3 O3 150.7(2) 1_656 4_455
La O3 O3 77.36(13) 2_566 4_455
O2 O3 O3 59.5(3) 2_455 4_455
O2 O3 O3 49.46(16) 4_455 4_455
O1 O3 O3 101.34(19) 2_566 4_455
O2 O3 O3 146.4(2) 1_655 4_455
O1 O3 O3 111.9(3) 1_545 4_455
O2 O3 O3 119.4(3) 5 4_455
O3 O3 O3 60.0 3_565 4_455
Ga3 O3 Ga2 168.7(4) 2_565 1_554
Nb O3 Ga2 77.6(3) . 1_554
Ga1 O3 Ga2 77.6(3) . 1_554
La O3 Ga2 30.55(16) . 1_554
Ga3 O3 Ga2 92.5(3) 4_446 1_554
O3 O3 Ga2 31.1(2) 6 1_554
O3 O3 Ga2 124.5(2) 4 1_554
O3 O3 Ga2 85.8(4) 3 1_554
O2 O3 Ga2 56.6(3) 5_445 1_554
O3 O3 Ga2 119.4(5) 6_556 1_554
O2 O3 Ga2 136.2(4) 2_565 1_554
O2 O3 Ga2 133.6(3) 3_566 1_554
O1 O3 Ga2 81.0(3) . 1_554
O3 O3 Ga2 83.7(4) 5 1_554
O2 O3 Ga2 62.0(3) 3_565 1_554
O3 O3 Ga2 166.7(3) 5_556 1_554
Ga2 O3 Ga2 103.2(2) 2_566 1_554
Ga3 O3 Ga2 128.5(2) 1_656 1_554
La O3 Ga2 98.5(2) 2_565 1_554
O2 O3 Ga2 55.4(2) 6 1_554
O3 O3 Ga2 70.7(3) 2 1_554
Ga3 O3 Ga2 62.36(14) 2_564 1_554
Ga2 O3 Ga2 63.24(15) . 1_554
O3 O3 Ga2 125.4(2) 2_556 1_554
Ga1 O3 Ga2 140.3(3) 1_556 1_554
Nb O3 Ga2 140.3(3) 1_556 1_554
O2 O3 Ga2 93.6(2) 1_556 1_554
La O3 Ga2 117.3(2) 4 1_554
O1 O3 Ga2 16.92(19) 2_455 1_554
Ga3 O3 Ga2 35.85(8) 4_445 1_554
La O3 Ga2 111.0(2) 1_556 1_554
O2 O3 Ga2 91.9(3) 4_446 1_554
O2 O3 Ga2 42.0(2) . 1_554
Ga2 O3 Ga2 144.3(3) 1_665 1_554
La O3 Ga2 40.60(9) 4_445 1_554
O2 O3 Ga2 41.8(2) 4_445 1_554
Ga2 O3 Ga2 53.78(11) 2_565 1_554
O2 O3 Ga2 109.4(2) 6_655 1_554
O1 O3 Ga2 84.0(2) 2_456 1_554
Ga3 O3 Ga2 72.04(14) 1_556 1_554
O1 O3 Ga2 106.4(3) 2_565 1_554
La O3 Ga2 76.20(14) 2 1_554
Ga3 O3 Ga2 74.39(14) 1_655 1_554
O3 O3 Ga2 44.40(15) 1_554 1_554
O3 O3 Ga2 135.60(15) 1_556 1_554
O2 O3 Ga2 111.4(3) 4_456 1_554
O2 O3 Ga2 142.4(3) 1_656 1_554
La O3 Ga2 142.81(19) 2_566 1_554
O2 O3 Ga2 49.68(15) 2_455 1_554
O2 O3 Ga2 71.0(2) 4_455 1_554
O1 O3 Ga2 159.4(3) 2_566 1_554
O2 O3 Ga2 94.5(2) 1_655 1_554
O1 O3 Ga2 65.47(18) 1_545 1_554
O2 O3 Ga2 137.8(3) 5 1_554
O3 O3 Ga2 106.36(13) 3_565 1_554
O3 O3 Ga2 65.55(19) 4_455 1_554
Ga3 O3 O2 46.3(4) 2_565 6_665
Nb O3 O2 102.4(5) . 6_665
Ga1 O3 O2 102.4(5) . 6_665
La O3 O2 108.2(4) . 6_665
Ga3 O3 O2 140.2(3) 4_446 6_665
O3 O3 O2 115.4(7) 6 6_665
O3 O3 O2 72.9(5) 4 6_665
O3 O3 O2 132.7(5) 3 6_665
O2 O3 O2 161.8(4) 5_445 6_665
O3 O3 O2 106.4(5) 6_556 6_665
O2 O3 O2 12.9(4) 2_565 6_665
O2 O3 O2 55.3(4) 3_566 6_665
O1 O3 O2 60.2(3) . 6_665
O3 O3 O2 71.0(2) 5 6_665
O2 O3 O2 66.2(3) 3_565 6_665
O3 O3 O2 65.9(2) 5_556 6_665
Ga2 O3 O2 60.8(2) 2_566 6_665
Ga3 O3 O2 91.4(3) 1_656 6_665
La O3 O2 28.89(19) 2_565 6_665
O2 O3 O2 118.1(3) 6 6_665
O3 O3 O2 111.5(2) 2 6_665
Ga3 O3 O2 76.4(3) 2_564 6_665
Ga2 O3 O2 137.9(3) . 6_665
O3 O3 O2 105.8(2) 2_556 6_665
Ga1 O3 O2 91.3(2) 1_556 6_665
Nb O3 O2 91.3(2) 1_556 6_665
O2 O3 O2 85.0(3) 1_556 6_665
La O3 O2 50.24(18) 4 6_665
O1 O3 O2 137.1(3) 2_455 6_665
Ga3 O3 O2 121.8(3) 4_445 6_665
La O3 O2 95.5(2) 1_556 6_665
O2 O3 O2 140.7(3) 4_446 6_665
O2 O3 O2 89.5(3) . 6_665
Ga2 O3 O2 18.19(16) 1_665 6_665
La O3 O2 167.7(3) 4_445 6_665
O2 O3 O2 142.9(3) 4_445 6_665
Ga2 O3 O2 73.6(3) 2_565 6_665
O2 O3 O2 102.9(3) 6_655 6_665
O1 O3 O2 125.9(3) 2_456 6_665
Ga3 O3 O2 99.8(2) 1_556 6_665
O1 O3 O2 32.0(2) 2_565 6_665
La O3 O2 131.6(3) 2 6_665
Ga3 O3 O2 94.7(2) 1_655 6_665
O3 O3 O2 93.73(18) 1_554 6_665
O3 O3 O2 86.27(18) 1_556 6_665
O2 O3 O2 52.0(3) 4_456 6_665
O2 O3 O2 77.4(2) 1_656 6_665
La O3 O2 46.38(15) 2_566 6_665
O2 O3 O2 148.0(2) 2_455 6_665
O2 O3 O2 58.2(4) 4_455 6_665
O1 O3 O2 33.25(19) 2_566 6_665
O2 O3 O2 81.6(3) 1_655 6_665
O1 O3 O2 158.6(3) 1_545 6_665
O2 O3 O2 29.90(16) 5 6_665
O3 O3 O2 29.7(3) 3_565 6_665
O3 O3 O2 89.5(3) 4_455 6_665
Ga2 O3 O2 127.3(3) 1_554 6_665
Ga3 O3 O2 166.4(6) 2_565 5_444
Nb O3 O2 58.8(3) . 5_444
Ga1 O3 O2 58.8(3) . 5_444
La O3 O2 47.3(2) . 5_444
Ga3 O3 O2 95.2(4) 4_446 5_444
O3 O3 O2 12.2(3) 6 5_444
O3 O3 O2 105.4(2) 4 5_444
O3 O3 O2 76.1(4) 3 5_444
O2 O3 O2 66.9(3) 5_445 5_444
O3 O3 O2 130.1(6) 6_556 5_444
O2 O3 O2 127.7(5) 2_565 5_444
O2 O3 O2 150.9(4) 3_566 5_444
O1 O3 O2 92.4(3) . 5_444
O3 O3 O2 66.2(4) 5 5_444
O2 O3 O2 58.0(4) 3_565 5_444
O3 O3 O2 156.4(3) 5_556 5_444
Ga2 O3 O2 119.2(2) 2_566 5_444
Ga3 O3 O2 114.1(2) 1_656 5_444
La O3 O2 97.2(3) 2_565 5_444
O2 O3 O2 74.6(2) 6 5_444
O3 O3 O2 52.6(3) 2 5_444
Ga3 O3 O2 48.9(2) 2_564 5_444
Ga2 O3 O2 79.3(2) . 5_444
O3 O3 O2 119.7(3) 2_556 5_444
Ga1 O3 O2 143.6(4) 1_556 5_444
Nb O3 O2 143.6(4) 1_556 5_444
O2 O3 O2 112.7(2) 1_556 5_444
La O3 O2 99.6(3) 4 5_444
O1 O3 O2 34.4(2) 2_455 5_444
Ga3 O3 O2 17.14(12) 4_445 5_444
La O3 O2 129.0(3) 1_556 5_444
O2 O3 O2 95.0(4) 4_446 5_444
O2 O3 O2 52.63(16) . 5_444
Ga2 O3 O2 135.7(4) 1_665 5_444
La O3 O2 45.0(2) 4_445 5_444
O2 O3 O2 31.2(4) 4_445 5_444
Ga2 O3 O2 55.9(2) 2_565 5_444
O2 O3 O2 94.3(2) 6_655 5_444
O1 O3 O2 99.7(3) 2_456 5_444
Ga3 O3 O2 91.20(19) 1_556 5_444
O1 O3 O2 95.3(4) 2_565 5_444
La O3 O2 63.9(2) 2 5_444
Ga3 O3 O2 55.09(15) 1_655 5_444
O3 O3 O2 30.4(2) 1_554 5_444
O3 O3 O2 149.6(2) 1_556 5_444
O2 O3 O2 126.0(2) 4_456 5_444
O2 O3 O2 126.1(3) 1_656 5_444
La O3 O2 157.3(3) 2_566 5_444
O2 O3 O2 64.72(17) 2_455 5_444
O2 O3 O2 75.34(19) 4_455 5_444
O1 O3 O2 154.6(4) 2_566 5_444
O2 O3 O2 75.2(2) 1_655 5_444
O1 O3 O2 62.1(3) 1_545 5_444
O2 O3 O2 123.0(4) 5 5_444
O3 O3 O2 111.4(2) 3_565 5_444
O3 O3 O2 83.0(2) 4_455 5_444
Ga2 O3 O2 19.29(11) 1_554 5_444
O2 O3 O2 123.1(4) 6_665 5_444
Ga3 O3 O2 105.9(5) 2_565 2_564
Nb O3 O2 58.3(4) . 2_564
Ga1 O3 O2 58.3(4) . 2_564
La O3 O2 78.0(4) . 2_564
Ga3 O3 O2 144.6(3) 4_446 2_564
O3 O3 O2 51.9(6) 6 2_564
O3 O3 O2 75.4(3) 4 2_564
O3 O3 O2 105.0(3) 3 2_564
O2 O3 O2 128.0(4) 5_445 2_564
O3 O3 O2 167.1(5) 6_556 2_564
O2 O3 O2 66.5(3) 2_565 2_564
O2 O3 O2 116.3(6) 3_566 2_564
O1 O3 O2 75.2(4) . 2_564
O3 O3 O2 26.0(2) 5 2_564
O2 O3 O2 25.2(3) 3_565 2_564
O3 O3 O2 116.2(5) 5_556 2_564
Ga2 O3 O2 102.4(3) 2_566 2_564
Ga3 O3 O2 103.5(3) 1_656 2_564
La O3 O2 46.1(2) 2_565 2_564
O2 O3 O2 114.5(3) 6 2_564
O3 O3 O2 63.2(3) 2 2_564
Ga3 O3 O2 12.64(15) 2_564 2_564
Ga2 O3 O2 134.8(3) . 2_564
O3 O3 O2 130.1(3) 2_556 2_564
Ga1 O3 O2 143.0(3) 1_556 2_564
Nb O3 O2 143.0(3) 1_556 2_564
O2 O3 O2 122.1(3) 1_556 2_564
La O3 O2 49.47(19) 4 2_564
O1 O3 O2 89.8(3) 2_455 2_564
Ga3 O3 O2 58.2(2) 4_445 2_564
La O3 O2 152.1(3) 1_556 2_564
O2 O3 O2 145.3(3) 4_446 2_564
O2 O3 O2 62.1(3) . 2_564
Ga2 O3 O2 74.5(2) 1_665 2_564
La O3 O2 105.4(2) 4_445 2_564
O2 O3 O2 80.7(3) 4_445 2_564
Ga2 O3 O2 41.01(19) 2_565 2_564
O2 O3 O2 94.1(3) 6_655 2_564
O1 O3 O2 154.0(3) 2_456 2_564
Ga3 O3 O2 115.4(3) 1_556 2_564
O1 O3 O2 34.2(2) 2_565 2_564
La O3 O2 91.9(2) 2 2_564
Ga3 O3 O2 46.0(2) 1_655 2_564
O3 O3 O2 30.74(15) 1_554 2_564
O3 O3 O2 149.26(15) 1_556 2_564
O2 O3 O2 99.4(3) 4_456 2_564
O2 O3 O2 101.2(3) 1_656 2_564
La O3 O2 109.5(3) 2_566 2_564
O2 O3 O2 122.7(3) 2_455 2_564
O2 O3 O2 49.07(16) 4_455 2_564
O1 O3 O2 93.5(3) 2_566 2_564
O2 O3 O2 51.0(3) 1_655 2_564
O1 O3 O2 111.5(3) 1_545 2_564
O2 O3 O2 64.6(2) 5 2_564
O3 O3 O2 67.6(2) 3_565 2_564
O3 O3 O2 96.04(19) 4_455 2_564
Ga2 O3 O2 73.24(19) 1_554 2_564
O2 O3 O2 63.76(19) 6_665 2_564
O2 O3 O2 61.2(3) 5_444 2_564
Ga3 O3 Ga2 107.8(5) 2_565 2_556
Nb O3 Ga2 74.4(4) . 2_556
Ga1 O3 Ga2 74.4(4) . 2_556
La O3 Ga2 99.7(4) . 2_556
Ga3 O3 Ga2 16.28(13) 4_446 2_556
O3 O3 Ga2 84.1(6) 6 2_556
O3 O3 Ga2 85.9(4) 4 2_556
O3 O3 Ga2 29.6(4) 3 2_556
O2 O3 Ga2 36.0(3) 5_445 2_556
O3 O3 Ga2 55.6(4) 6_556 2_556
O2 O3 Ga2 139.7(4) 2_565 2_556
O2 O3 Ga2 113.3(5) 3_566 2_556
O1 O3 Ga2 141.7(4) . 2_556
O3 O3 Ga2 110.38(12) 5 2_556
O2 O3 Ga2 137.8(3) 3_565 2_556
O3 O3 Ga2 86.51(19) 5_556 2_556
Ga2 O3 Ga2 125.6(3) 2_566 2_556
Ga3 O3 Ga2 62.24(18) 1_656 2_556
La O3 Ga2 175.2(3) 2_565 2_556
O2 O3 Ga2 81.6(3) 6 2_556
O3 O3 Ga2 67.5(2) 2 2_556
Ga3 O3 Ga2 118.3(2) 2_564 2_556
Ga2 O3 Ga2 55.72(17) . 2_556
O3 O3 Ga2 45.86(12) 2_556 2_556
Ga1 O3 Ga2 63.58(18) 1_556 2_556
Nb O3 Ga2 63.58(18) 1_556 2_556
O2 O3 Ga2 101.7(3) 1_556 2_556
La O3 Ga2 114.90(19) 4 2_556
O1 O3 Ga2 71.3(2) 2_455 2_556
Ga3 O3 Ga2 74.98(17) 4_445 2_556
La O3 Ga2 77.9(2) 1_556 2_556
O2 O3 Ga2 16.57(15) 4_446 2_556
O2 O3 Ga2 118.8(3) . 2_556
Ga2 O3 Ga2 133.5(2) 1_665 2_556
La O3 Ga2 39.82(11) 4_445 2_556
O2 O3 Ga2 51.81(19) 4_445 2_556
Ga2 O3 Ga2 133.9(2) 2_565 2_556
O2 O3 Ga2 55.5(2) 6_655 2_556
O1 O3 Ga2 55.95(15) 2_456 2_556
Ga3 O3 Ga2 95.4(2) 1_556 2_556
O1 O3 Ga2 145.1(2) 2_565 2_556
La O3 Ga2 39.38(9) 2 2_556
Ga3 O3 Ga2 85.76(15) 1_655 2_556
O3 O3 Ga2 105.07(12) 1_554 2_556
O3 O3 Ga2 74.93(12) 1_556 2_556
O2 O3 Ga2 130.6(3) 4_456 2_556
O2 O3 Ga2 75.2(2) 1_656 2_556
La O3 Ga2 117.5(2) 2_566 2_556
O2 O3 Ga2 52.87(19) 2_455 2_556
O2 O3 Ga2 150.1(3) 4_455 2_556
O1 O3 Ga2 120.1(2) 2_566 2_556
O2 O3 Ga2 90.2(2) 1_655 2_556
O1 O3 Ga2 18.90(17) 1_545 2_556
O2 O3 Ga2 125.7(2) 5 2_556
O3 O3 Ga2 163.0(2) 3_565 2_556
O3 O3 Ga2 111.2(3) 4_455 2_556
Ga2 O3 Ga2 80.22(17) 1_554 2_556
O2 O3 Ga2 151.6(3) 6_665 2_556
O2 O3 Ga2 80.1(3) 5_444 2_556
O2 O3 Ga2 129.3(2) 2_564 2_556
Ga3 O3 La 97.8(4) 2_565 4_455
Nb O3 La 128.7(5) . 4_455
Ga1 O3 La 128.7(5) . 4_455
La O3 La 42.12(19) . 4_455
Ga3 O3 La 132.4(4) 4_446 4_455
O3 O3 La 88.1(3) 6 4_455
O3 O3 La 138.8(6) 4 4_455
O3 O3 La 156.1(5) 3 4_455
O2 O3 La 99.3(3) 5_445 4_455
O3 O3 La 111.2(2) 6_556 4_455
O2 O3 La 82.0(4) 2_565 4_455
O2 O3 La 69.2(3) 3_566 4_455
O1 O3 La 10.08(19) . 4_455
O3 O3 La 100.0(2) 5 4_455
O2 O3 La 50.1(2) 3_565 4_455
O3 O3 La 119.58(18) 5_556 4_455
Ga2 O3 La 38.07(11) 2_566 4_455
Ga3 O3 La 159.5(3) 1_656 4_455
La O3 La 47.75(11) 2_565 4_455
O2 O3 La 53.8(2) 6 4_455
O3 O3 La 128.9(4) 2 4_455
Ga3 O3 La 77.51(19) 2_564 4_455
Ga2 O3 La 80.46(16) . 4_455
O3 O3 La 151.6(4) 2_556 4_455
Ga1 O3 La 124.2(2) 1_556 4_455
Nb O3 La 124.2(2) 1_556 4_455
O2 O3 La 48.74(18) 1_556 4_455
La O3 La 108.7(3) 4 4_455
O1 O3 La 71.47(14) 2_455 4_455
Ga3 O3 La 98.12(19) 4_445 4_455
La O3 La 81.19(14) 1_556 4_455
O2 O3 La 131.2(3) 4_446 4_455
O2 O3 La 30.5(2) . 4_455
Ga2 O3 La 85.69(18) 1_665 4_455
La O3 La 103.11(18) 4_445 4_455
O2 O3 La 112.5(3) 4_445 4_455
Ga2 O3 La 37.26(8) 2_565 4_455
O2 O3 La 167.7(3) 6_655 4_455
O1 O3 La 86.82(16) 2_456 4_455
Ga3 O3 La 43.61(8) 1_556 4_455
O1 O3 La 77.48(18) 2_565 4_455
La O3 La 146.8(2) 2 4_455
Ga3 O3 La 117.1(2) 1_655 4_455
O3 O3 La 77.43(12) 1_554 4_455
O3 O3 La 102.57(12) 1_556 4_455
O2 O3 La 43.06(19) 4_456 4_455
O2 O3 La 144.7(3) 1_656 4_455
La O3 La 74.27(13) 2_566 4_455
O2 O3 La 82.4(2) 2_455 4_455
O2 O3 La 25.38(14) 4_455 4_455
O1 O3 La 90.51(17) 2_566 4_455
O2 O3 La 124.9(3) 1_655 4_455
O1 O3 La 131.3(2) 1_545 4_455
O2 O3 La 98.2(3) 5 4_455
O3 O3 La 39.88(11) 3_565 4_455
O3 O3 La 25.05(9) 4_455 4_455
Ga2 O3 La 70.99(12) 1_554 4_455
O2 O3 La 69.1(2) 6_665 4_455
O2 O3 La 83.14(18) 5_444 4_455
O2 O3 La 74.1(2) 2_564 4_455
Ga2 O3 La 135.2(2) 2_556 4_455
Ga3 O3 La 18.6(2) 2_565 4_556
Nb O3 La 95.9(3) . 4_556
Ga1 O3 La 95.9(3) . 4_556
La O3 La 156.8(3) . 4_556
Ga3 O3 La 83.8(2) 4_446 4_556
O3 O3 La 143.5(2) 6 4_556
O3 O3 La 49.2(3) 4 4_556
O3 O3 La 87.3(3) 3 4_556
O2 O3 La 121.6(4) 5_445 4_556
O3 O3 La 60.8(3) 6_556 4_556
O2 O3 La 46.8(3) 2_565 4_556
O2 O3 La 53.4(2) 3_566 4_556
O1 O3 La 106.1(3) . 4_556
O3 O3 La 92.9(4) 5 4_556
O2 O3 La 120.6(4) 3_565 4_556
O3 O3 La 10.1(2) 5_556 4_556
Ga2 O3 La 84.07(19) 2_566 4_556
Ga3 O3 La 44.18(11) 1_656 4_556
La O3 La 85.9(2) 2_565 4_556
O2 O3 La 129.6(3) 6 4_556
O3 O3 La 102.4(3) 2 4_556
Ga3 O3 La 116.2(3) 2_564 4_556
Ga2 O3 La 118.4(3) . 4_556
O3 O3 La 49.19(19) 2_556 4_556
Ga1 O3 La 38.11(9) 1_556 4_556
Nb O3 La 38.11(9) 1_556 4_556
O2 O3 La 92.7(2) 1_556 4_556
La O3 La 59.76(13) 4 4_556
O1 O3 La 163.5(4) 2_455 4_556
Ga3 O3 La 137.6(2) 4_445 4_556
La O3 La 73.00(15) 1_556 4_556
O2 O3 La 84.5(3) 4_446 4_556
O2 O3 La 144.4(3) . 4_556
Ga2 O3 La 39.23(9) 1_665 4_556
La O3 La 134.7(3) 4_445 4_556
O2 O3 La 131.0(3) 4_445 4_556
Ga2 O3 La 130.5(3) 2_565 4_556
O2 O3 La 63.3(2) 6_655 4_556
O1 O3 La 97.9(3) 2_456 4_556
Ga3 O3 La 114.11(19) 1_556 4_556
O1 O3 La 74.5(2) 2_565 4_556
La O3 La 96.55(16) 2 4_556
Ga3 O3 La 99.92(18) 1_655 4_556
O3 O3 La 133.26(14) 1_554 4_556
O3 O3 La 46.74(14) 1_556 4_556
O2 O3 La 75.9(3) 4_456 4_556
O2 O3 La 30.3(2) 1_656 4_556
La O3 La 44.46(8) 2_566 4_556
O2 O3 La 130.9(3) 2_455 4_556
O2 O3 La 114.5(3) 4_455 4_556
O1 O3 La 26.54(9) 2_566 4_556
O2 O3 La 80.0(2) 1_655 4_556
O1 O3 La 108.6(2) 1_545 4_556
O2 O3 La 42.09(16) 5 4_556
O3 O3 La 79.9(3) 3_565 4_556
O3 O3 La 121.60(16) 4_455 4_556
Ga2 O3 La 172.67(19) 1_554 4_556
O2 O3 La 57.02(18) 6_665 4_556
O2 O3 La 154.6(2) 5_444 4_556
O2 O3 La 106.3(2) 2_564 4_556
Ga2 O3 La 94.90(17) 2_556 4_556
La O3 La 116.12(19) 4_455 4_556
Ga3 O3 O1 48.0(3) 2_565 1_556
Nb O3 O1 158.1(4) . 1_556
Ga1 O3 O1 158.1(4) . 1_556
La O3 O1 96.5(3) . 1_556
Ga3 O3 O1 86.1(3) 4_446 1_556
O3 O3 O1 153.33(12) 6 1_556
O3 O3 O1 111.9(3) 4 1_556
O3 O3 O1 122.75(19) 3 1_556
O2 O3 O1 92.6(4) 5_445 1_556
O3 O3 O1 48.0(3) 6_556 1_556
O2 O3 O1 74.0(4) 2_565 1_556
O2 O3 O1 15.5(3) 3_566 1_556
O1 O3 O1 62.9(2) . 1_556
O3 O3 O1 141.2(3) 5 1_556
O2 O3 O1 114.0(3) 3_565 1_556
O3 O3 O1 59.1(3) 5_556 1_556
Ga2 O3 O1 31.73(16) 2_566 1_556
Ga3 O3 O1 98.9(2) 1_656 1_556
La O3 O1 82.81(19) 2_565 1_556
O2 O3 O1 69.0(3) 6 1_556
O3 O3 O1 161.7(4) 2 1_556
Ga3 O3 O1 139.4(3) 2_564 1_556
Ga2 O3 O1 71.94(17) . 1_556
O3 O3 O1 82.6(3) 2_556 1_556
Ga1 O3 O1 54.95(14) 1_556 1_556
Nb O3 O1 54.95(14) 1_556 1_556
O2 O3 O1 30.09(18) 1_556 1_556
La O3 O1 112.5(2) 4 1_556
O1 O3 O1 110.3(3) 2_455 1_556
Ga3 O3 O1 159.2(3) 4_445 1_556
La O3 O1 25.32(7) 1_556 1_556
O2 O3 O1 85.6(2) 4_446 1_556
O2 O3 O1 97.2(3) . 1_556
Ga2 O3 O1 68.37(13) 1_665 1_556
La O3 O1 116.6(3) 4_445 1_556
O2 O3 O1 146.4(4) 4_445 1_556
Ga2 O3 O1 105.60(19) 2_565 1_556
O2 O3 O1 117.7(3) 6_655 1_556
O1 O3 O1 55.63(15) 2_456 1_556
Ga3 O3 O1 51.53(12) 1_556 1_556
O1 O3 O1 102.3(3) 2_565 1_556
La O3 O1 137.0(3) 2 1_556
Ga3 O3 O1 161.2(3) 1_655 1_556
O3 O3 O1 146.38(14) 1_554 1_556
O3 O3 O1 33.62(14) 1_556 1_556
O2 O3 O1 30.86(17) 4_456 1_556
O2 O3 O1 89.4(3) 1_656 1_556
La O3 O1 26.51(5) 2_566 1_556
O2 O3 O1 86.5(3) 2_455 1_556
O2 O3 O1 88.1(2) 4_455 1_556
O1 O3 O1 53.41(14) 2_566 1_556
O2 O3 O1 141.3(3) 1_655 1_556
O1 O3 O1 119.4(3) 1_545 1_556
O2 O3 O1 86.50(19) 5 1_556
O3 O3 O1 61.35(11) 3_565 1_556
O3 O3 O1 61.35(11) 4_455 1_556
Ga2 O3 O1 123.6(2) 1_554 1_556
O2 O3 O1 70.43(17) 6_665 1_556
O2 O3 O1 142.7(2) 5_444 1_556
O2 O3 O1 128.9(3) 2_564 1_556
Ga2 O3 O1 101.8(2) 2_556 1_556
La O3 O1 69.29(14) 4_455 1_556
La O3 O1 62.65(12) 4_556 1_556
Ga3 O3 O3 116.2(6) 2_565 4_554
Nb O3 O3 30.3(3) . 4_554
Ga1 O3 O3 30.3(3) . 4_554
La O3 O3 87.5(3) . 4_554
Ga3 O3 O3 116.0(3) 4_446 4_554
O3 O3 O3 38.4(4) 6 4_554
O3 O3 O3 61.95(14) 4 4_554
O3 O3 O3 76.40(6) 3 4_554
O2 O3 O3 110.9(3) 5_445 4_554
O3 O3 O3 149.5(4) 6_556 4_554
O2 O3 O3 83.2(5) 2_565 4_554
O2 O3 O3 140.6(6) 3_566 4_554
O1 O3 O3 102.4(4) . 4_554
O3 O3 O3 16.1(2) 5 4_554
O2 O3 O3 49.5(3) 3_565 4_554
O3 O3 O3 114.6(5) 5_556 4_554
Ga2 O3 O3 131.0(4) 2_566 4_554
Ga3 O3 O3 84.8(2) 1_656 4_554
La O3 O3 73.9(3) 2_565 4_554
O2 O3 O3 122.7(3) 6 4_554
O3 O3 O3 34.6(3) 2 4_554
Ga3 O3 O3 21.84(13) 2_564 4_554
Ga2 O3 O3 129.0(3) . 4_554
O3 O3 O3 108.2(4) 2_556 4_554
Ga1 O3 O3 131.7(3) 1_556 4_554
Nb O3 O3 131.7(3) 1_556 4_554
O2 O3 O3 147.9(4) 1_556 4_554
La O3 O3 49.1(2) 4 4_554
O1 O3 O3 84.8(2) 2_455 4_554
Ga3 O3 O3 39.20(8) 4_445 4_554
La O3 O3 179.1(4) 1_556 4_554
O2 O3 O3 116.8(3) 4_446 4_554
O2 O3 O3 78.6(3) . 4_554
Ga2 O3 O3 89.7(3) 1_665 4_554
La O3 O3 86.60(17) 4_445 4_554
O2 O3 O3 57.59(17) 4_445 4_554
Ga2 O3 O3 62.5(2) 2_565 4_554
O2 O3 O3 70.2(2) 6_655 4_554
O1 O3 O3 147.8(3) 2_456 4_554
Ga3 O3 O3 133.5(2) 1_556 4_554
O1 O3 O3 53.3(3) 2_565 4_554
La O3 O3 63.17(16) 2 4_554
Ga3 O3 O3 18.01(12) 1_655 4_554
O3 O3 O3 28.05(14) 1_554 4_554
O3 O3 O3 151.95(14) 1_556 4_554
O2 O3 O3 128.0(4) 4_456 4_554
O2 O3 O3 88.7(3) 1_656 4_554
La O3 O3 130.9(4) 2_566 4_554
O2 O3 O3 114.1(2) 2_455 4_554
O2 O3 O3 75.8(3) 4_455 4_554
O1 O3 O3 107.0(4) 2_566 4_554
O2 O3 O3 30.72(17) 1_655 4_554
O1 O3 O3 84.6(2) 1_545 4_554
O2 O3 O3 73.4(3) 5 4_554
O3 O3 O3 95.7(3) 3_565 4_554
O3 O3 O3 116.61(17) 4_455 4_554
Ga2 O3 O3 68.62(11) 1_554 4_554
O2 O3 O3 85.4(3) 6_665 4_554
O2 O3 O3 50.51(16) 5_444 4_554
O2 O3 O3 28.7(3) 2_564 4_554
Ga2 O3 O3 101.3(2) 2_556 4_554
La O3 O3 99.3(3) 4_455 4_554
La O3 O3 107.3(3) 4_556 4_554
O1 O3 O3 155.5(4) 1_556 4_554
Ga3 O3 O3 139.7(6) 2_565 3_554
Nb O3 O3 30.3(3) . 3_554
Ga1 O3 O3 30.3(3) . 3_554
La O3 O3 75.1(3) . 3_554
Ga3 O3 O3 95.8(3) 4_446 3_554
O3 O3 O3 18.3(2) 6 3_554
O3 O3 O3 76.40(6) 4 3_554
O3 O3 O3 61.95(14) 3 3_554
O2 O3 O3 83.7(4) 5_445 3_554
O3 O3 O3 135.0(5) 6_556 3_554
O2 O3 O3 110.3(5) 2_565 3_554
O2 O3 O3 166.8(5) 3_566 3_554
O1 O3 O3 110.9(4) . 3_554
O3 O3 O3 42.9(3) 5 3_554
O2 O3 O3 61.8(2) 3_565 3_554
O3 O3 O3 129.3(5) 5_556 3_554
Ga2 O3 O3 141.8(3) 2_566 3_554
Ga3 O3 O3 89.1(3) 1_656 3_554
La O3 O3 96.0(2) 2_565 3_554
O2 O3 O3 103.3(3) 6 3_554
O3 O3 O3 26.0(4) 2 3_554
Ga3 O3 O3 38.73(7) 2_564 3_554
Ga2 O3 O3 102.7(3) . 3_554
O3 O3 O3 103.9(4) 2_556 3_554
Ga1 O3 O3 131.7(3) 1_556 3_554
Nb O3 O3 131.7(3) 1_556 3_554
O2 O3 O3 141.6(4) 1_556 3_554
La O3 O3 73.7(2) 4 3_554
O1 O3 O3 62.2(3) 2_455 3_554
Ga3 O3 O3 13.29(12) 4_445 3_554
La O3 O3 152.0(4) 1_556 3_554
O2 O3 O3 96.2(3) 4_446 3_554
O2 O3 O3 75.1(3) . 3_554
Ga2 O3 O3 116.7(3) 1_665 3_554
La O3 O3 59.4(2) 4_445 3_554
O2 O3 O3 30.90(18) 4_445 3_554
Ga2 O3 O3 68.40(12) 2_565 3_554
O2 O3 O3 70.0(3) 6_655 3_554
O1 O3 O3 120.6(3) 2_456 3_554
Ga3 O3 O3 120.2(3) 1_556 3_554
O1 O3 O3 80.1(3) 2_565 3_554
La O3 O3 47.65(18) 2 3_554
Ga3 O3 O3 26.25(15) 1_655 3_554
O3 O3 O3 28.05(14) 1_554 3_554
O3 O3 O3 151.95(14) 1_556 3_554
O2 O3 O3 144.5(3) 4_456 3_554
O2 O3 O3 98.9(3) 1_656 3_554
La O3 O3 158.1(4) 2_566 3_554
O2 O3 O3 87.9(3) 2_455 3_554
O2 O3 O3 86.80(17) 4_455 3_554
O1 O3 O3 133.0(4) 2_566 3_554
O2 O3 O3 46.4(2) 1_655 3_554
O1 O3 O3 61.2(2) 1_545 3_554
O2 O3 O3 99.4(3) 5 3_554
O3 O3 O3 116.61(17) 3_565 3_554
O3 O3 O3 110.4(3) 4_455 3_554
Ga2 O3 O3 48.31(18) 1_554 3_554
O2 O3 O3 112.1(3) 6_665 3_554
O2 O3 O3 29.05(17) 5_444 3_554
O2 O3 O3 50.44(19) 2_564 3_554
Ga2 O3 O3 79.7(2) 2_556 3_554
La O3 O3 103.76(18) 4_455 3_554
La O3 O3 125.6(3) 4_556 3_554
O1 O3 O3 171.6(3) 1_556 3_554
O3 O3 O3 27.19(13) 4_554 3_554
Ga3 O3 O3 33.1(3) 2_565 4_556
Nb O3 O3 102.8(4) . 4_556
Ga1 O3 O3 102.8(4) . 4_556
La O3 O3 148.5(4) . 4_556
Ga3 O3 O3 61.5(2) 4_446 4_556
O3 O3 O3 148.8(5) 6 4_556
O3 O3 O3 61.95(14) 4 4_556
O3 O3 O3 76.40(6) 3 4_556
O2 O3 O3 97.6(4) 5_445 4_556
O3 O3 O3 37.3(3) 6_556 4_556
O2 O3 O3 70.0(3) 2_565 4_556
O2 O3 O3 53.9(3) 3_566 4_556
O1 O3 O3 114.5(4) . 4_556
O3 O3 O3 112.3(5) 5 4_556
O2 O3 O3 144.3(4) 3_565 4_556
O3 O3 O3 14.1(2) 5_556 4_556
Ga2 O3 O3 85.4(2) 2_566 4_556
Ga3 O3 O3 42.9(2) 1_656 4_556
La O3 O3 107.1(3) 2_565 4_556
O2 O3 O3 112.1(3) 6 4_556
O3 O3 O3 106.0(5) 2 4_556
Ga3 O3 O3 138.2(3) 2_564 4_556
Ga2 O3 O3 95.4(2) . 4_556
O3 O3 O3 32.6(3) 2_556 4_556
Ga1 O3 O3 13.87(7) 1_556 4_556
Nb O3 O3 13.87(7) 1_556 4_556
O2 O3 O3 83.8(2) 1_556 4_556
La O3 O3 81.2(2) 4 4_556
O1 O3 O3 139.2(4) 2_455 4_556
Ga3 O3 O3 138.8(3) 4_445 4_556
La O3 O3 56.14(10) 1_556 4_556
O2 O3 O3 62.0(3) 4_446 4_556
O2 O3 O3 152.9(4) . 4_556
Ga2 O3 O3 62.0(2) 1_665 4_556
La O3 O3 113.6(3) 4_445 4_556
O2 O3 O3 121.2(4) 4_445 4_556
Ga2 O3 O3 151.0(4) 2_565 4_556
O2 O3 O3 62.0(3) 6_655 4_556
O1 O3 O3 75.5(2) 2_456 4_556
Ga3 O3 O3 102.26(17) 1_556 4_556
O1 O3 O3 98.8(3) 2_565 4_556
La O3 O3 89.1(3) 2 4_556
Ga3 O3 O3 111.1(2) 1_655 4_556
O3 O3 O3 151.95(14) 1_554 4_556
O3 O3 O3 28.05(14) 1_556 4_556
O2 O3 O3 80.1(3) 4_456 4_556
O2 O3 O3 35.5(2) 1_656 4_556
La O3 O3 50.01(17) 2_566 4_556
O2 O3 O3 106.9(3) 2_455 4_556
O2 O3 O3 132.0(4) 4_455 4_556
O1 O3 O3 45.7(2) 2_566 4_556
O2 O3 O3 93.4(3) 1_655 4_556
O1 O3 O3 91.4(3) 1_545 4_556
O2 O3 O3 66.3(2) 5 4_556
O3 O3 O3 95.7(3) 3_565 4_556
O3 O3 O3 116.61(17) 4_455 4_556
Ga2 O3 O3 153.7(4) 1_554 4_556
O2 O3 O3 78.7(3) 6_665 4_556
O2 O3 O3 152.3(4) 5_444 4_556
O2 O3 O3 129.8(3) 2_564 4_556
Ga2 O3 O3 74.7(2) 2_556 4_556
La O3 O3 123.1(2) 4_455 4_556
La O3 O3 24.24(13) 4_556 4_556
O1 O3 O3 55.96(16) 1_556 4_556
O3 O3 O3 123.9(3) 4_554 4_556
O3 O3 O3 131.9(2) 3_554 4_556
Ga3 O3 O3 58.9(3) 2_565 3_556
Nb O3 O3 102.8(4) . 3_556
Ga1 O3 O3 102.8(4) . 3_556
La O3 O3 129.8(6) . 3_556
Ga3 O3 O3 35.3(2) 4_446 3_556
O3 O3 O3 133.6(7) 6 3_556
O3 O3 O3 76.40(6) 4 3_556
O3 O3 O3 61.95(14) 3 3_556
O2 O3 O3 70.5(4) 5_445 3_556
O3 O3 O3 18.3(2) 6_556 3_556
O2 O3 O3 97.2(3) 2_565 3_556
O2 O3 O3 67.1(3) 3_566 3_556
O1 O3 O3 123.8(4) . 3_556
O3 O3 O3 127.4(5) 5 3_556
O2 O3 O3 171.4(4) 3_565 3_556
O3 O3 O3 41.1(2) 5_556 3_556
Ga2 O3 O3 92.8(2) 2_566 3_556
Ga3 O3 O3 48.93(16) 1_656 3_556
La O3 O3 132.5(3) 2_565 3_556
O2 O3 O3 93.8(4) 6 3_556
O3 O3 O3 101.5(4) 2 3_556
Ga3 O3 O3 153.3(3) 2_564 3_556
Ga2 O3 O3 71.7(3) . 3_556
O3 O3 O3 23.7(3) 2_556 3_556
Ga1 O3 O3 13.87(7) 1_556 3_556
Nb O3 O3 13.87(7) 1_556 3_556
O2 O3 O3 80.2(3) 1_556 3_556
La O3 O3 102.8(2) 4 3_556
O1 O3 O3 112.3(4) 2_455 3_556
Ga3 O3 O3 123.6(3) 4_445 3_556
La O3 O3 47.63(18) 1_556 3_556
O2 O3 O3 35.7(3) 4_446 3_556
O2 O3 O3 146.2(4) . 3_556
Ga2 O3 O3 89.11(17) 1_665 3_556
La O3 O3 87.2(3) 4_445 3_556
O2 O3 O3 101.3(3) 4_445 3_556
Ga2 O3 O3 165.5(3) 2_565 3_556
O2 O3 O3 61.7(2) 6_655 3_556
O1 O3 O3 54.1(3) 2_456 3_556
Ga3 O3 O3 91.6(3) 1_556 3_556
O1 O3 O3 125.3(3) 2_565 3_556
La O3 O3 76.3(2) 2 3_556
Ga3 O3 O3 114.4(2) 1_655 3_556
O3 O3 O3 151.95(14) 1_554 3_556
O3 O3 O3 28.05(14) 1_556 3_556
O2 O3 O3 91.6(2) 4_456 3_556
O2 O3 O3 50.50(18) 1_656 3_556
La O3 O3 68.29(11) 2_566 3_556
O2 O3 O3 81.1(3) 2_455 3_556
O2 O3 O3 149.3(2) 4_455 3_556
O1 O3 O3 71.93(18) 2_566 3_556
O2 O3 O3 103.3(2) 1_655 3_556
O1 O3 O3 68.7(3) 1_545 3_556
O2 O3 O3 92.6(2) 5 3_556
O3 O3 O3 116.61(17) 3_565 3_556
O3 O3 O3 110.3(3) 4_455 3_556
Ga2 O3 O3 126.6(4) 1_554 3_556
O2 O3 O3 105.2(2) 6_665 3_556
O2 O3 O3 130.4(4) 5_444 3_556
O2 O3 O3 151.7(3) 2_564 3_556
Ga2 O3 O3 50.3(2) 2_556 3_556
La O3 O3 128.5(2) 4_455 3_556
La O3 O3 51.17(11) 4_556 3_556
O1 O3 O3 61.28(15) 1_556 3_556
O3 O3 O3 131.9(2) 4_554 3_556
O3 O3 O3 123.9(3) 3_554 3_556
O3 O3 O3 27.19(13) 4_556 3_556
Ga3 O3 O1 64.1(3) 2_565 1_655
Nb O3 O1 47.9(3) . 1_655
Ga1 O3 O1 47.9(3) . 1_655
La O3 O1 145.6(4) . 1_655
Ga3 O3 O1 95.1(2) 4_446 1_655
O3 O3 O1 93.5(3) 6 1_655
O3 O3 O1 7.5(3) 4 1_655
O3 O3 O1 66.7(4) 3 1_655
O2 O3 O1 128.3(3) 5_445 1_655
O3 O3 O1 99.6(2) 6_556 1_655
O2 O3 O1 54.8(4) 2_565 1_655
O2 O3 O1 99.9(3) 3_566 1_655
O1 O3 O1 124.9(4) . 1_655
O3 O3 O1 46.9(3) 5 1_655
O2 O3 O1 93.4(3) 3_565 1_655
O3 O3 O1 56.2(4) 5_556 1_655
Ga2 O3 O1 123.7(3) 2_566 1_655
Ga3 O3 O1 36.08(17) 1_656 1_655
La O3 O1 83.7(2) 2_565 1_655
O2 O3 O1 174.8(4) 6 1_655
O3 O3 O1 56.2(2) 2 1_655
Ga3 O3 O1 73.7(2) 2_564 1_655
Ga2 O3 O1 147.9(3) . 1_655
O3 O3 O1 62.6(2) 2_556 1_655
Ga1 O3 O1 75.9(2) 1_556 1_655
Nb O3 O1 75.9(2) 1_556 1_655
O2 O3 O1 141.2(3) 1_556 1_655
La O3 O1 23.29(10) 4 1_655
O1 O3 O1 137.2(2) 2_455 1_655
Ga3 O3 O1 88.9(2) 4_445 1_655
La O3 O1 121.5(2) 1_556 1_655
O2 O3 O1 96.3(3) 4_446 1_655
O2 O3 O1 131.3(3) . 1_655
Ga2 O3 O1 54.72(14) 1_665 1_655
La O3 O1 116.49(18) 4_445 1_655
O2 O3 O1 92.1(3) 4_445 1_655
Ga2 O3 O1 109.5(3) 2_565 1_655
O2 O3 O1 37.79(18) 6_655 1_655
O1 O3 O1 136.0(2) 2_456 1_655
Ga3 O3 O1 162.7(2) 1_556 1_655
O1 O3 O1 54.32(16) 2_565 1_655
La O3 O1 65.71(12) 2 1_655
Ga3 O3 O1 49.98(16) 1_655 1_655
O3 O3 O1 86.48(18) 1_554 1_655
O3 O3 O1 93.52(18) 1_556 1_655
O2 O3 O1 114.0(3) 4_456 1_655
O2 O3 O1 32.1(2) 1_656 1_655
La O3 O1 88.9(2) 2_566 1_655
O2 O3 O1 144.9(3) 2_455 1_655
O2 O3 O1 109.3(3) 4_455 1_655
O1 O3 O1 61.7(2) 2_566 1_655
O2 O3 O1 29.9(2) 1_655 1_655
O1 O3 O1 92.09(14) 1_545 1_655
O2 O3 O1 36.98(15) 5 1_655
O3 O3 O1 95.7(3) 3_565 1_655
O3 O3 O1 155.5(3) 4_455 1_655
Ga2 O3 O1 124.4(2) 1_554 1_655
O2 O3 O1 66.58(19) 6_665 1_655
O2 O3 O1 105.1(2) 5_444 1_655
O2 O3 O1 69.3(2) 2_564 1_655
Ga2 O3 O1 93.17(14) 2_556 1_655
La O3 O1 131.4(3) 4_455 1_655
La O3 O1 50.04(17) 4_556 1_655
O1 O3 O1 111.9(2) 1_556 1_655
O3 O3 O1 58.6(2) 4_554 1_655
O3 O3 O1 76.1(3) 3_554 1_655
O3 O3 O1 65.7(2) 4_556 1_655
O3 O3 O1 82.4(2) 3_556 1_655
Ga3 O3 La 91.9(5) 2_565 4_446
Nb O3 La 108.4(4) . 4_446
Ga1 O3 La 108.4(4) . 4_446
La O3 La 93.8(4) . 4_446
Ga3 O3 La 22.03(16) 4_446 4_446
O3 O3 La 109.0(7) 6 4_446
O3 O3 La 106.6(3) 4 4_446
O3 O3 La 62.1(4) 3 4_446
O2 O3 La 34.3(3) 5_445 4_446
O3 O3 La 29.7(4) 6_556 4_446
O2 O3 La 131.7(4) 2_565 4_446
O2 O3 La 82.4(4) 3_566 4_446
O1 O3 La 113.6(3) . 4_446
O3 O3 La 144.37(10) 5 4_446
O2 O3 La 149.8(3) 3_565 4_446
O3 O3 La 78.0(4) 5_556 4_446
Ga2 O3 La 91.6(3) 2_566 4_446
Ga3 O3 La 77.7(2) 1_656 4_446
La O3 La 150.6(2) 2_565 4_446
O2 O3 La 61.4(3) 6 4_446
O3 O3 La 101.7(3) 2 4_446
Ga3 O3 La 148.1(3) 2_564 4_446
Ga2 O3 La 35.75(12) . 4_446
O3 O3 La 51.68(14) 2_556 4_446
Ga1 O3 La 50.04(15) 1_556 4_446
Nb O3 La 50.04(15) 1_556 4_446
O2 O3 La 68.5(2) 1_556 4_446
La O3 La 136.8(2) 4 4_446
O1 O3 La 75.3(3) 2_455 4_446
Ga3 O3 La 102.5(2) 4_445 4_446
La O3 La 44.09(13) 1_556 4_446
O2 O3 La 20.93(18) 4_446 4_446
O2 O3 La 112.8(3) . 4_446
Ga2 O3 La 123.5(2) 1_665 4_446
La O3 La 55.63(15) 4_445 4_446
O2 O3 La 80.2(2) 4_445 4_446
Ga2 O3 La 135.0(2) 2_565 4_446
O2 O3 La 80.9(2) 6_655 4_446
O1 O3 La 24.61(9) 2_456 4_446
Ga3 O3 La 67.77(17) 1_556 4_446
O1 O3 La 162.7(3) 2_565 4_446
La O3 La 73.49(18) 2 4_446
Ga3 O3 La 120.0(2) 1_655 4_446
O3 O3 La 130.56(10) 1_554 4_446
O3 O3 La 49.44(10) 1_556 4_446
O2 O3 La 96.4(2) 4_456 4_446
O2 O3 La 84.7(2) 1_656 4_446
La O3 La 89.72(18) 2_566 4_446
O2 O3 La 43.65(16) 2_455 4_446
O2 O3 La 136.1(3) 4_455 4_446
O1 O3 La 104.7(3) 2_566 4_446
O2 O3 La 122.0(2) 1_655 4_446
O1 O3 La 50.50(18) 1_545 4_446
O2 O3 La 130.0(2) 5 4_446
O3 O3 La 128.85(15) 3_565 4_446
O3 O3 La 86.7(2) 4_455 4_446
Ga2 O3 La 90.77(19) 1_554 4_446
O2 O3 La 135.5(2) 6_665 4_446
O2 O3 La 100.4(3) 5_444 4_446
O2 O3 La 160.7(2) 2_564 4_446
Ga2 O3 La 34.24(9) 2_556 4_446
La O3 La 111.38(19) 4_455 4_446
La O3 La 88.15(17) 4_556 4_446
O1 O3 La 68.94(15) 1_556 4_446
O3 O3 La 135.1(3) 4_554 4_446
O3 O3 La 110.7(3) 3_554 4_446
O3 O3 La 63.91(15) 4_556 4_446
O3 O3 La 37.5(2) 3_556 4_446
O1 O3 La 113.8(2) 1_655 4_446
Ga3 O3 O2 70.5(4) 2_565 5_446
Nb O3 O2 123.9(5) . 5_446
Ga1 O3 O2 123.9(5) . 5_446
La O3 O2 103.7(4) . 5_446
Ga3 O3 O2 38.4(2) 4_446 5_446
O3 O3 O2 131.9(7) 6 5_446
O3 O3 O2 103.79(19) 4 5_446
O3 O3 O2 77.5(3) 3 5_446
O2 O3 O2 55.6(3) 5_445 5_446
O3 O3 O2 10.4(2) 6_556 5_446
O2 O3 O2 109.8(4) 2_565 5_446
O2 O3 O2 60.0(5) 3_566 5_446
O1 O3 O2 103.1(4) . 5_446
O3 O3 O2 154.5(3) 5 5_446
O2 O3 O2 154.5(3) 3_565 5_446
O3 O3 O2 61.0(4) 5_556 5_446
Ga2 O3 O2 75.1(3) 2_566 5_446
Ga3 O3 O2 76.2(2) 1_656 5_446
La O3 O2 130.5(3) 2_565 5_446
O2 O3 O2 66.9(3) 6 5_446
O3 O3 O2 119.4(4) 2 5_446
Ga3 O3 O2 171.2(3) 2_564 5_446
Ga2 O3 O2 47.88(19) . 5_446
O3 O3 O2 49.9(2) 2_556 5_446
Ga1 O3 O2 34.83(15) 1_556 5_446
Nb O3 O2 34.83(15) 1_556 5_446
O2 O3 O2 56.37(19) 1_556 5_446
La O3 O2 128.5(2) 4 5_446
O1 O3 O2 93.3(3) 2_455 5_446
Ga3 O3 O2 125.6(3) 4_445 5_446
La O3 O2 25.36(15) 1_556 5_446
O2 O3 O2 37.8(2) 4_446 5_446
O2 O3 O2 118.8(3) . 5_446
Ga2 O3 O2 101.8(2) 1_665 5_446
La O3 O2 78.4(3) 4_445 5_446
O2 O3 O2 103.0(3) 4_445 5_446
Ga2 O3 O2 139.2(2) 2_565 5_446
O2 O3 O2 86.8(2) 6_655 5_446
O1 O3 O2 28.0(2) 2_456 5_446
Ga3 O3 O2 64.54(18) 1_556 5_446
O1 O3 O2 142.2(3) 2_565 5_446
La O3 O2 90.9(2) 2 5_446
Ga3 O3 O2 136.2(2) 1_655 5_446
O3 O3 O2 152.95(18) 1_554 5_446
O3 O3 O2 27.05(18) 1_556 5_446
O2 O3 O2 77.6(2) 4_456 5_446
O2 O3 O2 77.5(2) 1_656 5_446
La O3 O2 66.69(19) 2_566 5_446
O2 O3 O2 60.4(2) 2_455 5_446
O2 O3 O2 129.50(19) 4_455 5_446
O1 O3 O2 82.8(2) 2_566 5_446
O2 O3 O2 129.7(3) 1_655 5_446
O1 O3 O2 72.1(3) 1_545 5_446
O2 O3 O2 112.2(2) 5 5_446
O3 O3 O2 109.12(16) 3_565 5_446
O3 O3 O2 83.72(18) 4_455 5_446
Ga2 O3 O2 110.0(3) 1_554 5_446
O2 O3 O2 112.4(3) 6_665 5_446
O2 O3 O2 122.5(4) 5_444 5_446
O2 O3 O2 176.2(3) 2_564 5_446
Ga2 O3 O2 54.03(19) 2_556 5_446
La O3 O2 104.8(2) 4_455 5_446
La O3 O2 70.74(17) 4_556 5_446
O1 O3 O2 47.79(18) 1_556 5_446
O3 O3 O2 153.9(3) 4_554 5_446
O3 O3 O2 133.2(3) 3_554 5_446
O3 O3 O2 47.62(14) 4_556 5_446
O3 O3 O2 27.41(19) 3_556 5_446
O1 O3 O2 109.6(2) 1_655 5_446
La O3 O2 23.11(14) 4_446 5_446
Ga3 O3 La 137.8(4) 2_565 2_455
Nb O3 La 109.3(4) . 2_455
Ga1 O3 La 109.3(4) . 2_455
La O3 La 28.1(2) . 2_455
Ga3 O3 La 78.4(3) 4_446 2_455
O3 O3 La 66.5(3) 6 2_455
O3 O3 La 153.4(5) 4 2_455
O3 O3 La 95.7(6) 3 2_455
O2 O3 La 38.9(3) 5_445 2_455
O3 O3 La 89.3(4) 6_556 2_455
O2 O3 La 144.0(4) 2_565 2_455
O2 O3 La 102.8(3) 3_566 2_455
O1 O3 La 71.0(2) . 2_455
O3 O3 La 118.8(4) 5 2_455
O2 O3 La 83.9(3) 3_565 2_455
O3 O3 La 139.4(5) 5_556 2_455
Ga2 O3 La 78.82(19) 2_566 2_455
Ga3 O3 La 136.6(3) 1_656 2_455
La O3 La 107.3(2) 2_565 2_455
O2 O3 La 21.0(2) 6 2_455
O3 O3 La 100.81(18) 2 2_455
Ga3 O3 La 94.90(18) 2_564 2_455
Ga2 O3 La 31.43(9) . 2_455
O3 O3 La 115.59(14) 2_556 2_455
Ga1 O3 La 113.6(3) 1_556 2_455
Nb O3 La 113.6(3) 1_556 2_455
O2 O3 La 61.6(2) 1_556 2_455
La O3 La 151.9(3) 4 2_455
O1 O3 La 20.43(17) 2_455 2_455
Ga3 O3 La 69.39(15) 4_445 2_455
La O3 La 75.48(18) 1_556 2_455
O2 O3 La 77.3(3) 4_446 2_455
O2 O3 La 47.94(17) . 2_455
Ga2 O3 La 146.4(2) 1_665 2_455
La O3 La 42.70(10) 4_445 2_455
O2 O3 La 64.9(3) 4_445 2_455
Ga2 O3 La 69.49(12) 2_565 2_455
O2 O3 La 125.5(3) 6_655 2_455
O1 O3 La 51.12(17) 2_456 2_455
Ga3 O3 La 40.31(9) 1_556 2_455
O1 O3 La 130.3(3) 2_565 2_455
La O3 La 93.44(19) 2 2_455
Ga3 O3 La 108.78(18) 1_655 2_455
O3 O3 La 78.48(12) 1_554 2_455
O3 O3 La 101.52(12) 1_556 2_455
O2 O3 La 88.4(2) 4_456 2_455
O2 O3 La 148.7(3) 1_656 2_455
La O3 La 113.99(18) 2_566 2_455
O2 O3 La 23.27(14) 2_455 2_455
O2 O3 La 77.6(2) 4_455 2_455
O1 O3 La 141.4(2) 2_566 2_455
O2 O3 La 128.8(2) 1_655 2_455
O1 O3 La 69.76(15) 1_545 2_455
O2 O3 La 159.9(3) 5 2_455
O3 O3 La 101.63(19) 3_565 2_455
O3 O3 La 43.1(2) 4_455 2_455
Ga2 O3 La 35.55(7) 1_554 2_455
O2 O3 La 131.2(3) 6_665 2_455
O2 O3 La 54.36(16) 5_444 2_455
O2 O3 La 103.4(2) 2_564 2_455
Ga2 O3 La 74.33(16) 2_556 2_455
La O3 La 62.15(10) 4_455 2_455
La O3 La 148.2(2) 4_556 2_455
O1 O3 La 89.85(16) 1_556 2_455
O3 O3 La 104.13(16) 4_554 2_455
O3 O3 La 82.6(2) 3_554 2_455
O3 O3 La 126.6(2) 4_556 2_455
O3 O3 La 102.9(3) 3_556 2_455
O1 O3 La 157.0(2) 1_655 2_455
La O3 La 65.95(14) 4_446 2_455
O2 O3 La 79.0(2) 5_446 2_455
Ga3 O3 O3 135.1(4) 2_565 2_455
Nb O3 O3 110.9(4) . 2_455
Ga1 O3 O3 110.9(4) . 2_455
La O3 O3 7.37(18) . 2_455
Ga3 O3 O3 101.0(2) 4_446 2_455
O3 O3 O3 62.51(19) 6 2_455
O3 O3 O3 156.3(2) 4 2_455
O3 O3 O3 113.8(5) 3 2_455
O2 O3 O3 61.4(3) 5_445 2_455
O3 O3 O3 106.6(3) 6_556 2_455
O2 O3 O3 123.6(4) 2_565 2_455
O2 O3 O3 99.5(3) 3_566 2_455
O1 O3 O3 52.4(3) . 2_455
O3 O3 O3 106.1(5) 5 2_455
O2 O3 O3 63.0(3) 3_565 2_455
O3 O3 O3 149.6(6) 5_556 2_455
Ga2 O3 O3 69.4(2) 2_566 2_455
Ga3 O3 O3 157.7(3) 1_656 2_455
La O3 O3 85.1(2) 2_565 2_455
O2 O3 O3 29.66(19) 6 2_455
O3 O3 O3 104.7(4) 2 2_455
Ga3 O3 O3 79.5(2) 2_564 2_455
Ga2 O3 O3 51.64(6) . 2_455
O3 O3 O3 138.06(18) 2_556 2_455
Ga1 O3 O3 130.8(3) 1_556 2_455
Nb O3 O3 130.8(3) 1_556 2_455
O2 O3 O3 60.9(2) 1_556 2_455
La O3 O3 134.5(3) 4 2_455
O1 O3 O3 29.22(7) 2_455 2_455
Ga3 O3 O3 69.33(18) 4_445 2_455
La O3 O3 85.3(2) 1_556 2_455
O2 O3 O3 99.9(3) 4_446 2_455
O2 O3 O3 25.6(2) . 2_455
Ga2 O3 O3 128.1(2) 1_665 2_455
La O3 O3 60.55(7) 4_445 2_455
O2 O3 O3 74.3(3) 4_445 2_455
Ga2 O3 O3 47.72(18) 2_565 2_455
O2 O3 O3 141.7(3) 6_655 2_455
O1 O3 O3 68.73(16) 2_456 2_455
Ga3 O3 O3 40.22(12) 1_556 2_455
O1 O3 O3 108.2(3) 2_565 2_455
La O3 O3 107.66(19) 2 2_455
Ga3 O3 O3 105.5(3) 1_655 2_455
O3 O3 O3 66.6(2) 1_554 2_455
O3 O3 O3 113.4(2) 1_556 2_455
O2 O3 O3 78.1(3) 4_456 2_455
O2 O3 O3 171.3(3) 1_656 2_455
La O3 O3 108.8(2) 2_566 2_455
O2 O3 O3 45.82(13) 2_455 2_455
O2 O3 O3 55.1(3) 4_455 2_455
O1 O3 O3 131.5(2) 2_566 2_455
O2 O3 O3 124.5(3) 1_655 2_455
O1 O3 O3 88.78(14) 1_545 2_455
O2 O3 O3 137.6(3) 5 2_455
O3 O3 O3 82.3(2) 3_565 2_455
O3 O3 O3 31.5(3) 4_455 2_455
Ga2 O3 O3 34.13(11) 1_554 2_455
O2 O3 O3 110.8(3) 6_665 2_455
O2 O3 O3 52.21(17) 5_444 2_455
O2 O3 O3 85.3(3) 2_564 2_455
Ga2 O3 O3 96.22(13) 2_556 2_455
La O3 O3 42.58(16) 4_455 2_455
La O3 O3 152.9(3) 4_556 2_455
O1 O3 O3 90.9(2) 1_556 2_455
O3 O3 O3 94.6(2) 4_554 2_455
O3 O3 O3 80.7(2) 3_554 2_455
O3 O3 O3 141.4(3) 4_556 2_455
O3 O3 O3 122.7(3) 3_556 2_455
O1 O3 O3 153.0(3) 1_655 2_455
La O3 O3 87.29(15) 4_446 2_455
O2 O3 O3 96.4(2) 5_446 2_455
La O3 O3 22.61(6) 2_455 2_455
Ga3 O3 O3 78.7(3) 2_565 2_565
Nb O3 O3 98.3(5) . 2_565
Ga1 O3 O3 98.3(5) . 2_565
La O3 O3 77.9(4) . 2_565
Ga3 O3 O3 172.1(4) 4_446 2_565
O3 O3 O3 87.8(7) 6 2_565
O3 O3 O3 92.2(4) 4 2_565
O3 O3 O3 144.4(4) 3 2_565
O2 O3 O3 143.7(4) 5_445 2_565
O3 O3 O3 132.8(5) 6_556 2_565
O2 O3 O3 43.8(2) 2_565 2_565
O2 O3 O3 75.2(4) 3_566 2_565
O1 O3 O3 41.9(3) . 2_565
O3 O3 O3 62.35(19) 5 2_565
O2 O3 O3 34.5(3) 3_565 2_565
O3 O3 O3 99.07(15) 5_556 2_565
Ga2 O3 O3 61.7(2) 2_566 2_565
Ga3 O3 O3 118.1(2) 1_656 2_565
La O3 O3 4.68(9) 2_565 2_565
O2 O3 O3 100.5(3) 6 2_565
O3 O3 O3 104.7(4) 2 2_565
Ga3 O3 O3 53.1(2) 2_564 2_565
Ga2 O3 O3 127.2(3) . 2_565
O3 O3 O3 138.06(18) 2_556 2_565
Ga1 O3 O3 123.5(2) 1_556 2_565
Nb O3 O3 123.5(2) 1_556 2_565
O2 O3 O3 85.0(3) 1_556 2_565
La O3 O3 61.99(10) 4 2_565
O1 O3 O3 104.8(4) 2_455 2_565
Ga3 O3 O3 96.7(3) 4_445 2_565
La O3 O3 110.2(3) 1_556 2_565
O2 O3 O3 171.9(4) 4_446 2_565
O2 O3 O3 58.1(3) . 2_565
Ga2 O3 O3 50.88(5) 1_665 2_565
La O3 O3 134.7(3) 4_445 2_565
O2 O3 O3 119.9(4) 4_445 2_565
Ga2 O3 O3 40.5(2) 2_565 2_565
O2 O3 O3 121.7(2) 6_655 2_565
O1 O3 O3 130.2(3) 2_456 2_565
Ga3 O3 O3 88.8(2) 1_556 2_565
O1 O3 O3 30.81(6) 2_565 2_565
La O3 O3 133.2(3) 2 2_565
Ga3 O3 O3 86.6(3) 1_655 2_565
O3 O3 O3 66.6(2) 1_554 2_565
O3 O3 O3 113.4(2) 1_556 2_565
O2 O3 O3 57.4(2) 4_456 2_565
O2 O3 O3 106.40(19) 1_656 2_565
La O3 O3 70.75(15) 2_566 2_565
O2 O3 O3 127.4(3) 2_455 2_565
O2 O3 O3 27.2(3) 4_455 2_565
O1 O3 O3 65.97(14) 2_566 2_565
O2 O3 O3 83.8(2) 1_655 2_565
O1 O3 O3 152.7(3) 1_545 2_565
O2 O3 O3 55.37(17) 5 2_565
O3 O3 O3 25.3(2) 3_565 2_565
O3 O3 O3 71.6(3) 4_455 2_565
Ga2 O3 O3 94.1(3) 1_554 2_565
O2 O3 O3 33.15(16) 6_665 2_565
O2 O3 O3 92.5(4) 5_444 2_565
O2 O3 O3 42.3(2) 2_564 2_565
Ga2 O3 O3 171.5(3) 2_556 2_565
La O3 O3 46.8(2) 4_455 2_565
La O3 O3 90.07(12) 4_556 2_565
O1 O3 O3 86.6(2) 1_556 2_565
O3 O3 O3 70.6(3) 4_554 2_565
O3 O3 O3 91.8(2) 3_554 2_565
O3 O3 O3 111.6(2) 4_556 2_565
O3 O3 O3 137.1(2) 3_556 2_565
O1 O3 O3 84.72(12) 1_655 2_565
La O3 O3 153.3(3) 4_446 2_565
O2 O3 O3 134.4(3) 5_446 2_565
La O3 O3 104.7(2) 2_455 2_565
O3 O3 O3 82.3(3) 2_455 2_565
Ga3 O3 O2 153.1(5) 2_565 6_554
Nb O3 O2 84.0(3) . 6_554
Ga1 O3 O2 84.0(3) . 6_554
La O3 O2 21.6(2) . 6_554
Ga3 O3 O2 108.7(3) 4_446 6_554
O3 O3 O2 35.55(16) 6 6_554
O3 O3 O2 128.15(15) 4 6_554
O3 O3 O2 101.5(4) 3 6_554
O2 O3 O2 70.8(3) 5_445 6_554
O3 O3 O2 129.9(4) 6_556 6_554
O2 O3 O2 120.6(4) 2_565 6_554
O2 O3 O2 123.6(3) 3_566 6_554
O1 O3 O2 65.9(3) . 6_554
O3 O3 O2 79.5(4) 5 6_554
O2 O3 O2 46.97(17) 3_565 6_554
O3 O3 O2 175.78(15) 5_556 6_554
Ga2 O3 O2 91.8(2) 2_566 6_554
Ga3 O3 O2 141.5(3) 1_656 6_554
La O3 O2 81.8(2) 2_565 6_554
O2 O3 O2 56.2(2) 6 6_554
O3 O3 O2 79.1(3) 2 6_554
Ga3 O3 O2 54.26(17) 2_564 6_554
Ga2 O3 O2 71.85(18) . 6_554
O3 O3 O2 142.4(2) 2_556 6_554
Ga1 O3 O2 153.7(3) 1_556 6_554
Nb O3 O2 153.7(3) 1_556 6_554
O2 O3 O2 88.3(3) 1_556 6_554
La O3 O2 111.4(3) 4 6_554
O1 O3 O2 28.8(2) 2_455 6_554
Ga3 O3 O2 43.96(13) 4_445 6_554
La O3 O2 113.1(2) 1_556 6_554
O2 O3 O2 108.0(3) 4_446 6_554
O2 O3 O2 26.1(3) . 6_554
Ga2 O3 O2 128.3(3) 1_665 6_554
La O3 O2 57.40(14) 4_445 6_554
O2 O3 O2 56.4(2) 4_445 6_554
Ga2 O3 O2 37.04(14) 2_565 6_554
O2 O3 O2 121.7(3) 6_655 6_554
O1 O3 O2 91.8(2) 2_456 6_554
Ga3 O3 O2 68.29(16) 1_556 6_554
O1 O3 O2 93.4(3) 2_565 6_554
La O3 O2 90.54(18) 2 6_554
Ga3 O3 O2 77.49(18) 1_655 6_554
O3 O3 O2 39.09(16) 1_554 6_554
O3 O3 O2 140.91(16) 1_556 6_554
O2 O3 O2 98.7(3) 4_456 6_554
O2 O3 O2 152.7(3) 1_656 6_554
La O3 O2 130.4(2) 2_566 6_554
O2 O3 O2 60.53(14) 2_455 6_554
O2 O3 O2 53.9(2) 4_455 6_554
O1 O3 O2 142.4(3) 2_566 6_554
O2 O3 O2 96.4(2) 1_655 6_554
O1 O3 O2 82.4(2) 1_545 6_554
O2 O3 O2 126.1(3) 5 6_554
O3 O3 O2 89.53(15) 3_565 6_554
O3 O3 O2 56.63(18) 4_455 6_554
Ga2 O3 O2 17.05(10) 1_554 6_554
O2 O3 O2 110.7(3) 6_665 6_554
O2 O3 O2 27.41(19) 5_444 6_554
O2 O3 O2 62.9(3) 2_564 6_554
Ga2 O3 O2 97.16(19) 2_556 6_554
La O3 O2 56.26(15) 4_455 6_554
La O3 O2 167.4(3) 4_556 6_554
O1 O3 O2 117.9(2) 1_556 6_554
O3 O3 O2 66.76(16) 4_554 6_554
O3 O3 O2 53.8(2) 3_554 6_554
O3 O3 O2 167.3(3) 4_556 6_554
O3 O3 O2 141.2(4) 3_556 6_554
O1 O3 O2 125.4(3) 1_655 6_554
La O3 O2 103.9(2) 4_446 6_554
O2 O3 O2 119.7(2) 5_446 6_554
La O3 O2 40.72(13) 2_455 6_554
O3 O3 O2 28.14(16) 2_455 6_554
O3 O3 O2 77.5(3) 2_565 6_554
Ga3 O3 O2 16.9(3) 2_565 2_566
Nb O3 O2 123.3(4) . 2_566
Ga1 O3 O2 123.3(4) . 2_566
La O3 O2 131.1(3) . 2_566
Ga3 O3 O2 82.5(3) 4_446 2_566
O3 O3 O2 170.9(4) 6 2_566
O3 O3 O2 76.9(3) 4 2_566
O3 O3 O2 103.4(2) 3 2_566
O2 O3 O2 110.0(4) 5_445 2_566
O3 O3 O2 46.9(4) 6_556 2_566
O2 O3 O2 55.4(3) 2_565 2_566
O2 O3 O2 28.1(2) 3_566 2_566
O1 O3 O2 87.6(3) . 2_566
O3 O3 O2 117.0(4) 5 2_566
O2 O3 O2 124.2(4) 3_565 2_566
O3 O3 O2 24.7(3) 5_556 2_566
Ga2 O3 O2 60.0(2) 2_566 2_566
Ga3 O3 O2 66.8(2) 1_656 2_566
La O3 O2 85.1(2) 2_565 2_566
O2 O3 O2 102.6(4) 6 2_566
O3 O3 O2 129.0(4) 2 2_566
Ga3 O3 O2 134.3(3) 2_564 2_566
Ga2 O3 O2 97.4(2) . 2_566
O3 O3 O2 59.5(3) 2_556 2_566
Ga1 O3 O2 34.67(15) 1_556 2_566
Nb O3 O2 34.67(15) 1_556 2_566
O2 O3 O2 65.1(2) 1_556 2_566
La O3 O2 83.6(2) 4 2_566
O1 O3 O2 142.5(4) 2_455 2_566
Ga3 O3 O2 164.4(3) 4_445 2_566
La O3 O2 47.85(15) 1_556 2_566
O2 O3 O2 82.7(3) 4_446 2_566
O2 O3 O2 127.1(2) . 2_566
Ga2 O3 O2 47.44(14) 1_665 2_566
La O3 O2 132.1(3) 4_445 2_566
O2 O3 O2 147.8(3) 4_445 2_566
Ga2 O3 O2 125.4(2) 2_565 2_566
O2 O3 O2 86.6(2) 6_655 2_566
O1 O3 O2 77.0(3) 2_456 2_566
Ga3 O3 O2 86.4(2) 1_556 2_566
O1 O3 O2 87.8(3) 2_565 2_566
La O3 O2 116.1(2) 2 2_566
Ga3 O3 O2 127.5(3) 1_655 2_566
O3 O3 O2 152.68(17) 1_554 2_566
O3 O3 O2 27.32(17) 1_556 2_566
O2 O3 O2 53.64(14) 4_456 2_566
O2 O3 O2 55.3(4) 1_656 2_566
La O3 O2 22.97(14) 2_566 2_566
O2 O3 O2 112.0(3) 2_455 2_566
O2 O3 O2 105.8(2) 4_455 2_566
O1 O3 O2 28.51(19) 2_566 2_566
O2 O3 O2 107.4(3) 1_655 2_566
O1 O3 O2 116.1(3) 1_545 2_566
O2 O3 O2 60.28(17) 5 2_566
O3 O3 O2 70.0(2) 3_565 2_566
O3 O3 O2 95.42(18) 4_455 2_566
Ga2 O3 O2 158.0(3) 1_554 2_566
O2 O3 O2 59.67(17) 6_665 2_566
O2 O3 O2 176.7(4) 5_444 2_566
O2 O3 O2 121.9(3) 2_564 2_566
Ga2 O3 O2 97.9(2) 2_556 2_566
La O3 O2 96.66(19) 4_455 2_566
La O3 O2 27.68(16) 4_556 2_566
O1 O3 O2 35.03(16) 1_556 2_566
O3 O3 O2 132.7(3) 4_554 2_566
O3 O3 O2 153.3(4) 3_554 2_566
O3 O3 O2 27.0(2) 4_556 2_566
O3 O3 O2 47.55(15) 3_556 2_566
O1 O3 O2 77.5(3) 1_655 2_566
La O3 O2 76.58(17) 4_446 2_566
O2 O3 O2 54.4(2) 5_446 2_566
La O3 O2 122.7(2) 2_455 2_566
O3 O3 O2 125.8(3) 2_455 2_566
O3 O3 O2 89.75(19) 2_565 2_566
O2 O3 O2 151.6(2) 6_554 2_566
Ga3 O3 La 74.9(4) 2_565 2_556
Nb O3 La 81.5(3) . 2_556
Ga1 O3 La 81.5(3) . 2_556
La O3 La 130.1(4) . 2_556
Ga3 O3 La 24.05(14) 4_446 2_556
O3 O3 La 111.8(5) 6 2_556
O3 O3 La 66.6(3) 4 2_556
O3 O3 La 39.02(9) 3 2_556
O2 O3 La 64.1(3) 5_445 2_556
O3 O3 La 38.0(3) 6_556 2_556
O2 O3 La 107.6(3) 2_565 2_556
O2 O3 La 89.8(4) 3_566 2_556
O1 O3 La 145.9(4) . 2_556
O3 O3 La 111.6(3) 5 2_556
O2 O3 La 161.1(3) 3_565 2_556
O3 O3 La 53.16(14) 5_556 2_556
Ga2 O3 La 115.4(3) 2_566 2_556
Ga3 O3 La 37.77(14) 1_656 2_556
La O3 La 147.4(3) 2_565 2_556
O2 O3 La 101.3(3) 6 2_556
O3 O3 La 79.1(3) 2 2_556
Ga3 O3 La 133.4(2) 2_564 2_556
Ga2 O3 La 75.0(2) . 2_556
O3 O3 La 13.43(12) 2_556 2_556
Ga1 O3 La 33.09(10) 1_556 2_556
Nb O3 La 33.09(10) 1_556 2_556
O2 O3 La 99.9(3) 1_556 2_556
La O3 La 96.92(16) 4 2_556
O1 O3 La 103.9(3) 2_455 2_556
Ga3 O3 La 101.6(2) 4_445 2_556
La O3 La 67.79(17) 1_556 2_556
O2 O3 La 25.1(2) 4_446 2_556
O2 O3 La 150.1(3) . 2_556
Ga2 O3 La 100.57(17) 1_665 2_556
La O3 La 73.17(17) 4_445 2_556
O2 O3 La 80.4(2) 4_445 2_556
Ga2 O3 La 166.9(2) 2_565 2_556
O2 O3 La 43.47(16) 6_655 2_556
O1 O3 La 63.47(18) 2_456 2_556
Ga3 O3 La 106.1(2) 1_556 2_556
O1 O3 La 126.5(2) 2_565 2_556
La O3 La 53.32(11) 2 2_556
Ga3 O3 La 93.63(15) 1_655 2_556
O3 O3 La 129.01(9) 1_554 2_556
O3 O3 La 50.99(9) 1_556 2_556
O2 O3 La 114.5(3) 4_456 2_556
O2 O3 La 46.56(14) 1_656 2_556
La O3 La 89.70(16) 2_566 2_556
O2 O3 La 79.1(2) 2_455 2_556
O2 O3 La 172.2(2) 4_455 2_556
O1 O3 La 86.88(19) 2_566 2_556
O2 O3 La 86.60(18) 1_655 2_556
O1 O3 La 49.33(17) 1_545 2_556
O2 O3 La 96.9(2) 5 2_556
O3 O3 La 137.47(16) 3_565 2_556
O3 O3 La 125.6(3) 4_455 2_556
Ga2 O3 La 113.6(2) 1_554 2_556
O2 O3 La 118.6(2) 6_665 2_556
O2 O3 La 111.1(3) 5_444 2_556
O2 O3 La 137.5(3) 2_564 2_556
Ga2 O3 La 33.37(8) 2_556 2_556
La O3 La 148.3(2) 4_455 2_556
La O3 La 61.59(11) 4_556 2_556
O1 O3 La 84.11(17) 1_556 2_556
O3 O3 La 111.6(2) 4_554 2_556
O3 O3 La 101.0(2) 3_554 2_556
O3 O3 La 42.05(17) 4_556 2_556
O3 O3 La 22.95(13) 3_556 2_556
O1 O3 La 73.80(15) 1_655 2_556
La O3 La 40.00(9) 4_446 2_556
O2 O3 La 43.58(14) 5_446 2_556
La O3 La 102.3(2) 2_455 2_556
O3 O3 La 124.9(2) 2_455 2_556
O3 O3 La 151.31(19) 2_565 2_556
O2 O3 La 130.5(2) 6_554 2_556
O2 O3 La 67.48(17) 2_566 2_556
Ga3 O3 O3 96.1(5) 2_565 2_456
Nb O3 O3 148.6(4) . 2_456
Ga1 O3 O3 148.6(4) . 2_456
La O3 O3 55.77(18) . 2_456
Ga3 O3 O3 76.3(3) 4_446 2_456
O3 O3 O3 107.7(2) 6 2_456
O3 O3 O3 154.5(3) 4 2_456
O3 O3 O3 113.4(5) 3 2_456
O2 O3 O3 54.8(2) 5_445 2_456
O3 O3 O3 61.0(2) 6_556 2_456
O2 O3 O3 116.2(5) 2_565 2_456
O2 O3 O3 62.1(4) 3_566 2_456
O1 O3 O3 59.4(3) . 2_456
O3 O3 O3 153.4(5) 5 2_456
O2 O3 O3 103.3(3) 3_565 2_456
O3 O3 O3 102.0(6) 5_556 2_456
Ga2 O3 O3 46.5(3) 2_566 2_456
Ga3 O3 O3 127.9(4) 1_656 2_456
La O3 O3 100.4(3) 2_565 2_456
O2 O3 O3 21.2(2) 6 2_456
O3 O3 O3 139.37(13) 2 2_456
Ga3 O3 O3 126.5(3) 2_564 2_456
Ga2 O3 O3 30.73(6) . 2_456
O3 O3 O3 101.4(4) 2_556 2_456
Ga1 O3 O3 83.5(3) 1_556 2_456
Nb O3 O3 83.5(3) 1_556 2_456
O2 O3 O3 22.8(3) 1_556 2_456
La O3 O3 157.4(2) 4 2_456
O1 O3 O3 62.09(17) 2_455 2_456
Ga3 O3 O3 111.06(18) 4_445 2_456
La O3 O3 36.71(19) 1_556 2_456
O2 O3 O3 75.1(3) 4_446 2_456
O2 O3 O3 67.4(2) . 2_456
Ga2 O3 O3 113.2(2) 1_665 2_456
La O3 O3 74.22(7) 4_445 2_456
O2 O3 O3 102.8(2) 4_445 2_456
Ga2 O3 O3 87.5(2) 2_565 2_456
O2 O3 O3 135.5(4) 6_655 2_456
O1 O3 O3 30.07(9) 2_456 2_456
Ga3 O3 O3 13.31(9) 1_556 2_456
O1 O3 O3 131.0(2) 2_565 2_456
La O3 O3 120.1(2) 2 2_456
Ga3 O3 O3 150.4(2) 1_655 2_456
O3 O3 O3 115.2(2) 1_554 2_456
O3 O3 O3 64.8(2) 1_556 2_456
O2 O3 O3 55.4(3) 4_456 2_456
O2 O3 O3 127.5(4) 1_656 2_456
La O3 O3 73.5(2) 2_566 2_456
O2 O3 O3 42.14(18) 2_455 2_456
O2 O3 O3 81.9(2) 4_455 2_456
O1 O3 O3 101.2(3) 2_566 2_456
O2 O3 O3 170.0(3) 1_655 2_456
O1 O3 O3 91.92(15) 1_545 2_456
O2 O3 O3 132.4(3) 5 2_456
O3 O3 O3 82.4(2) 3_565 2_456
O3 O3 O3 32.8(2) 4_455 2_456
Ga2 O3 O3 76.59(13) 1_554 2_456
O2 O3 O3 107.3(3) 6_665 2_456
O2 O3 O3 95.78(18) 5_444 2_456
O2 O3 O3 128.4(3) 2_564 2_456
Ga2 O3 O3 83.93(17) 2_556 2_456
La O3 O3 56.78(16) 4_455 2_456
La O3 O3 108.5(3) 4_556 2_456
O1 O3 O3 48.3(2) 1_556 2_456
O3 O3 O3 143.2(3) 4_554 2_456
O3 O3 O3 124.3(2) 3_554 2_456
O3 O3 O3 92.8(2) 4_556 2_456
O3 O3 O3 79.1(3) 3_556 2_456
O1 O3 O3 158.2(3) 1_655 2_456
La O3 O3 54.68(15) 4_446 2_456
O2 O3 O3 51.8(2) 5_446 2_456
La O3 O3 41.69(8) 2_455 2_456
O3 O3 O3 48.62(10) 2_455 2_456
O3 O3 O3 101.1(3) 2_565 2_456
O2 O3 O3 76.4(2) 6_554 2_456
O2 O3 O3 81.4(3) 2_566 2_456
La O3 O3 92.8(3) 2_556 2_456
Ga3 O3 O3 38.21(19) 2_565 2_566
Nb O3 O3 130.1(4) . 2_566
Ga1 O3 O3 130.1(4) . 2_566
La O3 O3 102.0(4) . 2_566
Ga3 O3 O3 123.5(4) 4_446 2_566
O3 O3 O3 136.2(8) 6 2_566
O3 O3 O3 92.1(4) 4 2_566
O3 O3 O3 143.3(3) 3 2_566
O2 O3 O3 133.6(4) 5_445 2_566
O3 O3 O3 84.4(5) 6_556 2_566
O2 O3 O3 35.4(4) 2_565 2_566
O2 O3 O3 28.0(4) 3_566 2_566
O1 O3 O3 50.1(3) . 2_566
O3 O3 O3 99.40(17) 5 2_566
O2 O3 O3 82.2(3) 3_565 2_566
O3 O3 O3 60.9(2) 5_556 2_566
Ga2 O3 O3 36.1(2) 2_566 2_566
Ga3 O3 O3 99.6(2) 1_656 2_566
La O3 O3 44.10(11) 2_565 2_566
O2 O3 O3 96.0(3) 6 2_566
O3 O3 O3 139.37(13) 2 2_566
Ga3 O3 O3 100.6(3) 2_564 2_566
Ga2 O3 O3 110.4(3) . 2_566
O3 O3 O3 101.4(4) 2_556 2_566
Ga1 O3 O3 77.7(2) 1_556 2_566
Nb O3 O3 77.7(2) 1_556 2_566
O2 O3 O3 58.1(3) 1_556 2_566
La O3 O3 76.66(8) 4 2_566
O1 O3 O3 130.1(3) 2_455 2_566
Ga3 O3 O3 145.3(4) 4_445 2_566
La O3 O3 67.7(2) 1_556 2_566
O2 O3 O3 123.3(3) 4_446 2_566
O2 O3 O3 89.0(3) . 2_566
Ga2 O3 O3 33.16(6) 1_665 2_566
La O3 O3 155.0(2) 4_445 2_566
O2 O3 O3 168.5(4) 4_445 2_566
Ga2 O3 O3 82.5(3) 2_565 2_566
O2 O3 O3 117.2(3) 6_655 2_566
O1 O3 O3 97.4(3) 2_456 2_566
Ga3 O3 O3 76.1(2) 1_556 2_566
O1 O3 O3 60.04(15) 2_565 2_566
La O3 O3 151.2(2) 2 2_566
Ga3 O3 O3 123.2(2) 1_655 2_566
O3 O3 O3 115.2(2) 1_554 2_566
O3 O3 O3 64.8(2) 1_556 2_566
O2 O3 O3 26.4(3) 4_456 2_566
O2 O3 O3 85.0(3) 1_656 2_566
La O3 O3 22.14(11) 2_566 2_566
O2 O3 O3 123.0(3) 2_455 2_566
O2 O3 O3 63.1(3) 4_455 2_566
O1 O3 O3 30.57(9) 2_566 2_566
O2 O3 O3 108.7(2) 1_655 2_566
O1 O3 O3 158.5(4) 1_545 2_566
O2 O3 O3 52.08(12) 5 2_566
O3 O3 O3 27.0(3) 3_565 2_566
O3 O3 O3 71.9(3) 4_455 2_566
Ga2 O3 O3 130.9(3) 1_554 2_566
O2 O3 O3 28.53(12) 6_665 2_566
O2 O3 O3 138.4(4) 5_444 2_566
O2 O3 O3 88.5(2) 2_564 2_566
Ga2 O3 O3 139.7(3) 2_556 2_566
La O3 O3 60.2(2) 4_455 2_566
La O3 O3 56.01(13) 4_556 2_566
O1 O3 O3 42.36(17) 1_556 2_566
O3 O3 O3 113.2(3) 4_554 2_566
O3 O3 O3 138.8(3) 3_554 2_566
O3 O3 O3 69.0(2) 4_556 2_566
O3 O3 O3 90.05(19) 3_556 2_566
O1 O3 O3 87.68(11) 1_655 2_566
La O3 O3 110.4(3) 4_446 2_566
O2 O3 O3 87.8(3) 5_446 2_566
La O3 O3 114.5(2) 2_455 2_566
O3 O3 O3 101.1(3) 2_455 2_566
O3 O3 O3 48.62(10) 2_565 2_566
O2 O3 O3 114.9(3) 6_554 2_566
O2 O3 O3 43.05(19) 2_566 2_566
La O3 O3 110.5(3) 2_556 2_566
O3 O3 O3 80.8(2) 2_456 2_566
Ga3 O3 La 84.1(3) 2_565 1_655
Nb O3 La 29.2(2) . 1_655
Ga1 O3 La 29.2(2) . 1_655
La O3 La 134.6(3) . 1_655
Ga3 O3 La 80.0(2) 4_446 1_655
O3 O3 La 77.79(10) 6 1_655
O3 O3 La 19.9(3) 4 1_655
O3 O3 La 44.7(4) 3 1_655
O2 O3 La 106.2(3) 5_445 1_655
O3 O3 La 99.04(16) 6_556 1_655
O2 O3 La 78.7(4) 2_565 1_655
O2 O3 La 120.3(3) 3_566 1_655
O1 O3 La 144.1(4) . 1_655
O3 O3 La 47.6(2) 5 1_655
O2 O3 La 98.5(3) 3_565 1_655
O3 O3 La 69.8(3) 5_556 1_655
Ga2 O3 La 147.5(3) 2_566 1_655
Ga3 O3 La 32.85(10) 1_656 1_655
La O3 La 102.5(3) 2_565 1_655
O2 O3 La 151.7(3) 6 1_655
O3 O3 La 35.4(2) 2 1_655
Ga3 O3 La 72.59(16) 2_564 1_655
Ga2 O3 La 129.0(3) . 1_655
O3 O3 La 57.2(2) 2_556 1_655
Ga1 O3 La 79.90(14) 1_556 1_655
Nb O3 La 79.90(14) 1_556 1_655
O2 O3 La 158.2(3) 1_556 1_655
La O3 La 41.72(8) 4 1_655
O1 O3 La 115.5(2) 2_455 1_655
Ga3 O3 La 70.63(13) 4_445 1_655
La O3 La 127.7(2) 1_556 1_655
O2 O3 La 81.2(2) 4_446 1_655
O2 O3 La 130.5(3) . 1_655
Ga2 O3 La 78.85(16) 1_665 1_655
La O3 La 92.37(15) 4_445 1_655
O2 O3 La 69.0(2) 4_445 1_655
Ga2 O3 La 113.5(2) 2_565 1_655
O2 O3 La 20.88(14) 6_655 1_655
O1 O3 La 126.2(2) 2_456 1_655
Ga3 O3 La 168.9(3) 1_556 1_655
O1 O3 La 71.73(15) 2_565 1_655
La O3 La 41.76(7) 2 1_655
Ga3 O3 La 36.73(7) 1_655 1_655
O3 O3 La 78.67(11) 1_554 1_655
O3 O3 La 101.33(11) 1_556 1_655
O2 O3 La 137.9(3) 4_456 1_655
O2 O3 La 39.55(19) 1_656 1_655
La O3 La 110.19(18) 2_566 1_655
O2 O3 La 121.9(2) 2_455 1_655
O2 O3 La 121.6(3) 4_455 1_655
O1 O3 La 84.28(15) 2_566 1_655
O2 O3 La 22.71(13) 1_655 1_655
O1 O3 La 68.95(11) 1_545 1_655
O2 O3 La 60.91(16) 5 1_655
O3 O3 La 118.1(4) 3_565 1_655
O3 O3 La 168.60(12) 4_455 1_655
Ga2 O3 La 106.12(16) 1_554 1_655
O2 O3 La 90.0(2) 6_665 1_655
O2 O3 La 87.75(17) 5_444 1_655
O2 O3 La 73.6(2) 2_564 1_655
Ga2 O3 La 73.51(12) 2_556 1_655
La O3 La 146.9(3) 4_455 1_655
La O3 La 67.05(11) 4_556 1_655
O1 O3 La 128.87(18) 1_556 1_655
O3 O3 La 52.01(15) 4_554 1_655
O3 O3 La 59.5(2) 3_554 1_655
O3 O3 La 74.4(2) 4_556 1_655
O3 O3 La 80.75(18) 3_556 1_655
O1 O3 La 24.13(6) 1_655 1_655
La O3 La 101.56(17) 4_446 1_655
O2 O3 La 106.95(18) 5_446 1_655
La O3 La 133.65(18) 2_455 1_655
O3 O3 La 140.0(3) 2_455 1_655
O3 O3 La 102.25(18) 2_565 1_655
O2 O3 La 113.2(2) 6_554 1_655
O2 O3 La 94.1(2) 2_566 1_655
La O3 La 64.18(10) 2_556 1_655
O3 O3 La 156.2(3) 2_456 1_655
O3 O3 La 111.70(13) 2_566 1_655
Ga2 O2 Ga3 119.7(6) 2_565 .
Ga2 O2 La 105.7(6) 2_565 .
Ga3 O2 La 120.1(6) . .
Ga2 O2 O3 117.2(7) 2_565 5_455
Ga3 O2 O3 62.7(5) . 5_455
La O2 O3 127.2(5) . 5_455
Ga2 O2 O2 39.9(2) 2_565 3_565
Ga3 O2 O2 143.9(7) . 3_565
La O2 O2 65.7(6) . 3_565
O3 O2 O2 146.2(8) 5_455 3_565
Ga2 O2 O2 39.9(2) 2_565 4_455
Ga3 O2 O2 129.5(8) . 4_455
La O2 O2 110.3(4) . 4_455
O3 O2 O2 86.9(8) 5_455 4_455
O2 O2 O2 60.000(1) 3_565 4_455
Ga2 O2 La 90.6(5) 2_565 4_455
Ga3 O2 La 112.7(7) . 4_455
La O2 La 103.1(4) . 4_455
O3 O2 La 50.2(4) 5_455 4_455
O2 O2 La 98.7(4) 3_565 4_455
O2 O2 La 50.6(4) 4_455 4_455
Ga2 O2 O3 159.0(6) 2_565 2_455
Ga3 O2 O3 39.3(3) . 2_455
La O2 O3 91.2(4) . 2_455
O3 O2 O3 57.5(4) 5_455 2_455
O2 O2 O3 154.2(9) 3_565 2_455
O2 O2 O3 144.2(9) 4_455 2_455
La O2 O3 97.8(5) 4_455 2_455
Ga2 O2 O1 84.1(4) 2_565 .
Ga3 O2 O1 153.9(7) . .
La O2 O1 55.8(2) . .
O3 O2 O1 98.2(5) 5_455 .
O2 O2 O1 61.3(2) 3_565 .
O2 O2 O1 61.3(2) 4_455 .
La O2 O1 52.1(3) 4_455 .
O3 O2 O1 116.2(5) 2_455 .
Ga2 O2 O2 101.5(6) 2_565 6_554
Ga3 O2 O2 39.8(6) . 6_554
La O2 O2 97.5(5) . 6_554
O3 O2 O2 102.5(3) 5_455 6_554
O2 O2 O2 106.5(4) 3_565 6_554
O2 O2 O2 136.5(4) 4_455 6_554
La O2 O2 152.3(2) 4_455 6_554
O3 O2 O2 63.2(5) 2_455 6_554
O1 O2 O2 153.0(5) . 6_554
Ga2 O2 O3 88.8(4) 2_565 4_454
Ga3 O2 O3 35.9(3) . 4_454
La O2 O3 154.4(6) . 4_454
O3 O2 O3 58.5(5) 5_455 4_454
O2 O2 O3 125.8(3) 3_565 4_454
O2 O2 O3 94.4(6) 4_455 4_454
La O2 O3 97.6(5) 4_455 4_454
O3 O2 O3 71.0(4) 2_455 4_454
O1 O2 O3 148.7(6) . 4_454
O2 O2 O3 58.3(4) 6_554 4_454
Ga2 O2 O1 30.9(3) 2_565 1_554
Ga3 O2 O1 89.3(4) . 1_554
La O2 O1 122.4(6) . 1_554
O3 O2 O1 110.0(5) 5_455 1_554
O2 O2 O1 63.2(2) 3_565 1_554
O2 O2 O1 63.2(2) 4_455 1_554
La O2 O1 109.0(4) 4_455 1_554
O3 O2 O1 128.5(5) 2_455 1_554
O1 O2 O1 114.9(3) . 1_554
O2 O2 O1 73.9(4) 6_554 1_554
O3 O2 O1 62.7(3) 4_454 1_554
Ga2 O2 O3 133.1(7) 2_565 4_455
Ga3 O2 O3 94.3(5) . 4_455
La O2 O3 79.2(4) . 4_455
O3 O2 O3 49.2(4) 5_455 4_455
O2 O2 O3 121.0(2) 3_565 4_455
O2 O2 O3 93.9(5) 4_455 4_455
La O2 O3 44.3(3) 4_455 4_455
O3 O2 O3 61.5(5) 2_455 4_455
O1 O2 O3 59.8(3) . 4_455
O2 O2 O3 124.5(4) 6_554 4_455
O3 O2 O3 106.4(5) 4_454 4_455
O1 O2 O3 151.9(5) 1_554 4_455
Ga2 O2 Nb 149.6(8) 2_565 1_455
Ga3 O2 Nb 61.5(4) . 1_455
La O2 Nb 97.1(3) . 1_455
O3 O2 Nb 33.3(2) 5_455 1_455
O2 O2 Nb 153.7(2) 3_565 1_455
O2 O2 Nb 113.1(7) 4_455 1_455
La O2 Nb 64.5(3) 4_455 1_455
O3 O2 Nb 33.4(3) 2_455 1_455
O1 O2 Nb 92.7(4) . 1_455
O2 O2 Nb 95.0(3) 6_554 1_455
O3 O2 Nb 78.3(3) 4_454 1_455
O1 O2 Nb 139.7(4) 1_554 1_455
O3 O2 Nb 32.9(2) 4_455 1_455
Ga2 O2 Ga1 149.6(8) 2_565 1_455
Ga3 O2 Ga1 61.5(4) . 1_455
La O2 Ga1 97.1(3) . 1_455
O3 O2 Ga1 33.3(2) 5_455 1_455
O2 O2 Ga1 153.7(2) 3_565 1_455
O2 O2 Ga1 113.1(7) 4_455 1_455
La O2 Ga1 64.5(3) 4_455 1_455
O3 O2 Ga1 33.4(3) 2_455 1_455
O1 O2 Ga1 92.7(4) . 1_455
O2 O2 Ga1 95.0(3) 6_554 1_455
O3 O2 Ga1 78.3(3) 4_454 1_455
O1 O2 Ga1 139.7(4) 1_554 1_455
O3 O2 Ga1 32.9(2) 4_455 1_455
Nb O2 Ga1 0.0 1_455 1_455
Ga2 O2 O1 127.7(8) 2_565 2_455
Ga3 O2 O1 75.6(4) . 2_455
La O2 O1 45.2(3) . 2_455
O3 O2 O1 114.0(3) 5_455 2_455
O2 O2 O1 96.5(7) 3_565 2_455
O2 O2 O1 154.1(6) 4_455 2_455
La O2 O1 132.1(4) 4_455 2_455
O3 O2 O1 57.7(3) 2_455 2_455
O1 O2 O1 99.1(3) . 2_455
O2 O2 O1 56.5(4) 6_554 2_455
O3 O2 O1 109.3(4) 4_454 2_455
O1 O2 O1 118.4(5) 1_554 2_455
O3 O2 O1 89.4(4) 4_455 2_455
Nb O2 O1 82.7(2) 1_455 2_455
Ga1 O2 O1 82.7(2) 1_455 2_455
Ga2 O2 Ga2 111.6(7) 2_565 1_554
Ga3 O2 Ga2 60.0(4) . 1_554
La O2 Ga2 68.4(4) . 1_554
O3 O2 Ga2 117.3(3) 5_455 1_554
O2 O2 Ga2 96.4(7) 3_565 1_554
O2 O2 Ga2 151.3(6) 4_455 1_554
La O2 Ga2 157.6(4) 4_455 1_554
O3 O2 Ga2 62.7(3) 2_455 1_554
O1 O2 Ga2 124.2(4) . 1_554
O2 O2 Ga2 29.2(2) 6_554 1_554
O3 O2 Ga2 86.7(4) 4_454 1_554
O1 O2 Ga2 92.6(4) 1_554 1_554
O3 O2 Ga2 113.3(3) 4_455 1_554
Nb O2 Ga2 95.2(2) 1_455 1_554
Ga1 O2 Ga2 95.2(2) 1_455 1_554
O1 O2 Ga2 28.7(3) 2_455 1_554
Ga2 O2 O2 140.9(4) 2_565 6
Ga3 O2 O2 97.4(5) . 6
La O2 O2 38.8(3) . 6
O3 O2 O2 89.4(3) 5_455 6
O2 O2 O2 102.3(2) 3_565 6
O2 O2 O2 123.1(4) 4_455 6
La O2 O2 85.5(4) 4_455 6
O3 O2 O2 59.4(4) 2_455 6
O1 O2 O2 63.1(4) . 6
O2 O2 O2 99.6(6) 6_554 6
O3 O2 O2 130.2(3) 4_454 6
O1 O2 O2 160.3(4) 1_554 6
O3 O2 O2 46.3(3) 4_455 6
Nb O2 O2 58.32(18) 1_455 6
Ga1 O2 O2 58.32(18) 1_455 6
O1 O2 O2 46.8(3) 2_455 6
Ga2 O2 O2 75.1(4) 1_554 6
Ga2 O2 O3 80.4(6) 2_565 6
Ga3 O2 O3 114.3(7) . 6
La O2 O3 36.6(3) . 6
O3 O2 O3 161.8(5) 5_455 6
O2 O2 O3 46.5(6) 3_565 6
O2 O2 O3 106.2(6) 4_455 6
La O2 O3 130.0(4) 4_455 6
O3 O2 O3 107.9(5) 2_455 6
O1 O2 O3 78.0(3) . 6
O2 O2 O3 76.9(3) 6_554 6
O3 O2 O3 130.8(5) 4_454 6
O1 O2 O3 87.5(4) 1_554 6
O3 O2 O3 115.9(4) 4_455 6
Nb O2 O3 128.5(4) 1_455 6
Ga1 O2 O3 128.5(4) 1_455 6
O1 O2 O3 50.2(3) 2_455 6
Ga2 O2 O3 54.6(3) 1_554 6
O2 O2 O3 72.9(3) 6 6
Ga2 O2 La 64.4(4) 2_565 1_554
Ga3 O2 La 68.5(4) . 1_554
La O2 La 103.0(5) . 1_554
O3 O2 La 122.2(4) 5_455 1_554
O2 O2 La 75.5(3) 3_565 1_554
O2 O2 La 102.3(2) 4_455 1_554
La O2 La 147.9(3) 4_455 1_554
O3 O2 La 100.1(4) 2_455 1_554
O1 O2 La 136.5(4) . 1_554
O2 O2 La 37.3(3) 6_554 1_554
O3 O2 La 63.9(4) 4_454 1_554
O1 O2 La 39.9(2) 1_554 1_554
O3 O2 La 161.6(3) 4_455 1_554
Nb O2 La 129.7(3) 1_455 1_554
Ga1 O2 La 129.7(3) 1_455 1_554
O1 O2 La 80.0(4) 2_455 1_554
Ga2 O2 La 52.8(2) 1_554 1_554
O2 O2 La 126.6(5) 6 1_554
O3 O2 La 68.2(3) 6 1_554
Ga2 O2 Ga3 107.8(5) 2_565 2_464
Ga3 O2 Ga3 48.8(4) . 2_464
La O2 Ga3 144.6(4) . 2_464
O3 O2 Ga3 20.9(3) 5_455 2_464
O2 O2 Ga3 146.3(6) 3_565 2_464
O2 O2 Ga3 88.8(7) 4_455 2_464
La O2 Ga3 65.8(3) 4_455 2_464
O3 O2 Ga3 59.4(3) 2_455 2_464
O1 O2 Ga3 117.0(5) . 2_464
O2 O2 Ga3 86.8(2) 6_554 2_464
O3 O2 Ga3 37.6(3) 4_454 2_464
O1 O2 Ga3 92.6(3) 1_554 2_464
O3 O2 Ga3 69.7(3) 4_455 2_464
Nb O2 Ga3 47.48(18) 1_455 2_464
Ga1 O2 Ga3 47.48(18) 1_455 2_464
O1 O2 Ga3 116.2(3) 2_455 2_464
Ga2 O2 Ga3 108.5(3) 1_554 2_464
O2 O2 Ga3 105.80(14) 6 2_464
O3 O2 Ga3 163.1(4) 6 2_464
La O2 Ga3 101.5(2) 1_554 2_464
Ga2 O2 La 56.6(3) 2_565 4_454
Ga3 O2 La 68.4(3) . 4_454
La O2 La 158.9(5) . 4_454
O3 O2 La 73.8(4) 5_455 4_454
O2 O2 La 95.9(2) 3_565 4_454
O2 O2 La 64.7(4) 4_455 4_454
La O2 La 89.4(3) 4_455 4_454
O3 O2 La 104.0(4) 2_455 4_454
O1 O2 La 125.8(4) . 4_454
O2 O2 La 77.2(4) 6_554 4_454
O3 O2 La 33.3(2) 4_454 4_454
O1 O2 La 36.49(14) 1_554 4_454
O3 O2 La 120.8(4) 4_455 4_454
Nb O2 La 103.6(3) 1_455 4_454
Ga1 O2 La 103.6(3) 1_455 4_454
O1 O2 La 133.7(4) 2_455 4_454
Ga2 O2 La 105.5(3) 1_554 4_454
O2 O2 La 161.63(17) 6 4_454
O3 O2 La 123.0(4) 6 4_454
La O2 La 60.51(16) 1_554 4_454
Ga3 O2 La 56.22(16) 2_464 4_454
Ga2 O2 Ga3 44.0(4) 2_565 2_564
Ga3 O2 Ga3 125.1(7) . 2_564
La O2 Ga3 66.7(3) . 2_564
O3 O2 Ga3 161.0(4) 5_455 2_564
O2 O2 Ga3 19.7(3) 3_565 2_564
O2 O2 Ga3 75.1(4) 4_455 2_564
La O2 Ga3 118.2(3) 4_455 2_564
O3 O2 Ga3 140.6(6) 2_455 2_564
O1 O2 Ga3 78.9(3) . 2_564
O2 O2 Ga3 86.8(2) 6_554 2_564
O3 O2 Ga3 115.9(4) 4_454 2_564
O1 O2 Ga3 56.2(2) 1_554 2_564
O3 O2 Ga3 136.8(3) 4_455 2_564
Nb O2 Ga3 163.8(3) 1_455 2_564
Ga1 O2 Ga3 163.8(3) 1_455 2_564
O1 O2 Ga3 85.0(3) 2_455 2_564
Ga2 O2 Ga3 78.6(3) 1_554 2_564
O2 O2 Ga3 105.49(14) 6 2_564
O3 O2 Ga3 36.4(3) 6 2_564
La O2 Ga3 57.6(2) 1_554 2_564
Ga3 O2 Ga3 148.7(3) 2_464 2_564
La O2 Ga3 92.5(2) 4_454 2_564
Ga2 O2 O3 52.8(5) 2_565 1_554
Ga3 O2 O3 100.2(6) . 1_554
La O2 O3 77.0(5) . 1_554
O3 O2 O3 154.6(4) 5_455 1_554
O2 O2 O3 44.3(4) 3_565 1_554
O2 O2 O3 91.5(4) 4_455 1_554
La O2 O3 140.3(4) 4_455 1_554
O3 O2 O3 121.8(6) 2_455 1_554
O1 O2 O3 103.3(4) . 1_554
O2 O2 O3 62.4(2) 6_554 1_554
O3 O2 O3 96.4(5) 4_454 1_554
O1 O2 O3 48.0(3) 1_554 1_554
O3 O2 O3 156.0(4) 4_455 1_554
Nb O2 O3 155.1(4) 1_455 1_554
Ga1 O2 O3 155.1(4) 1_455 1_554
O1 O2 O3 76.1(4) 2_455 1_554
Ga2 O2 O3 60.0(3) 1_554 1_554
O2 O2 O3 112.3(3) 6 1_554
O3 O2 O3 40.5(4) 6 1_554
La O2 O3 33.8(2) 1_554 1_554
Ga3 O2 O3 133.8(3) 2_464 1_554
La O2 O3 82.5(3) 4_454 1_554
Ga3 O2 O3 24.94(16) 2_564 1_554
Ga2 O2 La 49.5(3) 2_565 2_565
Ga3 O2 La 168.7(4) . 2_565
La O2 La 69.8(2) . 2_565
O3 O2 La 116.9(5) 5_455 2_565
O2 O2 La 31.9(2) 3_565 2_565
O2 O2 La 41.1(3) 4_455 2_565
La O2 La 67.3(2) 4_455 2_565
O3 O2 La 151.2(5) 2_455 2_565
O1 O2 La 35.1(2) . 2_565
O2 O2 La 138.4(3) 6_554 2_565
O3 O2 La 133.2(3) 4_454 2_565
O1 O2 La 80.2(3) 1_554 2_565
O3 O2 La 92.9(3) 4_455 2_565
Nb O2 La 125.1(4) 1_455 2_565
Ga1 O2 La 125.1(4) 1_455 2_565
O1 O2 La 113.2(3) 2_455 2_565
Ga2 O2 La 124.3(4) 1_554 2_565
O2 O2 La 93.9(4) 6 2_565
O3 O2 La 69.8(3) 6 2_565
La O2 La 105.1(3) 1_554 2_565
Ga3 O2 La 126.9(4) 2_464 2_565
La O2 La 100.4(2) 4_454 2_565
Ga3 O2 La 51.59(13) 2_564 2_565
O3 O2 La 76.1(2) 1_554 2_565
Ga2 O2 Ga3 138.1(5) 2_565 1_556
Ga3 O2 Ga3 100.7(4) . 1_556
La O2 Ga3 57.3(2) . 1_556
O3 O2 Ga3 70.1(4) 5_455 1_556
O2 O2 Ga3 109.8(2) 3_565 1_556
O2 O2 Ga3 105.5(3) 4_455 1_556
La O2 Ga3 61.7(2) 4_455 1_556
O3 O2 Ga3 62.0(3) 2_455 1_556
O1 O2 Ga3 54.3(3) . 1_556
O2 O2 Ga3 117.7(5) 6_554 1_556
O3 O2 Ga3 123.4(4) 4_454 1_556
O1 O2 Ga3 168.3(4) 1_554 1_556
O3 O2 Ga3 22.5(2) 4_455 1_556
Nb O2 Ga3 45.08(14) 1_455 1_556
Ga1 O2 Ga3 45.08(14) 1_455 1_556
O1 O2 Ga3 70.4(3) 2_455 1_556
Ga2 O2 Ga3 97.6(2) 1_554 1_556
O2 O2 Ga3 24.55(19) 6 1_556
O3 O2 Ga3 93.8(3) 6 1_556
La O2 Ga3 150.3(4) 1_554 1_556
Ga3 O2 Ga3 89.6(3) 2_464 1_556
La O2 Ga3 143.2(4) 4_454 1_556
Ga3 O2 Ga3 120.3(3) 2_564 1_556
O3 O2 Ga3 134.2(4) 1_554 1_556
La O2 Ga3 89.3(2) 2_565 1_556
Ga2 O2 Ga3 37.3(4) 2_565 4_455
Ga3 O2 Ga3 116.1(5) . 4_455
La O2 Ga3 123.7(3) . 4_455
O3 O2 Ga3 82.2(4) 5_455 4_455
O2 O2 Ga3 67.2(4) 3_565 4_455
O2 O2 Ga3 14.2(3) 4_455 4_455
La O2 Ga3 56.3(2) 4_455 4_455
O3 O2 Ga3 138.6(5) 2_455 4_455
O1 O2 Ga3 75.4(3) . 4_455
O2 O2 Ga3 124.4(5) 6_554 4_455
O3 O2 Ga3 80.5(3) 4_454 4_455
O1 O2 Ga3 53.50(19) 1_554 4_455
O3 O2 Ga3 100.6(4) 4_455 4_455
Nb O2 Ga3 112.7(4) 1_455 4_455
Ga1 O2 Ga3 112.7(4) 1_455 4_455
O1 O2 Ga3 163.6(4) 2_455 4_455
Ga2 O2 Ga3 145.9(4) 1_554 4_455
O2 O2 Ga3 136.0(6) 6 4_455
O3 O2 Ga3 113.4(3) 6 4_455
La O2 Ga3 93.4(2) 1_554 4_455
Ga3 O2 Ga3 79.7(2) 2_464 4_455
La O2 Ga3 50.57(12) 4_454 4_455
Ga3 O2 Ga3 78.83(17) 2_564 4_455
O3 O2 Ga3 90.0(3) 1_554 4_455
La O2 Ga3 53.84(13) 2_565 4_455
Ga3 O2 Ga3 115.8(4) 1_556 4_455
Ga2 O2 O3 120.2(5) 2_565 3_454
Ga3 O2 O3 1.7(3) . 3_454
La O2 O3 118.6(4) . 3_454
O3 O2 O3 64.0(3) 5_455 3_454
O2 O2 O3 143.1(5) 3_565 3_454
O2 O2 O3 131.1(6) 4_455 3_454
La O2 O3 114.2(4) 4_455 3_454
O3 O2 O3 38.9(4) 2_455 3_454
O1 O2 O3 154.2(5) . 3_454
O2 O2 O3 38.5(3) 6_554 3_454
O3 O2 O3 37.2(3) 4_454 3_454
O1 O2 O3 89.6(3) 1_554 3_454
O3 O2 O3 94.8(3) 4_455 3_454
Nb O2 O3 62.0(2) 1_455 3_454
Ga1 O2 O3 62.0(2) 1_455 3_454
O1 O2 O3 74.0(3) 2_455 3_454
Ga2 O2 O3 58.4(2) 1_554 3_454
O2 O2 O3 96.6(4) 6 3_454
O3 O2 O3 112.7(4) 6 3_454
La O2 O3 67.9(2) 1_554 3_454
Ga3 O2 O3 50.37(19) 2_464 3_454
La O2 O3 69.5(2) 4_454 3_454
Ga3 O2 O3 124.1(4) 2_564 3_454
O3 O2 O3 99.2(4) 1_554 3_454
La O2 O3 169.5(3) 2_565 3_454
Ga3 O2 O3 100.5(3) 1_556 3_454
Ga3 O2 O3 117.5(3) 4_455 3_454
Ga2 O2 Ga2 96.8(4) 2_565 2_566
Ga3 O2 Ga2 141.9(5) . 2_566
La O2 Ga2 51.6(2) . 2_566
O3 O2 Ga2 92.4(4) 5_455 2_566
O2 O2 Ga2 71.98(11) 3_565 2_566
O2 O2 Ga2 71.98(11) 4_455 2_566
La O2 Ga2 52.05(19) 4_455 2_566
O3 O2 Ga2 103.6(4) 2_455 2_566
O1 O2 Ga2 12.71(19) . 2_566
O2 O2 Ga2 147.7(5) 6_554 2_566
O3 O2 Ga2 149.0(6) 4_454 2_566
O1 O2 Ga2 127.6(3) 1_554 2_566
O3 O2 Ga2 49.2(2) 4_455 2_566
Nb O2 Ga2 81.7(3) 1_455 2_566
Ga1 O2 Ga2 81.7(3) 1_455 2_566
O1 O2 Ga2 91.3(3) 2_455 2_566
Ga2 O2 Ga2 118.7(3) 1_554 2_566
O2 O2 Ga2 51.4(4) 6 2_566
O3 O2 Ga2 80.2(3) 6 2_566
La O2 Ga2 145.0(4) 1_554 2_566
Ga3 O2 Ga2 112.7(4) 2_464 2_566
La O2 Ga2 134.9(3) 4_454 2_566
Ga3 O2 Ga2 88.1(2) 2_564 2_566
O3 O2 Ga2 111.3(3) 1_554 2_566
La O2 Ga2 47.69(12) 2_565 2_566
Ga3 O2 Ga2 41.62(11) 1_556 2_566
Ga3 O2 Ga2 85.6(2) 4_455 2_566
O3 O2 Ga2 142.0(3) 3_454 2_566
Ga2 O2 O3 87.5(4) 2_565 .
Ga3 O2 O3 138.9(6) . .
La O2 O3 19.8(2) . .
O3 O2 O3 134.6(4) 5_455 .
O2 O2 O3 48.0(4) 3_565 .
O2 O2 O3 91.4(4) 4_455 .
La O2 O3 95.8(3) 4_455 .
O3 O2 O3 110.6(4) 2_455 .
O1 O2 O3 43.97(19) . .
O2 O2 O3 109.4(4) 6_554 .
O3 O2 O3 166.1(6) 4_454 .
O1 O2 O3 109.4(4) 1_554 .
O3 O2 O3 85.7(3) 4_455 .
Nb O2 O3 110.9(3) 1_455 .
Ga1 O2 O3 110.9(3) 1_455 .
O1 O2 O3 63.2(3) 2_455 .
Ga2 O2 O3 82.2(3) 1_554 .
O2 O2 O3 54.4(3) 6 .
O3 O2 O3 35.3(3) 6 .
La O2 O3 102.5(4) 1_554 .
Ga3 O2 O3 155.4(4) 2_464 .
La O2 O3 143.8(3) 4_454 .
Ga3 O2 O3 53.7(2) 2_564 .
O3 O2 O3 70.8(3) 1_554 .
La O2 O3 50.4(2) 2_565 .
Ga3 O2 O3 66.7(2) 1_556 .
Ga3 O2 O3 104.2(3) 4_455 .
O3 O2 O3 137.3(4) 3_454 .
Ga2 O2 O3 44.85(15) 2_566 .
Ga2 O2 O2 89.4(8) 2_565 5_444
Ga3 O2 O2 75.5(5) . 5_444
La O2 O2 67.7(3) . 5_444
O3 O2 O2 137.4(5) 5_455 5_444
O2 O2 O2 75.2(7) 3_565 5_444
O2 O2 O2 128.6(7) 4_455 5_444
La O2 O2 170.4(5) 4_455 5_444
O3 O2 O2 85.5(4) 2_455 5_444
O1 O2 O2 118.3(4) . 5_444
O2 O2 O2 36.5(3) 6_554 5_444
O3 O2 O2 92.0(5) 4_454 5_444
O1 O2 O2 75.3(5) 1_554 5_444
O3 O2 O2 132.5(4) 4_455 5_444
Nb O2 O2 118.2(3) 1_455 5_444
Ga1 O2 O2 118.2(3) 1_455 5_444
O1 O2 O2 43.2(2) 2_455 5_444
Ga2 O2 O2 22.92(10) 1_554 5_444
O2 O2 O2 88.4(3) 6 5_444
O3 O2 O2 40.6(2) 6 5_444
La O2 O2 38.6(4) 1_554 5_444
Ga3 O2 O2 123.3(4) 2_464 5_444
La O2 O2 98.6(5) 4_454 5_444
Ga3 O2 O2 56.5(4) 2_564 5_444
O3 O2 O2 37.1(4) 1_554 5_444
La O2 O2 105.7(4) 2_565 5_444
Ga3 O2 O2 112.9(2) 1_556 5_444
Ga3 O2 O2 125.8(5) 4_455 5_444
O3 O2 O2 74.0(3) 3_454 5_444
Ga2 O2 O2 118.4(3) 2_566 5_444
O3 O2 O2 74.6(3) . 5_444
Ga2 O2 O2 51.4(4) 2_565 5_454
Ga3 O2 O2 92.6(5) . 5_454
La O2 O2 147.3(5) . 5_454
O3 O2 O2 66.0(4) 5_455 5_454
O2 O2 O2 88.1(4) 3_565 5_454
O2 O2 O2 37.0(4) 4_455 5_454
La O2 O2 60.0(2) 4_455 5_454
O3 O2 O2 117.4(5) 2_455 5_454
O1 O2 O2 95.2(4) . 5_454
O2 O2 O2 109.0(6) 6_554 5_454
O3 O2 O2 57.6(4) 4_454 5_454
O1 O2 O2 52.0(3) 1_554 5_454
O3 O2 O2 100.0(4) 4_455 5_454
Nb O2 O2 99.2(4) 1_455 5_454
Ga1 O2 O2 99.2(4) 1_455 5_454
O1 O2 O2 165.5(5) 2_455 5_454
Ga2 O2 O2 137.2(4) 1_554 5_454
O2 O2 O2 145.3(6) 6 5_454
O3 O2 O2 131.8(5) 6 5_454
La O2 O2 88.0(3) 1_554 5_454
Ga3 O2 O2 58.2(3) 2_464 5_454
La O2 O2 31.9(2) 4_454 5_454
Ga3 O2 O2 95.4(3) 2_564 5_454
O3 O2 O2 98.3(4) 1_554 5_454
La O2 O2 77.6(3) 2_565 5_454
Ga3 O2 O2 120.8(4) 1_556 5_454
Ga3 O2 O2 23.78(14) 4_455 5_454
O3 O2 O2 94.1(4) 3_454 5_454
Ga2 O2 O2 103.2(3) 2_566 5_454
O3 O2 O2 128.0(4) . 5_454
O2 O2 O2 126.3(6) 5_444 5_454
Ga2 O2 La 160.9(8) 2_565 2_455
Ga3 O2 La 59.7(3) . 2_455
La O2 La 64.7(2) . 2_455
O3 O2 La 80.3(3) 5_455 2_455
O2 O2 La 127.7(7) 3_565 2_455
O2 O2 La 157.2(4) 4_455 2_455
La O2 La 107.4(3) 4_455 2_455
O3 O2 La 27.0(2) 2_455 2_455
O1 O2 La 101.7(3) . 2_455
O2 O2 La 65.4(4) 6_554 2_455
O3 O2 La 94.9(3) 4_454 2_455
O1 O2 La 139.2(4) 1_554 2_455
O3 O2 La 63.5(3) 4_455 2_455
Nb O2 La 49.11(12) 1_455 2_455
Ga1 O2 La 49.11(12) 1_455 2_455
O1 O2 La 33.82(12) 2_455 2_455
Ga2 O2 La 50.20(14) 1_554 2_455
O2 O2 La 38.7(3) 6 2_455
O3 O2 La 83.0(3) 6 2_455
La O2 La 100.6(3) 1_554 2_455
Ga3 O2 La 86.0(2) 2_464 2_455
La O2 La 128.0(2) 4_454 2_455
Ga3 O2 La 118.7(4) 2_564 2_455
O3 O2 La 108.1(4) 1_554 2_455
La O2 La 131.5(2) 2_565 2_455
Ga3 O2 La 52.36(11) 1_556 2_455
Ga3 O2 La 161.7(4) 4_455 2_455
O3 O2 La 58.67(19) 3_454 2_455
Ga2 O2 La 89.60(18) 2_566 2_455
O3 O2 La 84.4(3) . 2_455
O2 O2 La 71.80(18) 5_444 2_455
O2 O2 La 144.2(4) 5_454 2_455
Ga2 O2 O2 84.7(4) 2_565 2_464
Ga3 O2 O2 62.2(4) . 2_464
La O2 O2 163.5(7) . 2_464
O3 O2 O2 37.2(4) 5_455 2_464
O2 O2 O2 123.3(4) 3_565 2_464
O2 O2 O2 69.3(6) 4_455 2_464
La O2 O2 63.2(4) 4_455 2_464
O3 O2 O2 82.0(4) 2_455 2_464
O1 O2 O2 114.0(6) . 2_464
O2 O2 O2 92.9(4) 6_554 2_464
O3 O2 O2 34.7(3) 4_454 2_464
O1 O2 O2 72.9(3) 1_554 2_464
O3 O2 O2 84.3(5) 4_455 2_464
Nb O2 O2 69.0(4) 1_455 2_464
Ga1 O2 O2 69.0(4) 1_455 2_464
O1 O2 O2 136.59(19) 2_455 2_464
Ga2 O2 O2 120.3(3) 1_554 2_464
O2 O2 O2 126.6(4) 6 2_464
O3 O2 O2 159.8(5) 6 2_464
La O2 O2 93.1(3) 1_554 2_464
Ga3 O2 O2 23.20(18) 2_464 2_464
La O2 O2 36.94(18) 4_454 2_464
Ga3 O2 O2 127.0(3) 2_564 2_464
O3 O2 O2 119.4(4) 1_554 2_464
La O2 O2 110.0(3) 2_565 2_464
Ga3 O2 O2 106.4(5) 1_556 2_464
Ga3 O2 O2 58.19(16) 4_455 2_464
O3 O2 O2 63.9(2) 3_454 2_464
Ga2 O2 O2 115.3(5) 2_566 2_464
O3 O2 O2 157.5(5) . 2_464
O2 O2 O2 126.3(5) 5_444 2_464
O2 O2 O2 35.5(3) 5_454 2_464
La O2 O2 108.8(2) 2_455 2_464
Ga2 O2 O3 167.9(7) 2_565 3_455
Ga3 O2 O3 68.3(4) . 3_455
La O2 O3 75.1(3) . 3_455
O3 O2 O3 56.6(4) 5_455 3_455
O2 O2 O3 138.8(4) 3_565 3_455
O2 O2 O3 128.1(6) 4_455 3_455
La O2 O3 77.6(3) 4_455 3_455
O3 O2 O3 29.7(4) 2_455 3_455
O1 O2 O3 86.6(4) . 3_455
O2 O2 O3 90.3(4) 6_554 3_455
O3 O2 O3 95.2(3) 4_454 3_455
O1 O2 O3 157.2(4) 1_554 3_455
O3 O2 O3 34.8(3) 4_455 3_455
Nb O2 O3 23.34(16) 1_455 3_455
Ga1 O2 O3 23.34(16) 1_455 3_455
O1 O2 O3 61.6(2) 2_455 3_455
Ga2 O2 O3 80.1(2) 1_554 3_455
O2 O2 O3 36.8(3) 6 3_455
O3 O2 O3 105.2(3) 6 3_455
La O2 O3 127.5(3) 1_554 3_455
Ga3 O2 O3 69.8(3) 2_464 3_455
La O2 O3 124.8(4) 4_454 3_455
Ga3 O2 O3 140.9(3) 2_564 3_455
O3 O2 O3 137.5(5) 1_554 3_455
La O2 O3 121.7(3) 2_565 3_455
Ga3 O2 O3 32.44(18) 1_556 3_455
Ga3 O2 O3 132.2(4) 4_455 3_455
O3 O2 O3 68.1(2) 3_454 3_455
Ga2 O2 O3 74.0(2) 2_566 3_455
O3 O2 O3 91.2(4) . 3_455
O2 O2 O3 101.9(3) 5_444 3_455
O2 O2 O3 122.2(5) 5_454 3_455
La O2 O3 30.08(14) 2_455 3_455
O2 O2 O3 92.1(4) 2_464 3_455
Ga2 O2 O1 82.9(5) 2_565 2_465
Ga3 O2 O1 95.4(6) . 2_465
La O2 O1 128.8(5) . 2_465
O3 O2 O1 39.2(3) 5_455 2_465
O2 O2 O1 107.1(6) 3_565 2_465
O2 O2 O1 47.9(5) 4_455 2_465
La O2 O1 25.7(2) 4_455 2_465
O3 O2 O1 96.3(4) 2_455 2_465
O1 O2 O1 75.8(4) . 2_465
O2 O2 O1 130.9(3) 6_554 2_465
O3 O2 O1 73.0(4) 4_454 2_465
O1 O2 O1 90.8(3) 1_554 2_465
O3 O2 O1 61.1(4) 4_455 2_465
Nb O2 O1 67.0(3) 1_455 2_465
Ga1 O2 O1 67.0(3) 1_455 2_465
O1 O2 O1 148.8(5) 2_455 2_465
Ga2 O2 O1 155.1(3) 1_554 2_465
O2 O2 O1 106.9(4) 6 2_465
O3 O2 O1 150.2(3) 6 2_465
La O2 O1 125.1(3) 1_554 2_465
Ga3 O2 O1 46.74(19) 2_464 2_465
La O2 O1 64.7(3) 4_454 2_465
Ga3 O2 O1 123.0(2) 2_564 2_465
O3 O2 O1 135.1(3) 1_554 2_465
La O2 O1 80.5(2) 2_565 2_465
Ga3 O2 O1 82.4(3) 1_556 2_465
Ga3 O2 O1 45.67(17) 4_455 2_465
O3 O2 O1 97.0(3) 3_454 2_465
Ga2 O2 O1 77.5(3) 2_566 2_465
O3 O2 O1 119.7(4) . 2_465
O2 O2 O1 163.2(4) 5_444 2_465
O2 O2 O1 38.8(2) 5_454 2_465
La O2 O1 116.1(3) 2_455 2_465
O2 O2 O1 38.3(3) 2_464 2_465
O3 O2 O1 87.3(3) 3_455 2_465
Ga2 O2 Nb 98.9(4) 2_565 1_454
Ga3 O2 Nb 23.3(2) . 1_454
La O2 Nb 142.0(4) . 1_454
O3 O2 Nb 60.4(3) 5_455 1_454
O2 O2 Nb 132.46(13) 3_565 1_454
O2 O2 Nb 107.2(5) 4_455 1_454
La O2 Nb 105.3(4) 4_455 1_454
O3 O2 Nb 60.4(3) 2_455 1_454
O1 O2 Nb 157.4(5) . 1_454
O2 O2 Nb 48.6(2) 6_554 1_454
O3 O2 Nb 12.8(2) 4_454 1_454
O1 O2 Nb 70.4(2) 1_554 1_454
O3 O2 Nb 104.5(3) 4_455 1_454
Nb O2 Nb 73.43(19) 1_455 1_454
Ga1 O2 Nb 73.43(19) 1_455 1_454
O1 O2 Nb 96.8(3) 2_455 1_454
Ga2 O2 Nb 75.7(2) 1_554 1_454
O2 O2 Nb 119.7(3) 6 1_454
O3 O2 Nb 124.6(4) 6 1_454
La O2 Nb 62.37(16) 1_554 1_454
Ga3 O2 Nb 40.74(10) 2_464 1_454
La O2 Nb 45.16(10) 4_454 1_454
Ga3 O2 Nb 118.6(3) 2_564 1_454
O3 O2 Nb 96.1(3) 1_554 1_454
La O2 Nb 145.5(2) 2_565 1_454
Ga3 O2 Nb 117.7(3) 1_556 1_454
Ga3 O2 Nb 93.3(2) 4_455 1_454
O3 O2 Nb 24.55(14) 3_454 1_454
Ga2 O2 Nb 152.6(4) 2_566 1_454
O3 O2 Nb 157.8(4) . 1_454
O2 O2 Nb 84.2(4) 5_444 1_454
O2 O2 Nb 70.3(3) 5_454 1_454
La O2 Nb 82.89(17) 2_455 1_454
O2 O2 Nb 44.69(15) 2_464 1_454
O3 O2 Nb 86.9(3) 3_455 1_454
O1 O2 Nb 82.3(2) 2_465 1_454
Ga2 O2 Ga1 98.9(4) 2_565 1_454
Ga3 O2 Ga1 23.3(2) . 1_454
La O2 Ga1 142.0(4) . 1_454
O3 O2 Ga1 60.4(3) 5_455 1_454
O2 O2 Ga1 132.46(13) 3_565 1_454
O2 O2 Ga1 107.2(5) 4_455 1_454
La O2 Ga1 105.3(4) 4_455 1_454
O3 O2 Ga1 60.4(3) 2_455 1_454
O1 O2 Ga1 157.4(5) . 1_454
O2 O2 Ga1 48.6(2) 6_554 1_454
O3 O2 Ga1 12.8(2) 4_454 1_454
O1 O2 Ga1 70.4(2) 1_554 1_454
O3 O2 Ga1 104.5(3) 4_455 1_454
Nb O2 Ga1 73.43(19) 1_455 1_454
Ga1 O2 Ga1 73.43(19) 1_455 1_454
O1 O2 Ga1 96.8(3) 2_455 1_454
Ga2 O2 Ga1 75.7(2) 1_554 1_454
O2 O2 Ga1 119.7(3) 6 1_454
O3 O2 Ga1 124.6(4) 6 1_454
La O2 Ga1 62.37(16) 1_554 1_454
Ga3 O2 Ga1 40.74(10) 2_464 1_454
La O2 Ga1 45.16(10) 4_454 1_454
Ga3 O2 Ga1 118.6(3) 2_564 1_454
O3 O2 Ga1 96.1(3) 1_554 1_454
La O2 Ga1 145.5(2) 2_565 1_454
Ga3 O2 Ga1 117.7(3) 1_556 1_454
Ga3 O2 Ga1 93.3(2) 4_455 1_454
O3 O2 Ga1 24.55(14) 3_454 1_454
Ga2 O2 Ga1 152.6(4) 2_566 1_454
O3 O2 Ga1 157.8(4) . 1_454
O2 O2 Ga1 84.2(4) 5_444 1_454
O2 O2 Ga1 70.3(3) 5_454 1_454
La O2 Ga1 82.89(17) 2_455 1_454
O2 O2 Ga1 44.69(15) 2_464 1_454
O3 O2 Ga1 86.9(3) 3_455 1_454
O1 O2 Ga1 82.3(2) 2_465 1_454
Nb O2 Ga1 0.0 1_454 1_454
Ga2 O2 O3 139.8(6) 2_565 6_455
Ga3 O2 O3 41.9(4) . 6_455
La O2 O3 114.1(4) . 6_455
O3 O2 O3 28.8(3) 5_455 6_455
O2 O2 O3 173.9(6) 3_565 6_455
O2 O2 O3 115.6(7) 4_455 6_455
La O2 O3 75.3(3) 4_455 6_455
O3 O2 O3 29.2(3) 2_455 6_455
O1 O2 O3 113.2(4) . 6_455
O2 O2 O3 79.6(2) 6_554 6_455
O3 O2 O3 57.1(4) 4_454 6_455
O1 O2 O3 119.5(4) 1_554 6_455
O3 O2 O3 53.8(3) 4_455 6_455
Nb O2 O3 21.75(16) 1_455 6_455
Ga1 O2 O3 21.75(16) 1_455 6_455
O1 O2 O3 86.8(3) 2_455 6_455
Ga2 O2 O3 89.0(2) 1_554 6_455
O2 O2 O3 76.3(2) 6 6_455
O3 O2 O3 137.0(4) 6 6_455
La O2 O3 110.2(3) 1_554 6_455
Ga3 O2 O3 32.05(19) 2_464 6_455
La O2 O3 85.3(3) 4_454 6_455
Ga3 O2 O3 166.4(4) 2_564 6_455
O3 O2 O3 141.7(3) 1_554 6_455
La O2 O3 142.0(4) 2_565 6_455
Ga3 O2 O3 66.6(2) 1_556 6_455
Ga3 O2 O3 109.6(3) 4_455 6_455
O3 O2 O3 42.7(3) 3_454 6_455
Ga2 O2 O3 103.0(3) 2_566 6_455
O3 O2 O3 130.6(2) . 6_455
O2 O2 O3 110.5(3) 5_444 6_455
O2 O2 O3 89.8(4) 5_454 6_455
La O2 O3 54.5(2) 2_455 6_455
O2 O2 O3 55.2(3) 2_464 6_455
O3 O2 O3 39.5(4) 3_455 6_455
O1 O2 O3 68.0(2) 2_465 6_455
Nb O2 O3 51.67(18) 1_454 6_455
Ga1 O2 O3 51.67(18) 1_454 6_455
Ga2 O2 Ga2 72.9(4) 2_565 1_564
Ga3 O2 Ga2 84.2(5) . 1_564
La O2 Ga2 149.2(5) . 1_564
O3 O2 Ga2 44.2(3) 5_455 1_564
O2 O2 Ga2 106.8(5) 3_565 1_564
O2 O2 Ga2 48.6(6) 4_455 1_564
La O2 Ga2 46.8(2) 4_455 1_564
O3 O2 Ga2 99.0(4) 2_455 1_564
O1 O2 Ga2 93.8(4) . 1_564
O2 O2 Ga2 113.1(3) 6_554 1_564
O3 O2 Ga2 55.0(3) 4_454 1_564
O1 O2 Ga2 72.4(2) 1_554 1_564
O3 O2 Ga2 80.3(4) 4_455 1_564
Nb O2 Ga2 77.2(3) 1_455 1_564
Ga1 O2 Ga2 77.2(3) 1_455 1_564
O1 O2 Ga2 156.5(3) 2_455 1_564
Ga2 O2 Ga2 141.7(3) 1_554 1_564
O2 O2 Ga2 126.6(4) 6 1_564
O3 O2 Ga2 152.8(3) 6 1_564
La O2 Ga2 103.8(2) 1_554 1_564
Ga3 O2 Ga2 40.36(14) 2_464 1_564
La O2 Ga2 43.28(13) 4_454 1_564
Ga3 O2 Ga2 116.9(2) 2_564 1_564
O3 O2 Ga2 119.9(3) 1_554 1_564
La O2 Ga2 88.5(2) 2_565 1_564
Ga3 O2 Ga2 102.4(3) 1_556 1_564
Ga3 O2 Ga2 39.67(12) 4_455 1_564
O3 O2 Ga2 85.8(3) 3_454 1_564
Ga2 O2 Ga2 97.6(3) 2_566 1_564
O3 O2 Ga2 135.8(3) . 1_564
O2 O2 Ga2 141.7(4) 5_444 1_564
O2 O2 Ga2 22.11(15) 5_454 1_564
La O2 Ga2 124.2(3) 2_455 1_564
O2 O2 Ga2 22.01(16) 2_464 1_564
O3 O2 Ga2 100.1(3) 3_455 1_564
O1 O2 Ga2 21.49(19) 2_465 1_564
Nb O2 Ga2 66.09(16) 1_454 1_564
Ga1 O2 Ga2 66.09(16) 1_454 1_564
O3 O2 Ga2 70.0(3) 6_455 1_564
Ga2 O2 Ga3 136.7(4) 2_565 4_345
Ga3 O2 Ga3 21.4(3) . 4_345
La O2 Ga3 114.0(3) . 4_345
O3 O2 Ga3 47.5(2) 5_455 4_345
O2 O2 Ga3 164.3(6) 3_565 4_345
O2 O2 Ga3 129.8(7) 4_455 4_345
La O2 Ga3 96.5(4) 4_455 4_345
O3 O2 Ga3 23.3(3) 2_455 4_345
O1 O2 Ga3 132.6(4) . 4_345
O2 O2 Ga3 57.8(2) 6_554 4_345
O3 O2 Ga3 47.9(2) 4_454 4_345
O1 O2 Ga3 108.3(3) 1_554 4_345
O3 O2 Ga3 73.0(3) 4_455 4_345
Nb O2 Ga3 40.14(11) 1_455 4_345
Ga1 O2 Ga3 40.14(11) 1_455 4_345
O1 O2 Ga3 75.59(19) 2_455 4_345
Ga2 O2 Ga3 70.15(17) 1_554 4_345
O2 O2 Ga3 82.3(3) 6 4_345
O3 O2 Ga3 123.3(4) 6 4_345
La O2 Ga3 89.7(2) 1_554 4_345
Ga3 O2 Ga3 41.01(11) 2_464 4_345
La O2 Ga3 80.75(18) 4_454 4_345
Ga3 O2 Ga3 144.7(4) 2_564 4_345
O3 O2 Ga3 120.1(4) 1_554 4_345
La O2 Ga3 163.7(4) 2_565 4_345
Ga3 O2 Ga3 80.67(19) 1_556 4_345
Ga3 O2 Ga3 119.7(3) 4_455 4_345
O3 O2 Ga3 21.88(15) 3_454 4_345
Ga2 O2 Ga3 121.0(3) 2_566 4_345
O3 O2 Ga3 133.7(3) . 4_345
O2 O2 Ga3 90.1(3) 5_444 4_345
O2 O2 Ga3 96.5(3) 5_454 4_345
La O2 Ga3 49.34(10) 2_455 4_345
O2 O2 Ga3 61.47(16) 2_464 4_345
O3 O2 Ga3 48.9(2) 3_455 4_345
O1 O2 Ga3 85.4(2) 2_465 4_345
Nb O2 Ga3 38.13(8) 1_454 4_345
Ga1 O2 Ga3 38.13(8) 1_454 4_345
O3 O2 Ga3 21.72(14) 6_455 4_345
Ga2 O2 Ga3 81.2(2) 1_564 4_345
Ga2 O2 Ga3 81.3(5) 2_565 4_445
Ga3 O2 Ga3 97.1(6) . 4_445
La O2 Ga3 51.9(3) . 4_445
O3 O2 Ga3 157.1(4) 5_455 4_445
O2 O2 Ga3 56.7(6) 3_565 4_445
O2 O2 Ga3 115.5(6) 4_455 4_445
La O2 Ga3 149.1(3) 4_455 4_445
O3 O2 Ga3 100.3(4) 2_455 4_445
O1 O2 Ga3 97.2(3) . 4_445
O2 O2 Ga3 58.33(15) 6_554 4_445
O3 O2 Ga3 111.9(5) 4_454 4_445
O1 O2 Ga3 78.3(3) 1_554 4_445
O3 O2 Ga3 128.5(3) 4_455 4_445
Nb O2 Ga3 129.0(3) 1_455 4_445
Ga1 O2 Ga3 129.0(3) 1_455 4_445
O1 O2 Ga3 46.4(2) 2_455 4_445
Ga2 O2 Ga3 39.80(18) 1_554 4_445
O2 O2 Ga3 82.4(2) 6 4_445
O3 O2 Ga3 19.19(17) 6 4_445
La O2 Ga3 51.1(2) 1_554 4_445
Ga3 O2 Ga3 145.1(3) 2_464 4_445
La O2 Ga3 110.1(3) 4_454 4_445
Ga3 O2 Ga3 40.36(15) 2_564 4_445
O3 O2 Ga3 30.9(2) 1_554 4_445
La O2 Ga3 85.1(2) 2_565 4_445
Ga3 O2 Ga3 106.1(2) 1_556 4_445
Ga3 O2 Ga3 118.2(3) 4_455 4_445
O3 O2 Ga3 95.5(3) 3_454 4_445
Ga2 O2 Ga3 99.1(2) 2_566 4_445
O3 O2 Ga3 54.3(2) . 4_445
O2 O2 Ga3 21.84(16) 5_444 4_445
O2 O2 Ga3 129.2(4) 5_454 4_445
La O2 Ga3 79.9(2) 2_455 4_445
O2 O2 Ga3 144.2(5) 2_464 4_445
O3 O2 Ga3 107.6(3) 3_455 4_445
O1 O2 Ga3 163.3(2) 2_465 4_445
Nb O2 Ga3 105.4(3) 1_454 4_445
Ga1 O2 Ga3 105.4(3) 1_454 4_445
O3 O2 Ga3 128.4(3) 6_455 4_445
Ga2 O2 Ga3 150.7(3) 1_564 4_445
Ga3 O2 Ga3 109.9(3) 4_345 4_445
Ga2 O2 O2 62.3(4) 2_565 1_554
Ga3 O2 O2 58.4(4) . 1_554
La O2 O2 130.6(4) . 1_554
O3 O2 O2 97.3(3) 5_455 1_554
O2 O2 O2 90.001(1) 3_565 1_554
O2 O2 O2 90.000(2) 4_455 1_554
La O2 O2 123.5(2) 4_455 1_554
O3 O2 O2 97.2(4) 2_455 1_554
O1 O2 O2 146.4(3) . 1_554
O2 O2 O2 47.0(4) 6_554 1_554
O3 O2 O2 39.5(4) 4_454 1_554
O1 O2 O2 31.4(3) 1_554 1_554
O3 O2 O2 145.9(2) 4_455 1_554
Nb O2 O2 116.02(17) 1_455 1_554
Ga1 O2 O2 116.02(17) 1_455 1_554
O1 O2 O2 101.5(3) 2_455 1_554
Ga2 O2 O2 72.80(16) 1_554 1_554
O2 O2 O2 146.6(4) 6 1_554
O3 O2 O2 95.3(3) 6 1_554
La O2 O2 27.6(2) 1_554 1_554
Ga3 O2 O2 76.51(18) 2_464 1_554
La O2 O2 34.1(2) 4_454 1_554
Ga3 O2 O2 76.77(15) 2_564 1_554
O3 O2 O2 57.3(2) 1_554 1_554
La O2 O2 111.51(16) 2_565 1_554
Ga3 O2 O2 159.09(14) 1_556 1_554
Ga3 O2 O2 77.40(17) 4_455 1_554
O3 O2 O2 58.6(2) 3_454 1_554
Ga2 O2 O2 159.07(13) 2_566 1_554
O3 O2 O2 128.1(2) . 1_554
O2 O2 O2 64.7(3) 5_444 1_554
O2 O2 O2 64.7(3) 5_454 1_554
La O2 O2 110.26(16) 2_455 1_554
O2 O2 O2 65.5(4) 2_464 1_554
O3 O2 O2 126.7(2) 3_455 1_554
O1 O2 O2 98.6(2) 2_465 1_554
Nb O2 O2 42.59(17) 1_454 1_554
Ga1 O2 O2 42.59(17) 1_454 1_554
O3 O2 O2 94.3(2) 6_455 1_554
Ga2 O2 O2 77.10(16) 1_564 1_554
Ga3 O2 O2 78.59(14) 4_345 1_554
Ga3 O2 O2 78.75(12) 4_445 1_554
Ga2 O2 O2 117.7(4) 2_565 1_556
Ga3 O2 O2 121.6(4) . 1_556
La O2 O2 49.4(4) . 1_556
O3 O2 O2 82.7(3) 5_455 1_556
O2 O2 O2 90.000(1) 3_565 1_556
O2 O2 O2 89.999(2) 4_455 1_556
La O2 O2 56.5(2) 4_455 1_556
O3 O2 O2 82.8(4) 2_455 1_556
O1 O2 O2 33.6(3) . 1_556
O2 O2 O2 133.0(4) 6_554 1_556
O3 O2 O2 140.5(4) 4_454 1_556
O1 O2 O2 148.6(3) 1_554 1_556
O3 O2 O2 34.1(2) 4_455 1_556
Nb O2 O2 63.98(17) 1_455 1_556
Ga1 O2 O2 63.98(17) 1_455 1_556
O1 O2 O2 78.5(3) 2_455 1_556
Ga2 O2 O2 107.20(16) 1_554 1_556
O2 O2 O2 33.4(4) 6 1_556
O3 O2 O2 84.7(3) 6 1_556
La O2 O2 152.4(2) 1_554 1_556
Ga3 O2 O2 103.49(18) 2_464 1_556
La O2 O2 145.9(2) 4_454 1_556
Ga3 O2 O2 103.23(15) 2_564 1_556
O3 O2 O2 122.7(2) 1_554 1_556
La O2 O2 68.49(16) 2_565 1_556
Ga3 O2 O2 20.91(14) 1_556 1_556
Ga3 O2 O2 102.60(17) 4_455 1_556
O3 O2 O2 121.4(2) 3_454 1_556
Ga2 O2 O2 20.93(13) 2_566 1_556
O3 O2 O2 51.9(2) . 1_556
O2 O2 O2 115.3(3) 5_444 1_556
O2 O2 O2 115.3(3) 5_454 1_556
La O2 O2 69.74(16) 2_455 1_556
O2 O2 O2 114.5(4) 2_464 1_556
O3 O2 O2 53.3(2) 3_455 1_556
O1 O2 O2 81.4(2) 2_465 1_556
Nb O2 O2 137.41(17) 1_454 1_556
Ga1 O2 O2 137.41(17) 1_454 1_556
O3 O2 O2 85.7(2) 6_455 1_556
Ga2 O2 O2 102.90(16) 1_564 1_556
Ga3 O2 O2 101.40(14) 4_345 1_556
Ga3 O2 O2 101.25(12) 4_445 1_556
O2 O2 O2 179.998(3) 1_554 1_556
Ga2 O2 O3 18.5(3) 2_565 3_564
Ga3 O2 O3 114.2(4) . 3_564
La O2 O3 120.0(4) . 3_564
O3 O2 O3 98.7(4) 5_455 3_564
O2 O2 O3 55.5(4) 3_565 3_564
O2 O2 O3 27.93(17) 4_455 3_564
La O2 O3 76.3(3) 4_455 3_564
O3 O2 O3 148.8(4) 2_455 3_564
O1 O2 O3 84.7(3) . 3_564
O2 O2 O3 108.9(4) 6_554 3_564
O3 O2 O3 79.3(3) 4_454 3_564
O1 O2 O3 35.2(2) 1_554 3_564
O3 O2 O3 120.6(4) 4_455 3_564
Nb O2 O3 131.2(4) 1_455 3_564
Ga1 O2 O3 131.2(4) 1_455 3_564
O1 O2 O3 145.9(5) 2_455 3_564
Ga2 O2 O3 126.1(4) 1_554 3_564
O2 O2 O3 147.6(5) 6 3_564
O3 O2 O3 98.6(4) 6 3_564
La O2 O3 74.5(2) 1_554 3_564
Ga3 O2 O3 91.0(3) 2_464 3_564
La O2 O3 46.09(19) 4_454 3_564
Ga3 O2 O3 62.4(2) 2_564 3_564
O3 O2 O3 70.2(2) 1_554 3_564
La O2 O3 54.5(2) 2_565 3_564
Ga3 O2 O3 133.3(4) 1_556 3_564
Ga3 O2 O3 20.33(12) 4_455 3_564
O3 O2 O3 115.2(3) 3_454 3_564
Ga2 O2 O3 96.7(3) 2_566 3_564
O3 O2 O3 100.52(19) . 3_564
O2 O2 O3 105.4(5) 5_444 3_564
O2 O2 O3 33.3(2) 5_454 3_564
La O2 O3 173.6(3) 2_455 3_564
O2 O2 O3 67.9(2) 2_464 3_564
O3 O2 O3 152.3(5) 3_455 3_564
O1 O2 O3 65.1(2) 2_465 3_564
Nb O2 O3 91.2(2) 1_454 3_564
Ga1 O2 O3 91.2(2) 1_454 3_564
O3 O2 O3 123.0(3) 6_455 3_564
Ga2 O2 O3 54.5(2) 1_564 3_564
Ga3 O2 O3 125.8(3) 4_345 3_564
Ga3 O2 O3 99.6(3) 4_445 3_564
O2 O2 O3 63.5(2) 1_554 3_564
O2 O2 O3 116.5(2) 1_556 3_564
Ga2 O2 O2 116.7(6) 2_565 5_445
Ga3 O2 O2 107.2(4) . 5_445
La O2 O2 13.05(18) . 5_445
O3 O2 O2 121.3(5) 5_455 5_445
O2 O2 O2 77.1(7) 3_565 5_445
O2 O2 O2 123.1(5) 4_455 5_445
La O2 O2 108.7(4) 4_455 5_445
O3 O2 O2 78.9(3) 2_455 5_445
O1 O2 O2 66.1(4) . 5_445
O2 O2 O2 88.2(3) 6_554 5_445
O3 O2 O2 142.3(4) 4_454 5_445
O1 O2 O2 128.2(5) 1_554 5_445
O3 O2 O2 77.1(3) 4_455 5_445
Nb O2 O2 88.9(3) 1_455 5_445
Ga1 O2 O2 88.9(3) 1_455 5_445
O1 O2 O2 33.3(2) 2_455 5_445
Ga2 O2 O2 58.96(10) 1_554 5_445
O2 O2 O2 32.1(2) 6 5_445
O3 O2 O2 40.8(2) 6 5_445
La O2 O2 100.9(3) 1_554 5_445
Ga3 O2 O2 135.3(4) 2_464 5_445
La O2 O2 161.3(4) 4_454 5_445
Ga3 O2 O2 75.0(3) 2_564 5_445
O3 O2 O2 80.5(4) 1_554 5_445
La O2 O2 82.9(3) 2_565 5_445
Ga3 O2 O2 54.5(2) 1_556 5_445
Ga3 O2 O2 136.6(3) 4_455 5_445
O3 O2 O2 105.8(3) 3_454 5_445
Ga2 O2 O2 59.8(2) 2_566 5_445
O3 O2 O2 32.8(3) . 5_445
O2 O2 O2 62.97(7) 5_444 5_445
O2 O2 O2 160.1(5) 5_454 5_445
La O2 O2 52.05(15) 2_455 5_445
O2 O2 O2 158.0(5) 2_464 5_445
O3 O2 O2 65.9(3) 3_455 5_445
O1 O2 O2 133.8(4) 2_465 5_445
Nb O2 O2 129.6(3) 1_454 5_445
Ga1 O2 O2 129.6(3) 1_454 5_445
O3 O2 O2 103.5(3) 6_455 5_445
Ga2 O2 O2 155.3(4) 1_564 5_445
Ga3 O2 O2 101.3(2) 4_345 5_445
Ga3 O2 O2 51.60(16) 4_445 5_445
O2 O2 O2 127.6(2) 1_554 5_445
O2 O2 O2 52.4(2) 1_556 5_445
O3 O2 O2 132.3(4) 3_564 5_445
Ga2 O2 O2 84.9(4) 2_565 5_455
Ga3 O2 O2 123.8(7) . 5_455
La O2 O2 95.5(5) . 5_455
O3 O2 O2 61.2(4) 5_455 5_455
O2 O2 O2 88.3(4) 3_565 5_455
O2 O2 O2 45.6(2) 4_455 5_455
La O2 O2 11.04(5) 4_455 5_455
O3 O2 O2 106.2(6) 2_455 5_455
O1 O2 O2 42.1(4) . 5_455
O2 O2 O2 163.3(2) 6_554 5_455
O3 O2 O2 106.9(4) 4_454 5_455
O1 O2 O2 107.5(3) 1_554 5_455
O3 O2 O2 48.4(4) 4_455 5_455
Nb O2 O2 73.0(4) 1_455 5_455
Ga1 O2 O2 73.0(4) 1_455 5_455
O1 O2 O2 130.6(5) 2_455 5_455
Ga2 O2 O2 159.2(4) 1_554 5_455
O2 O2 O2 84.1(6) 6 5_455
O3 O2 O2 119.5(4) 6 5_455
La O2 O2 147.4(3) 1_554 5_455
Ga3 O2 O2 76.6(3) 2_464 5_455
La O2 O2 94.10(16) 4_454 5_455
Ga3 O2 O2 107.9(3) 2_564 5_455
O3 O2 O2 131.3(4) 1_554 5_455
La O2 O2 56.6(2) 2_565 5_455
Ga3 O2 O2 61.9(4) 1_556 5_455
Ga3 O2 O2 54.07(11) 4_455 5_455
O3 O2 O2 125.2(4) 3_454 5_455
Ga2 O2 O2 43.9(3) 2_566 5_455
O3 O2 O2 86.1(4) . 5_455
O2 O2 O2 160.1(5) 5_444 5_455
O2 O2 O2 62.97(7) 5_454 5_455
La O2 O2 111.7(4) 2_455 5_455
O2 O2 O2 72.2(3) 2_464 5_455
O3 O2 O2 83.0(4) 3_455 5_455
O1 O2 O2 33.92(18) 2_465 5_455
Nb O2 O2 115.5(3) 1_454 5_455
Ga1 O2 O2 115.5(3) 1_454 5_455
O3 O2 O2 85.7(4) 6_455 5_455
Ga2 O2 O2 53.71(8) 1_564 5_455
Ga3 O2 O2 107.1(4) 4_345 5_455
Ga3 O2 O2 138.3(3) 4_445 5_455
O2 O2 O2 127.6(2) 1_554 5_455
O2 O2 O2 52.4(2) 1_556 5_455
O3 O2 O2 73.0(2) 3_564 5_455
O2 O2 O2 102.8(4) 5_445 5_455
Ga2 O2 O3 110.0(4) 2_565 1_454
Ga3 O2 O3 30.3(4) . 1_454
La O2 O3 143.3(4) . 1_454
O3 O2 O3 37.8(3) 5_455 1_454
O2 O2 O3 149.3(3) 3_565 1_454
O2 O2 O3 102.5(7) 4_455 1_454
La O2 O3 85.1(4) 4_455 1_454
O3 O2 O3 52.1(4) 2_455 1_454
O1 O2 O3 135.8(5) . 1_454
O2 O2 O3 67.4(2) 6_554 1_454
O3 O2 O3 24.5(2) 4_454 1_454
O1 O2 O3 86.7(3) 1_554 1_454
O3 O2 O3 82.7(3) 4_455 1_454
Nb O2 O3 53.9(2) 1_455 1_454
Ga1 O2 O3 53.9(2) 1_455 1_454
O1 O2 O3 103.4(3) 2_455 1_454
Ga2 O2 O3 90.3(2) 1_554 1_454
O2 O2 O3 108.4(2) 6 1_454
O3 O2 O3 144.1(4) 6 1_454
La O2 O3 85.1(2) 1_554 1_454
Ga3 O2 O3 19.38(13) 2_464 1_454
La O2 O3 53.5(2) 4_454 1_454
Ga3 O2 O3 140.1(3) 2_564 1_454
O3 O2 O3 118.8(4) 1_554 1_454
La O2 O3 143.2(4) 2_565 1_454
Ga3 O2 O3 98.9(3) 1_556 1_454
Ga3 O2 O3 90.9(3) 4_455 1_454
O3 O2 O3 31.96(17) 3_454 1_454
Ga2 O2 O3 129.8(4) 2_566 1_454
O3 O2 O3 162.5(4) . 1_454
O2 O2 O3 103.9(4) 5_444 1_454
O2 O2 O3 67.3(3) 5_454 1_454
La O2 O3 78.7(2) 2_455 1_454
O2 O2 O3 33.25(19) 2_464 1_454
O3 O2 O3 71.91(17) 3_455 1_454
O1 O2 O3 65.3(3) 2_465 1_454
Nb O2 O3 22.78(13) 1_454 1_454
Ga1 O2 O3 22.78(13) 1_454 1_454
O3 O2 O3 32.9(3) 6_455 1_454
Ga2 O2 O3 54.7(2) 1_564 1_454
Ga3 O2 O3 29.42(17) 4_345 1_454
Ga3 O2 O3 125.7(3) 4_445 1_454
O2 O2 O3 63.4(2) 1_554 1_454
O2 O2 O3 116.6(2) 1_556 1_454
O3 O2 O3 96.7(4) 3_564 1_454
O2 O2 O3 130.7(3) 5_445 1_454
O2 O2 O3 96.0(3) 5_455 1_454
Ga2 O2 O2 111.4(6) 2_565 2_465
Ga3 O2 O2 95.3(6) . 2_465
La O2 O2 102.8(4) . 2_465
O3 O2 O2 34.3(3) 5_455 2_465
O2 O2 O2 119.0(4) 3_565 2_465
O2 O2 O2 71.8(5) 4_455 2_465
La O2 O2 22.0(2) 4_455 2_465
O3 O2 O2 75.9(4) 2_455 2_465
O1 O2 O2 63.9(3) . 2_465
O2 O2 O2 134.41(7) 6_554 2_465
O3 O2 O2 90.9(5) 4_454 2_465
O1 O2 O2 124.0(4) 1_554 2_465
O3 O2 O2 27.9(3) 4_455 2_465
Nb O2 O2 42.5(2) 1_455 2_465
Ga1 O2 O2 42.5(2) 1_455 2_465
O1 O2 O2 116.7(3) 2_455 2_465
Ga2 O2 O2 136.9(2) 1_554 2_465
O2 O2 O2 74.0(4) 6 2_465
O3 O2 O2 137.7(4) 6 2_465
La O2 O2 154.0(4) 1_554 2_465
Ga3 O2 O2 54.0(3) 2_464 2_465
La O2 O2 95.1(4) 4_454 2_465
Ga3 O2 O2 138.7(2) 2_564 2_465
O3 O2 O2 162.2(2) 1_554 2_465
La O2 O2 87.1(2) 2_565 2_465
Ga3 O2 O2 49.6(2) 1_556 2_465
Ga3 O2 O2 75.2(3) 4_455 2_465
O3 O2 O2 96.4(3) 3_454 2_465
Ga2 O2 O2 58.7(2) 2_566 2_465
O3 O2 O2 102.9(3) . 2_465
O2 O2 O2 159.0(3) 5_444 2_465
O2 O2 O2 72.1(3) 5_454 2_465
La O2 O2 87.3(2) 2_455 2_465
O2 O2 O2 61.0(4) 2_464 2_465
O3 O2 O2 57.2(2) 3_455 2_465
O1 O2 O2 33.2(2) 2_465 2_465
Nb O2 O2 94.6(3) 1_454 2_465
Ga1 O2 O2 94.6(3) 1_454 2_465
O3 O2 O2 54.9(2) 6_455 2_465
Ga2 O2 O2 52.8(2) 1_564 2_465
Ga3 O2 O2 76.6(2) 4_345 2_465
Ga3 O2 O2 154.6(3) 4_445 2_465
O2 O2 O2 126.5(2) 1_554 2_465
O2 O2 O2 53.5(2) 1_556 2_465
O3 O2 O2 95.5(3) 3_564 2_465
O2 O2 O2 103.4(4) 5_445 2_465
O2 O2 O2 31.1(2) 5_455 2_465
O3 O2 O2 72.1(3) 1_454 2_465
Ga2 O2 O2 116.6(8) 2_565 2_454
Ga3 O2 O2 47.8(3) . 2_454
La O2 O2 78.5(4) . 2_454
O3 O2 O2 106.0(3) 5_455 2_454
O2 O2 O2 107.4(8) 3_565 2_454
O2 O2 O2 155.7(5) 4_455 2_454
La O2 O2 151.6(4) 4_455 2_454
O3 O2 O2 53.9(2) 2_455 2_454
O1 O2 O2 134.0(5) . 2_454
O2 O2 O2 21.6(3) 6_554 2_454
O3 O2 O2 76.1(4) 4_454 2_454
O1 O2 O2 92.8(5) 1_554 2_454
O3 O2 O2 110.2(3) 4_455 2_454
Nb O2 O2 87.18(15) 1_455 2_454
Ga1 O2 O2 87.18(15) 1_455 2_454
O1 O2 O2 35.3(3) 2_455 2_454
Ga2 O2 O2 12.25(16) 1_554 2_454
O2 O2 O2 78.4(4) 6 2_454
O3 O2 O2 66.9(4) 6 2_454
La O2 O2 53.5(3) 1_554 2_454
Ga3 O2 O2 96.2(2) 2_464 2_454
La O2 O2 98.6(3) 4_454 2_454
Ga3 O2 O2 88.8(5) 2_564 2_454
O3 O2 O2 68.0(5) 1_554 2_454
La O2 O2 136.4(5) 2_565 2_454
Ga3 O2 O2 98.3(2) 1_556 2_454
Ga3 O2 O2 145.4(4) 4_455 2_454
O3 O2 O2 46.16(18) 3_454 2_454
Ga2 O2 O2 126.5(3) 2_566 2_454
O3 O2 O2 93.6(4) . 2_454
O2 O2 O2 32.3(3) 5_444 2_454
O2 O2 O2 130.3(5) 5_454 2_454
La O2 O2 47.09(8) 2_455 2_454
O2 O2 O2 108.7(3) 2_464 2_454
O3 O2 O2 75.54(19) 3_455 2_454
O1 O2 O2 142.9(4) 2_465 2_454
Nb O2 O2 64.47(19) 1_454 2_454
Ga1 O2 O2 64.47(19) 1_454 2_454
O3 O2 O2 78.2(2) 6_455 2_454
Ga2 O2 O2 130.5(3) 1_564 2_454
Ga3 O2 O2 58.50(12) 4_345 2_454
Ga3 O2 O2 51.4(3) 4_445 2_454
O2 O2 O2 68.3(2) 1_554 2_454
O2 O2 O2 111.7(2) 1_556 2_454
O3 O2 O2 127.9(4) 3_564 2_454
O2 O2 O2 67.89(15) 5_445 2_454
O2 O2 O2 158.5(5) 5_455 2_454
O3 O2 O2 78.1(2) 1_454 2_454
O2 O2 O2 129.7(3) 2_465 2_454
Ga2 O2 O2 25.2(2) 2_565 2_564
Ga3 O2 O2 124.8(7) . 2_564
La O2 O2 83.7(4) . 2_564
O3 O2 O2 142.3(5) 5_455 2_564
O2 O2 O2 21.9(2) 3_565 2_564
O2 O2 O2 59.6(2) 4_455 2_564
La O2 O2 107.7(3) 4_455 2_564
O3 O2 O2 154.5(7) 2_455 2_564
O1 O2 O2 81.3(2) . 2_564
O2 O2 O2 92.6(4) 6_554 2_564
O3 O2 O2 104.2(4) 4_454 2_564
O1 O2 O2 41.7(2) 1_554 2_564
O3 O2 O2 140.7(4) 4_455 2_564
Nb O2 O2 172.1(5) 1_455 2_564
Ga1 O2 O2 172.1(5) 1_455 2_564
O1 O2 O2 103.1(5) 2_455 2_564
Ga2 O2 O2 92.3(5) 1_554 2_564
O2 O2 O2 122.1(2) 6 2_564
O3 O2 O2 55.3(4) 6 2_564
La O2 O2 57.2(3) 1_554 2_564
Ga3 O2 O2 131.4(3) 2_464 2_564
La O2 O2 76.2(2) 4_454 2_564
Ga3 O2 O2 18.89(17) 2_564 2_564
O3 O2 O2 32.7(3) 1_554 2_564
La O2 O2 47.84(9) 2_565 2_564
Ga3 O2 O2 131.7(3) 1_556 2_564
Ga3 O2 O2 61.02(13) 4_455 2_564
O3 O2 O2 124.4(4) 3_454 2_564
Ga2 O2 O2 92.8(2) 2_566 2_564
O3 O2 O2 68.1(3) . 2_564
O2 O2 O2 69.4(5) 5_444 2_564
O2 O2 O2 76.5(3) 5_454 2_564
La O2 O2 137.0(5) 2_455 2_564
O2 O2 O2 108.7(3) 2_464 2_564
O3 O2 O2 158.8(4) 3_455 2_564
O1 O2 O2 106.4(3) 2_465 2_564
Nb O2 O2 110.6(3) 1_454 2_564
Ga1 O2 O2 110.6(3) 1_454 2_564
O3 O2 O2 161.2(4) 6_455 2_564
Ga2 O2 O2 98.1(2) 1_564 2_564
Ga3 O2 O2 146.1(4) 4_345 2_564
Ga3 O2 O2 57.2(3) 4_445 2_564
O2 O2 O2 68.3(2) 1_554 2_564
O2 O2 O2 111.7(2) 1_556 2_564
O3 O2 O2 43.59(17) 3_564 2_564
O2 O2 O2 93.2(5) 5_445 2_564
O2 O2 O2 99.2(2) 5_455 2_564
O3 O2 O2 128.3(3) 1_454 2_564
O2 O2 O2 129.7(3) 2_465 2_564
O2 O2 O2 100.6(6) 2_454 2_564
Ga2 O2 La 14.4(3) 2_565 2_564
Ga3 O2 La 106.9(4) . 2_564
La O2 La 110.1(4) . 2_564
O3 O2 La 119.2(4) 5_455 2_564
O2 O2 La 46.72(19) 3_565 2_564
O2 O2 La 52.5(2) 4_455 2_564
La O2 La 102.5(3) 4_455 2_564
O3 O2 La 145.9(4) 2_455 2_564
O1 O2 La 97.8(3) . 2_564
O2 O2 La 87.2(4) 6_554 2_564
O3 O2 La 79.4(3) 4_454 2_564
O1 O2 La 17.67(18) 1_554 2_564
O3 O2 La 146.4(4) 4_455 2_564
Nb O2 La 152.1(3) 1_455 2_564
Ga1 O2 La 152.1(3) 1_455 2_564
O1 O2 La 120.6(4) 2_455 2_564
Ga2 O2 La 99.9(3) 1_554 2_564
O2 O2 La 148.59(14) 6 2_564
O3 O2 La 79.1(3) 6 2_564
La O2 La 50.44(13) 1_554 2_564
Ga3 O2 La 105.2(2) 2_464 2_564
La O2 La 49.78(11) 4_454 2_564
Ga3 O2 La 43.90(11) 2_564 2_564
O3 O2 La 44.7(2) 1_554 2_564
La O2 La 62.81(13) 2_565 2_564
Ga3 O2 La 152.0(3) 1_556 2_564
Ga3 O2 La 46.75(10) 4_455 2_564
O3 O2 La 107.2(3) 3_454 2_564
Ga2 O2 La 110.5(2) 2_566 2_564
O3 O2 La 94.3(3) . 2_564
O2 O2 La 79.0(4) 5_444 2_564
O2 O2 La 54.3(2) 5_454 2_564
La O2 La 150.1(4) 2_455 2_564
O2 O2 La 83.1(2) 2_464 2_564
O3 O2 La 174.5(3) 3_455 2_564
O1 O2 La 90.6(2) 2_465 2_564
Nb O2 La 87.82(17) 1_454 2_564
Ga1 O2 La 87.82(17) 1_454 2_564
O3 O2 La 135.1(3) 6_455 2_564
Ga2 O2 La 76.43(14) 1_564 2_564
Ga3 O2 La 125.9(2) 4_345 2_564
Ga3 O2 La 75.2(2) 4_445 2_564
O2 O2 La 48.70(12) 1_554 2_564
O2 O2 La 131.30(12) 1_556 2_564
O3 O2 La 26.43(12) 3_564 2_564
O2 O2 La 118.9(4) 5_445 2_564
O2 O2 La 98.0(2) 5_455 2_564
O3 O2 La 102.6(2) 1_454 2_564
O2 O2 La 121.9(2) 2_465 2_564
O2 O2 La 103.4(4) 2_454 2_564
O2 O2 La 26.49(13) 2_564 2_564
Ga2 O2 O3 34.1(4) 2_565 2_565
Ga3 O2 O3 143.5(5) . 2_565
La O2 O3 95.6(3) . 2_565
O3 O2 O3 102.7(4) 5_455 2_565
O2 O2 O3 43.7(4) 3_565 2_565
O2 O2 O3 16.9(4) 4_455 2_565
La O2 O3 60.6(2) 4_455 2_565
O3 O2 O3 158.3(6) 2_455 2_565
O1 O2 O3 53.6(3) . 2_565
O2 O2 O3 135.6(4) 6_554 2_565
O3 O2 O3 107.7(3) 4_454 2_565
O1 O2 O3 63.3(3) 1_554 2_565
O3 O2 O3 99.6(3) 4_455 2_565
Nb O2 O3 125.1(4) 1_455 2_565
Ga1 O2 O3 125.1(4) 1_455 2_565
O1 O2 O3 137.5(3) 2_455 2_565
Ga2 O2 O3 138.8(4) 1_554 2_565
O2 O2 O3 116.6(5) 6 2_565
O3 O2 O3 89.4(2) 6 2_565
La O2 O3 98.4(2) 1_554 2_565
Ga3 O2 O3 105.7(3) 2_464 2_565
La O2 O3 75.5(2) 4_454 2_565
Ga3 O2 O3 60.26(15) 2_564 2_565
O3 O2 O3 79.8(3) 1_554 2_565
La O2 O3 25.83(13) 2_565 2_565
Ga3 O2 O3 105.1(3) 1_556 2_565
Ga3 O2 O3 28.18(15) 4_455 2_565
O3 O2 O3 144.8(3) 3_454 2_565
Ga2 O2 O3 65.87(19) 2_566 2_565
O3 O2 O3 76.1(3) . 2_565
O2 O2 O3 116.1(4) 5_444 2_565
O2 O2 O3 52.0(3) 5_454 2_565
La O2 O3 155.3(3) 2_455 2_565
O2 O2 O3 85.8(2) 2_464 2_565
O3 O2 O3 134.1(3) 3_455 2_565
O1 O2 O3 63.51(19) 2_465 2_565
Nb O2 O3 120.3(3) 1_454 2_565
Ga1 O2 O3 120.3(3) 1_454 2_565
O3 O2 O3 131.5(4) 6_455 2_565
Ga2 O2 O3 65.5(2) 1_564 2_565
Ga3 O2 O3 146.7(3) 4_345 2_565
Ga3 O2 O3 100.1(2) 4_445 2_565
O2 O2 O3 93.82(18) 1_554 2_565
O2 O2 O3 86.18(18) 1_556 2_565
O3 O2 O3 31.1(3) 3_564 2_565
O2 O2 O3 108.7(3) 5_445 2_565
O2 O2 O3 52.7(2) 5_455 2_565
O3 O2 O3 118.9(3) 1_454 2_565
O2 O2 O3 82.6(2) 2_465 2_565
O2 O2 O3 147.7(5) 2_454 2_565
O2 O2 O3 47.12(16) 2_564 2_565
La O2 O3 48.46(15) 2_564 2_565
Ga2 O2 Ga2 134.3(5) 2_565 .
Ga3 O2 Ga2 99.0(3) . .
La O2 Ga2 28.86(16) . .
O3 O2 Ga2 101.2(3) 5_455 .
O2 O2 Ga2 94.4(5) 3_565 .
O2 O2 Ga2 127.24(17) 4_455 .
La O2 Ga2 96.3(3) 4_455 .
O3 O2 Ga2 64.1(3) 2_455 .
O1 O2 Ga2 65.9(2) . .
O2 O2 Ga2 92.9(4) 6_554 .
O3 O2 Ga2 134.3(3) 4_454 .
O1 O2 Ga2 147.9(5) 1_554 .
O3 O2 Ga2 58.8(2) 4_455 .
Nb O2 Ga2 69.13(16) 1_455 .
Ga1 O2 Ga2 69.13(16) 1_455 .
O1 O2 Ga2 37.2(3) 2_455 .
Ga2 O2 Ga2 65.97(17) 1_554 .
O2 O2 Ga2 12.52(14) 6 .
O3 O2 Ga2 60.8(3) 6 .
La O2 Ga2 115.5(3) 1_554 .
Ga3 O2 Ga2 116.2(2) 2_464 .
La O2 Ga2 167.4(3) 4_454 .
Ga3 O2 Ga2 94.7(2) 2_564 .
O3 O2 Ga2 99.9(4) 1_554 .
La O2 Ga2 92.20(18) 2_565 .
Ga3 O2 Ga2 36.66(8) 1_556 .
Ga3 O2 Ga2 141.3(3) 4_455 .
O3 O2 Ga2 97.9(2) 3_454 .
Ga2 O2 Ga2 55.81(11) 2_566 .
O3 O2 Ga2 46.9(2) . .
O2 O2 Ga2 76.93(18) 5_444 .
O2 O2 Ga2 156.3(4) 5_454 .
La O2 Ga2 39.41(8) 2_455 .
O2 O2 Ga2 138.1(4) 2_464 .
O3 O2 Ga2 46.44(19) 3_455 .
O1 O2 Ga2 118.9(3) 2_465 .
Nb O2 Ga2 122.3(2) 1_454 .
Ga1 O2 Ga2 122.3(2) 1_454 .
O3 O2 Ga2 85.2(2) 6_455 .
Ga2 O2 Ga2 139.0(3) 1_564 .
Ga3 O2 Ga2 87.41(15) 4_345 .
Ga3 O2 Ga2 69.91(18) 4_445 .
O2 O2 Ga2 138.78(17) 1_554 .
O2 O2 Ga2 41.22(17) 1_556 .
O3 O2 Ga2 146.3(3) 3_564 .
O2 O2 Ga2 20.03(14) 5_445 .
O2 O2 Ga2 93.5(4) 5_455 .
O3 O2 Ga2 115.6(2) 1_454 .
O2 O2 Ga2 86.3(2) 2_465 .
O2 O2 Ga2 71.3(2) 2_454 .
O2 O2 Ga2 112.4(4) 2_564 .
La O2 Ga2 138.6(3) 2_564 .
O3 O2 Ga2 117.1(2) 2_565 .
Ga2 O2 O3 62.2(4) 2_565 3_565
Ga3 O2 O3 152.5(7) . 3_565
La O2 O3 82.1(3) . 3_565
O3 O2 O3 91.4(4) 5_455 3_565
O2 O2 O3 57.2(3) 3_565 3_565
O2 O2 O3 32.44(19) 4_455 3_565
La O2 O3 41.7(2) 4_455 3_565
O3 O2 O3 134.2(5) 2_455 3_565
O1 O2 O3 29.0(2) . 3_565
O2 O2 O3 162.5(3) 6_554 3_565
O3 O2 O3 123.5(4) 4_454 3_565
O1 O2 O3 91.5(3) 1_554 3_565
O3 O2 O3 72.8(3) 4_455 3_565
Nb O2 O3 102.4(4) 1_455 3_565
Ga1 O2 O3 102.4(4) 1_455 3_565
O1 O2 O3 127.0(3) 2_455 3_565
Ga2 O2 O3 147.3(4) 1_554 3_565
O2 O2 O3 91.0(5) 6 3_565
O3 O2 O3 93.2(3) 6 3_565
La O2 O3 125.6(3) 1_554 3_565
Ga3 O2 O3 103.7(4) 2_464 3_565
La O2 O3 96.8(3) 4_454 3_565
Ga3 O2 O3 76.9(2) 2_564 3_565
O3 O2 O3 100.7(2) 1_554 3_565
La O2 O3 25.65(14) 2_565 3_565
Ga3 O2 O3 76.9(2) 1_556 3_565
Ga3 O2 O3 46.40(17) 4_455 3_565
O3 O2 O3 154.1(5) 3_454 3_565
Ga2 O2 O3 39.65(15) 2_566 3_565
O3 O2 O3 65.94(19) . 3_565
O2 O2 O3 131.2(4) 5_444 3_565
O2 O2 O3 66.8(3) 5_454 3_565
La O2 O3 128.5(3) 2_455 3_565
O2 O2 O3 91.8(3) 2_464 3_565
O3 O2 O3 106.4(3) 3_455 3_565
O1 O2 O3 57.1(3) 2_465 3_565
Nb O2 O3 135.6(3) 1_454 3_565
Ga1 O2 O3 135.6(3) 1_454 3_565
O3 O2 O3 116.7(3) 6_455 3_565
Ga2 O2 O3 69.9(2) 1_564 3_565
Ga3 O2 O3 138.2(4) 4_345 3_565
Ga3 O2 O3 110.0(3) 4_445 3_565
O2 O2 O3 121.24(15) 1_554 3_565
O2 O2 O3 58.76(15) 1_556 3_565
O3 O2 O3 57.71(17) 3_564 3_565
O2 O2 O3 93.8(3) 5_445 3_565
O2 O2 O3 31.1(2) 5_455 3_565
O3 O2 O3 122.3(4) 1_454 3_565
O2 O2 O3 61.9(2) 2_465 3_565
O2 O2 O3 159.4(5) 2_454 3_565
O2 O2 O3 69.93(18) 2_564 3_565
La O2 O3 76.58(17) 2_564 3_565
O3 O2 O3 28.2(2) 2_565 3_565
Ga2 O2 O3 94.9(2) . 3_565
Ga2 O2 O3 140.1(7) 2_565 1_455
Ga3 O2 O3 70.9(4) . 1_455
La O2 O3 98.5(3) . 1_455
O3 O2 O3 28.9(3) 5_455 1_455
O2 O2 O3 145.1(3) 3_565 1_455
O2 O2 O3 101.9(7) 4_455 1_455
La O2 O3 52.8(3) 4_455 1_455
O3 O2 O3 45.1(3) 2_455 1_455
O1 O2 O3 84.0(4) . 1_455
O2 O2 O3 106.3(3) 6_554 1_455
O3 O2 O3 82.1(3) 4_454 1_455
O1 O2 O3 138.9(4) 1_554 1_455
O3 O2 O3 25.01(18) 4_455 1_455
Nb O2 O3 11.69(15) 1_455 1_455
Ga1 O2 O3 11.69(15) 1_455 1_455
O1 O2 O3 91.8(3) 2_455 1_455
Ga2 O2 O3 106.6(2) 1_554 1_455
O2 O2 O3 60.56(19) 6 1_455
O3 O2 O3 133.3(2) 6 1_455
La O2 O3 139.4(3) 1_554 1_455
Ga3 O2 O3 47.2(2) 2_464 1_455
La O2 O3 102.6(3) 4_454 1_455
Ga3 O2 O3 161.8(3) 2_564 1_455
O3 O2 O3 166.6(5) 1_554 1_455
La O2 O3 114.6(4) 2_565 1_455
Ga3 O2 O3 42.42(18) 1_556 1_455
Ga3 O2 O3 102.8(4) 4_455 1_455
O3 O2 O3 71.62(18) 3_454 1_455
Ga2 O2 O3 74.1(2) 2_566 1_455
O3 O2 O3 109.0(3) . 1_455
O2 O2 O3 129.5(3) 5_444 1_455
O2 O2 O3 92.2(4) 5_454 1_455
La O2 O3 58.95(18) 2_455 1_455
O2 O2 O3 66.1(4) 2_464 1_455
O3 O2 O3 30.35(18) 3_455 1_455
O1 O2 O3 57.3(3) 2_465 1_455
Nb O2 O3 79.5(2) 1_454 1_455
Ga1 O2 O3 79.5(2) 1_454 1_455
O3 O2 O3 29.3(2) 6_455 1_455
Ga2 O2 O3 70.1(3) 1_564 1_455
Ga3 O2 O3 49.91(16) 4_345 1_455
Ga3 O2 O3 138.0(3) 4_445 1_455
O2 O2 O3 121.40(16) 1_554 1_455
O2 O2 O3 58.60(16) 1_556 1_455
O3 O2 O3 122.3(4) 3_564 1_455
O2 O2 O3 92.5(3) 5_445 1_455
O2 O2 O3 61.3(4) 5_455 1_455
O3 O2 O3 58.02(19) 1_454 1_455
O2 O2 O3 30.8(2) 2_465 1_455
O2 O2 O3 98.8(2) 2_454 1_455
O2 O2 O3 160.5(4) 2_564 1_455
La O2 O3 146.5(3) 2_564 1_455
O3 O2 O3 113.4(3) 2_565 1_455
Ga2 O2 O3 72.48(19) . 1_455
O3 O2 O3 91.0(4) 3_565 1_455
Ga2 O2 Nb 76.9(4) 2_565 .
Ga3 O2 Nb 130.1(7) . .
La O2 Nb 30.6(2) . .
O3 O2 Nb 155.5(4) 5_455 .
O2 O2 Nb 38.1(5) 3_565 .
O2 O2 Nb 94.4(5) 4_455 .
La O2 Nb 113.7(3) 4_455 .
O3 O2 Nb 116.4(4) 2_455 .
O1 O2 Nb 61.8(2) . .
O2 O2 Nb 93.4(2) 6_554 .
O3 O2 Nb 145.4(5) 4_454 .
O1 O2 Nb 92.1(3) 1_554 .
O3 O2 Nb 106.3(3) 4_455 .
Nb O2 Nb 127.7(2) 1_455 .
Ga1 O2 Nb 127.7(2) 1_455 .
O1 O2 Nb 60.2(2) 2_455 .
Ga2 O2 Nb 70.1(2) 1_554 .
O2 O2 Nb 69.37(11) 6 .
O3 O2 Nb 16.44(17) 6 .
La O2 Nb 81.5(3) 1_554 .
Ga3 O2 Nb 175.1(2) 2_464 .
La O2 Nb 128.5(3) 4_454 .
Ga3 O2 Nb 36.12(11) 2_564 .
O3 O2 Nb 49.9(2) 1_554 .
La O2 Nb 55.27(14) 2_565 .
Ga3 O2 Nb 86.03(18) 1_556 .
Ga3 O2 Nb 104.2(2) 4_455 .
O3 O2 Nb 128.5(4) 3_454 .
Ga2 O2 Nb 65.08(14) 2_566 .
O3 O2 Nb 21.09(16) . .
O2 O2 Nb 57.0(2) 5_444 .
O2 O2 Nb 126.1(3) 5_454 .
La O2 Nb 89.7(2) 2_455 .
O2 O2 Nb 161.40(17) 2_464 .
O3 O2 Nb 105.4(3) 3_455 .
O1 O2 Nb 134.4(3) 2_465 .
Nb O2 Nb 140.7(4) 1_454 .
Ga1 O2 Nb 140.7(4) 1_454 .
O3 O2 Nb 143.3(3) 6_455 .
Ga2 O2 Nb 143.0(2) 1_564 .
Ga3 O2 Nb 135.8(3) 4_345 .
Ga3 O2 Nb 35.39(10) 4_445 .
O2 O2 Nb 107.11(15) 1_554 .
O2 O2 Nb 72.89(15) 1_556 .
O3 O2 Nb 93.5(3) 3_564 .
O2 O2 Nb 39.9(2) 5_445 .
O2 O2 Nb 103.1(3) 5_455 .
O3 O2 Nb 160.3(4) 1_454 .
O2 O2 Nb 123.7(3) 2_465 .
O2 O2 Nb 82.3(4) 2_454 .
O2 O2 Nb 53.5(3) 2_564 .
La O2 Nb 79.70(19) 2_564 .
O3 O2 Nb 77.51(17) 2_565 .
Ga2 O2 Nb 58.94(13) . .
O3 O2 Nb 77.33(19) 3_565 .
O3 O2 Nb 128.3(2) 1_455 .
Ga2 O2 Ga1 76.9(4) 2_565 .
Ga3 O2 Ga1 130.1(7) . .
La O2 Ga1 30.6(2) . .
O3 O2 Ga1 155.5(4) 5_455 .
O2 O2 Ga1 38.1(5) 3_565 .
O2 O2 Ga1 94.4(5) 4_455 .
La O2 Ga1 113.7(3) 4_455 .
O3 O2 Ga1 116.4(4) 2_455 .
O1 O2 Ga1 61.8(2) . .
O2 O2 Ga1 93.4(2) 6_554 .
O3 O2 Ga1 145.4(5) 4_454 .
O1 O2 Ga1 92.1(3) 1_554 .
O3 O2 Ga1 106.3(3) 4_455 .
Nb O2 Ga1 127.7(2) 1_455 .
Ga1 O2 Ga1 127.7(2) 1_455 .
O1 O2 Ga1 60.2(2) 2_455 .
Ga2 O2 Ga1 70.1(2) 1_554 .
O2 O2 Ga1 69.37(11) 6 .
O3 O2 Ga1 16.44(17) 6 .
La O2 Ga1 81.5(3) 1_554 .
Ga3 O2 Ga1 175.1(2) 2_464 .
La O2 Ga1 128.5(3) 4_454 .
Ga3 O2 Ga1 36.12(11) 2_564 .
O3 O2 Ga1 49.9(2) 1_554 .
La O2 Ga1 55.27(14) 2_565 .
Ga3 O2 Ga1 86.03(18) 1_556 .
Ga3 O2 Ga1 104.2(2) 4_455 .
O3 O2 Ga1 128.5(4) 3_454 .
Ga2 O2 Ga1 65.08(14) 2_566 .
O3 O2 Ga1 21.09(16) . .
O2 O2 Ga1 57.0(2) 5_444 .
O2 O2 Ga1 126.1(3) 5_454 .
La O2 Ga1 89.7(2) 2_455 .
O2 O2 Ga1 161.40(17) 2_464 .
O3 O2 Ga1 105.4(3) 3_455 .
O1 O2 Ga1 134.4(3) 2_465 .
Nb O2 Ga1 140.7(4) 1_454 .
Ga1 O2 Ga1 140.7(4) 1_454 .
O3 O2 Ga1 143.3(3) 6_455 .
Ga2 O2 Ga1 143.0(2) 1_564 .
Ga3 O2 Ga1 135.8(3) 4_345 .
Ga3 O2 Ga1 35.39(10) 4_445 .
O2 O2 Ga1 107.11(15) 1_554 .
O2 O2 Ga1 72.89(15) 1_556 .
O3 O2 Ga1 93.5(3) 3_564 .
O2 O2 Ga1 39.9(2) 5_445 .
O2 O2 Ga1 103.1(3) 5_455 .
O3 O2 Ga1 160.3(4) 1_454 .
O2 O2 Ga1 123.7(3) 2_465 .
O2 O2 Ga1 82.3(4) 2_454 .
O2 O2 Ga1 53.5(3) 2_564 .
La O2 Ga1 79.70(19) 2_564 .
O3 O2 Ga1 77.51(17) 2_565 .
Ga2 O2 Ga1 58.94(13) . .
O3 O2 Ga1 77.33(19) 3_565 .
O3 O2 Ga1 128.3(2) 1_455 .
Nb O2 Ga1 0.0 . .
Ga2 O2 O3 55.6(4) 2_565 5
Ga3 O2 O3 136.3(7) . 5
La O2 O3 51.2(3) . 5
O3 O2 O3 160.9(5) 5_455 5
O2 O2 O3 18.0(5) 3_565 5
O2 O2 O3 77.6(5) 4_455 5
La O2 O3 110.8(3) 4_455 5
O3 O2 O3 136.2(4) 2_455 5
O1 O2 O3 64.6(3) . 5
O2 O2 O3 96.5(2) 6_554 5
O3 O2 O3 133.1(4) 4_454 5
O1 O2 O3 72.9(3) 1_554 5
O3 O2 O3 120.1(3) 4_455 5
Nb O2 O3 147.4(3) 1_455 5
Ga1 O2 O3 147.4(3) 1_455 5
O1 O2 O3 78.6(3) 2_455 5
Ga2 O2 O3 80.8(3) 1_554 5
O2 O2 O3 89.71(17) 6 5
O3 O2 O3 28.6(3) 6 5
La O2 O3 72.7(3) 1_554 5
Ga3 O2 O3 163.4(3) 2_464 5
La O2 O3 108.6(3) 4_454 5
Ga3 O2 O3 17.28(14) 2_564 5
O3 O2 O3 38.9(3) 1_554 5
La O2 O3 44.18(16) 2_565 5
Ga3 O2 O3 103.1(2) 1_556 5
Ga3 O2 O3 85.15(18) 4_455 5
O3 O2 O3 134.9(4) 3_454 5
Ga2 O2 O3 72.4(2) 2_566 5
O3 O2 O3 36.6(3) . 5
O2 O2 O3 61.6(3) 5_444 5
O2 O2 O3 105.6(3) 5_454 5
La O2 O3 110.2(3) 2_455 5
O2 O2 O3 140.3(2) 2_464 5
O3 O2 O3 126.3(3) 3_455 5
O1 O2 O3 123.7(2) 2_465 5
Nb O2 O3 134.9(4) 1_454 5
Ga1 O2 O3 134.9(4) 1_454 5
O3 O2 O3 164.5(3) 6_455 5
Ga2 O2 O3 124.8(2) 1_564 5
Ga3 O2 O3 150.9(4) 4_345 5
Ga3 O2 O3 41.08(18) 4_445 5
O2 O2 O3 93.82(19) 1_554 5
O2 O2 O3 86.18(19) 1_556 5
O3 O2 O3 72.5(2) 3_564 5
O2 O2 O3 61.2(3) 5_445 5
O2 O2 O3 99.8(3) 5_455 5
O3 O2 O3 157.2(3) 1_454 5
O2 O2 O3 127.9(3) 2_465 5
O2 O2 O3 92.5(5) 2_454 5
O2 O2 O3 32.5(2) 2_564 5
La O2 O3 58.97(17) 2_564 5
O3 O2 O3 61.0(2) 2_565 5
Ga2 O2 O3 79.9(2) . 5
O3 O2 O3 69.54(19) 3_565 5
O3 O2 O3 144.7(2) 1_455 5
Nb O2 O3 21.31(12) . 5
Ga1 O2 O3 21.31(12) . 5
Ga2 O2 O3 51.6(4) 2_565 6_565
Ga3 O2 O3 122.2(5) . 6_565
La O2 O3 116.2(4) . 6_565
O3 O2 O3 74.1(4) 5_455 6_565
O2 O2 O3 72.5(5) 3_565 6_565
O2 O2 O3 13.0(5) 4_455 6_565
La O2 O3 39.61(18) 4_455 6_565
O3 O2 O3 131.3(5) 2_455 6_565
O1 O2 O3 62.5(3) . 6_565
O2 O2 O3 140.4(5) 6_554 6_565
O3 O2 O3 89.4(4) 4_454 6_565
O1 O2 O3 70.8(3) 1_554 6_565
O3 O2 O3 83.8(4) 4_455 6_565
Nb O2 O3 100.4(4) 1_455 6_565
Ga1 O2 O3 100.4(4) 1_455 6_565
O1 O2 O3 161.3(4) 2_455 6_565
Ga2 O2 O3 162.8(4) 1_554 6_565
O2 O2 O3 119.5(5) 6 6_565
O3 O2 O3 118.1(3) 6 6_565
La O2 O3 110.7(2) 1_554 6_565
Ga3 O2 O3 77.7(3) 2_464 6_565
La O2 O3 63.9(2) 4_454 6_565
Ga3 O2 O3 88.1(2) 2_564 6_565
O3 O2 O3 103.9(3) 1_554 6_565
La O2 O3 50.10(18) 2_565 6_565
Ga3 O2 O3 98.5(3) 1_556 6_565
Ga3 O2 O3 17.34(14) 4_455 6_565
O3 O2 O3 123.8(3) 3_454 6_565
Ga2 O2 O3 71.1(2) 2_566 6_565
O3 O2 O3 98.8(3) . 6_565
O2 O2 O3 140.9(5) 5_444 6_565
O2 O2 O3 32.7(2) 5_454 6_565
La O2 O3 146.9(4) 2_455 6_565
O2 O2 O3 60.1(2) 2_464 6_565
O3 O2 O3 116.9(3) 3_455 6_565
O1 O2 O3 34.97(13) 2_465 6_565
Nb O2 O3 101.8(3) 1_454 6_565
Ga1 O2 O3 101.8(3) 1_454 6_565
O3 O2 O3 102.9(3) 6_455 6_565
Ga2 O2 O3 38.39(15) 1_564 6_565
Ga3 O2 O3 118.5(3) 4_345 6_565
Ga3 O2 O3 128.4(3) 4_445 6_565
O2 O2 O3 93.73(18) 1_554 6_565
O2 O2 O3 86.27(18) 1_556 6_565
O3 O2 O3 36.8(2) 3_564 6_565
O2 O2 O3 128.0(3) 5_445 6_565
O2 O2 O3 36.73(16) 5_455 6_565
O3 O2 O3 93.1(3) 1_454 6_565
O2 O2 O3 59.8(2) 2_465 6_565
O2 O2 O3 162.0(4) 2_454 6_565
O2 O2 O3 72.4(2) 2_564 6_565
La O2 O3 62.89(17) 2_564 6_565
O3 O2 O3 28.9(2) 2_565 6_565
Ga2 O2 O3 126.6(3) . 6_565
O3 O2 O3 34.3(3) 3_565 6_565
O3 O2 O3 89.4(3) 1_455 6_565
Nb O2 O3 105.1(2) . 6_565
Ga1 O2 O3 105.1(2) . 6_565
O3 O2 O3 89.78(17) 5 6_565
Ga2 O2 O3 78.6(4) 2_565 5_454
Ga3 O2 O3 43.9(3) . 5_454
La O2 O3 155.8(6) . 5_454
O3 O2 O3 66.9(3) 5_455 5_454
O2 O2 O3 115.12(19) 3_565 5_454
O2 O2 O3 88.4(4) 4_455 5_454
La O2 O3 100.6(4) 4_455 5_454
O3 O2 O3 80.9(3) 2_455 5_454
O1 O2 O3 147.6(4) . 5_454
O2 O2 O3 58.5(3) 6_554 5_454
O3 O2 O3 10.7(3) 4_454 5_454
O1 O2 O3 52.0(2) 1_554 5_454
O3 O2 O3 115.7(4) 4_455 5_454
Nb O2 O3 88.8(3) 1_455 5_454
Ga1 O2 O3 88.8(3) 1_455 5_454
O1 O2 O3 113.2(4) 2_455 5_454
Ga2 O2 O3 87.7(2) 1_554 5_454
O2 O2 O3 140.3(3) 6 5_454
O3 O2 O3 124.8(5) 6 5_454
La O2 O3 56.7(2) 1_554 5_454
Ga3 O2 O3 46.09(19) 2_464 5_454
La O2 O3 24.55(12) 4_454 5_454
Ga3 O2 O3 105.7(3) 2_564 5_454
O3 O2 O3 87.7(3) 1_554 5_454
La O2 O3 124.8(2) 2_565 5_454
Ga3 O2 O3 133.8(3) 1_556 5_454
Ga3 O2 O3 74.26(18) 4_455 5_454
O3 O2 O3 45.0(2) 3_454 5_454
Ga2 O2 O3 152.5(4) 2_566 5_454
O3 O2 O3 158.5(4) . 5_454
O2 O2 O3 88.8(4) 5_444 5_454
O2 O2 O3 52.8(3) 5_454 5_454
La O2 O3 103.6(2) 2_455 5_454
O2 O2 O3 37.7(2) 2_464 5_454
O3 O2 O3 105.8(4) 3_455 5_454
O1 O2 O3 75.1(3) 2_465 5_454
Nb O2 O3 20.82(11) 1_454 5_454
Ga1 O2 O3 20.82(11) 1_454 5_454
O3 O2 O3 67.74(17) 6_455 5_454
Ga2 O2 O3 55.04(19) 1_564 5_454
Ga3 O2 O3 58.10(16) 4_345 5_454
Ga3 O2 O3 106.8(3) 4_445 5_454
O2 O2 O3 30.4(2) 1_554 5_454
O2 O2 O3 149.6(2) 1_556 5_454
O3 O2 O3 70.4(2) 3_564 5_454
O2 O2 O3 146.2(3) 5_445 5_454
O2 O2 O3 108.6(3) 5_455 5_454
O3 O2 O3 35.0(3) 1_454 5_454
O2 O2 O3 97.5(4) 2_465 5_454
O2 O2 O3 78.4(3) 2_454 5_454
O2 O2 O3 93.6(3) 2_564 5_454
La O2 O3 68.72(18) 2_564 5_454
O3 O2 O3 100.0(2) 2_565 5_454
Ga2 O2 O3 142.8(2) . 5_454
O3 O2 O3 119.6(3) 3_565 5_454
O3 O2 O3 92.1(3) 1_455 5_454
Nb O2 O3 137.5(4) . 5_454
Ga1 O2 O3 137.5(4) . 5_454
O3 O2 O3 123.0(4) 5 5_454
O3 O2 O3 85.4(2) 6_565 5_454
Ga2 O2 O3 92.9(4) 2_565 2_454
Ga3 O2 O3 28.0(3) . 2_454
La O2 O3 127.8(5) . 2_454
O3 O2 O3 80.8(3) 5_455 2_454
O2 O2 O3 117.6(3) 3_565 2_454
O2 O2 O3 114.7(3) 4_455 2_454
La O2 O3 125.5(4) 4_455 2_454
O3 O2 O3 66.5(3) 2_455 2_454
O1 O2 O3 176.0(4) . 2_454
O2 O2 O3 30.4(3) 6_554 2_454
O3 O2 O3 28.2(3) 4_454 2_454
O1 O2 O3 62.1(3) 1_554 2_454
O3 O2 O3 121.3(3) 4_455 2_454
Nb O2 O3 88.6(2) 1_455 2_454
Ga1 O2 O3 88.6(2) 1_455 2_454
O1 O2 O3 84.8(4) 2_455 2_454
Ga2 O2 O3 59.4(2) 1_554 2_454
O2 O2 O3 120.7(5) 6 2_454
O3 O2 O3 104.1(4) 6 2_454
La O2 O3 43.21(16) 1_554 2_454
Ga3 O2 O3 61.46(16) 2_464 2_454
La O2 O3 50.20(15) 4_454 2_454
Ga3 O2 O3 100.8(3) 2_564 2_454
O3 O2 O3 76.8(3) 1_554 2_454
La O2 O3 142.2(3) 2_565 2_454
Ga3 O2 O3 128.4(2) 1_556 2_454
Ga3 O2 O3 100.6(2) 4_455 2_454
O3 O2 O3 28.0(3) 3_454 2_454
Ga2 O2 O3 170.0(3) 2_566 2_454
O3 O2 O3 138.7(4) . 2_454
O2 O2 O3 64.1(3) 5_444 2_454
O2 O2 O3 80.9(3) 5_454 2_454
La O2 O3 82.0(2) 2_455 2_454
O2 O2 O3 63.0(2) 2_464 2_454
O3 O2 O3 96.0(3) 3_455 2_454
O1 O2 O3 101.2(3) 2_465 2_454
Nb O2 O3 20.72(11) 1_454 2_454
Ga1 O2 O3 20.72(11) 1_454 2_454
O3 O2 O3 67.60(17) 6_455 2_454
Ga2 O2 O3 82.75(18) 1_564 2_454
Ga3 O2 O3 49.01(15) 4_345 2_454
Ga3 O2 O3 84.9(3) 4_445 2_454
O2 O2 O3 30.73(16) 1_554 2_454
O2 O2 O3 149.26(16) 1_556 2_454
O3 O2 O3 91.6(3) 3_564 2_454
O2 O2 O3 117.7(3) 5_445 2_454
O2 O2 O3 135.1(3) 5_455 2_454
O3 O2 O3 43.1(2) 1_454 2_454
O2 O2 O3 115.1(3) 2_465 2_454
O2 O2 O3 49.8(2) 2_454 2_454
O2 O2 O3 97.1(3) 2_564 2_454
La O2 O3 79.44(19) 2_564 2_454
O3 O2 O3 122.7(3) 2_565 2_454
Ga2 O2 O3 118.1(3) . 2_454
O3 O2 O3 147.0(3) 3_565 2_454
O3 O2 O3 96.8(2) 1_455 2_454
Nb O2 O3 120.1(3) . 2_454
Ga1 O2 O3 120.1(3) . 2_454
O3 O2 O3 115.7(3) 5 2_454
O3 O2 O3 113.6(3) 6_565 2_454
O3 O2 O3 28.56(19) 5_454 2_454
Ga2 O2 La 110.5(5) 2_565 2_454
Ga3 O2 La 26.2(4) . 2_454
La O2 La 104.3(4) . 2_454
O3 O2 La 88.8(3) 5_455 2_454
O2 O2 La 120.3(6) 3_565 2_454
O2 O2 La 139.4(2) 4_455 2_454
La O2 La 138.9(4) 4_455 2_454
O3 O2 La 51.9(3) 2_455 2_454
O1 O2 La 158.9(4) . 2_454
O2 O2 La 13.87(18) 6_554 2_454
O3 O2 La 50.3(3) 4_454 2_454
O1 O2 La 80.7(3) 1_554 2_454
O3 O2 La 113.2(3) 4_455 2_454
Nb O2 La 82.22(18) 1_455 2_454
Ga1 O2 La 82.22(18) 1_455 2_454
O1 O2 La 60.0(3) 2_455 2_454
Ga2 O2 La 36.96(11) 1_554 2_454
O2 O2 La 97.2(4) 6 2_454
O3 O2 La 89.1(3) 6 2_454
La O2 La 48.36(14) 1_554 2_454
Ga3 O2 La 74.19(16) 2_464 2_454
La O2 La 75.27(17) 4_454 2_454
Ga3 O2 La 100.6(3) 2_564 2_454
O3 O2 La 76.0(3) 1_554 2_454
La O2 La 152.1(4) 2_565 2_454
Ga3 O2 La 110.90(19) 1_556 2_454
Ga3 O2 La 125.5(2) 4_455 2_454
O3 O2 La 24.78(17) 3_454 2_454
Ga2 O2 La 148.6(2) 2_566 2_454
O3 O2 La 119.1(4) . 2_454
O2 O2 La 49.4(2) 5_444 2_454
O2 O2 La 105.9(3) 5_454 2_454
La O2 La 59.69(14) 2_455 2_454
O2 O2 La 83.4(2) 2_464 2_454
O3 O2 La 80.6(2) 3_455 2_454
O1 O2 La 120.0(2) 2_465 2_454
Nb O2 La 38.80(9) 1_454 2_454
Ga1 O2 La 38.80(9) 1_454 2_454
O3 O2 La 65.80(18) 6_455 2_454
Ga2 O2 La 104.88(19) 1_564 2_454
Ga3 O2 La 44.08(9) 4_345 2_454
Ga3 O2 La 71.1(2) 4_445 2_454
O2 O2 La 50.57(10) 1_554 2_454
O2 O2 La 129.43(10) 1_556 2_454
O3 O2 La 114.1(2) 3_564 2_454
O2 O2 La 93.18(19) 5_445 2_454
O2 O2 La 150.0(4) 5_455 2_454
O3 O2 La 54.99(15) 1_454 2_454
O2 O2 La 120.6(2) 2_465 2_454
O2 O2 La 25.81(13) 2_454 2_454
O2 O2 La 105.2(4) 2_564 2_454
La O2 La 96.1(2) 2_564 2_454
O3 O2 La 144.0(3) 2_565 2_454
Ga2 O2 La 93.21(19) . 2_454
O3 O2 La 171.7(2) 3_565 2_454
O3 O2 La 93.14(19) 1_455 2_454
Nb O2 La 105.4(3) . 2_454
Ga1 O2 La 105.4(3) . 2_454
O3 O2 La 110.2(3) 5 2_454
O3 O2 La 138.6(2) 6_565 2_454
O3 O2 La 53.16(14) 5_454 2_454
O3 O2 La 25.12(13) 2_454 2_454
Ga2 O2 O2 152.0(3) 2_565 4_345
Ga3 O2 O2 32.4(3) . 4_345
La O2 O2 95.2(4) . 4_345
O3 O2 O2 59.3(2) 5_455 4_345
O2 O2 O2 154.1(8) 3_565 4_345
O2 O2 O2 145.9(8) 4_455 4_345
La O2 O2 102.8(3) 4_455 4_345
O3 O2 O2 7.3(4) 2_455 4_345
O1 O2 O2 123.5(3) . 4_345
O2 O2 O2 56.6(3) 6_554 4_345
O3 O2 O2 65.3(2) 4_454 4_345
O1 O2 O2 121.3(3) 1_554 4_345
O3 O2 O2 68.4(2) 4_455 4_345
Nb O2 O2 38.90(10) 1_455 4_345
Ga1 O2 O2 38.90(10) 1_455 4_345
O1 O2 O2 58.2(2) 2_455 4_345
Ga2 O2 O2 59.1(2) 1_554 4_345
O2 O2 O2 65.6(4) 6 4_345
O3 O2 O2 107.8(4) 6 4_345
La O2 O2 93.2(2) 1_554 4_345
Ga3 O2 O2 58.10(15) 2_464 4_345
La O2 O2 98.56(18) 4_454 4_345
Ga3 O2 O2 137.7(4) 2_564 4_345
O3 O2 O2 116.8(4) 1_554 4_345
La O2 O2 158.42(15) 2_565 4_345
Ga3 O2 O2 69.28(13) 1_556 4_345
Ga3 O2 O2 137.7(4) 4_455 4_345
O3 O2 O2 31.9(2) 3_454 4_345
Ga2 O2 O2 110.87(13) 2_566 4_345
O3 O2 O2 114.9(3) . 4_345
O2 O2 O2 81.4(3) 5_444 4_345
O2 O2 O2 115.1(4) 5_454 4_345
La O2 O2 30.56(18) 2_455 4_345
O2 O2 O2 79.8(3) 2_464 4_345
O3 O2 O2 37.0(2) 3_455 4_345
O1 O2 O2 98.5(3) 2_465 4_345
Nb O2 O2 54.12(13) 1_454 4_345
Ga1 O2 O2 54.12(13) 1_454 4_345
O3 O2 O2 30.46(19) 6_455 4_345
Ga2 O2 O2 98.4(3) 1_564 4_345
Ga3 O2 O2 18.83(12) 4_345 4_345
Ga3 O2 O2 98.0(3) 4_445 4_345
O2 O2 O2 90.000(1) 1_554 4_345
O2 O2 O2 90.000(1) 1_556 4_345
O3 O2 O2 144.3(3) 3_564 4_345
O2 O2 O2 82.5(3) 5_445 4_345
O2 O2 O2 111.8(4) 5_455 4_345
O3 O2 O2 48.2(2) 1_454 4_345
O2 O2 O2 81.0(2) 2_465 4_345
O2 O2 O2 49.22(15) 2_454 4_345
O2 O2 O2 148.9(4) 2_564 4_345
La O2 O2 138.67(13) 2_564 4_345
O3 O2 O2 162.0(4) 2_565 4_345
Ga2 O2 O2 69.2(2) . 4_345
O3 O2 O2 140.9(3) 3_565 4_345
O3 O2 O2 50.52(15) 1_455 4_345
Nb O2 O2 118.1(3) . 4_345
Ga1 O2 O2 118.1(3) . 4_345
O3 O2 O2 136.4(4) 5 4_345
O3 O2 O2 133.3(4) 6_565 4_345
O3 O2 O2 74.86(17) 5_454 4_345
O3 O2 O2 59.27(15) 2_454 4_345
La O2 O2 44.86(13) 2_454 4_345
Ga2 O2 O2 112.7(7) 2_565 3_465
Ga3 O2 O2 58.8(4) . 3_465
La O2 O2 134.3(3) . 3_465
O3 O2 O2 7.4(3) 5_455 3_465
O2 O2 O2 145.9(8) 3_565 3_465
O2 O2 O2 85.9(8) 4_455 3_465
La O2 O2 54.1(3) 4_455 3_465
O3 O2 O2 59.3(2) 2_455 3_465
O1 O2 O2 104.0(5) . 3_465
O2 O2 O2 98.20(17) 6_554 3_465
O3 O2 O2 51.4(4) 4_454 3_465
O1 O2 O2 103.2(4) 1_554 3_465
O3 O2 O2 56.6(2) 4_455 3_465
Nb O2 O2 38.90(10) 1_455 3_465
Ga1 O2 O2 38.90(10) 1_455 3_465
O1 O2 O2 116.8(2) 2_455 3_465
Ga2 O2 O2 116.1(2) 1_554 3_465
O2 O2 O2 96.16(9) 6 3_465
O3 O2 O2 166.8(4) 6 3_465
La O2 O2 115.26(16) 1_554 3_465
Ga3 O2 O2 13.79(16) 2_464 3_465
La O2 O2 66.8(3) 4_454 3_465
Ga3 O2 O2 156.7(4) 2_564 3_465
O3 O2 O2 147.2(2) 1_554 3_465
La O2 O2 119.3(5) 2_565 3_465
Ga3 O2 O2 77.45(14) 1_556 3_465
Ga3 O2 O2 79.6(4) 4_455 3_465
O3 O2 O2 60.26(16) 3_454 3_465
Ga2 O2 O2 99.0(3) 2_566 3_465
O3 O2 O2 141.9(3) . 3_465
O2 O2 O2 134.2(3) 5_444 3_465
O2 O2 O2 61.4(4) 5_454 3_465
La O2 O2 83.80(14) 2_455 3_465
O2 O2 O2 30.5(4) 2_464 3_465
O3 O2 O2 62.20(17) 3_455 3_465
O1 O2 O2 39.4(3) 2_465 3_465
Nb O2 O2 54.12(13) 1_454 3_465
Ga1 O2 O2 54.12(13) 1_454 3_465
O3 O2 O2 30.1(2) 6_455 3_465
Ga2 O2 O2 40.4(3) 1_564 3_465
Ga3 O2 O2 46.04(8) 4_345 3_465
Ga3 O2 O2 155.5(3) 4_445 3_465
O2 O2 O2 90.0 1_554 3_465
O2 O2 O2 90.0 1_556 3_465
O3 O2 O2 94.6(4) 3_564 3_465
O2 O2 O2 127.7(3) 5_445 3_465
O2 O2 O2 65.2(3) 5_455 3_465
O3 O2 O2 31.84(15) 1_454 3_465
O2 O2 O2 40.4(3) 2_465 3_465
O2 O2 O2 104.24(14) 2_454 3_465
O2 O2 O2 137.8(5) 2_564 3_465
La O2 O2 113.3(3) 2_564 3_465
O3 O2 O2 102.3(4) 2_565 3_465
Ga2 O2 O2 107.68(12) . 3_465
O3 O2 O2 94.4(4) 3_565 3_465
O3 O2 O2 35.80(17) 1_455 3_465
Nb O2 O2 162.89(14) . 3_465
Ga1 O2 O2 162.89(14) . 3_465
O3 O2 O2 163.0(4) 5 3_465
O3 O2 O2 73.5(4) 6_565 3_465
O3 O2 O2 59.6(2) 5_454 3_465
O3 O2 O2 74.74(13) 2_454 3_465
La O2 O2 84.90(12) 2_454 3_465
O2 O2 O2 60.0 4_345 3_465
Ga2 O2 O1 88.2(5) 2_565 2_454
Ga3 O2 O1 50.6(4) . 2_454
La O2 O1 98.1(5) . 2_454
O3 O2 O1 112.1(3) 5_455 2_454
O2 O2 O1 94.2(5) 3_565 2_454
O2 O2 O1 125.1(2) 4_455 2_454
La O2 O1 158.3(3) 4_455 2_454
O3 O2 O1 76.9(4) 2_455 2_454
O1 O2 O1 148.9(5) . 2_454
O2 O2 O1 13.7(2) 6_554 2_454
O3 O2 O1 60.7(4) 4_454 2_454
O1 O2 O1 61.9(3) 1_554 2_454
O3 O2 O1 138.1(3) 4_455 2_454
Nb O2 O1 108.5(2) 1_455 2_454
Ga1 O2 O1 108.5(2) 1_455 2_454
O1 O2 O1 62.8(3) 2_455 2_454
Ga2 O2 O1 34.07(16) 1_554 2_454
O2 O2 O1 108.7(5) 6 2_454
O3 O2 O1 71.0(3) 6 2_454
La O2 O1 23.77(11) 1_554 2_454
Ga3 O2 O1 94.1(2) 2_464 2_454
La O2 O1 71.9(2) 4_454 2_454
Ga3 O2 O1 74.7(3) 2_564 2_454
O3 O2 O1 49.9(2) 1_554 2_454
La O2 O1 125.8(3) 2_565 2_454
Ga3 O2 O1 129.4(3) 1_556 2_454
Ga3 O2 O1 114.5(2) 4_455 2_454
O3 O2 O1 49.5(2) 3_454 2_454
Ga2 O2 O1 149.6(3) 2_566 2_454
O3 O2 O1 105.8(4) . 2_454
O2 O2 O1 31.3(3) 5_444 2_454
O2 O2 O1 103.3(3) 5_454 2_454
La O2 O1 77.5(2) 2_455 2_454
O2 O2 O1 95.1(3) 2_464 2_454
O3 O2 O1 103.8(3) 3_455 2_454
O1 O2 O1 133.0(3) 2_465 2_454
Nb O2 O1 53.62(15) 1_454 2_454
Ga1 O2 O1 53.62(15) 1_454 2_454
O3 O2 O1 91.9(2) 6_455 2_454
Ga2 O2 O1 112.5(2) 1_564 2_454
Ga3 O2 O1 70.22(15) 4_345 2_454
Ga3 O2 O1 51.86(17) 4_445 2_454
O2 O2 O1 38.74(14) 1_554 2_454
O2 O2 O1 141.27(14) 1_556 2_454
O3 O2 O1 97.1(2) 3_564 2_454
O2 O2 O1 91.2(2) 5_445 2_454
O2 O2 O1 166.0(3) 5_455 2_454
O3 O2 O1 74.98(18) 1_454 2_454
O2 O2 O1 145.8(3) 2_465 2_454
O2 O2 O1 31.1(2) 2_454 2_454
O2 O2 O1 79.0(4) 2_564 2_454
La O2 O1 74.1(2) 2_564 2_454
O3 O2 O1 122.1(3) 2_565 2_454
Ga2 O2 O1 100.0(3) . 2_454
O3 O2 O1 148.8(3) 3_565 2_454
O3 O2 O1 119.5(2) 1_455 2_454
Nb O2 O1 87.1(3) . 2_454
Ga1 O2 O1 87.1(3) . 2_454
O3 O2 O1 86.2(3) 5 2_454
O3 O2 O1 131.6(3) 6_565 2_454
O3 O2 O1 57.9(2) 5_454 2_454
O3 O2 O1 33.09(14) 2_454 2_454
La O2 O1 26.38(7) 2_454 2_454
O2 O2 O1 70.32(18) 4_345 2_454
O2 O2 O1 106.76(13) 3_465 2_454
Ga2 O2 Ga3 129.1(6) 2_565 2_465
Ga3 O2 Ga3 89.3(5) . 2_465
La O2 Ga3 90.7(4) . 2_465
O3 O2 Ga3 38.3(3) 5_455 2_465
O2 O2 Ga3 126.8(3) 3_565 2_465
O2 O2 Ga3 89.2(5) 4_455 2_465
La O2 Ga3 38.52(18) 4_455 2_465
O3 O2 Ga3 61.5(4) 2_455 2_465
O1 O2 Ga3 65.9(3) . 2_465
O2 O2 Ga3 124.1(3) 6_554 2_465
O3 O2 Ga3 96.3(4) 4_454 2_465
O1 O2 Ga3 141.7(4) 1_554 2_465
O3 O2 Ga3 11.5(2) 4_455 2_465
Nb O2 Ga3 29.16(14) 1_455 2_465
Ga1 O2 Ga3 29.16(14) 1_455 2_465
O1 O2 Ga3 98.1(3) 2_455 2_465
Ga2 O2 Ga3 119.3(2) 1_554 2_465
O2 O2 Ga3 57.3(2) 6 2_465
O3 O2 Ga3 127.4(3) 6 2_465
La O2 Ga3 157.6(3) 1_554 2_465
Ga3 O2 Ga3 59.1(2) 2_464 2_465
La O2 Ga3 109.3(3) 4_454 2_465
Ga3 O2 Ga3 144.8(3) 2_564 2_465
O3 O2 Ga3 167.1(3) 1_554 2_465
La O2 Ga3 96.2(3) 2_565 2_465
Ga3 O2 Ga3 33.98(13) 1_556 2_465
Ga3 O2 Ga3 93.6(3) 4_455 2_465
O3 O2 Ga3 90.1(3) 3_454 2_465
Ga2 O2 Ga3 56.86(17) 2_566 2_465
O3 O2 Ga3 96.4(2) . 2_465
O2 O2 Ga3 140.6(3) 5_444 2_465
O2 O2 Ga3 89.9(3) 5_454 2_465
La O2 Ga3 69.15(17) 2_455 2_465
O2 O2 Ga3 72.8(4) 2_464 2_465
O3 O2 Ga3 39.13(17) 3_455 2_465
O1 O2 Ga3 51.3(2) 2_465 2_465
Nb O2 Ga3 96.0(2) 1_454 2_465
Ga1 O2 Ga3 96.0(2) 1_454 2_465
O3 O2 Ga3 47.50(18) 6_455 2_465
Ga2 O2 Ga3 69.4(2) 1_564 2_465
Ga3 O2 Ga3 68.37(18) 4_345 2_465
Ga3 O2 Ga3 139.7(2) 4_445 2_465
O2 O2 Ga3 135.58(11) 1_554 2_465
O2 O2 Ga3 44.41(11) 1_556 2_465
O3 O2 Ga3 114.0(3) 3_564 2_465
O2 O2 Ga3 88.5(3) 5_445 2_465
O2 O2 Ga3 45.1(3) 5_455 2_465
O3 O2 Ga3 73.5(2) 1_454 2_465
O2 O2 Ga3 18.61(12) 2_465 2_465
O2 O2 Ga3 113.8(2) 2_454 2_465
O2 O2 Ga3 143.3(3) 2_564 2_465
La O2 Ga3 140.4(3) 2_564 2_465
O3 O2 Ga3 97.8(3) 2_565 2_465
Ga2 O2 Ga3 69.77(14) . 2_465
O3 O2 Ga3 73.3(2) 3_565 2_465
O3 O2 Ga3 18.46(13) 1_455 2_465
Nb O2 Ga3 117.23(19) . 2_465
Ga1 O2 Ga3 117.23(19) . 2_465
O3 O2 Ga3 129.1(2) 5 2_465
O3 O2 Ga3 77.8(2) 6_565 2_465
O3 O2 Ga3 105.1(3) 5_454 2_465
O3 O2 Ga3 114.5(2) 2_454 2_465
La O2 Ga3 111.36(19) 2_454 2_465
O2 O2 Ga3 67.64(12) 4_345 2_465
O2 O2 Ga3 45.66(11) 3_465 2_465
O1 O2 Ga3 137.6(2) 2_454 2_465
Ga2 O2 O2 39.0(3) 2_565 3_564
Ga3 O2 O2 86.1(4) . 3_564
La O2 O2 111.8(6) . 3_564
O3 O2 O2 120.9(4) 5_455 3_564
O2 O2 O2 61.12(15) 3_565 3_564
O2 O2 O2 76.02(7) 4_455 3_564
La O2 O2 123.8(4) 4_455 3_564
O3 O2 O2 123.0(5) 2_455 3_564
O1 O2 O2 119.8(3) . 3_564
O2 O2 O2 62.6(3) 6_554 3_564
O3 O2 O2 66.9(3) 4_454 3_564
O1 O2 O2 15.14(10) 1_554 3_564
O3 O2 O2 167.0(5) 4_455 3_564
Nb O2 O2 144.8(3) 1_455 3_564
Ga1 O2 O2 144.8(3) 1_455 3_564
O1 O2 O2 103.3(6) 2_455 3_564
Ga2 O2 O2 78.2(4) 1_554 3_564
O2 O2 O2 146.6(5) 6 3_564
O3 O2 O2 75.4(4) 6 3_564
La O2 O2 26.24(18) 1_554 3_564
Ga3 O2 O2 101.39(18) 2_464 3_564
La O2 O2 47.52(8) 4_454 3_564
Ga3 O2 O2 49.1(2) 2_564 3_564
O3 O2 O2 35.0(2) 1_554 3_564
La O2 O2 84.9(2) 2_565 3_564
Ga3 O2 O2 169.0(4) 1_556 3_564
Ga3 O2 O2 67.76(17) 4_455 3_564
O3 O2 O2 86.0(3) 3_454 3_564
Ga2 O2 O2 131.9(3) 2_566 3_564
O3 O2 O2 102.5(4) . 3_564
O2 O2 O2 60.1(5) 5_444 3_564
O2 O2 O2 67.0(2) 5_454 3_564
La O2 O2 126.8(4) 2_455 3_564
O2 O2 O2 84.4(3) 2_464 3_564
O3 O2 O2 152.4(4) 3_455 3_564
O1 O2 O2 105.8(3) 2_465 3_564
Nb O2 O2 71.42(16) 1_454 3_564
Ga1 O2 O2 71.42(16) 1_454 3_564
O3 O2 O2 123.1(2) 6_455 3_564
Ga2 O2 O2 86.82(19) 1_564 3_564
Ga3 O2 O2 107.0(2) 4_345 3_564
Ga3 O2 O2 64.2(3) 4_445 3_564
O2 O2 O2 28.88(15) 1_554 3_564
O2 O2 O2 151.12(15) 1_556 3_564
O3 O2 O2 48.41(18) 3_564 3_564
O2 O2 O2 115.3(5) 5_445 3_564
O2 O2 O2 121.4(3) 5_455 3_564
O3 O2 O2 91.3(2) 1_454 3_564
O2 O2 O2 139.1(4) 2_465 3_564
O2 O2 O2 79.7(5) 2_454 3_564
O2 O2 O2 39.5(3) 2_564 3_564
La O2 O2 24.63(13) 2_564 3_564
O3 O2 O2 73.1(2) 2_565 3_564
Ga2 O2 O2 134.1(5) . 3_564
O3 O2 O2 101.1(2) 3_565 3_564
O3 O2 O2 148.5(3) 1_455 3_564
Nb O2 O2 83.0(3) . 3_564
Ga1 O2 O2 83.0(3) . 3_564
O3 O2 O2 66.4(3) 5 3_564
O3 O2 O2 84.9(3) 6_565 3_564
O3 O2 O2 56.65(18) 5_454 3_564
O3 O2 O2 58.1(2) 2_454 3_564
La O2 O2 71.8(3) 2_454 3_564
O2 O2 O2 115.8(2) 4_345 3_564
O2 O2 O2 113.6(3) 3_465 3_564
O1 O2 O2 49.6(3) 2_454 3_564
Ga3 O2 O2 156.1(4) 2_465 3_564
Ga2 O2 O2 39.0(3) 2_565 4_454
Ga3 O2 O2 81.3(3) . 4_454
La O2 O2 137.5(6) . 4_454
O3 O2 O2 94.9(4) 5_455 4_454
O2 O2 O2 76.02(7) 3_565 4_454
O2 O2 O2 61.12(15) 4_455 4_454
La O2 O2 100.2(3) 4_455 4_454
O3 O2 O2 120.2(4) 2_455 4_454
O1 O2 O2 119.8(3) . 4_454
O2 O2 O2 75.7(3) 6_554 4_454
O3 O2 O2 50.3(3) 4_454 4_454
O1 O2 O2 15.14(10) 1_554 4_454
O3 O2 O2 139.3(5) 4_455 4_454
Nb O2 O2 125.0(4) 1_455 4_454
Ga1 O2 O2 125.0(4) 1_455 4_454
O1 O2 O2 127.6(4) 2_455 4_454
Ga2 O2 O2 99.5(2) 1_554 4_454
O2 O2 O2 174.2(6) 6 4_454
O3 O2 O2 102.5(4) 6 4_454
La O2 O2 47.69(8) 1_554 4_454
Ga3 O2 O2 77.6(3) 2_464 4_454
La O2 O2 21.43(14) 4_454 4_454
Ga3 O2 O2 71.1(3) 2_564 4_454
O3 O2 O2 62.5(3) 1_554 4_454
La O2 O2 87.5(3) 2_565 4_454
Ga3 O2 O2 161.2(4) 1_556 4_454
Ga3 O2 O2 48.75(19) 4_455 4_454
O3 O2 O2 82.0(2) 3_454 4_454
Ga2 O2 O2 131.9(3) 2_566 4_454
O3 O2 O2 123.5(4) . 4_454
O2 O2 O2 85.8(4) 5_444 4_454
O2 O2 O2 40.5(3) 5_454 4_454
La O2 O2 138.4(2) 2_455 4_454
O2 O2 O2 57.8(2) 2_464 4_454
O3 O2 O2 145.2(4) 3_455 4_454
O1 O2 O2 78.9(3) 2_465 4_454
Nb O2 O2 59.9(2) 1_454 4_454
Ga1 O2 O2 59.9(2) 1_454 4_454
O3 O2 O2 105.9(4) 6_455 4_454
Ga2 O2 O2 59.0(2) 1_564 4_454
Ga3 O2 O2 97.8(3) 4_345 4_454
Ga3 O2 O2 92.1(3) 4_445 4_454
O2 O2 O2 28.88(15) 1_554 4_454
O2 O2 O2 151.12(15) 1_556 4_454
O3 O2 O2 35.2(2) 3_564 4_454
O2 O2 O2 143.0(5) 5_445 4_454
O2 O2 O2 101.3(3) 5_455 4_454
O3 O2 O2 73.3(3) 1_454 4_454
O2 O2 O2 111.7(4) 2_465 4_454
O2 O2 O2 96.7(3) 2_454 4_454
O2 O2 O2 55.4(2) 2_564 4_454
La O2 O2 29.31(19) 2_564 4_454
O3 O2 O2 66.2(3) 2_565 4_454
Ga2 O2 O2 162.0(4) . 4_454
O3 O2 O2 92.7(2) 3_565 4_454
O3 O2 O2 123.8(4) 1_455 4_454
Nb O2 O2 107.1(4) . 4_454
Ga1 O2 O2 107.1(4) . 4_454
O3 O2 O2 87.4(3) 5 4_454
O3 O2 O2 65.6(2) 6_565 4_454
O3 O2 O2 39.8(2) 5_454 4_454
O3 O2 O2 56.6(2) 2_454 4_454
La O2 O2 79.07(14) 2_454 4_454
O2 O2 O2 113.6(3) 4_345 4_454
O2 O2 O2 88.0(4) 3_465 4_454
O1 O2 O2 66.08(14) 2_454 4_454
Ga3 O2 O2 128.2(4) 2_465 4_454
O2 O2 O2 27.95(13) 3_564 4_454
Ga2 O2 O2 92.1(4) 2_565 3_566
Ga3 O2 O2 148.1(4) . 3_566
La O2 O2 39.8(2) . 3_566
O3 O2 O2 106.8(4) 5_455 3_566
O2 O2 O2 61.12(15) 3_565 3_566
O2 O2 O2 76.02(7) 4_455 3_566
La O2 O2 65.8(2) 4_455 3_566
O3 O2 O2 108.9(4) 2_455 3_566
O1 O2 O2 16.11(12) . 3_566
O2 O2 O2 137.3(5) 6_554 3_566
O3 O2 O2 163.4(6) 4_454 3_566
O1 O2 O2 121.9(4) 1_554 3_566
O3 O2 O2 61.58(19) 4_455 3_566
Nb O2 O2 92.80(18) 1_455 3_566
Ga1 O2 O2 92.80(18) 1_455 3_566
O1 O2 O2 83.1(3) 2_455 3_566
Ga2 O2 O2 108.2(4) 1_554 3_566
O2 O2 O2 51.10(19) 6 3_566
O3 O2 O2 65.6(3) 6 3_566
La O2 O2 130.9(4) 1_554 3_566
Ga3 O2 O2 127.3(4) 2_464 3_566
La O2 O2 140.7(4) 4_454 3_566
Ga3 O2 O2 75.3(2) 2_564 3_566
O3 O2 O2 97.3(3) 1_554 3_566
La O2 O2 43.0(2) 2_565 3_566
Ga3 O2 O2 49.13(12) 1_556 3_566
Ga3 O2 O2 90.2(3) 4_455 3_566
O3 O2 O2 147.5(3) 3_454 3_566
Ga2 O2 O2 14.70(7) 2_566 3_566
O3 O2 O2 30.32(19) . 3_566
O2 O2 O2 104.6(4) 5_444 3_566
O2 O2 O2 111.0(4) 5_454 3_566
La O2 O2 89.6(2) 2_455 3_566
O2 O2 O2 128.9(6) 2_464 3_566
O3 O2 O2 80.8(2) 3_455 3_566
O1 O2 O2 90.6(3) 2_465 3_566
Nb O2 O2 166.1(3) 1_454 3_566
Ga1 O2 O2 166.1(3) 1_454 3_566
O3 O2 O2 114.5(2) 6_455 3_566
Ga2 O2 O2 109.6(4) 1_564 3_566
Ga3 O2 O2 129.7(2) 4_345 3_566
Ga3 O2 O2 84.6(3) 4_445 3_566
O2 O2 O2 151.12(15) 1_554 3_566
O2 O2 O2 28.88(15) 1_556 3_566
O3 O2 O2 96.7(3) 3_564 3_566
O2 O2 O2 50.0(3) 5_445 3_566
O2 O2 O2 56.7(3) 5_455 3_566
O3 O2 O2 143.8(3) 1_454 3_566
O2 O2 O2 73.3(2) 2_465 3_566
O2 O2 O2 117.9(5) 2_454 3_566
O2 O2 O2 82.8(3) 2_564 3_566
La O2 O2 104.3(2) 2_564 3_566
O3 O2 O2 65.9(3) 2_565 3_566
Ga2 O2 O2 51.6(2) . 3_566
O3 O2 O2 44.3(2) 3_565 3_566
O3 O2 O2 86.57(18) 1_455 3_566
Nb O2 O2 50.38(19) . 3_566
Ga1 O2 O2 50.38(19) . 3_566
O3 O2 O2 58.8(2) 5 3_566
O3 O2 O2 78.3(3) 6_565 3_566
O3 O2 O2 163.7(4) 5_454 3_566
O3 O2 O2 167.6(5) 2_454 3_566
La O2 O2 143.1(4) 2_454 3_566
O2 O2 O2 115.8(2) 4_345 3_566
O2 O2 O2 113.6(3) 3_465 3_566
O1 O2 O2 135.9(4) 2_454 3_566
Ga3 O2 O2 70.35(12) 2_465 3_566
O2 O2 O2 122.2(3) 3_564 3_566
O2 O2 O2 130.5(2) 4_454 3_566
Ga2 O2 O2 92.1(4) 2_565 4_456
Ga3 O2 O2 140.0(7) . 4_456
La O2 O2 66.3(2) . 4_456
O3 O2 O2 82.1(5) 5_455 4_456
O2 O2 O2 76.02(7) 3_565 4_456
O2 O2 O2 61.12(15) 4_455 4_456
La O2 O2 37.9(2) 4_455 4_456
O3 O2 O2 106.3(5) 2_455 4_456
O1 O2 O2 16.11(12) . 4_456
O2 O2 O2 161.4(5) 6_554 4_456
O3 O2 O2 135.5(6) 4_454 4_456
O1 O2 O2 121.9(4) 1_554 4_456
O3 O2 O2 46.2(3) 4_455 4_456
Nb O2 O2 78.8(4) 1_455 4_456
Ga1 O2 O2 78.8(4) 1_455 4_456
O1 O2 O2 105.0(3) 2_455 4_456
Ga2 O2 O2 133.0(3) 1_554 4_456
O2 O2 O2 62.1(4) 6 4_456
O3 O2 O2 93.1(3) 6 4_456
La O2 O2 151.4(4) 1_554 4_456
Ga3 O2 O2 101.2(5) 2_464 4_456
La O2 O2 121.2(4) 4_454 4_456
Ga3 O2 O2 94.4(2) 2_564 4_456
O3 O2 O2 119.1(3) 1_554 4_456
La O2 O2 46.74(16) 2_565 4_456
Ga3 O2 O2 46.44(18) 1_556 4_456
Ga3 O2 O2 73.9(3) 4_455 4_456
O3 O2 O2 140.7(5) 3_454 4_456
Ga2 O2 O2 14.70(7) 2_566 4_456
O3 O2 O2 58.11(16) . 4_456
O2 O2 O2 132.5(3) 5_444 4_456
O2 O2 O2 89.4(4) 5_454 4_456
La O2 O2 98.2(2) 2_455 4_456
O2 O2 O2 101.0(5) 2_464 4_456
O3 O2 O2 77.0(3) 3_455 4_456
O1 O2 O2 63.0(4) 2_465 4_456
Nb O2 O2 141.9(5) 1_454 4_456
Ga1 O2 O2 141.9(5) 1_454 4_456
O3 O2 O2 98.3(4) 6_455 4_456
Ga2 O2 O2 82.9(3) 1_564 4_456
Ga3 O2 O2 118.8(4) 4_345 4_456
Ga3 O2 O2 112.2(3) 4_445 4_456
O2 O2 O2 151.12(15) 1_554 4_456
O2 O2 O2 28.88(15) 1_556 4_456
O3 O2 O2 87.9(3) 3_564 4_456
O2 O2 O2 74.3(2) 5_445 4_456
O2 O2 O2 29.2(3) 5_455 4_456
O3 O2 O2 119.8(5) 1_454 4_456
O2 O2 O2 47.8(2) 2_465 4_456
O2 O2 O2 139.8(3) 2_454 4_456
O2 O2 O2 94.5(2) 2_564 4_456
La O2 O2 106.5(2) 2_564 4_456
O3 O2 O2 58.6(2) 2_565 4_456
Ga2 O2 O2 68.51(11) . 4_456
O3 O2 O2 30.49(17) 3_565 4_456
O3 O2 O2 69.1(3) 1_455 4_456
Nb O2 O2 77.24(18) . 4_456
Ga1 O2 O2 77.24(18) . 4_456
O3 O2 O2 80.7(2) 5 4_456
O3 O2 O2 58.2(2) 6_565 4_456
O3 O2 O2 137.9(4) 5_454 4_456
O3 O2 O2 162.7(5) 2_454 4_456
La O2 O2 157.3(3) 2_454 4_456
O2 O2 O2 113.6(3) 4_345 4_456
O2 O2 O2 88.0(4) 3_465 4_456
O1 O2 O2 163.9(4) 2_454 4_456
Ga3 O2 O2 50.8(3) 2_465 4_456
O2 O2 O2 130.5(2) 3_564 4_456
O2 O2 O2 122.2(3) 4_454 4_456
O2 O2 O2 27.95(13) 3_566 4_456
Ga2 O2 O2 144.3(7) 2_565 2_455
Ga3 O2 O2 81.5(2) . 2_455
La O2 O2 41.4(3) . 2_455
O3 O2 O2 97.9(4) 5_455 2_455
O2 O2 O2 105.7(7) 3_565 2_455
O2 O2 O2 145.45(19) 4_455 2_455
La O2 O2 108.1(4) 4_455 2_455
O3 O2 O2 50.0(2) 2_455 2_455
O1 O2 O2 84.1(3) . 2_455
O2 O2 O2 76.0(4) 6_554 2_455
O3 O2 O2 117.3(3) 4_454 2_455
O1 O2 O2 142.4(6) 1_554 2_455
O3 O2 O2 65.5(3) 4_455 2_455
Nb O2 O2 64.59(18) 1_455 2_455
Ga1 O2 O2 64.59(18) 1_455 2_455
O1 O2 O2 24.1(2) 2_455 2_455
Ga2 O2 O2 51.4(2) 1_554 2_455
O2 O2 O2 23.9(2) 6 2_455
O3 O2 O2 64.1(4) 6 2_455
La O2 O2 103.8(4) 1_554 2_455
Ga3 O2 O2 107.6(3) 2_464 2_455
La O2 O2 149.4(3) 4_454 2_455
Ga3 O2 O2 100.5(4) 2_564 2_455
O3 O2 O2 97.8(5) 1_554 2_455
La O2 O2 109.4(3) 2_565 2_455
Ga3 O2 O2 46.51(18) 1_556 2_455
Ga3 O2 O2 159.3(4) 4_455 2_455
O3 O2 O2 80.29(17) 3_454 2_455
Ga2 O2 O2 73.6(2) 2_566 2_455
O3 O2 O2 61.1(3) . 2_455
O2 O2 O2 67.16(17) 5_444 2_455
O2 O2 O2 163.6(6) 5_454 2_455
La O2 O2 23.27(7) 2_455 2_455
O2 O2 O2 130.8(4) 2_464 2_455
O3 O2 O2 41.49(19) 3_455 2_455
O1 O2 O2 126.2(5) 2_465 2_455
Nb O2 O2 104.84(14) 1_454 2_455
Ga1 O2 O2 104.84(14) 1_454 2_455
O3 O2 O2 75.6(3) 6_455 2_455
Ga2 O2 O2 141.5(5) 1_564 2_455
Ga3 O2 O2 72.62(9) 4_345 2_455
Ga3 O2 O2 66.9(3) 4_445 2_455
O2 O2 O2 122.9(3) 1_554 2_455
O2 O2 O2 57.1(3) 1_556 2_455
O3 O2 O2 161.1(4) 3_564 2_455
O2 O2 O2 28.9(2) 5_445 2_455
O2 O2 O2 107.8(5) 5_455 2_455
O3 O2 O2 101.9(2) 1_454 2_455
O2 O2 O2 93.2(3) 2_465 2_455
O2 O2 O2 54.56(16) 2_454 2_455
O2 O2 O2 119.4(6) 2_564 2_455
La O2 O2 142.0(5) 2_564 2_455
O3 O2 O2 134.9(3) 2_565 2_455
Ga2 O2 O2 18.28(13) . 2_455
O3 O2 O2 113.0(3) 3_565 2_455
O3 O2 O2 71.5(3) 1_455 2_455
Nb O2 O2 67.8(3) . 2_455
Ga1 O2 O2 67.8(3) . 2_455
O3 O2 O2 88.9(4) 5 2_455
O3 O2 O2 143.4(4) 6_565 2_455
O3 O2 O2 124.99(19) 5_454 2_455
O3 O2 O2 99.8(2) 2_454 2_455
La O2 O2 75.14(18) 2_454 2_455
O2 O2 O2 53.83(13) 4_345 2_455
O2 O2 O2 102.84(14) 3_465 2_455
O1 O2 O2 84.8(3) 2_454 2_455
Ga3 O2 O2 74.8(3) 2_465 2_455
O2 O2 O2 127.3(6) 3_564 2_455
O2 O2 O2 150.9(4) 4_454 2_455
O2 O2 O2 69.8(3) 3_566 2_455
O2 O2 O2 85.5(3) 4_456 2_455
Ga2 O2 O2 65.8(2) 2_565 2_565
Ga3 O2 O2 167.0(7) . 2_565
La O2 O2 48.0(3) . 2_565
O3 O2 O2 127.1(6) 5_455 2_565
O2 O2 O2 33.0(2) 3_565 2_565
O2 O2 O2 62.8(3) 4_455 2_565
La O2 O2 78.0(3) 4_455 2_565
O3 O2 O2 134.8(4) 2_455 2_565
O1 O2 O2 29.93(16) . 2_565
O2 O2 O2 129.7(4) 6_554 2_565
O3 O2 O2 154.0(3) 4_454 2_565
O1 O2 O2 94.2(3) 1_554 2_565
O3 O2 O2 88.5(4) 4_455 2_565
Nb O2 O2 120.7(4) 1_455 2_565
Ga1 O2 O2 120.7(4) 1_455 2_565
O1 O2 O2 91.7(4) 2_455 2_565
Ga2 O2 O2 107.2(4) 1_554 2_565
O2 O2 O2 75.4(4) 6 2_565
O3 O2 O2 53.4(3) 6 2_565
La O2 O2 106.7(4) 1_554 2_565
Ga3 O2 O2 143.3(5) 2_464 2_565
La O2 O2 120.71(16) 4_454 2_565
Ga3 O2 O2 49.1(2) 2_564 2_565
O3 O2 O2 73.3(3) 1_554 2_565
La O2 O2 21.89(6) 2_565 2_565
Ga3 O2 O2 77.4(3) 1_556 2_565
Ga3 O2 O2 75.73(11) 4_455 2_565
O3 O2 O2 165.3(5) 3_454 2_565
Ga2 O2 O2 39.24(19) 2_566 2_565
O3 O2 O2 28.6(2) . 2_565
O2 O2 O2 93.3(5) 5_444 2_565
O2 O2 O2 99.5(2) 5_454 2_565
La O2 O2 110.9(3) 2_455 2_565
O2 O2 O2 130.8(4) 2_464 2_565
O3 O2 O2 108.6(3) 3_455 2_565
O1 O2 O2 97.1(3) 2_465 2_565
Nb O2 O2 164.5(3) 1_454 2_565
Ga1 O2 O2 164.5(3) 1_454 2_565
O3 O2 O2 142.2(5) 6_455 2_565
Ga2 O2 O2 108.8(3) 1_564 2_565
Ga3 O2 O2 157.4(3) 4_345 2_565
Ga3 O2 O2 71.5(3) 4_445 2_565
O2 O2 O2 122.9(3) 1_554 2_565
O2 O2 O2 57.1(3) 1_556 2_565
O3 O2 O2 74.71(18) 3_564 2_565
O2 O2 O2 61.0(4) 5_445 2_565
O2 O2 O2 67.0(3) 5_455 2_565
O3 O2 O2 162.4(5) 1_454 2_565
O2 O2 O2 93.2(3) 2_465 2_565
O2 O2 O2 119.4(6) 2_454 2_565
O2 O2 O2 54.56(16) 2_564 2_565
La O2 O2 76.70(17) 2_564 2_565
O3 O2 O2 47.68(14) 2_565 2_565
Ga2 O2 O2 71.6(2) . 2_565
O3 O2 O2 40.12(19) 3_565 2_565
O3 O2 O2 113.2(4) 1_455 2_565
Nb O2 O2 37.3(2) . 2_565
Ga1 O2 O2 37.3(2) . 2_565
O3 O2 O2 34.9(2) 5 2_565
O3 O2 O2 70.7(2) 6_565 2_565
O3 O2 O2 144.3(2) 5_454 2_565
O3 O2 O2 149.9(5) 2_454 2_565
La O2 O2 142.5(5) 2_454 2_565
O2 O2 O2 140.7(2) 4_345 2_565
O2 O2 O2 132.0(5) 3_465 2_565
O1 O2 O2 120.8(5) 2_454 2_565
Ga3 O2 O2 95.6(3) 2_465 2_565
O2 O2 O2 94.0(3) 3_564 2_565
O2 O2 O2 104.7(3) 4_454 2_565
O2 O2 O2 28.3(3) 3_566 2_565
O2 O2 O2 45.85(15) 4_456 2_565
O2 O2 O2 88.1(3) 2_455 2_565
Ga2 O2 Ga3 83.3(3) 2_565 2_565
Ga3 O2 Ga3 151.1(5) . 2_565
La O2 Ga3 31.14(18) . 2_565
O3 O2 Ga3 125.1(4) 5_455 2_565
O2 O2 Ga3 46.9(2) 3_565 2_565
O2 O2 Ga3 79.3(3) 4_455 2_565
La O2 Ga3 82.0(2) 4_455 2_565
O3 O2 Ga3 116.8(4) 2_455 2_565
O1 O2 Ga3 29.87(18) . 2_565
O2 O2 Ga3 123.8(3) 6_554 2_565
O3 O2 Ga3 172.2(3) 4_454 2_565
O1 O2 Ga3 110.0(3) 1_554 2_565
O3 O2 Ga3 78.8(2) 4_455 2_565
Nb O2 Ga3 108.3(2) 1_455 2_565
Ga1 O2 Ga3 108.3(2) 1_455 2_565
O1 O2 Ga3 76.2(2) 2_455 2_565
Ga2 O2 Ga3 96.6(3) 1_554 2_565
O2 O2 Ga3 57.6(3) 6 2_565
O3 O2 Ga3 48.3(2) 6 2_565
La O2 Ga3 112.6(3) 1_554 2_565
Ga3 O2 Ga3 145.5(4) 2_464 2_565
La O2 Ga3 139.0(2) 4_454 2_565
Ga3 O2 Ga3 58.24(13) 2_564 2_565
O3 O2 Ga3 79.3(2) 1_554 2_565
La O2 Ga3 39.51(9) 2_565 2_565
Ga3 O2 Ga3 63.31(13) 1_556 2_565
Ga3 O2 Ga3 92.86(18) 4_455 2_565
O3 O2 Ga3 149.6(3) 3_454 2_565
Ga2 O2 Ga3 32.86(8) 2_566 2_565
O3 O2 Ga3 14.48(15) . 2_565
O2 O2 Ga3 88.4(3) 5_444 2_565
O2 O2 Ga3 116.2(3) 5_454 2_565
La O2 Ga3 92.64(17) 2_455 2_565
O2 O2 Ga3 143.0(4) 2_464 2_565
O3 O2 Ga3 92.4(2) 3_455 2_565
O1 O2 Ga3 105.4(3) 2_465 2_565
Nb O2 Ga3 172.3(4) 1_454 2_565
Ga1 O2 Ga3 172.3(4) 1_454 2_565
O3 O2 Ga3 129.9(3) 6_455 2_565
Ga2 O2 Ga3 121.5(3) 1_564 2_565
Ga3 O2 Ga3 139.9(2) 4_345 2_565
Ga3 O2 Ga3 67.47(16) 4_445 2_565
O2 O2 Ga3 135.01(14) 1_554 2_565
O2 O2 Ga3 44.99(14) 1_556 2_565
O3 O2 Ga3 93.0(2) 3_564 2_565
O2 O2 Ga3 43.9(2) 5_445 2_565
O2 O2 Ga3 72.0(3) 5_455 2_565
O3 O2 Ga3 161.6(3) 1_454 2_565
O2 O2 Ga3 91.5(2) 2_465 2_565
O2 O2 Ga3 107.9(4) 2_454 2_565
O2 O2 Ga3 68.6(2) 2_564 2_565
La O2 Ga3 93.05(17) 2_564 2_565
O3 O2 Ga3 65.26(16) 2_565 2_565
Ga2 O2 Ga3 53.34(10) . 2_565
O3 O2 Ga3 51.84(16) 3_565 2_565
O3 O2 Ga3 103.6(2) 1_455 2_565
Nb O2 Ga3 32.48(7) . 2_565
Ga1 O2 Ga3 32.48(7) . 2_565
O3 O2 Ga3 41.27(15) 5 2_565
O3 O2 Ga3 85.4(2) 6_565 2_565
O3 O2 Ga3 161.7(3) 5_454 2_565
O3 O2 Ga3 152.4(4) 2_454 2_565
La O2 Ga3 133.5(3) 2_454 2_565
O2 O2 Ga3 122.5(2) 4_345 2_565
O2 O2 Ga3 131.8(2) 3_465 2_565
O1 O2 Ga3 119.3(3) 2_454 2_565
Ga3 O2 Ga3 88.24(17) 2_465 2_565
O2 O2 Ga3 106.8(3) 3_564 2_565
O2 O2 Ga3 122.0(3) 4_454 2_565
O2 O2 Ga3 18.28(13) 3_566 2_565
O2 O2 Ga3 44.82(13) 4_456 2_565
O2 O2 Ga3 70.0(2) 2_455 2_565
O2 O2 Ga3 18.29(14) 2_565 2_565
Ga2 O2 La 118.4(6) 2_565 4_445
Ga3 O2 La 87.7(5) . 4_445
La O2 La 34.4(2) . 4_445
O3 O2 La 124.4(3) 5_455 4_445
O2 O2 La 84.5(6) 3_565 4_445
O2 O2 La 141.5(6) 4_455 4_445
La O2 La 130.8(3) 4_455 4_445
O3 O2 La 69.7(3) 2_455 4_445
O1 O2 La 89.9(3) . 4_445
O2 O2 La 64.1(3) 6_554 4_445
O3 O2 La 120.1(4) 4_454 4_445
O1 O2 La 115.7(4) 1_554 4_445
O3 O2 La 92.2(3) 4_455 4_445
Nb O2 La 91.8(2) 1_455 4_445
Ga1 O2 La 91.8(2) 1_455 4_445
O1 O2 La 12.67(11) 2_455 4_445
Ga2 O2 La 34.88(12) 1_554 4_445
O2 O2 La 46.5(2) 6 4_445
O3 O2 La 38.7(2) 6 4_445
La O2 La 80.7(3) 1_554 4_445
Ga3 O2 La 128.7(2) 2_464 4_445
La O2 La 139.4(3) 4_454 4_445
Ga3 O2 La 74.5(2) 2_564 4_445
O3 O2 La 69.6(3) 1_554 4_445
La O2 La 100.7(2) 2_565 4_445
Ga3 O2 La 71.07(15) 1_556 4_445
Ga3 O2 La 151.6(3) 4_455 4_445
O3 O2 La 86.1(3) 3_454 4_445
Ga2 O2 La 83.83(17) 2_566 4_445
O3 O2 La 51.2(2) . 4_445
O2 O2 La 42.11(15) 5_444 4_445
O2 O2 La 167.7(4) 5_454 4_445
La O2 La 44.34(12) 2_455 4_445
O2 O2 La 149.23(12) 2_464 4_445
O3 O2 La 69.3(2) 3_455 4_445
O1 O2 La 153.3(3) 2_465 4_445
Nb O2 La 107.9(2) 1_454 4_445
Ga1 O2 La 107.9(2) 1_454 4_445
O3 O2 La 98.5(2) 6_455 4_445
Ga2 O2 La 168.5(2) 1_564 4_445
Ga3 O2 La 88.24(17) 4_345 4_445
Ga3 O2 La 38.70(11) 4_445 4_445
O2 O2 La 105.47(13) 1_554 4_445
O2 O2 La 74.53(13) 1_556 4_445
O3 O2 La 136.8(3) 3_564 4_445
O2 O2 La 24.08(9) 5_445 4_445
O2 O2 La 126.4(3) 5_455 4_445
O3 O2 La 116.0(2) 1_454 4_445
O2 O2 La 120.2(2) 2_465 4_445
O2 O2 La 44.2(2) 2_454 4_445
O2 O2 La 93.2(4) 2_564 4_445
La O2 La 113.9(3) 2_564 4_445
O3 O2 La 124.9(2) 2_565 4_445
Ga2 O2 La 34.82(8) . 4_445
O3 O2 La 116.4(2) 3_565 4_445
O3 O2 La 99.5(2) 1_455 4_445
Nb O2 La 47.61(12) . 4_445
Ga1 O2 La 47.61(12) . 4_445
O3 O2 La 66.5(2) 5 4_445
O3 O2 La 150.0(2) 6_565 4_445
O3 O2 La 122.4(3) 5_454 4_445
O3 O2 La 93.9(3) 2_454 4_445
La O2 La 69.91(17) 2_454 4_445
O2 O2 La 70.6(3) 4_345 4_445
O2 O2 La 128.1(2) 3_465 4_445
O1 O2 La 67.6(2) 2_454 4_445
Ga3 O2 La 102.40(15) 2_465 4_445
O2 O2 La 100.8(4) 3_564 4_445
O2 O2 La 127.7(3) 4_454 4_445
O2 O2 La 73.7(3) 3_566 4_445
O2 O2 La 98.30(16) 4_456 4_445
O2 O2 La 28.2(2) 2_455 4_445
O2 O2 La 79.5(3) 2_565 4_445
Ga3 O2 La 64.76(13) 2_565 4_445
Ga2 O2 O3 126.6(6) 2_565 5_456
Ga3 O2 O3 103.0(5) . 5_456
La O2 O3 74.7(3) . 5_456
O3 O2 O3 55.6(3) 5_455 5_456
O2 O2 O3 112.39(16) 3_565 5_456
O2 O2 O3 88.6(4) 4_455 5_456
La O2 O3 41.2(2) 4_455 5_456
O3 O2 O3 69.4(4) 2_455 5_456
O1 O2 O3 51.1(3) . 5_456
O2 O2 O3 131.8(4) 6_554 5_456
O3 O2 O3 113.7(5) 4_454 5_456
O1 O2 O3 150.1(4) 1_554 5_456
O3 O2 O3 8.68(18) 4_455 5_456
Nb O2 O3 41.57(19) 1_455 5_456
Ga1 O2 O3 41.57(19) 1_455 5_456
O1 O2 O3 91.2(3) 2_455 5_456
Ga2 O2 O3 117.2(2) 1_554 5_456
O2 O2 O3 45.6(3) 6 5_456
O3 O2 O3 111.0(3) 6 5_456
La O2 O3 169.0(3) 1_554 5_456
Ga3 O2 O3 76.5(3) 2_464 5_456
La O2 O3 124.1(4) 4_454 5_456
Ga3 O2 O3 128.6(2) 2_564 5_456
O3 O2 O3 149.8(3) 1_554 5_456
La O2 O3 84.4(2) 2_565 5_456
Ga3 O2 O3 21.08(13) 1_556 5_456
Ga3 O2 O3 96.9(3) 4_455 5_456
O3 O2 O3 103.5(3) 3_454 5_456
Ga2 O2 O3 40.68(15) 2_566 5_456
O3 O2 O3 79.0(2) . 5_456
O2 O2 O3 133.9(3) 5_444 5_456
O2 O2 O3 99.8(4) 5_454 5_456
La O2 O3 68.59(17) 2_455 5_456
O2 O2 O3 88.8(5) 2_464 5_456
O3 O2 O3 41.5(2) 3_455 5_456
O1 O2 O3 61.3(3) 2_465 5_456
Nb O2 O3 112.7(3) 1_454 5_456
Ga1 O2 O3 112.7(3) 1_454 5_456
O3 O2 O3 62.4(2) 6_455 5_456
Ga2 O2 O3 81.8(3) 1_564 5_456
Ga3 O2 O3 81.7(2) 4_345 5_456
Ga3 O2 O3 125.8(2) 4_445 5_456
O2 O2 O3 152.95(17) 1_554 5_456
O2 O2 O3 27.05(17) 1_556 5_456
O3 O2 O3 116.1(3) 3_564 5_456
O2 O2 O3 74.3(3) 5_445 5_456
O2 O2 O3 43.2(3) 5_455 5_456
O3 O2 O3 90.6(3) 1_454 5_456
O2 O2 O3 29.09(18) 2_465 5_456
O2 O2 O3 115.7(2) 2_454 5_456
O2 O2 O3 132.1(3) 2_564 5_456
La O2 O3 140.6(3) 2_564 5_456
O3 O2 O3 92.6(2) 2_565 5_456
Ga2 O2 O3 57.55(15) . 5_456
O3 O2 O3 65.2(2) 3_565 5_456
O3 O2 O3 33.4(2) 1_455 5_456
Nb O2 O3 99.93(19) . 5_456
Ga1 O2 O3 99.93(19) . 5_456
O3 O2 O3 112.2(2) 5 5_456
O3 O2 O3 79.7(3) 6_565 5_456
O3 O2 O3 122.5(4) 5_454 5_456
O3 O2 O3 130.0(2) 2_454 5_456
La O2 O3 121.27(19) 2_454 5_456
O2 O2 O3 76.45(14) 4_345 5_456
O2 O2 O3 62.96(17) 3_465 5_456
O1 O2 O3 145.2(2) 2_454 5_456
Ga3 O2 O3 17.40(12) 2_465 5_456
O2 O2 O3 164.5(4) 3_564 5_456
O2 O2 O3 140.2(4) 4_454 5_456
O2 O2 O3 53.43(14) 3_566 5_456
O2 O2 O3 37.7(2) 4_456 5_456
O2 O2 O3 67.1(3) 2_455 5_456
O2 O2 O3 79.9(3) 2_565 5_456
Ga3 O2 O3 71.05(16) 2_565 5_456
La O2 O3 92.13(17) 4_445 5_456
Ga2 O2 O3 60.4(5) 2_565 6_554
Ga3 O2 O3 79.8(5) . 6_554
La O2 O3 92.0(5) . 6_554
O3 O2 O3 135.1(4) 5_455 6_554
O2 O2 O3 64.2(4) 3_565 6_554
O2 O2 O3 100.2(4) 4_455 6_554
La O2 O3 150.2(3) 4_455 6_554
O3 O2 O3 107.5(5) 2_455 6_554
O1 O2 O3 124.3(4) . 6_554
O2 O2 O3 44.6(2) 6_554 6_554
O3 O2 O3 76.7(4) 4_454 6_554
O1 O2 O3 42.2(3) 1_554 6_554
O3 O2 O3 165.4(4) 4_455 6_554
Nb O2 O3 139.5(3) 1_455 6_554
Ga1 O2 O3 139.5(3) 1_455 6_554
O1 O2 O3 76.2(4) 2_455 6_554
Ga2 O2 O3 52.2(2) 1_554 6_554
O2 O2 O3 120.7(4) 6 6_554
O3 O2 O3 56.2(2) 6 6_554
La O2 O3 12.90(13) 1_554 6_554
Ga3 O2 O3 114.3(3) 2_464 6_554
La O2 O3 69.7(2) 4_454 6_554
Ga3 O2 O3 45.52(19) 2_564 6_554
O3 O2 O3 21.1(2) 1_554 6_554
La O2 O3 95.0(3) 2_565 6_554
Ga3 O2 O3 145.2(3) 1_556 6_554
Ga3 O2 O3 94.0(2) 4_455 6_554
O3 O2 O3 79.0(3) 3_454 6_554
Ga2 O2 O3 132.2(3) 2_566 6_554
O3 O2 O3 89.9(4) . 6_554
O2 O2 O3 33.0(3) 5_444 6_554
O2 O2 O3 93.7(3) 5_454 6_554
La O2 O3 102.2(3) 2_455 6_554
O2 O2 O3 104.4(4) 2_464 6_554
O3 O2 O3 131.6(4) 3_455 6_554
O1 O2 O3 132.4(3) 2_465 6_554
Nb O2 O3 75.2(2) 1_454 6_554
Ga1 O2 O3 75.2(2) 1_454 6_554
O3 O2 O3 121.7(3) 6_455 6_554
Ga2 O2 O3 112.2(2) 1_564 6_554
Ga3 O2 O3 100.5(2) 4_345 6_554
Ga3 O2 O3 40.46(17) 4_445 6_554
O2 O2 O3 39.09(16) 1_554 6_554
O2 O2 O3 140.91(16) 1_556 6_554
O3 O2 O3 73.9(2) 3_564 6_554
O2 O2 O3 91.7(3) 5_445 6_554
O2 O2 O3 145.3(3) 5_455 6_554
O3 O2 O3 98.0(2) 1_454 6_554
O2 O2 O3 164.8(3) 2_465 6_554
O2 O2 O3 56.1(3) 2_454 6_554
O2 O2 O3 48.0(3) 2_564 6_554
La O2 O3 47.85(19) 2_564 6_554
O3 O2 O3 92.8(2) 2_565 6_554
Ga2 O2 O3 108.6(3) . 6_554
O3 O2 O3 117.9(3) 3_565 6_554
O3 O2 O3 150.4(3) 1_455 6_554
Nb O2 O3 68.8(2) . 6_554
Ga1 O2 O3 68.8(2) . 6_554
O3 O2 O3 60.0(2) 5 6_554
O3 O2 O3 110.7(3) 6_565 6_554
O3 O2 O3 69.0(3) 5_454 6_554
O3 O2 O3 55.7(2) 2_454 6_554
La O2 O3 57.32(17) 2_454 6_554
O2 O2 O3 101.1(2) 4_345 6_554
O2 O2 O3 128.05(15) 3_465 6_554
O1 O2 O3 31.03(13) 2_454 6_554
Ga3 O2 O3 168.7(2) 2_465 6_554
O2 O2 O3 27.1(3) 3_564 6_554
O2 O2 O3 53.5(2) 4_454 6_554
O2 O2 O3 118.0(3) 3_566 6_554
O2 O2 O3 139.9(4) 4_456 6_554
O2 O2 O3 100.2(4) 2_455 6_554
O2 O2 O3 94.4(4) 2_565 6_554
Ga3 O2 O3 99.7(3) 2_565 6_554
La O2 O3 74.2(2) 4_445 6_554
O3 O2 O3 166.0(3) 5_456 6_554
Ga2 O2 O3 144.9(5) 2_565 2_456
Ga3 O2 O3 94.4(4) . 2_456
La O2 O3 58.0(3) . 2_456
O3 O2 O3 69.2(3) 5_455 2_456
O2 O2 O3 114.6(2) 3_565 2_456
O2 O2 O3 112.0(3) 4_455 2_456
La O2 O3 66.7(2) 4_455 2_456
O3 O2 O3 55.4(3) 2_455 2_456
O1 O2 O3 60.9(3) . 2_456
O2 O2 O3 111.0(4) 6_554 2_456
O3 O2 O3 119.3(4) 4_454 2_456
O1 O2 O3 175.2(4) 1_554 2_456
O3 O2 O3 24.7(3) 4_455 2_456
Nb O2 O3 41.37(16) 1_455 2_456
Ga1 O2 O3 41.37(16) 1_455 2_456
O1 O2 O3 65.6(3) 2_455 2_456
Ga2 O2 O3 91.9(2) 1_554 2_456
O2 O2 O3 21.75(17) 6 2_456
O3 O2 O3 93.7(3) 6 2_456
La O2 O3 144.7(3) 1_554 2_456
Ga3 O2 O3 87.6(2) 2_464 2_456
La O2 O3 143.1(4) 4_454 2_456
Ga3 O2 O3 123.2(2) 2_564 2_456
O3 O2 O3 133.9(3) 1_554 2_456
La O2 O3 95.8(3) 2_565 2_456
Ga3 O2 O3 6.92(14) 1_556 2_456
Ga3 O2 O3 121.9(3) 4_455 2_456
O3 O2 O3 94.2(3) 3_454 2_456
Ga2 O2 O3 48.19(19) 2_566 2_456
O3 O2 O3 69.58(19) . 2_456
O2 O2 O3 108.6(3) 5_444 2_456
O2 O2 O3 124.6(4) 5_454 2_456
La O2 O3 45.60(15) 2_455 2_456
O2 O2 O3 106.2(4) 2_464 2_456
O3 O2 O3 26.2(3) 3_455 2_456
O1 O2 O3 85.8(3) 2_465 2_456
Nb O2 O3 112.5(2) 1_454 2_456
Ga1 O2 O3 112.5(2) 1_454 2_456
O3 O2 O3 62.25(17) 6_455 2_456
Ga2 O2 O3 104.9(3) 1_564 2_456
Ga3 O2 O3 74.89(19) 4_345 2_456
Ga3 O2 O3 104.2(2) 4_445 2_456
O2 O2 O3 152.68(17) 1_554 2_456
O2 O2 O3 27.32(17) 1_556 2_456
O3 O2 O3 140.0(3) 3_564 2_456
O2 O2 O3 53.4(2) 5_445 2_456
O2 O2 O3 67.8(4) 5_455 2_456
O3 O2 O3 95.0(3) 1_454 2_456
O2 O2 O3 52.6(2) 2_465 2_456
O2 O2 O3 91.9(2) 2_454 2_456
O2 O2 O3 136.4(3) 2_564 2_456
La O2 O3 158.6(3) 2_564 2_456
O3 O2 O3 112.0(3) 2_565 2_456
Ga2 O2 O3 34.26(11) . 2_456
O3 O2 O3 83.8(3) 3_565 2_456
O3 O2 O3 40.6(2) 1_455 2_456
Nb O2 O3 87.80(17) . 2_456
Ga1 O2 O3 87.80(17) . 2_456
O3 O2 O3 106.2(3) 5 2_456
O3 O2 O3 104.5(3) 6_565 2_456
O3 O2 O3 130.0(2) 5_454 2_456
O3 O2 O3 121.9(3) 2_454 2_456
La O2 O3 104.0(2) 2_454 2_456
O2 O2 O3 62.69(17) 4_345 2_456
O2 O2 O3 76.33(12) 3_465 2_456
O1 O2 O3 122.9(2) 2_454 2_456
Ga3 O2 O3 35.52(12) 2_465 2_456
O2 O2 O3 168.3(4) 3_564 2_456
O2 O2 O3 163.6(4) 4_454 2_456
O2 O2 O3 54.77(18) 3_566 2_456
O2 O2 O3 53.4(2) 4_456 2_456
O2 O2 O3 41.5(2) 2_455 2_456
O2 O2 O3 82.8(3) 2_565 2_456
Ga3 O2 O3 67.77(17) 2_565 2_456
La O2 O3 67.54(14) 4_445 2_456
O3 O2 O3 25.58(17) 5_456 2_456
O3 O2 O3 141.6(3) 6_554 2_456
Ga2 O2 O2 95.9(7) 2_565 4_445
Ga3 O2 O2 94.2(4) . 4_445
La O2 O2 41.5(4) . 4_445
O3 O2 O2 145.7(3) 5_455 4_445
O2 O2 O2 66.7(8) 3_565 4_445
O2 O2 O2 126.7(8) 4_455 4_445
La O2 O2 144.4(3) 4_455 4_445
O3 O2 O2 88.5(3) 2_455 4_445
O1 O2 O2 93.7(4) . 4_445
O2 O2 O2 59.6(3) 6_554 4_445
O3 O2 O2 117.4(4) 4_454 4_445
O1 O2 O2 93.5(4) 1_554 4_445
O3 O2 O2 113.9(3) 4_455 4_445
Nb O2 O2 114.5(2) 1_455 4_445
Ga1 O2 O2 114.5(2) 1_455 4_445
O1 O2 O2 31.95(11) 2_455 4_445
Ga2 O2 O2 34.18(8) 1_554 4_445
O2 O2 O2 67.6(3) 6 4_445
O3 O2 O2 21.1(3) 6 4_445
La O2 O2 62.8(2) 1_554 4_445
Ga3 O2 O2 142.4(2) 2_464 4_445
La O2 O2 123.2(3) 4_454 4_445
Ga3 O2 O2 53.1(3) 2_564 4_445
O3 O2 O2 46.4(3) 1_554 4_445
La O2 O2 90.8(4) 2_565 4_445
Ga3 O2 O2 91.77(17) 1_556 4_445
Ga3 O2 O2 132.0(4) 4_455 4_445
O3 O2 O2 92.6(2) 3_454 4_445
Ga2 O2 O2 92.4(3) 2_566 4_445
O3 O2 O2 49.8(3) . 4_445
O2 O2 O2 26.2(3) 5_444 4_445
O2 O2 O2 144.7(4) 5_454 4_445
La O2 O2 65.77(11) 2_455 4_445
O2 O2 O2 152.1(3) 2_464 4_445
O3 O2 O2 92.4(2) 3_455 4_445
O1 O2 O2 169.5(2) 2_465 4_445
Nb O2 O2 108.18(16) 1_454 4_445
Ga1 O2 O2 108.18(16) 1_454 4_445
O3 O2 O2 117.6(3) 6_455 4_445
Ga2 O2 O2 165.8(2) 1_564 4_445
Ga3 O2 O2 102.28(17) 4_345 4_445
Ga3 O2 O2 15.46(14) 4_445 4_445
O2 O2 O2 90.0 1_554 4_445
O2 O2 O2 90.0 1_556 4_445
O3 O2 O2 114.3(4) 3_564 4_445
O2 O2 O2 38.2(2) 5_445 4_445
O2 O2 O2 135.7(3) 5_455 4_445
O3 O2 O2 124.5(2) 1_454 4_445
O2 O2 O2 141.31(19) 2_465 4_445
O2 O2 O2 46.40(17) 2_454 4_445
O2 O2 O2 71.2(5) 2_564 4_445
La O2 O2 90.6(3) 2_564 4_445
O3 O2 O2 110.2(4) 2_565 4_445
Ga2 O2 O2 55.20(14) . 4_445
O3 O2 O2 113.2(4) 3_565 4_445
O3 O2 O2 122.7(2) 1_455 4_445
Nb O2 O2 35.9(3) . 4_445
Ga1 O2 O2 35.9(3) . 4_445
O3 O2 O2 49.2(3) 5 4_445
O3 O2 O2 139.0(4) 6_565 4_445
O3 O2 O2 115.0(2) 5_454 4_445
O3 O2 O2 89.21(16) 2_454 4_445
La O2 O2 70.25(9) 2_454 4_445
O2 O2 O2 87.4(2) 4_345 4_445
O2 O2 O2 147.4(2) 3_465 4_445
O1 O2 O2 57.19(12) 2_454 4_445
Ga3 O2 O2 124.75(11) 2_465 4_445
O2 O2 O2 79.0(4) 3_564 4_445
O2 O2 O2 106.8(3) 4_454 4_445
O2 O2 O2 79.0(4) 3_566 4_445
O2 O2 O2 106.8(3) 4_456 4_445
O2 O2 O2 51.5(2) 2_455 4_445
O2 O2 O2 73.1(5) 2_565 4_445
Ga3 O2 O2 64.2(3) 2_565 4_445
La O2 O2 23.27(8) 4_445 4_445
O3 O2 O2 112.26(15) 5_456 4_445
O3 O2 O2 53.8(2) 6_554 4_445
O3 O2 O2 89.29(14) 2_456 4_445
Ga2 O2 O2 144.4(6) 2_565 3_455
Ga3 O2 O2 45.7(3) . 3_455
La O2 O2 74.5(3) . 3_455
O3 O2 O2 86.5(3) 5_455 3_455
O2 O2 O2 126.7(8) 3_565 3_455
O2 O2 O2 173.3(8) 4_455 3_455
La O2 O2 124.5(3) 4_455 3_455
O3 O2 O2 29.3(3) 2_455 3_455
O1 O2 O2 120.6(3) . 3_455
O2 O2 O2 44.8(4) 6_554 3_455
O3 O2 O2 81.4(3) 4_454 3_455
O1 O2 O2 118.6(3) 1_554 3_455
O3 O2 O2 82.4(3) 4_455 3_455
Nb O2 O2 61.1(2) 1_455 3_455
Ga1 O2 O2 61.1(2) 1_455 3_455
O1 O2 O2 31.95(11) 2_455 3_455
Ga2 O2 O2 34.18(7) 1_554 3_455
O2 O2 O2 57.7(4) 6 3_455
O3 O2 O2 80.5(3) 6 3_455
La O2 O2 80.63(16) 1_554 3_455
Ga3 O2 O2 84.7(3) 2_464 3_455
La O2 O2 112.43(19) 4_454 3_455
Ga3 O2 O2 111.4(3) 2_564 3_455
O3 O2 O2 94.2(3) 1_554 3_455
La O2 O2 144.3(3) 2_565 3_455
Ga3 O2 O2 72.99(17) 1_556 3_455
Ga3 O2 O2 161.8(3) 4_455 3_455
O3 O2 O2 44.3(2) 3_454 3_455
Ga2 O2 O2 109.15(13) 2_566 3_455
O3 O2 O2 93.9(3) . 3_455
O2 O2 O2 57.09(13) 5_444 3_455
O2 O2 O2 138.1(4) 5_454 3_455
La O2 O2 20.64(17) 2_455 3_455
O2 O2 O2 104.71(17) 2_464 3_455
O3 O2 O2 47.7(2) 3_455 3_455
O1 O2 O2 125.6(3) 2_465 3_455
Nb O2 O2 68.64(17) 1_454 3_455
Ga1 O2 O2 68.64(17) 1_454 3_455
O3 O2 O2 57.7(3) 6_455 3_455
Ga2 O2 O2 125.0(3) 1_564 3_455
Ga3 O2 O2 43.75(17) 4_345 3_455
Ga3 O2 O2 71.06(18) 4_445 3_455
O2 O2 O2 90.000(1) 1_554 3_455
O2 O2 O2 90.0 1_556 3_455
O3 O2 O2 153.4(2) 3_564 3_455
O2 O2 O2 61.57(12) 5_445 3_455
O2 O2 O2 130.7(4) 5_455 3_455
O3 O2 O2 71.6(2) 1_454 3_455
O2 O2 O2 102.95(15) 2_465 3_455
O2 O2 O2 27.8(2) 2_454 3_455
O2 O2 O2 126.4(5) 2_564 3_455
La O2 O2 131.0(2) 2_564 3_455
O3 O2 O2 169.5(3) 2_565 3_455
Ga2 O2 O2 55.20(14) . 3_455
O3 O2 O2 148.67(15) 3_565 3_455
O3 O2 O2 72.4(2) 1_455 3_455
Nb O2 O2 92.0(2) . 3_455
Ga1 O2 O2 92.0(2) . 3_455
O3 O2 O2 109.0(3) 5 3_455
O3 O2 O2 160.5(4) 6_565 3_455
O3 O2 O2 88.19(17) 5_454 3_455
O3 O2 O2 63.30(17) 2_454 3_455
La O2 O2 39.61(11) 2_454 3_455
O2 O2 O2 27.4(2) 4_345 3_455
O2 O2 O2 87.4(2) 3_465 3_455
O1 O2 O2 57.19(12) 2_454 3_455
Ga3 O2 O2 86.17(19) 2_465 3_455
O2 O2 O2 106.8(3) 3_564 3_455
O2 O2 O2 118.67(16) 4_454 3_455
O2 O2 O2 106.8(3) 3_566 3_455
O2 O2 O2 118.67(16) 4_456 3_455
O2 O2 O2 36.96(18) 2_455 3_455
O2 O2 O2 122.4(3) 2_565 3_455
Ga3 O2 O2 105.33(19) 2_565 3_455
La O2 O2 44.62(12) 4_445 3_455
O3 O2 O2 88.38(15) 5_456 3_455
O3 O2 O2 83.97(18) 6_554 3_455
O3 O2 O2 66.20(18) 2_456 3_455
O2 O2 O2 60.000(1) 4_445 3_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.375(10) 6
La O3 2.375(10) .
La O2 2.398(12) 6
La O2 2.398(12) .
La O1 2.516(5) 2_455
La O1 2.516(5) .
La O2 2.827(17) 5_445
La O2 2.827(17) 3_565
La Ga2 3.3733(14) .
La Ga2 3.3733(14) 2_565
La Nb 3.4604(9) .
La Ga1 3.4604(9) .
Ga1 O3 1.964(10) 4
Ga1 O3 1.964(10) .
Ga1 O3 1.964(10) 3
Ga1 O3 1.964(10) 2
Ga1 O3 1.964(10) 5
Ga1 O3 1.964(10) 6
Ga1 La 3.4604(9) 2
Ga1 La 3.4604(9) 4
Ga1 O2 3.557(13) 1_655
Ga1 O2 3.557(13) 4_445
Ga1 O2 3.557(13) 2_565
Ga2 O1 1.784(16) 2_456
Ga2 O2 1.812(10) 6
Ga2 O2 1.812(10) 2_455
Ga2 O2 1.812(10) 5_445
Ga2 O1 3.254(16) 2_455
Ga2 La 3.3732(14) 4_445
Ga2 La 3.3732(14) 2_455
Ga2 O3 3.425(9) 6_556
Ga2 O3 3.425(9) 5_446
Ga2 O3 3.425(9) 2_456
Ga2 La 3.5425(15) 4_446
Ga3 O3 1.812(10) 2_455
Ga3 O3 1.812(10) 4_454
Ga3 O2 1.830(10) .
Ga3 O2 1.830(10) 6_554
Ga3 O3 2.527(14) 3_454
Ga3 O3 2.527(14) 5_455
Ga3 Nb 3.1280(10) 1_454
Ga3 Nb 3.1280(10) 1_455
Ga3 O1 3.561(7) 1_554
Ga3 O1 3.561(7) 2_455
Ga3 O3 3.609(10) 6_455
Ga3 O3 3.609(10) 1_454
Nb O3 1.964(10) 4
Nb O3 1.964(10) .
Nb O3 1.964(10) 3
Nb O3 1.964(10) 2
Nb O3 1.964(10) 5
Nb O3 1.964(10) 6
Nb Ga3 3.1280(10) 4_445
Nb Ga3 3.1280(10) 4_446
Nb Ga3 3.1280(10) 2_565
Nb Ga3 3.1280(10) 2_564
Nb Ga3 3.1280(10) 1_656
Nb Ga3 3.1280(10) 1_655
O1 Ga2 1.784(16) 2_566
O1 La 2.516(5) 2_565
O1 La 2.516(5) 4_455
O1 O2 2.896(17) 3_565
O1 O2 2.896(18) .
O1 O2 2.896(17) 4_455
O1 O2 3.077(17) 3_566
O1 O2 3.077(17) 1_556
O1 O2 3.077(17) 4_456
O1 O3 3.133(10) .
O1 O3 3.133(10) 3_565
O1 O3 3.133(10) 4_455
O1 Ga2 3.254(16) 2_565
O1 Ga3 3.561(7) 1_556
O1 Ga3 3.561(7) 2_565
O1 Ga3 3.561(7) 4_456
O1 O2 3.544(14) 6
O1 O2 3.544(14) 5_455
O1 O2 3.544(14) 2_565
O1 O3 4.287(13) 6
O1 O3 4.287(13) 2_565
O1 O3 4.287(13) 5_455
O1 Ga3 4.611(11) 2_564
O1 Ga3 4.611(11) 4_455
O1 Ga1 4.691(3) 1_455
O1 Nb 4.691(3) 1_455
O1 Ga1 4.691(3) 1_565
O1 Nb 4.691(3) 1_565
O1 O2 4.746(17) 2_465
O1 O2 4.746(17) 5_445
O1 O2 4.746(17) 6_665
O1 O3 4.799(18) 6_556
O1 O3 4.799(18) 2_566
O1 O3 4.799(18) 5_456
O1 La 4.809(13) 1_556
O1 La 4.809(13) 2_566
O1 La 4.809(13) 4_456
O1 O3 4.844(17) 5
O1 O3 4.844(17) 2_455
O1 O3 4.844(17) 6_565
O1 Ga2 4.867(5) 1_665
O1 Ga2 4.867(5) 1_565
O1 O1 4.917(11) 2_565
O1 O1 4.917(11) 2_455
O1 O1 4.917(11) 2_465
O1 O1 5.0374 1_556
O1 O1 5.0374 1_554
O1 Ga3 5.244(5) 2_465
O1 Ga3 5.244(5) 4_446
O1 Ga3 5.244(5) 1_666
O1 O3 5.302(14) 5_556
O1 O3 5.302(14) 2_456
O1 O3 5.302(14) 6_566
O1 O3 5.317(12) 4
O1 O3 5.317(12) 3_455
O1 O3 5.317(12) 1_565
O1 O2 5.55(2) 6_554
O1 O2 5.55(2) 5_454
O1 O2 5.55(2) 2_564
O1 O3 5.623(15) 1_554
O1 O3 5.623(15) 4_454
O1 O3 5.623(15) 3_564
O1 O1 5.693(18) 2_566
O1 O1 5.693(18) 2_456
O1 O1 5.693(18) 2_466
O1 O3 5.775(11) 3
O1 O3 5.775(11) 4_565
O1 O3 5.775(11) 1_455
O1 La 5.829(2) 4
O1 La 5.829(2) 2_455
O1 La 5.829(2) 1_565
O1 O2 6.164(10) 6_565
O1 O2 6.164(10) 5
O1 O2 6.164(10) 2_455
O1 O3 6.226(17) 1_556
O3 Ga3 1.812(10) 2_565
O3 Ga3 2.527(14) 4_446
O3 O3 2.60(2) 6
O3 O3 2.684(16) 4
O3 O3 2.684(16) 3
O3 O2 2.78(2) 5_445
O3 O3 2.80(3) 6_556
O3 O2 2.807(16) 2_565
O3 O2 2.943(14) 3_566
O3 O3 3.18(3) 5
O3 O2 3.341(19) 3_565
O3 O3 3.34(2) 5_556
O3 Ga2 3.425(9) 2_566
O3 Ga3 3.609(10) 1_656
O3 La 3.731(14) 2_565
O3 O2 3.821(19) 6
O3 O3 3.875(19) 2
O3 Ga3 3.929(13) 2_564
O3 O3 4.01(2) 2_556
O3 Ga1 4.133(12) 1_556
O3 Nb 4.133(12) 1_556
O3 O2 4.201(19) 1_556
O3 La 4.246(13) 4
O3 O1 4.287(13) 2_455
O3 Ga3 4.305(10) 4_445
O3 La 4.343(12) 1_556
O3 O2 4.355(18) 4_446
O3 O2 4.488(16) .
O3 Ga2 4.545(12) 1_665
O3 La 4.637(12) 4_445
O3 O2 4.633(16) 4_445
O3 Ga2 4.766(12) 2_565
O3 O2 4.759(17) 6_655
O3 O1 4.799(18) 2_456
O3 Ga3 4.869(11) 1_556
O3 O1 4.844(17) 2_565
O3 La 4.880(10) 2
O3 Ga3 5.018(11) 1_655
O3 O3 5.0374 1_554
O3 O3 5.0374 1_556
O3 O2 5.095(14) 4_456
O3 O2 5.069(16) 1_656
O3 La 5.210(10) 2_566
O3 O2 5.314(17) 2_455
O3 O2 5.335(18) 4_455
O3 O1 5.302(14) 2_566
O3 O2 5.309(18) 1_655
O3 O1 5.317(12) 1_545
O3 O2 5.32(2) 5
O3 O3 5.392(17) 3_565
O3 O3 5.392(17) 4_455
O3 Ga2 5.376(10) 1_554
O3 O2 5.445(18) 6_665
O3 O2 5.432(15) 5_444
O3 O2 5.449(18) 2_564
O3 Ga2 5.494(13) 2_556
O3 La 5.541(10) 4_455
O3 La 5.590(10) 4_556
O3 O1 5.623(15) 1_556
O3 O3 5.708(7) 4_554
O3 O3 5.708(7) 3_554
O3 O3 5.708(7) 4_556
O3 O3 5.708(7) 3_556
O3 O1 5.775(11) 1_655
O3 La 5.892(15) 4_446
O3 O2 6.05(2) 5_446
O3 La 6.041(11) 2_455
O3 O3 6.074(16) 2_455
O3 O3 6.074(16) 2_565
O3 O2 6.034(18) 6_554
O3 O2 6.068(15) 2_566
O3 La 6.086(12) 2_556
O3 O3 6.161(15) 2_456
O3 O3 6.161(15) 2_566
O3 La 6.141(10) 1_655
O2 Ga2 1.812(10) 2_565
O2 O3 2.78(2) 5_455
O2 O2 2.779(17) 3_565
O2 O2 2.779(17) 4_455
O2 La 2.827(17) 4_455
O2 O3 2.807(16) 2_455
O2 O2 2.81(3) 6_554
O2 O3 2.943(14) 4_454
O2 O1 3.077(17) 1_554
O2 O3 3.341(19) 4_455
O2 Nb 3.557(13) 1_455
O2 Ga1 3.557(13) 1_455
O2 O1 3.544(14) 2_455
O2 Ga2 3.635(16) 1_554
O2 O2 3.74(2) 6
O2 O3 3.821(19) 6
O2 La 3.925(15) 1_554
O2 Ga3 4.110(14) 2_464
O2 La 4.201(10) 4_454
O2 Ga3 4.189(14) 2_564
O2 O3 4.200(19) 1_554
O2 La 4.255(10) 2_565
O2 Ga3 4.367(12) 1_556
O2 Ga3 4.392(12) 4_455
O2 O3 4.355(18) 3_454
O2 Ga2 4.491(12) 2_566
O2 O2 4.479(11) 5_444
O2 O2 4.479(11) 5_454
O2 La 4.507(10) 2_455
O2 O2 4.63(3) 2_464
O2 O3 4.633(16) 3_455
O2 O1 4.746(17) 2_465
O2 Nb 4.723(10) 1_454
O2 Ga1 4.723(10) 1_454
O2 O3 4.759(17) 6_455
O2 Ga2 4.814(15) 1_564
O2 Ga3 4.847(11) 4_345
O2 Ga3 4.914(17) 4_445
O2 O2 5.0374 1_554
O2 O2 5.0374 1_556
O2 O3 5.095(14) 3_564
O2 O2 5.111(14) 5_445
O2 O2 5.111(14) 5_455
O2 O3 5.069(16) 1_454
O2 O2 5.24(3) 2_465
O2 O2 5.19(2) 2_454
O2 O2 5.19(2) 2_564
O2 La 5.269(11) 2_564
O2 O3 5.314(17) 2_565
O2 O3 5.335(18) 3_565
O2 O3 5.310(18) 1_455
O2 O3 5.32(2) 5
O2 O3 5.445(18) 6_565
O2 O3 5.432(15) 5_454
O2 O3 5.449(18) 2_454
O2 La 5.474(13) 2_454
O2 O2 5.54(2) 4_345
O2 O2 5.54(2) 3_465
O2 O1 5.55(2) 2_454
O2 Ga3 5.710(16) 2_465
O2 O2 5.753(8) 3_564
O2 O2 5.753(8) 4_454
O2 O2 5.753(8) 3_566
O2 O2 5.753(8) 4_456
O2 O2 5.746(16) 2_455
O2 O2 5.746(16) 2_565
O2 Ga3 5.768(11) 2_565
O2 La 5.850(14) 4_445
O2 O3 6.05(2) 5_456
O2 O3 6.034(18) 6_554
O2 O3 6.068(15) 2_456
O2 O2 6.01(3) 4_445
O2 O2 6.01(3) 3_455
